Dental Materials and Their Selection - 3rd Ed. (2002) by William J. OBrien
DENTAL MATERIALS AND THEIR SELECTION - 3rd Ed. (2002)Front MatterTitle PageEdited byWilliam J. OBrien, PhD, FADMProfessor, Department of Biologic and Materials SciencesDirector, Biomaterials Graduate ProgramSchool of DentistryUniversity of MichiganAnn Arbor, Michigan Quintessence Publishing Co, IncChicago, Berlin, Tokyo, Copenhagen, London, Paris, Milan, Barcelona, Istanbul, SaoPaulo, New Dehli, Moscow, Prague, and WarsawLibrary of Congress Cataloging-in-Publication DataDental materials and their selection / edited by William J. OBrien.3rd ed.p.; cm.Includes bibliographical references and index.ISBN 0-86715-406-3 (hardback)1. Dental materials.[DNLM: 1. Dental Materials. WU 190 D4152 2002] I. OBrien, WilliamJ. (William Joseph), 1940-RK652.5. D454 2002617.695dc21 2002003731 2002 by Quintessence Publishing Co, IncQuintessence Publishing Co, Inc4350 Chandler DriveHanover Park, IL 60133www.quintpub.com
All rights reserved. This book or any part thereof may not be reproduced, stored in aretrieval system, or transmitted in any form or by any means, electronic, mechanical,photocopying, recording, or otherwise, without prior written permission of the publisher.Editor: Arinne DicksonProduction: Eric PrzybylskiPrinted in CanadaTable of Contents Contributors vii Acknowledgments ix Introduction x1 A Comparison of Metals, Ceramics, and Polymers 12 Physical Properties and Biocompatibility 123 Color and Appearance 244 Gypsum Products 375 Surface Phenomena and Adhesion to Tooth Structure 626 Polymers and Polymerization 747 Impression Materials 908 Polymeric Restorative Materials 1139 Dental Cements 13210 Abrasion, Polishing, and Bleaching 15611 Structure and Properties of Metals and Alloys 16512 Dental Amalgams 17513 Precious Metal Casting Alloys 19214 Alloys for Porcelain-Fused-to-Metal Restorations 20015 Dental Porcelain 21016 Base Metal Casting Alloys 22517 Casting 23918 Soldering, Welding, and Electroplating 249
19 High-Temperature Investments 25820 Waxes 26721 Orthodontic Wires 27122 Endodontic Materials 28723 Implant and Bone Augmentation Materials 294 Appendix A Tabulated Values of Physical and Mechanical Properties 309 Appendix B Biocompatibility Tests 391 Appendix C Periodic Chart of the Elements 393 Appendix D Units and Conversion Factors 394 Appendix E Answers to Study Questions 395ContributorsKenzo Asaoka, PhDProfessor and ChairDepartment of Dental EngineeringSchool of DentistryUniversity of TokushimaTokushima, JapanCh 19 High-Temperature InvestmentsRaymond L. Bertolotti, DDS, PhDClinical Professor of Restorative DentistrySchool of DentistryUniversity of CaliforniaSan Francisco, CaliforniaCh 14 Alloys for Porcelain-Fused-to-Metal RestorationsWilliam A. Brantley, PhDProfessorSection of Restorative Dentistry, Prosthodontics, and EndodonticsCollege of DentistryOhio State UniversityColumbus, OhioCh 21 Orthodontic WiresGordon Christensen, DDS, MSD, PhDSenior ConsultantClinical Research AssociatesProvo, UtahLongevity of Restorations
Richard G. Earnshaw, PhD, MDScHonorary AssociateFaculty of DentistryUniversity of SydneySydney, AustraliaCh 4 Gypsum ProductsGerald N. Glickman, DDS, MS, MBAProfessor and ChairmanDepartment of EndodonticsDirector, Graduate Program in EndodonticsSchool of DentistryUniversity of WashingtonSeattle, WashingtonCh 22 Endodontic MaterialsEugene F. Huget, BS, DDS, MSProfessorDepartment of Restorative DentistryCollege of DentistryUniversity of TennesseeMemphis, TennesseeCh 16 Base Metal Casting AlloysAbraham Jarjoura, DDSDepartment of Biologic and Materials SciencesSchool of DentistryUniversity of MichiganAnn Arbor, MichiganCh 22 Endodontic MaterialsDavid H. Kohn, PhDAssociate ProfessorDepartment of Biologic and Materials SciencesSchool of DentistryDepartment of Biomedical EngineeringSchool of EngineeringUniversity of MichiganAnn Arbor, MichiganCh 23 Implant and Bone Augmentation MaterialsJ. Rodway Mackert, Jr, DMD, PhDProfessor of Dental MaterialsDepartment of Oral RehabilitationSchool of DentistryMedical College of GeorgiaAugusta, GeorgiaCh 1 A Comparison of Metals, Ceramics, and PolymersCh 2 Physical Properties and Biocompatibility
Peter C. Moon, MS, PhDProfessor of Restorative DentistrySchool of DentistryMedical College of VirginiaVirginia Commonwealth UniversityRichmond, VirginiaCh 11 Structure and Properties of Metals and AlloysAnn-Marie L. Neme, DDS, MSAssociate ProfessorDepartment of Restorative DentistrySchool of DentistryUniversity of Detroit MercyDetroit, MichiganCh 8 Polymeric Restorative MaterialsOsamu Okuno, PhDProfessor and ChairDivision of Biomaterials ScienceGraduate School of DentistryTohoko UniversitySendai, JapanCh 19 High-Temperature InvestmentsStephen T. Rasmussen, PhDResearch AssociateDepartment of Biologic and Materials SciencesSchool of DentistryUniversity of MichiganAnn Arbor, MichiganCh 18 Soldering, Welding, and ElectroplatingDennis C. Smith, MSc, PhD, FRISProfessor EmeritusFaculty of DentistryUniversity of TorontoToronto, Ontario, CanadaCh 9 Dental CementsKenneth W. Stoffers, DMD, MSClinical Associate ProfessorDepartment of Cariology, Restorative Sciences, and EndodonticsSchool of DentistryUniversity of MichiganAnn Arbor, MichiganClinical Decision-Making ScenariosJohn A. Tesk, BS, MS, PhDCoordinatorBiomaterials Program Polymers DivisionNational Institute of Standards and TechnologyGaithersburg, Maryland
AcknowledgmentsI would like to thank the many contributors to the third edition who took the time andused their expertise to keep this book current in a field that has seen many changes inrecent years. Several contributors to the second edition are also recognized for theirvaluable contributions: Dr Pui L. Fan, Dr Evan H. Greener, Carole L. Groh, Dr Valerie A.Lee, and Dr Mathijs M. A. Vrijhoef.I appreciate the many people who contributed data to the biomaterials properties tables,especially Drs Hal OKray and Abe Jarjoura, who provided major additions to the data onrestorative and impression materials, respectively. Chris Jung contributed many excellentillustrations, and Elizabeth Rodriguiz was invaluable in preparing the manuscript. Finally,I want to acknowledge the staff at Quintessence for their expert assistance in helping meprepare the book for publication.IntroductionIn revising this book for a third edition, the current situation confronting academic dentalmaterials was considered. On one hand, dental materials is one of the most popularsubjects among those who pursue continuing education seminars and read the dentalliterature. On the other hand, most dental students think of dental materials as a basicscience course, filled with facts and concepts that have little application to clinicaldentistry. A perusal of current dental textbooks on restorative dentistry andprosthodontics reveals that such texts cover much of the subject matter formerly taughtonly in dental materials courses. This sign of our success in integrating dental materialsinto dental education and research is also a sign that the dental materials curriculum mustcontinue to evolve to maintain its vital position as an intellectual leader in dentaleducation. More and more of the traditional approach simply will not do for this thirdedition. Instead, we must seize the opportunity to move the field of dental materialseducation forward to tackle two major challenges in dentistry: the proliferation ofproducts and techniques and the information explosion in science and technology. Therecent proliferation of dental products may lead to improved patient care, but keeping upwith the new technology is a challenge to dental materials specialists and educators.Dental materials textbooks have evolved significantly over the past century. An earlytextbook on dental materials provided recipes for a handful of materials (three cements,amalgam alloys, gold foil, vulcanized rubber, and gold casting materials) and emphasizedformulation, techniques, and crude testing. Then came the research and developmentperiod, when dental materials properties were optimized by the dentist according to theresults of laboratory testing and ADA standards were developed. Dental materials havebeen further refined to offer simpler techniques for clinicians and to meet the increasingesthetic demands of middle-class patients in developed countries.Another dimension to proliferation is the large number of products and techniquesavailable for each type of material, which only intensifies the need for dentists to staycurrent with the literature. To ease this burden, publications such as Clinical ResearchAssociates Newsletter, Dental Advisor, and Reality compile new information and providemonthly updates for dental practitioners. Perhaps the greatest drawback of proliferation isthat many new materials are not sufficiently tested prior to full-scale marketing, therebyincreasing the risk of clinical failures.As a result of this product explosion, dental materials education has an opportunity to
become a more integral part of the overall curriculum, but to do so it must revise itsapproach to teaching. A long-standing problem is that dental materials courses aregrouped with basic sciences, which tends to encourage memorization of facts rather thanunderstanding of clinical application. A new approach (Fig 1)would be more pragmatic, integrating problem-based learning and evidence-baseddentistry with the traditional overview of clinical materials and materials scienceconcepts, which is still important. Table 1 Table 1 Longevity of Restorations Commonly Used in Dentistry Gordon J. Christensen, DDS, MSD, PhDMaterial /Estimated Indications Contraindications Strengths WeaknesseslongevityAmalgam, Incipient, Large intracoronal Good marginal Objectionablesilver /14 y moderate- restorations (cusp seal; strength; color; stains sized, and replacement); longevity; tooth; marginal some large endodontically manipulability; breakdown; lesions in treated teeth cariostatic alleged health adolescents activity challenges and adultsCast gold Large lesions; Adolescents; high Reproduces Time required(inlays, teeth caries activity; anatomy well; for placement;onlays, and requiring persons who object onlays and high fee; poorcrowns) / 20 additional to gold display crowns may esthetics;y strength; teeth increase strength thermal used in of tooth; sensitivity rebuilding or longevity; wears changing occlusally
occlusion similar to enamelCeramic Restoration of Heavy occlusal Esthetics; no Have onlycrowns /15 y teeth stress; bruxism; metal content moderate requiring fixed prosthesis strength; require good longer than three resin bonding for appearance teeth strength and moderate strengthCeramic Class 2 and 5 Teeth that are Esthetic May create toothinlays and locations grossly broken potential sensitivity ifonlays (fired where high down and require extremely high; bonding agentsor pressed) / esthetics is crowns properly etched are not used10 y desired tooth and properly; may restoration may fracture during increase strength service of tooth; onlays stronger than inlaysCompacted Initial Class 3 Periodontally Marginal Time-golds (gold and 5lesions unstable teeth; high integrity; consuming; poorfoil, for patients of caries activity; longevity estheticspowdered all ages persons who objectgold, mat to gold displaygold) / 24 yCompomer / Moderate to Occlusal stress; Moderate Color degrades10 y high caries locations where fluoride release; activity; color stability is easy to use repair of necessary crowns; pediatricGlass Class 1 and 2 Areas of high High fluoride Only fairionomer / 8 y High caries esthetic need; areas release esthetics; activity; of difficult moisture difficult and crown repairs control time- consuming to placeHybrid High caries Occlusal stress; High fluoride Somewhationomer / 10 activity; locations where release; tri- difficult to use;y repair of color stability is cured; sets in color degrades crowns; necessary dark pediatric Class 1 and 2Porcelain- Teeth that Heavy occlusal Strength; good Appearance notfused-to- require full stress; bruxism marginal fit; as good as somemetal crowns coverage and acceptable to others; possible/ 20 y are subject to excellent wear of opposing heavy esthetic result teeth occlusal forces; fixed prosthesisResin Class 1 and 2 Bruxers and Esthetics; may Wear of
edition incorporates the hierarchy of evidence as a tool for material selection.The level of evidence needed to evaluate a new material or technology depends on thelevel of innovation or the level of risk as compared with the conventional material ortechnology. The higher the level of innovation and the greater the potential for harm orfinancial loss to the patient or dentist, the higher the standard for evidence. Materials andtechnology that are entirely new for a given application have the highest level ofinnovation and risk. For example, dentin etching for the purpose of bonding compositematerials to dentin was highly innovative and had many risks when it was firstintroduced. The next, lower level of innovation includes major product changes in aconventional material, such as with high-copper amalgam alloys in the 1970s or hybridionomer cements in the 1990s. Decreasing levels of innovation and risk include minorproduct improvements (eg, more shades for a resin restorative material). The majority of"new products" fall into this category.Each category in the hierarchy of evidence is described below.Large-scale, long-term clinical trialsA well-designed clinical trial will have a clearly stated hypothesis about the clinicalperformance of a new material when compared with a control material. It will have alarge number of subjects to be sufficiently definitive. A good design will also reducesubjectivity by using methods such as calibration of observers, double-blind procedures,and randomization, and the institutional review board of the organization will protect thestudy participants. These studies are indicated for adoption of brand new innovations andmajor product changes.Other clinical studiesOther types of clinical study generally are not as decisive as full clinical trials, but theynevertheless provide valuable information. A cohort study would follow a group ofpatients who receive biomaterials, for instance, and record successes and failures relatedto their characteristics. Follow-up studies evaluate product longevity and causes of failurein patients who are treated in a clinic. A significant finding might be one in which aresearcher discovers a high failure rate of a new biomaterial as patients return forreplacement within a short period of time. Short-term clinical studies performed for newdental restorative materials by manufacturers are common and useful, but they miss long-term effects and less frequent problems that are usually only evident in larger groups ofpatients. Studies in this category are indicated for product improvements and newtechniques.Animal experimentsSeveral of the biocompatibility tests for new materials involve animal testing. Animaltests are valuable, but they are often difficult to interpret. Cytotoxicity screening testswith cell cultures will detect gross toxicity of a material, but subtle effects require expertinterpretation. Animal tests are required for new compositions or techniques withquestionable biocompatibility.Physical properties dataThe publication of physical properties data on new biomaterials is essential for predicting
successful performance, as compared with a standard material. However, since conditionsin the body are highly complex, data from laboratory tests cannot always be extrapolatedto clinical performance. For example, a new material may be strong when tested in thelaboratory, but it may deteriorate more rapidly in body fluids and thus may not be animprovement when compared with a standard material. It is important to evaluate allapplicable physical properties of a new material alongside its clinical trials. Physicalproperties data are usually necessary for minor improvements in materials, but they areinsufficient for products with a higher level of innovation.In vitro experimentsThe biomaterials literature has many examples of laboratory experiments designed tosimulate the clinical situation. For instance, the wear resistance of biomaterials is oftenassessed with toothbrushing machines that use thousands of cycles to simulate years ofdaily brushing. Although useful, these experiments are tricky to interpret. In one suchstudy using a toothbrushing test, a new porcelain glaze was reported to be more resistantto wear than the current glazes. It was later disclosed that no dentifrice had been used.Thermocycling, marginal leakage, adhesion testing, and corrosion testing are a fewexamples of in vitro tests. They are useful for all new products and techniques.Deductions from clinical experiments and scientific theoriesDeductive reasoning is frequently used to support the superiority of new materials, but itcan be unreliable without supporting data. One example is the conclusion that the cariesrate will be reduced when fluoride-containing materials are used. Original clinicalresearch on fluoride-containing silicate cements reported that these materials wereassociated with a low caries rate. The deduction that other fluoride-containing restorativematerials provide equal caries protection is often unsupported by clinical data. Anotherexample is the claim that a new high-strength ceramic will have a low clinical failure ratefor posterior crowns. It may be strong, but dental laboratory fabrication and the oralenvironment may contribute to clinical failure. This type of evidence is useful duringproduct development, but very speculative for new products.Product literature from the manufacturerThere are too many fallacies and extreme claims in dental advertising for this to be areliable source of evidence. Advertisements that provide references to the publishedliterature are more reliable than those that do not cite published studies.Popular media, rumors, and mythsNone of these is reliable.Recommended ReadingNiederman R, Badovinac R (l999). Tradition-based dental care and evidence-based dentalcare. J Dent Res 78:1288-1291.Sackett DL, Straus SE, Richardson WS, Rosenberg W, Haynes RB (2000). Evidence-Based Medicine: How to Practice and Teach EBM (ed 2). New York: Churchill-Livingstone.
influence their selection for use in dentistry. For example, metals are inherently strong, ingeneral, and have good stiffness (modulus of elasticity). These properties would tend torecommend them as restorative materials. On the other hand, metals conduct heat rapidlyand are opaque (nonesthetic), limiting their usefulness in restorative dentistry. Ceramicsand polymers are thermally insulating and tend to be more translucent. Hence, thesematerials insulate the pulp from extremes of heat and cold and offer the potential of morelifelike esthetics. They tend to have lower toughness than metals, however, and polymershave much lower strength.Because no one class of materials possesses all the desired properties, it is not surprisingthat materials tend to be used in combination. The porcelain-fused-to-metal restorationcombines the strength and ductility of metal with the esthetics of dental porcelain. Aceramic or polymer base is used to insulate the pulp from a thermal-conductive metallicrestoration. A high thermal-expansion, low-strength, low-elastic-modulus polymer isreinforced with a low thermally expanding, high-strength, high-elastic-modulus ceramicfiller to form a dental resin composite material. An understanding of the advantages andlimitations of the various types of materials enables us to make selections based on thebest compromise of desired properties versus inherent limitations.Predicted Versus Actual StrengthsIt is possible to predict the strength of a material from the strengths of the individualbonds between the atoms in the material. The values of strength obtained by such aprediction are typically 1 million to 3 million pounds per square inch (psi), or about 7 to21 GPa. Actual strengths of most materials are ten to 100 times lower.Why do materials fail to exhibit the strengths one would expect from the bonds betweenatoms? Why do ceramics break suddenly without yielding, whereas metals often yieldand distort to 120% or more of their original length before fracturing? Why are polymersso much weaker and more flexible than metals and ceramics? Why do metals conductheat and electricity, whereas polymers and ceramics do not? As will be seen in thischapter, many of the answers to these questions can be understood by knowing only a fewthings about the structures of these materials. There is one key concept, for example, thatwill not only explain the tendency for ceramics to be brittle, but will also explain all ofthe methods used to strengthen ceramics. Similarly, one key concept will explain whypolymers expand about ten times as much as metals or ceramics when heated the sameamount, why polymers are generally weak, why they are ten times more flexible thanmetals or ceramics, and why they tend to absorb water and other fluids.CeramicsIntroductionConsider a block of material as depicted in Fig 1-2(a)
Fig 1-2 Stress raisers and the effect of their shape on stress concentration. (a) If no stressraiser is present, the stress is constant across cross section A. (b) If a rounded notch ispresent, the stress is constant over most of the cross section. (c) As the notch becomessharper, the stress concentration becomes greater. If this block is stretched by applying a force, F, the stress at any point on cross section Ais the same as the average stress, ave. For example, if the cross-sectional dimensions ofthe block are 1/2 in 1/2 in = 1/4 in2 (1.27 cm 1.27 cm = 1.61 cm2), and a force of3,000 lb (13 kN) is applied, the average stress along cross section A is 12,000 psi (83MPa). However, if a semicircular groove were machined across one side of the block ofmaterial, as depicted in Fig 1-2(b), the stress at each point across a plane passing throughthis groove would not be the same as the average stress. The stress would be constantover most of the cross section, but near the groove, the stress would suddenly rise andreach a maximum right at the edge of the groove. This phenomenon occurs around anyirregularity in a block of material. The groove or other irregularity is called a stressraiser. The stress around a stress raiser can be many times higher than the average stressin the body. The amount of increased stress depends on the shape of the stress raiser. Forexample, if the stress raiser in our block of material were a sharp notch rather than asemicircular groove, the stress would increase greatly at the tip of the sharp notch (Fig 1-2(c)). As the tip of the notch becomes smaller (ie, the notch becomes sharper), the stressconcentration at the tip of the notch becomes greater.The minute scratches present on the surfaces of nearly all materials behave as sharpnotches whose tips are as narrow as the spacing between atoms in the material. Thus, the
Understanding the effect of stress concentration is the key to understanding the failure ofbrittle materials, such as ceramics, which influences their selection as dental materials anddictates the design of restorations fabricated from these materials.The tendency for ceramics to fail in a brittle manner at stresses that are far below thetheoretical strengths of these materials can be understood in light of the concept of stressconcentration at surface scratches and other defects. Most of the techniques forstrengthening ceramics can also be understood by virtue of this concept.* Actually, the exceeding of the theoretical strength of the material at the crack tip is anecessary but insufficient condition for crack propagation. The remaining conditioninvolves a balance between the surface energy required to form the two new surfaces ofthe crack, and the elastic strain energy arising from the applied stress. This is called theGriffith energy balance, discussion of which is beyond the scope of this book.Clinical applications of ceramicsCeramics are inherently brittle and must be used in such a way as to minimize the effectof this property. Ceramic restorations must not be subjected, for example, to large tensilestresses, to avoid catastrophic failure. A method for reducing the influence of thebrittleness of ceramics is to fuse them to a material of greater toughness (eg, metal), as isdone with porcelain-fused-to-metal (PFM) restorations. Ceramics also may be reinforcedwith dispersions of high-toughness materials, as is the case with the alumina (Al2O3)-reinforced porcelain used in porcelain jacket crowns.Fig 1-4 Brittle fracture (arrows) of ceramic (dental porcelain) due to mismatch in thecoefficient of thermal expansion between porcelain and metal. (Photo courtesy of R. P.OConnor, DMD.)Figure 1-4 shows brittle fractures that occurred in the porcelain of two PFM crowns dueto the mismatch in thermal expansion between the porcelain and metal.
MetalsEffect of ductility on stress concentrationAs discussed in the previous section, stress raisers at the surface of a material can causethe stress in a localized region around the tip of the stress raiser to reach the theoreticalstrength of the material. When this happens in a brittle material, a crack propagatesthrough the material, resulting in fracture (see the footnote on page 3). In a ductilematerial, something happens before the theoretical strength of the material is reached atthe tip of the stress raiser that accounts for the tremendous difference in behaviorbetween, for example, a glass and a metal. As discussed previously, the magnitude of thestress concentration at the tip of a notch, surface scratch, or other stress raiser isdetermined by the sharpness of the stress raiser. If a sharp notch or scratch is present inthe surface of a brittle material, the stress concentration around this notch would besomething like that shown in Fig 1-5(a).Fig 1-5 Rounding or blunting of stress raisers that occurs in ductile materials. Stressconcentration is self-limiting in ductile materials because the region under greatest stress,the tip of the sharp stress raiser (a), yields to round or blunt the stress raiser and lower thestress (b). If a stress raiser is present in a ductile metal, however, the material at the tip of the stressraiser deforms under stress so the sharp notch becomes a rounded groove, as shown in Fig
1-5(b). Because the tip of the stress raiser is now rounded rather than sharp, the stressconcentration at the tip of this stress raiser is much lower. There are two important factsto recognize in this process:1. As with brittle materials, the actual strengths of ductile materials are many times lessthan those predicted from strengths of bonds between atoms.2. Unlike the behavior around the notch in a brittle material, the stress concentrationblunts the sharp tip of the stress raiser, thus lowering the stress concentration effect.Mechanism of ductile behaviorWhat, then, is responsible for the ductile behavior of a metal? Consideration of what ishappening on an atomic level provides insights into the difference between brittlematerials and ductile ones. A schematic of the arrangement of atoms in a piece of metal isshown in Fig 1-6.Fig 1-6 Tensile stress on a piece of material can be considered stress normal (n)(perpendicular) to plane A-A, together with stress parallel (s) to plane A-A. The stressparallel to plane A-A tends to cause the atoms along the plane to slide (shear) past eachother.If this piece of metal is subjected to a tensile stress as shown, this stress can be resolvedinto two components when considered relative to the plane A-A. One component tends tomove the rows of atoms on either side of the plane A-A apart from each other, and the
other component tends to cause the planes to slide past one another along the plane A-A.The component of the stress that tends to cause the planes to slide past one another is theone that causes a material to deform plastically. Scientists are able to calculate, from thebond strengths between the atoms, the stresses that would be required to make one planeof atoms slide past another plane; these stresses are 100 or more times higher than thoseactually observed. If, however, the bonds were to break one at a time and re-formimmediately with the adjacent atom, one plane could move past the other at very lowstress levels.The mechanism of this process is shown in Fig 1-7.Fig 1-7 Figure 1-7 (a) through (f) show how the shearing stress can cause a dislocation to
pass through the network of atoms, breaking only one row of bonds at a time. For theatoms along plane A-A to slide past one another all at once would require enormousstress. The fact that metals yield to stresses much lower than expected is explained by thebreaking of only one row of bonds (perpendicular to the page) at a time. Figure 1-7 (a) through (f) show how, by breaking and re-forming bonds, an extra plane ofatoms can move along plane A-A until this "ripple" in the crystal lattice passescompletely through the material. Multiple repetitions of this process along many planessimilar to A-A allow a metal to yield to an applied stress without fracturing. This ripplein the lattice structure is called a dislocation, and it is responsible for the ductile behaviorof metals.Metals can be hardened and strengthened by a variety of treatments that make it moredifficult for dislocations to move through the metal lattice. Alloying, cold-working, andformation of second phases in a metal are all ways of impeding dislocation motion. Somecrystal structures of metals, such as intermetallic compounds, make it difficult fordislocations to move. The passage of a dislocation through the ordered structure of anintermetallic compound would result in an unfavorable atomic arrangement, sodislocations move only with difficulty.With metals, it is important to remember that their ability to yield without fracturing, aswell as all of the methods for making metals harder and stronger, is understandable inlight of the concept of dislocations in the metal structure.Other properties of metals, such as their electrical and thermal conductivity, can beunderstood as resulting from the metallic bond. In the metallic bond some of theelectrons are free to move rapidly through the lattice of metal ions. This unusual aspect ofthe metallic bond enables metals to conduct heat and electricity.The electronic structure of the metallic bond also accounts for the opacity of metals.Figure 1-8 illustrates the metallic bond with its lattice of positively charged metal ioncores and electrons that are free to move between the ion cores.
Fig 1-8 Representation of the metallic bond showing the metal ion cores surrounded byfree electrons. (After Lewis and Secker, 1965.)Dislocations in ceramic materials and in intermetallic compoundsWhy do ceramic materials not yield in the same manner as metals? The answer to thisquestion involves consideration of two types of ceramic materials:1. Amorphous materials (glasses)Glassy materials do not possess an orderedcrystalline structure as do metals. Therefore, dislocations of a crystalline lattice cannotexist in glassy materials. Thus, glasses have no mechanism for yielding without fracture.2. Crystalline ceramic materialsDislocations exist in crystalline ceramic materials, buttheir mobility is severely limited, because their movement would require that atoms oflike charge be brought adjacent to one another, as seen in Fig 1-9. The energy required todo this is so large that dislocations are essentially immobile in crystalline ceramicmaterials.Intermetallic compounds, unlike ordinary metal alloys, have a specific formula (eg,Ag3Sn, the main component of dental amalgam alloy powder) and an orderedarrangement of atoms. The movement of a dislocation through this ordered structurewould produce a disruption of the order similar to that shown in Fig 1-9 for crystallineceramic materials. Hence, dislocations move only with difficulty in intermetalliccompounds, and this property renders them more brittle than ordinary metal alloys.
Fig 1-9 The alternating charges of an ionic structure (crystalline ceramic) do not allowdislocations to move along plane A-A. If a dislocation were to pass through such astructure, it would result in ions of like charge coming into direct contact, which wouldrequire too much energy.Clinical applications of metalsMetals are generally ductile and tough when compared to ceramics, although a few typesof metals, such as dental amalgams, are markedly more brittle than others. This ductilityallows the margins of castings to be burnished, orthodontic wires to be bent, and partialdenture clasps to be adjusted. Figure 1-10 shows how the ductility of metal allows thewire clasp for a partial denture framework to be bent permanently to provide the desiredretention. The ductile behavior of the partial denture alloy can be contrasted with thebrittle behavior of the intermetallic material, dental amalgam, as shown in Fig 1-11.
Fig 1-10 Ductility of metal as illustrated by the adaptation (bending) of a partial denturewrought wire clasp.Fig 1-11 Brittle fracture of an amalgam post and core that had supported a PFM crown.Set dental amalgam is a mixture of several intermetallic compounds. Intermetalliccompounds tend to be brittle rather than ductile. (Photo courtesy of R. P. OConnor,DMD.)Polymers
IntroductionThe behavior of polymers is fundamentally different from both ceramics and metals. Tounderstand this difference, it is useful to consider the modulus of elasticity and thestrength of polymers at a molecular level.Modulus of elasticityWhen chains of polyethylene are aligned parallel to one another and are subjected to atensile stress along their long axes (Fig 1-12(a)), the stress required to stretch the atoms inthe chains farther apart is surprisingly high. In fact, the modulus of elasticity ofpolyethylene when measured in this way is 30 million psi, about the same as steel!However, if the applied stress is perpendicular to the long axes of the chains (Fig 1-12(b)), the modulus of elasticity is only about 0.5 million psi. The high modulus ofelasticity (30 million psi) in the first case results from the strong bonds between the atomswithin polymer chains. The low elastic modulus (0.5 million psi) in the second caseresults from the weak bonds between atoms in adjacent chains.Bulk polymers have their polymer molecules in a more random, tangled arrangement, andhence there are somewhat fewer secondary bonds between chains than when the chainsare perfectly aligned. The tangling and coiling of the polymer molecules make polymerseven more flexible, because of the lower stress required to straighten out a coiledmolecule compared to the stress necessary to stretch the atoms in a molecule farther apart.
Fig 1-12 (a) Strong (primary) bonds between atoms within a polymer chain result in ahigh stiffness (modulus of elasticity) when aligned chains are stretched along theirlengths. (b) Weak (hydrogen) bonds between atoms in adjacent chains result in a lowmodulus of elasticity when aligned chains are stretched perpendicular to their lengths.StrengthThe low strength of polymers when compared to ceramics and metals can also beunderstood in terms of the strong bonds within polymer chains and the weak bondsbetween polymer chains. If the rule-of-thumb value for theoretical strength, 0.1E, isapplied to the oriented polyethylene fiber shown in Fig 1-12(a), a value of 3 million psi isobtained for the theoretical strength of polyethylene. Typical bulk polymers, however,seldom have tensile strengths of more than 10,000 psi. The weak secondary bondsbetween polymer chains allow these chains to slide past one another at much lowerstresses than those required to break the bonds within the chains.Thermal expansionThe increase of the temperature of a material as the result of increased atomic vibrationwithin it is a familiar concept. This atomic vibration is limited by the bonds betweenatoms in a material such that when strong bonds are present between atoms, the atoms
vibrate over a small amplitude, and when weak bonds are present, the atoms vibrate overa large amplitude. Ceramics and metals are characterized by strong bonds between atoms,and the secondary bonds play an insignificant role in their properties. As a result, mostceramics and metals expand relatively little when heatedthat is, their coefficients ofthermal expansion are relatively low. Polymers, however, are characterized by strongbonds within polymer chains and weak bonds between polymer chains. Thus, thevibration of carbon atoms within the polymer chain is restricted in the directions parallelto the long axis of the chain, but the atoms are free to vibrate in the two directionsperpendicular to the long axis of the polymer chain. As a result, when a polymer isheated, the chains must move farther apart to allow for the larger-amplitude vibration,which occurs perpendicular to the long axes of the polymer chains. This phenomenonaccounts for the large coefficient of thermal expansion exhibited by polymers. Figure 1-13 illustrates the different thermal expansion behaviors of a polymeric material and acrystalline material.Fig 1-13 The different thermal expansion behaviors of a polymeric material and acrystalline material.Water absorptionBecause of the weak secondary bonds in polymer materials, water molecules are able topenetrate between the polymer chains in a process called water absorption. Waterabsorption has both positive and negative aspects. On the positive side, it is the mainfactor in correcting the 0.5% processing shrinkage that occurs during the fabrication ofheat-cured denture bases. When the acrylic polymer absorbs water, the polymermolecules are forced apart slightly, causing the denture base to expand. This expansionduring water absorption compensates for the processing shrinkage.On the negative side, water is responsible for the hydrolytic degradation of polymers. Inaddition, the ions carried by the water may cause the polymer to break down morequickly or to become stained or malodorous.Effect of cross-linking
Because many of the undesirable properties of polymers are due to weak bonds betweenpolymer chains, it would seem that a way to improve them would be to link chainstogether with primary chemical bonds. In fact, this method, called cross-linking, iswidely used to improve strength, resistance to water absorption, abrasion resistance, andother properties of polymers. Because of the small number of primary bonds in a givenvolume of polymer material as compared to ceramics or metals, however, polymerproperties remain generally inferior even with cross-linking.The key to understanding polymers is that the low strengths and elastic moduli ofpolymers, as well as many other distinctive properties, can be seen in light of the conceptof strong bonds within polymer chains and weak bonds between polymer chains.Clinical applications of polymersPolymers have had limited use as restorative materials by themselves because of their lowstrength and high thermal expansion. Some of the unfavorable properties of polymershave been mitigated by the incorporation of inorganic fillers to form composite materials.Modification of the polymer resins themselves to make them hydrophobic has improvedtheir resistance to water absorption. The properties of polymers may be further improvedby increasing their crystallinity, but the bonds between chains in crystalline polymers arestill only secondary bonds. The intrinsic weaknesses of polymers will probably continueto limit their use as restorative materials. The incisal fracture of a Class 4 microfilledcomposite restoration is shown in Fig 1-14. Microfilled resin composites tend to haveconsiderably lower levels of the stronger inorganic filler, and so the stresses are bornemore heavily by the weaker resin matrix. In Class 4 restorations, microfills generally haveinsufficient strength to withstand the stresses that may be encountered.Fig 1-14 Fracture of a Class 4 microfilled composite restoration. The low filler content ofmost microfills leaves the polymer matrix bearing the majority of the stress. Polymers aregenerally too weak for bearing large stresses. (Photo courtesy of C. D. Smith, DDS.)Glossaryalloy A material that exhibits metallic properties and is composed of one or moreelementsat least one of which is a metal. For example, steel is an alloy of iron and
carbon, brass is an alloy of copper and zinc, and bronze is an alloy of copper and tin.amorphous Literally, "without form." Atoms in crystalline solids exhibit an orderedarrangement, whereas atoms in amorphous solids lack this long-range periodicity.ceramic In the broadest sense, a compound of metallic and nonmetallic elements. By thisdefinition, materials ranging from aluminum oxide (Al2O3) to table salt (NaCl) areclassified as ceramics. In dentistry, gypsum (CaSO4 2H2O), many dental cements (eg,zinc phosphate), and porcelains are examples of ceramic materials.cross-linking A method for making a polymer stronger and more rigid by creatingchemical bonds between the molecular chains in the polymer.crystalline Having atoms or molecules arranged in a regular, repeating three-dimensionalpattern. Metals are nearly always crystalline; ceramics and polymers can be crystalline ornoncrystalline (amorphous).dislocation A defect in a crystal that is caused by an extra plane of atoms in the structure(see Fig 1-7). The movement of dislocations is responsible for the ability of metals tobend without breaking.intermetallic compound A chemical compound whose components are metals. Thegamma phase of amalgam, Ag3Sn, is an example of an intermetallic compound.metal A crystalline material that consists of positively charged ions in an ordered, closelypacked arrangement and bonded with a cloud of free electrons. This type of bond, called ametallic bond, is responsible for many of the properties of metalselectrical and thermalconductivity, metallic luster, and (usually) high strength.metallic bond One of the three types of primary (strong) chemical bond. (Ionic andcovalent are the other two.) Metallic bonds involve the sharing of valence electronsamong all atoms in the metal. Metallic bonds are responsible for many of the distinctiveproperties of metals, including electrical conductivity.modulus of elasticity A measure of the stiffness or flexibility of a material. A stiffmaterial has a high modulus of elasticity, and a flexible material has a low modulus ofelasticity. Also called Youngs modulus. (See chapter 2 for more detail.)polymer A material that is made up of repeating units, or mers. Most polymers are basedon a carbon (-C-C-C-C-) backbone in the polymer chain, although a silicone (-O-Si-O-Si-O-) backbone is important in many polymers.stress raiser An irregularity on the surface or in the interior of an object that causesapplied stress to concentrate in a localized area of the object. Other things being equal,the sharper the stress raiser, the greater the localized stress around it.water absorption The penetration of water into the structure of a material. Waterabsorption by polymers can help offset the effects of processing or polymerizationshrinkage (as in heat-processed denture bases), but it can also have detrimental effects,such as discoloration and leaching of unreacted components. For water to be absorbedinto the structure of a material, it must first be adsorbed onto the surface. Because bothphenomena occur when water is absorbed, the process is often referred to simply as water
Chapter 2. Physical Properties and BiocompatibilityIntroductionPhysical properties determine how materials respond to changes in their environments,and biocompatibility relates to the effect a material has on the tissue it contacts. Therelationships among the various properties are classified according to the scheme in Fig2-1.Fig 2-1 A tree diagram classifying physical properties.Mechanical PropertiesIntroductionThe concepts of stress, strain, modulus of elasticity, plastic deformation, and otherproperties were introduced in chapter 1. Because of the unfamiliarity and abstruse natureof many of these concepts, they will be discussed here in somewhat greater depth, andsome additional concepts will be introduced as necessary to understand the physical
behavior of materials.StressConsider again the block of material described in the previous chapter that was 1/2 in 1/2 in (1.27 cm 1.27 cm) in cross section and was subjected to a 3,000-lb (about 13 kN)load. As was pointed out in that example, the stress experienced by thatblockdetermined by dividing the force by the cross-sectional area of the blockis12,000 psi, or 83 MPa. Stress () is the force (F) divided by the cross-sectional area (A):Now consider a similar block, but with smaller dimensions1/4 in 1/4 in (about 0.6 cm 0.6 cm) in cross section (area of 1/16 in2, or about 0.4 cm2). If this new block issubjected to the same 3,000-lb (13-kN) tensile load, the stress in this case is 3,000 lb (13kN) divided by 1/16 in2 (about 0.4 cm2) = 48,000 psi (about 330 MPa).Thus, the usefulness of the concept of stress is apparent. It is not sufficient merely to statethe load or force that is being applied to a dental material, because the stress that isproduced in the material depends just as much on the cross-sectional area on which theload is acting as it does on the load itself. For instance, if the block that measured 1/4 in 1/4 in in cross section is subjected to a load of 12,000 lb (about 53 kN) instead of 3,000 lb(about 13 kN), the stress is 48,000 psi (about 330 MPa). If the cross-sectional area ismade 4 times smaller (1/4 as large), or if the load is made 4 times larger, the stress isincreased by a factor of 4. Thus, the stress is said to be inversely proportional to the cross-sectional area and directly proportional to the load.The basic types of stresses produced in dental structures under a force are tensile,compressive, and shear. All three are present in a beam loaded in the center. If the valueof these stresses exceeds the strength of the material, the structure will fail. It is thereforeimportant to know the strength values of materials. It is rare that an object will be subjectto the pure tensile, compressive, or shear stresses experienced by test specimens in amaterials testing laboratory. As shown in Fig 2-2, however, wherever bending forces arepresent, tensile stresses are present in critical areas, which could result in failure.
Fig 2-2 (a) Tensile stress (ST) at the isthmus of a two-surface amalgam restoration. (b)Tensile stress at the occlusal surface of a beveled amalgam restoration. (c) Tensile stressat the junctions of a partial denture clasp. (d) Tensile and compressive stresses (SC) in asoldering bridge. F = force; A = area. (From Mahler and Terkla, 1958. Reprinted withpermission.)StrainWhen a block of material is subjected to a tensile stress as described in the precedingsection, it temporarily becomes longer by a certain amount. This temporary increase inlength is called strain. A few examples will illustrate how strain is described. Considerthe block with the cross section of 1/4 in 1/4 in = 1/16 in2 (0.6 cm 0.6 cm = 0.4 cm2)and assume it has a length of 10 in (25.40 cm) when no load is applied. If the length ismeasured while the 3,000-lb (13-kN) load is being applied and the new length is 10.016in (25.441 cm), the strain is computed by dividing the increase in length (0.016 in, 0.041cm) by the original length (10.000 in, 25.40 cm) to obtain 0.0016. Strain is adimensionless quantity because we are dividing unit length by unit length, but sometimesit is written as "in/in" or "cm/cm." Strain can also be expressed in a percentage, in whichcase the dimensionless value is multiplied by 100%. In the given example, the strainwould be 0.16%.If a piece of the same material with the same cross section but 11 in (27.940 cm) long
were subjected to the same load (3,000 lb, about 13 kN), and the length of the block ofmaterial were measured while the load was being applied, it would be 11.0176 in(27.9847 cm). To compute the strain produced, the change in length (0.0176 in, 0.0447cm) is divided by the original length (11.0000 in, 27.9400 cm); the strain is determined tobe 0.0016 (or 0.16%), the same value obtained above for the block of material measuring10 in (25.4 cm). Thus, it can be seen that strain is independent of the length of thespecimen.Now consider a bar of high-strength steel, 1/4 in 1/4 in = 1/16 in2 (0.6 cm 0.6 cm =0.4 cm2) in cross section and 10 in (25.4 cm) long, that is capable of supporting a tensileload of 6,000 lb (about 27 kN). If the length of this bar were measured while under this6,000-lb (27-kN) load, it would be 10.032 in (25.4813 cm). If the strain is computed asbefore, the change in length (0.032 in, 0.0813 cm) divided by the original length (10.000in, 25.4 cm) is found to be 0.0032 or 0.32%. Hence, it can be seen that if the cross-sectional area of the block of material is kept the same and the applied load is doubled,the strain experienced by the material is doubled.ElasticityThe preceding examples showed that both stress and strain are directly proportional to theload applied when the cross-sectional area is kept the same. Hence, if the load is doubled,both the stress and the strain likewise will be doubled. It can be seen that the ratiobetween stress () and strain () is the same, thus:The property of having a constant ratio of stress to strain is called elasticity, and theconstant that is the ratio of stress to strain is called the modulus of elasticity. To gain aclearer understanding of the concept of elasticity and to see what it means for twomaterials to have different moduli of elasticity, it is helpful to consider the analogy of twosprings of different stiffnesses, as shown in Fig 2-3. Spring 2 is stiffer than spring 1;therefore, when they support equal weights, the stiffer spring is extended a smalleramount. Increasing the load from 1 lb (4.4 N) to 2 lb (8.9 N) causes each spring to extendtwice as much as it did under the 1-lb (4.4-N) load. Subjecting both springs to a 3-lb (13-N) load causes each one to extend 3 times as much as it did under a 1-lb (4.4-N) load, andso on. It can be seen that, irrespective of the load applied for either spring 1 or spring 2,the ratio of the extension to the load is a constant for that spring. However, the constantsfor the two springs are different. In this analogy, the extension of the spring correspondsto strain, the load or weight on the spring corresponds to stress, and the spring constantcorresponds to the modulus of elasticity.It is obvious that more weight cannot be added to a spring indefinitely and still have theextension increase proportionately. At some point the spring will become "stretched out"and will not return to its original size when the weight is removed. In the same way, whena material is stressed above a certain point, stress is no longer proportional to strain. Thehighest stress at which stress is proportional to strain is called the elastic limit, or theproportional limit. Because this stress is difficult to determine precisely, as it wouldentail looking for an infinitely small deviation from proportionality, it is customary todesignate a certain permanent deformation or offset (usually 0.002, or 0.2%) and to reportthe yield strength of the material at this strain. Thus the terms "elastic limit" and"proportional limit" are synonymous, whereas "yield strength" has a slightly different
meaning. The yield strength of a material is always slightly higher than the elastic limit.If a material continues to have more and more weight applied to it, it will of courseeventually break. If the material is being stretched (tensile loading), the stress at breakageis called the ultimate tensile strength (UTS). When many metals are stressed above theirproportional limits, they undergo a process called work hardening, and actually becomestronger and harder. But with the increased strength provided by work hardening comesincreased brittleness. It is thus very important to avoid overdoing it when bending a wireor a partial denture clasptoo much bending of the metal back and forth will make itharder and more brittle.The modulus of elasticity is an inherent property of the material and cannot be alteredappreciably by heat treatment, work hardening, or any other kind of conditioning. Thisproperty is called structure insensitivity, because it is not sensitive to any alteration to thestructure (meaning the microstructure) of the material. The modulus of elasticity is one ofthe few properties that is not sensitive to any alteration of the structure of the material.The yield strength of a material, for example, is sensitive to work hardening and willincrease with increasing amounts of work hardening.Fig 2-3 The concept of modulus of elasticity using the analogy of springs. Spring 1 is aflexible spring, representing a material with a low modulus of elasticity. Spring 2 is a stiffspring, representing a material with a high modulus of elasticity. When the same load is
applied to both springs, they stretch different amounts. The weight applied to the spring isanalogous to the stress (), the amount the spring stretches is analogous to the strain (),and the stiffness of the spring is analogous to the modulus of elasticity (E).PlasticityWhen the elastic or proportional limit is exceeded in a material, it is said to exhibit plasticbehavior. (The term "plastic" means "moldable," but the term has come to be associatedwith polymers.) Materials that experience a large amount of plastic behavior orpermanent deformation are said to be ductile. Materials that undergo little or no plasticbehavior are said to be brittle. If stress is plotted against strain, with stress as the ordinate(y axis) and strain as the abscissa (x axis), a diagram such as the one in Fig 2-4 is theresult. It can be seen that stress is proportional to strength up to the elastic (orproportional) limit. Above this stress, stress and strain are no longer proportional. If amaterial is stressed into the plastic region or region of permanent deformation and thenthe stress is removed, the material will have a permanent set, or deformation. If stress iscontinuously increased, the material will undergo more and more plastic deformation andwill ultimately fracture. The highest stress achieved during this process is called theultimate tensile strength of the material, as mentioned previously. The total strain atfracture (elastic strain + plastic strain) is called the elongation. Elongation of metals isimportant in several situations in dentistry. When one is burnishing the margin of acrown, the property that most comes into play is the elongation, although the yieldstrength is also important. For example, gold alloys are generally easy to burnish becausethey have a lower yield strength. Nickel-chromium and cobalt-chromium alloys may haveadequate elongation for burnishing, but their yield strengths are so high that they makeburnishing difficult. Another example of the importance of elongation is the bending of apartial denture clasp to adjust the retention.The entire area under the stress-strain curve is a measure of the energy required tofracture the material, or its toughness. The area under only the elastic region of the stress-strain curve is a measure of the ability of the material to store elastic energy (the way acompressed spring does). This is called the resilience of the material.Tabulated data for (Youngs) modulus of elasticity, yield strength, ultimate tensilestrength, percent elongation, and other mechanical properties are listed in Appendix A.
Fig 2-4 Measurement of stress and strain on an object being stretched. In the regionlabeled "elastic deformation," stress is proportional to strain, whereas in the regionlabeled "plastic deformation," stress and strain are no longer proportional (strain increasesfaster than stress does). The highest stress at which stress and strain are still proportionalis called the proportional limit, and the maximum stress just before the object breaks iscalled the ultimate tensile strength. The total amount that the object stretches (ie, the totalstrain), which is the sum of the elastic deformation and the plastic deformation, is calledthe percent elongation.FatigueWhen materials are subjected to cycles of loading and unloading, as during mastication,they may fail due to fatigue at stresses below the ultimate tensile strength. Usually, smallcracks at the surface or within the material gradually grow larger upon cycling, andeventually the material fails. Fatigue curves, such as the one shown in Fig 2-5, show theexperimentally determined number of cycles to failure at different stress levels. Thehigher the stress placed on and off the material, the fewer the number of cycles untilfailure.
Fig 2-5 Fatigue curves for glass-filled resin composite restorative material. (Courtesy ofR. A. Draughn, PhD.)Viscous flowMany dental materials are in a fluid state when they are formed, and viscous flowphenomena are important considerations. Our understanding of the behavior ofimpression materials and amalgam involve viscoelastic phenomena. When shear stress-strain rate (flow rate) plots are obtained, they enable viscous materials to be classified inseveral ways. A newtonian fluid shows a constant viscosity, , which is independent ofstrain rate:where is the viscosity in poise, is the shear stress acting on the fluid, and is thestrain, or flow rate.Actual fluids differ from these in their flow responses to the level of stress applied. Plasticfluids (eg, putty) dont flow at all until a minimum stress is applied. Pseudoplastic fluids(eg, fluoride gels) show an instantaneous decrease in apparent viscosity or consistency(become more free-flowing) with increasing shear rate. Dilatant fluids (eg, fluid denturebase resins) show an increase in rigidity as more pressure is applied. Thixotropic fluids(eg, fluoride gels, house paints) flow more freely when vibrated, shaken, or stirred than ifallowed to sit undisturbed. Formulation of the various suspensions and gels used indentistry to impart one or more of these properties can make them easier to handle. Forexample, impression materials that do not run off impression trays but are less viscousunder pressure in a syringe have a definite advantage.Viscoelastic behaviorMany materials, including elastic impression materials, waxes, and even hardenedamalgam, show a combination of elasticity and viscous flow. Figure 2-6 is a model ofhow a viscoelastic material acts under stress, the so-called spring-and-dashpot (or Voigt)model. (A dashpot is an oil-filled cylinder with a loosely fitted pistonmost automobileshock absorbers are of a dashpot design.) As the model is stretched, the spring component
on the left stretches and the piston of the dashpot also moves through the viscous liquid.The strain under stress and after release of the stress is time-dependent. The straingradually builds up until the release of stress, and then it gradually goes back to zero asthe spring element returns to its original length but is dampened by the dashpot element.Elastic impression materials are viscoelastic; initially they are strained upon removalfrom the mouth and require a short period of time to recover before models or dies arepoured.Fig 2-6 (a) Voight model for viscoelastic behavior. (b) Response of (a) to stress. Strainincreases with time and decreases after force (F) is released at t1, but is slow due to thedamping effect of the dashpot or the elastic action of the spring element. (From OBrienand Ryge, 1978. Reprinted with permission.)HardnessThe resistance of a material to indentation or penetration is called hardness. Thetechnical definition of hardness varies little, if at all, from the familiar definition, with thepossible exception that the technical definition carries with it the connotation of a methodof measurement. Most of the methods for measuring hardness consist of making a dent inthe surface of a material with a specified force in a controlled and reproducible mannerand measuring the size of the dent. For the measurement methods discussed in thissection, as the hardness increases, the respective hardness number increases also. Forexample, Fig 2-7 indicates the relative positions of a variety of dental and other materialson a Knoop hardness scale ranging from soft on the left to hard on the right. The positionsof the different materials on the line indicate their relative hardnesses.Brinell hardness number (BHN)The indenter for the Brinell hardness test is a small, hardened steel ball, which is forcedinto the surface of a material under a specified load. This indentation process leaves around dent in the material, and hardness is determined by measuring the diameter of the
dent. Brinell hardness values for selected metals are listed in Appendix A.Vickers hardness number (VHN) or diamond pyramid hardness (DPH)The Vickers hardness indenter is a square, pyramid-shaped diamond, which leaves asquare, diamond-shaped indentation in the surface of the material being tested. Hardnessis determined by measuring the diagonals of the square and taking the average of the twodimensions. The Vickers hardness test is also called the diamond pyramid hardness test.The Brinell and Vickers hardness tests are both used to measure the hardness of dentalalloys, and hardness values on alloy packages are expressed in either Vickers or Brinellhardness numbers. To compare Vickers and Brinell numbers, use the followingrelationship:For example, if a package of casting alloy lists a Vickers hardness of 242 and you want tocompare it with a different brand that lists the Brinell hardness, you would divide theVHN by 1.05 to obtain a BHN of 230. Diamond pyramid (Vickers) hardness values forseveral types of materials are listed in Appendix A.Knoop hardness (KHN)The indenter for the Knoop hardness test is also made of a diamond, but its outline issomewhat different from the Vickers indenter; although it is diamond shaped, onediagonal is much longer than the other. Only the long diagonal is measured to determinethe Knoop hardness number. Knoop hardness numbers for a variety of materials are listedin Appendix A.Rockwell hardness (RA, RB, . . . RG)The Rockwell hardness test is used primarily for determining the hardnesses of steels andis the most widely used hardness test in the United States. The Vickers, Brinell, andKnoop hardness tests are more commonly used for dental materials, however. Rockwelluses different hardened steel balls or diamond cones and different loads. Eachcombination forms a specific Rockwell scale (A, B, and C scales are the most common).The different scales are used for materials of different hardness ranges.Shore A durometerThe Shore A hardness test is used to measure the hardness of rubbers and soft plastics.The Shore A scale is between 0 and 100 units, with complete penetration of the materialby the indenter yielding a value of 0, and no penetration yielding a value of 100. Shore Ahardness values for several polymeric materials are listed in Appendix A.
Fig 2-7 Relative hardnesses of a variety of dental materials and tooth substances.Thermal PropertiesHeat flow through a materialMetals tend to be good conductors of heat, and this property must be taken intoconsideration when placing metallic restorations. Dentin is a thermal insulator (poorconductor of heat); thus, when a sufficient thickness of dentin is present, the patient feelsno sensitivity to heat and cold through a metallic restoration. However, when only a thinlayer of dentin remains, some thermal protection must be provided for the pulp. A goodrule of thumb in determining the thickness of cement base necessary in a given situationis to visualize how much dentin would have to be present in the excavation site so no basewould be necessary and then to apply base up to this level. The rate at which heat flowsthrough a material is expressed as thermal conductivity or thermal diffusivity. Thedifference between these two terms is described in the following subsections.Thermal conductivityThermal conductivity (k) is a measure of the speed at which heat travels (in calories persecond) through a given thickness of material (1 cm), when one side of the material ismaintained at a constant temperature that is 1C higher than the other side. Thermalconductivity is expressed in units of cal/cm sec C. Thermal conductivity values for avariety of materials are listed in Appendix A.Thermal diffusivityWhereas thermal conductivity gives an idea of the relative rates at which heat flowsthrough various materials, it fails to take into account the fact that various materialsrequire different amounts of heat (calories) to raise their temperatures an equal amount.For example, 1 gram of water requires 1.000 calorie to raise its temperature 1C, whereas1 gram of dentin requires only 0.28 calorie, and 1 gram of gold requires only 0.031calorie to produce a 1C temperature increase. Thus, thermal conductivity alone will nottell us, for instance, how rapidly the interior surface under a crown will heat up when theexterior surface is heated. To know how quickly the interior of the crown will approach
the temperature of the exterior, we need to know the thermal diffusivity of the alloy. Thethermal diffusivity (h) of a material (expressed in units of mm2/sec) is dependent on itsthermal conductivity, heat capacity (Cp), and density ():The relative thermal diffusivities of several dental materials are shown in Fig 2-8, andtabular data on a variety of materials are included in Appendix A.Fig 2-8 Thermal diffusivities of restorative materials.Thermal expansionThere are several situations in dentistry in which the thermal expansion of materials isimportant. Some restorative materials have coefficients of thermal expansion that aremarkedly different from tooth structure. In such cases, temperature fluctuations that occurin the mouth can cause percolation at the tooth-restoration interface as the restorationcontracts and expands. The porcelain and metal in a porcelain-fused-to-metal (PFM)restoration must contract at the same rate upon cooling from the porcelain firingtemperature if the buildup of large residual stresses is to be avoided. The cooling of adenture base from the processing temperature to room temperature is primarilyresponsible for the processing shrinkage that occurs. The thermal expansion behavior ofdental wax, gold alloy, investment, and so on are all important in producing properlyfitting castings. Figure 2-9 illustrates the relative values of linear coefficient of thermalexpansion for tooth, amalgam, composite, and acrylic resin. The diagram is onlyschematicthe expansion has been magnified to make it visible; the actual thermalexpansion would be too small to see. The thermal expansion coefficients, or the fractionalchanges in length per degree celsius, are given in parentheses. Tabular thermal expansiondata on a variety of materials are included in Appendix A.
Fig 2-9 Relative thermal expansions of several restorative materials and tooth structure.The relative amounts the materials expand when heated the same amount are representedby the dashed lines. The amount of expansion is magnified to make it visible forcomparison of the materials.Electrical and Electrochemical PropertiesElectrode potentialsAn electrochemical series is a listing of elements according to their tendency to gain orlose electrons in solution. The series is referenced versus the potential of a standardhydrogen electrode, which is arbitrarily assigned a value of 0.000 volts. If the elementsare listed according to the tendency of their atoms to lose electrons, the potentials aretermed oxidation potentials. If they are listed according to the tendency of their ions togain electrons, the potentials are termed reduction potentials. Reduction potentials at25C and 1 atmosphere of pressure are termed standard electrode potentials (Table 2-1). Table 2-1 Standard electrode potentialsHalf-reaction E0 (volts) +Li + e = Li -3.04K+ + e = K -2.93 2+Ca + 2e = Ca -2.87 +Na + e = Na -2.71Mg2+ + 2e = Mg -2.37 3+Al + 3e = Al -1.662 2+Zn + 2e = Zn -0.762Cr3+ + 3e = Cr -0.744Fe2+ + 2e = Fe -0.447 2+Ni + 2e = Ni -0.257Sn2+ + 2e = Sn -0.1375 2+Pb + 2e = Pb -0.1262 3+Fe + 3e = Fe -0.037H+ + e = H 0.000 (reference) 2+Cu + 2e = Cu +0.342
Cu+ + e = Cu +0.521Ag+ + e = Ag +0.800Hg2+ + 2e = Hg +0.851Pt2+ + 2e = Pt +1.118Au+ + e = Au +1.692Metals with a large positive electrode potential, such as platinum and gold, are moreresistant to oxidation and corrosion in the oral cavity. If there is a large differencebetween the electrode potentials of two metals in contact with the same solution, such asbetween gold and aluminum, an electrolytic cell may develop. If this occurs in the mouth,the patient may experience discomfort.The exact nature of tarnish and corrosion of restorative materials in vivo is extremelycomplex and involves much more than electrode potentials of materials. A possiblesource of the corrosion of gold alloys is accidental contamination of the surface withcopper during pickling, and subsequent tarnishing in saliva (Fig 2-10).Fig 2-10 Accidental plating of copper during pickling of gold casting. The model of thecell is formed by iron tongs and gold alloy (right). (From OBrien, 1962. Reprinted withpermission.)Electrical resistivityElectrical resistivity measures the resistance of a material to the flow of an electricalcurrent. The relationship between the resistance (R) in ohms, the resistivity (), the length(l), and the cross-sectional area (A) is as follows:Electrical resistivity values for several materials are given in Table 2-2. Table 2-2 Electrical resistivity of several materials
Material Resistivity (ohm-cm)Copper 1.7 10-6SiO2 (glass) > 1014Human enamel ~4 106Human dentin ~3 104Zinc phosphate cement 2 105Zinc oxide-eugenol 5 109 The low resistivity of metallic restorative materials is responsible for discomfort to thepulp if dissimilar metals generate a voltage. The insulating properties of cements help toreduce this problem.BiocompatibilityA material that is designed to be implanted in the body for the repair or replacement of adiseased or damaged tissue is called a biomaterial. Biomaterials must be biocompatible.All materials used in medicine and dentistry interact with tissues, producing changes inboth the materials and the surrounding tissues; there is no such thing as an "inert"material.Several factors affect the biocompatibility of a material. The chemical composition andstructure of the material affect the type and quantities of chemical species released. Therelative abundance of chemical species in a material will not reliably predict the amountsor even the proportions of the chemical species released. For this reason, thebiocompatibility of a material is usually determined empirically. The characteristics of thesite of use also affect a materials biocompatibility. For example, the presence of manyfactors in the oral environment affect the release of components from dental materials.Chemical factors, such as bacterial metabolic products, water, enzymes, and polar andnonpolar solvents, can accelerate the release of components. Mechanical factors in thesite of use can also affect the biocompatibility of a material. For example, under mostconditions, high-molecular-weight polyethylene elicits little if any tissue reaction whenimplanted. When it is used for the acetabular (socket) side of a total hip replacement,however, it can generate wear debris over time that produces an inflammatory responsethat eventually causes loosening of the prosthesis and failure of the implant.Evidence on a new product for use in the body must first be presented to governmentagencies that document possible adverse reactions the material might cause. Thisinformation includes the history of the material, its chemical composition, and resultsfrom a series of biocompatibility tests. A product that is a new version of an oldcomposition used successfully in similar applications may be classified under the FederalDrug Administration (FDA) classification of 510(k), which requires less extensive testingfor premarket approval. Another strategic qualification is whether the new product hastemporary or long-term contact with the body. The FDA has different categories formaterials with short-term contact, such as an impression material, than for materials usedfor long-term service, such as a cemented crown or an implant. The more potential forharm, the greater the burden of testing required. The testing required depends on manyfactors, including the results of initial minimal screening tests. A brief description ofthese tests is provided in Appendix B.Glossary
biocompatible A material is considered biocompatible if it does not produce harmful ortoxic reactions in the tissues it contacts or adverse systemic reactions as a result ofelements, ions, and/or compounds it releases.biomaterial A material that is designed to be implanted in the body for the repair orreplacement of a diseased or damaged tissue.brittle A material that tends to fracture without appreciable plastic deformation is said tobe brittle.compressive stress Two forces applied toward one another in the same straight line.ductility Ability of a material to be plastically strained in tension.elasticity Ability to sustain deformation without permanent change in size or shape.electrical resistivity Ability of a material to resist conduction of an electric current.elongation Overall deformation (elastic + plastic) as a result of tensile force application.fatigue Tendency to fracture under cyclic stresses.hardness Resistance to permanent indentation on the surface.linear coefficient of thermal expansion Change in length per unit original length for a1C temperature change.modulus of elasticity Stiffness of a material within the elastic range. Numerically, it isthe ratio of stress and strain.percolation The pumping of oral fluids in and out at the tooth-restoration interface as therestoration contracts and expands with temperature changes. Percolation occurs when thethermal expansion coefficient of the restoration is markedly different from that of toothstructure.proportional limit (elastic limit) The maximum stress at which the straight-linerelationship between stress and strain is valid.resilience Energy needed to deform a material to the proportional limit.shear stress Two forces applied toward one another but not in the same straight line.strain (nominal) Change in length per unit original length.stress (nominal) Force per unit area.tensile stress Two forces applied away from one another in the same straight line.thermal conductivity The quantity of heat passing through a material 1 cm thick with across section of 1 cm2, having a temperature difference of 1C.
thermal diffusivity Measure of the heat transfer of a material in the time-dependent state.toughness Amount of energy needed for fracture.ultimate tensile strength The maximum strength obtained based on the originaldimensions of the sample.viscoelastic Having both elastic and viscous properties.viscous Resistant to flow (referring to a fluid).work hardening The increase in strength and hardness, with accompanying decrease inductility, that occurs in a ductile metal as it is plastically deformed. Also called strainhardening.yield strength Strength measured at the stress at which a small amount of plastic strainoccurs. Also called yield point.Discussion Questions1. What is galvanic action in the mouth and how can it be minimized?2. Why is thermal diffusivity more relevant to insulation of the pulp than thermalconductivity?3. Explain why fixed partial dentures may fail under tensile stresses when under bitingforces that appear to be compressive?4. How is the leakage of oral fluids around a composite restoration related to thecoefficient of thermal expansion and temperature changes in the mouth?5. Why is time so important in the behavior of viscoelastic materials such as impressionmaterials and waxes?6. Why is there a hierarchy of biocompatibility tests?7. Why can biocompatibility tests be difficult to interpret?Study Questions(See Appendix E for answers.)1. Discuss why a knowledge and understanding of the physical and mechanical propertiesof biomaterials is important in dentistry.2. Explain why the thermal diffusivity of a material is more applicable to behavior in vivothan is its thermal conductivity.3. Draw and label a stress-strain diagram including the proportional limit, yield point, andultimate tensile strength.4. Define hardness and its relation to other mechanical properties.
5. Compare materials a and b on the basis of the two stress-strain curves below, obtainedby pulling the materials in tension.6. Why are laboratory biocompatibility tests run prior to clinical trials?Recommended ReadingASTM (1995). Practice for direct contact cell culture evaluation of materials for medicaldevices. Annual Book of ASTM Standards, 13.01, F813, 233-236.ASTM (1995). Standard test method for agar diffusion cell culture screening forcytotoxicity. Annual Book of ASTM Standards 13.01, F895, 247-250.Babich H, Borenfreund E (1987). Structure-activity relationship (SAR) modelsestablished in vitro with the neutral red cytotoxicity assay. Toxicol In Vitro 1:3-9.Billmeyer FW Jr (1984). Textbook of Polymer Science, ed 3. New York: John Wiley &Sons.Borenfreund E, Puerner JA (1987). Short-term quantitative in vitro cytotoxicity assayinvolving an S-9 activating system. Cancer Lett 34:243-248.Callister WD Jr (1999). Materials Science and Engineering: an introduction, ed 5. NewYork: John Wiley & Sons.Chappell RP, Spencer P, Eick JD (1994). The effects of current dentinal adhesives on thedentinal surface. Quintessence Int 25:851-859.Chiang Y-M, Birnie D III, Kingery WD (1997). Physical Ceramics. New York: JohnWiley & Sons.Dieter GE (1986). Mechanical Metallurgy, ed 3. New York: McGraw-Hill.Doremus RH (1994). Glass Science, ed 2. New York: John Wiley & Sons.
Ferracane JL, Condon JR (1990). Rate of elution of leachable components fromcomposites. Dent Mat 6:282-287.Hanks CT, Wataha JC, Sun Z (1996). In vitro models of biocompatibility: a review. DentMater 12:186-193.ISO (1992). "In vitro" method of test for cytotoxicity of medical and dental materials anddevices. Pforzheim, Germany: International Standards Organization, ISO/10993-5.Mahler DB, Terkla LG (1958). Analysis of stress in dental structures. Dent Clin NorthAm (Nov).OBrien WJ (1962). Electrochemical corrosion of gold alloys. Dent Abstracts 7:46.OBrien WJ, Ryge G (1978). Outline of Dental Materials. Philadelphia: WB Saunders.Rathbun MA, Craig RG, Hanks CT, Filisko FE (1991). Cytotoxicity of a bis-GMA dentalcomposite before and after leaching in organic solvents. J Biomed Mater Res 25:443-457.Ratner BD, et al (eds) (1996). Biomaterials Science: An Introduction to Materials inMedicine. San Diego: Academic Press.Reed-Hill RE, Abbaschian R (1991). Physical Metallurgy Principles. Boston: PWS-Kent.Tyas MJ (1977). A method for the in vitro toxicity testing of dental restorative materials.J Dent Res 56:1285-1290.Williams D (ed) (1990). Concise Encyclopedia of Medical and Dental Materials. Oxford:Pergamon Press. Chapter 3. Color and AppearanceIntroductionAmong the important factors that influence esthetic appearances of restorations are color,translucency, gloss, and fluorescence. Each of these factors, as perceived by an observersuch as a dentist, technician, or patient, is influenced by (1) the illuminant (light source),(2) the inherent optical parameters of the restorative materials that dictate the interactionof the light from the illuminant with the material, and (3) the interpretation of theobserver (Fig 3-1). An understanding of these factors in restorative materials, and properconsideration and communication of this information, will greatly assist the choice andfabrication of esthetic restorations.
Fig 3-1 Illuminant, object, and observer interaction.IlluminantIntroductionLight waves emitted from the illuminant interact with the object and are perceived by theobserver. The color content of the illuminant interacts with the object being perceived.The color content of the illuminant is the intensity of light emitted at each wavelength(spectral distribution). This is dependent on the type of illuminant. The wavelengths oflight are associated with hues, commonly referred to as color (Fig 3-2).Fig 3-2 Wavelength and hue. (Adapted from Billmeyer and Saltzman, 1960.)White light contains a mixture of wavelengths (colors). It is dispersed into componentswhen it passes through a prism, as shown in Fig 3-3.
Fig 3-3 Dispersion of white light by a prism.Different illuminants have different intensity distributions, or spectra, with respect towavelength, as illustrated in Figs 3-4a and 3-4b.Fig 3-4a Intensity distributions of illuminant A.
Fig 3-4b Intensity distributions of fluorescent light.Illuminants are sometimes described by their color temperature (in degrees Kelvin). Thisis based on the equivalence of the illuminant as compared to a radiating body with atemperature equal to the color temperature.The characteristics of an illuminant are important in color evaluation because the intensitydistribution, with respect to wavelength, identifies the light spectrum available to interactwith the object and then be perceived by the observer. In any color description the type ofilluminant used needs to be defined. Furthermore, the appropriate illuminant needs to beused in shade selection and shade matching. Illuminants that closely approximate daylightare preferred because color considerations for restorations, when seen under theseilluminants, are close to those seen under natural light. Several "daylight" sourcesintended for use in dental operatories are available. Representative spectral distributionsof some of these illuminants are shown in Figs 3-5a and 3-5b.
Fig 3-5a Spectral distribution of Neylite (J.M. Ney), a device used for dental shadematching.Fig 3-5b Spectral distribution of Vita-Lite (Duro Test), a fluorescent lamp for dentaloperatories.Color-rendering indexAnother parameter used in characterizing an illuminant is the color-rendering index.Color rendering of a light source is the effect that the source (illuminant) has on the colorappearance of objects in comparison with their color appearance under a reference source.The color-rendering index is a measure of the degree to which the illuminant can impartthe color of an object as compared to the reference source. A color-rendering index of 100is considered ideal. For an adequate color-matching environment, the illuminant shouldhave a color-rendering index of 90 or above (Preston et al, 1978). A summary of color-rendering indices of some illuminants used in dentistry is shown in Table 3-1. Table 3-1 Color-rendering indices of illuminantsIlluminant (manufacturer) Color-rendering indexChroma 50 (General Electric) 92Chroma 75 (General Electric) 94
Cool white (General Electric) 65Hanau Viewing Lamp (Teledyne Hanau) 93Neylite (J.M. Ney) 98Verilux (Verilux) 93Vita-Lite (Duro Test) 87, 91Surroundings in a dental operatory may modify the actual light reaching the object.Colors of walls, clothing, and soft tissues such as lips contribute to the color of the lightincident on teeth, shade guides, and restorative materials.ObjectIntroductionThe inherent color property of an object is its characteristic interactions with the lightfrom the illuminant. These interactions include reflection, transmission, and theabsorption involved in both processes.ReflectionA material gains its reflective color by reflecting that part of the spectrum of lightincident upon it and absorbing the other parts of the light spectrum. A blue surfacereflects only the blue part of the light spectrum and absorbs all other colors (Fig 3-6).Fig 3-6 Reflected color. A blue object reflects only blue light and absorbs all othercolors.A white object reflects all incident wavelengths. A black object absorbs all wavelengthsand reflects none. An object also appears black when no light is reflected from it; forexample, a blue object appears black when viewed in red light. Materials of differentreflected color have different color reflectance spectra (Fig 3-7). Reflection spectra ofobjects are usually obtained using a spectrophotometer.
Fig 3-7 Color reflectance of a blue object and a yellow object. (Adapted fromBillmeyer and Saltzman, 1960.)Mixing of reflected colorsTo obtain a desired esthetic appearance for a restoration, it is often necessary to use morethan one colorant. Each colorant has its own characteristic reflected color because of itsreflection spectrum and its absorption of other parts of the spectrum. The mixing of twocolorants with different reflected colors, and therefore different absorptions, results in areflection of the part or parts of the light spectrum common to both colorants. In otherwords, each colorant will absorb the part of the light spectrum as if it were by itself. Theparts of the light spectrum that are not absorbed by either colorant are, therefore, theresultant reflected color of the mixture of the two.TransmissionA translucent material gains its transmitted color by the resultant spectrum it transmits.As a beam of light passes through a translucent material (eg, glass), it can be changed bythe color of the material or scattered by fine particles, giving a milky appearance.Wavelengths that are not transmitted are absorbed. For example, a green filter transmitslight in the green wavelength region of the light spectrum and absorbs all otherwavelengths.ObserverThe observer receives the light reflected or transmitted by the object and then interpretsthe results. In many cases, the observer uses the human eye as the detector. Eye responsesvary among individuals. The human eye response varies with wavelength. It is mostsensitive in the green color region (Fig 3-8). The human eye is best in detecting colordifferences by comparison.
Fig 3-8 Relative response of a human eye at different wavelengths. (Adapted fromBillmeyer and Saltzman, 1960.)The detection of color by the human eye results from stimuli received by cone-shapedcells in the retina. Color blindnessthe inability to distinguish certain colorsis due toabnormalities in these cells. Constant stimulus of one color decreases the response of theeye to that color. This is sometimes known as color fatigue. After removal of thestimulus, a complementary color image may persist.Other detectors may be used as an observer in place of the human eye. These are usuallyphotodetectors, such as spectrophotometers or colorimeters. The response ofphotodetectors varies among types, and they differ from the response of the human eye.Color-measuring devices are designed to minimize the effect of photodetector responses.In color measurements and parametric color determinations, the CIE (CommissionInternationale de lEclairage) Standard Colorimetric Observer is often referenced.Color SystemsIntroductionColor systems are used to describe the color parameters of objects. The following areexamples of some color systems used in describing the color of dental materials.
Munsell color systemThe Munsell color system uses a three-dimensional system with hue, value, and chromaas coordinates (Fig 3-9).Fig 3-9 Munsell color system with hue, value, and chroma as coordinates.Hue is commonly referred to as color; examples are blue, yellow, and red. Hue is alsoassociated with the wavelengths of the light observed.Value is the lightness or darkness of a color. A tooth of low value appears gray andnonvital. Value is the most important color factor in tooth color matching.Chroma is a measurement of color intensity; that is, the amount of hue saturation in acolor. An example is a beaker of water containing one drop of colorant; it is lower inchroma than a beaker of water containing ten drops of the same colorant.CIE color systemsThe CIE tristimulus values system uses three parameters, X, Y, and Z, which are based onthe spectral response functions defined by the CIE observer. A CIE chromaticity diagramis also sometimes used to define color.Another CIE color system (CIE L*a*b*) uses the three parameters L*, a*, and b* todefine color. The L*, a*, and b* values can be calculated from the tristimulus X, Y, and Zvalues. The advantage of this color system is that its arrangement is an approximatelyuniform three-dimensional color space whose elements are equally spaced on the basis ofvisual color perception. A unit change in each of the three color parameters is
approximately equally perceived. The quality L* correlates to lightness, similar to valuein the Munsell system. The a* and b* coordinates describe the chromatic component (Fig3-10).Fig 3-10 CIE and Munsell color arrangements. (From Seghi et al, 1986. Reprintedwith permission.)The color difference, E*, in the CIE L*a*b* system is defined as:where L*, a*, and b* are the differences between the CIE L*a*b* color parameter oftwo samples. An advantage of E* is that it can serve as a tolerance for color matching.Clinical color matching between teeth and restorations may be rated according to E*values, as given in Table 3-2, based on clinical studies. Shade guides are held to atolerance of a E* of 1 according to an American Dental Association (ADA) standard.Although these E* values can serve as approximate tolerances, some individualsperceive color differences as low as 0.5, whereas others do not see differences of 4. Thisis often a source of disagreement among patients, dentists, and laboratory technicians.Color MeasurementsApart from visual comparison using color standards such as Munsell color chips, colormeasurements can be made using either spectrophotometric or colorimetric methods.Spectrophotometers measure the amount of light reflected at each wavelength. Adouble-beam spectrophotometer compares the responses from the object and a referencestandard. From the spectral response, color parameters for the object can be calculated.Spectrophotometric measurements have been used to evaluate the color parameters for
restorative resins, denture teeth, porcelains, shade guides, and color changes in dentalmaterials. Figure 3-11 shows one model of a spectrophotometer.Fig 3-11 Spectrophotometer for laboratory measurement of color parameters(Macbeth 7000, Gretag-Macbeth.)Colorimeters measure the amount of light reflected at selected colors (eg, red, green,blue). The selections are based on the CIE tristimulus value standard observers. There areseveral instruments available, and applications of their measurement methods for dentalmaterials have been reported (Powers et al, 1980; OBrien et al, 1983; Stanford et al,1985). The instruments give readings in tristimulus values (X, Y, Z) or CIE L*a*b*values.The major technical problem in using such instruments to measure the color parametersof teeth is the edge effect. Dental enamel is a translucent material that scatters theincident light from the instrument at many angles. As a result, the light reflected back intothe instrument for analysis is not reliable and presents major errors in shade selection.A new approach to tooth shade selection is the use of photography in combination with aspectrophotometer. Although accurate instrumental measurements of color parameters oftranslucent materials are difficult to use, color measurements on photographs are routine.This procedure of photocolorimetry involves the following steps:
1. The clinician or assistant holds the 3 or 4 closest-matching shade guide teeth next tothe patients teeth and photographs them with a 35-mm camera under a balanced lightsource (Fig 3-12).Fig 3-12 Photograph of patients teeth compared with the closest-matching shadeguide teeth.2. The photograph is sent to the dental laboratory along with the impression. Thelaboratory technician measures the color of the patients teeth and shade guide teeth in thephotograph. A computer program then aids in selecting the closest match.This approach has been tested in a clinical study (Groh et al, 1999) in comparison withvisual matching of 30 patients. The difference in color parameters between shadesselected by experienced observers and those selected by photocolorimetry resulted in aE* of 1.88, which is within the color tolerance of a E* of 2.00 for shade guide teeth. Inanother study (OBrien et al, 1983), the accuracy of matching one Vita shade guide wassignificantly higher with photocolorimetry than with visual matching by dental facultyand technicians.Several chairside colorimeters have been introduced in the past 3 years (Fig 3-13). Theseinstruments determine tooth shade by direct application to a patients tooth. Theiraccuracy is difficult to assess and depends on the angle at which the instrument ispositioned and other operator variables. A dental professional who can match shades well(eg, two shade guides at 90%) is still the standard, but technology is improving. Highprices of these instruments ($6,000 to $15,000) limit adoption.
Fig 3-13 Chairside colorimeter. The angle of instrument is controlled by the dentist.(Shade-Eye EX, Shofu; courtesy of Shofu.)MetamerismThe change in color matching of two objects under different light sources is calledmetamerism. Two objects that are matched under one light source but not under otherlight sources form a metameric pair (Fig 3-14). They have different color reflectancecurves. An example of metamerism is when a shade-guide tooth matches the tooth underfluorescent light but not under incandescent light. Metamerism results from possibledifferences in illumination between the dental clinic and the dental laboratory, causingpoor matching in a fabricated restoration, such as a porcelain crown.Standardization of illuminations (usually similar to the patients environment) in colormatching diminishes the effect of metamerism in shade matching. The ideal situation, ofcourse, is to have the objects possess the same color reflectance curve. The objects arethen an isomeric pair; they are color matched under all light sources.
Fig 3-14 Metamerism. Objects 1 and 2 match under light source A but do not matchunder light source B.TranslucencyThe translucency of an object is the amount of incident light transmitted and scattered bythat object. A high translucency gives a lighter color appearance. A more translucentmaterial will show more of the backing in the color and appearance. Translucencydecreases with increasing scattering within the material.The opposite of translucency is opacity. Light scattering in a material is the result ofscattering centers that cause the incident light to be scattered in all directions. Examplesof scattering centers are air bubbles and opacifiers such as titanium dioxide. Anotherexample is the filler particles in a resin composite matrix. The effect of scattering isdependent on the size, shape, and number of scattering centers. Scattering is alsodependent on the difference in refractive indices between the scattering centers and thematrix in which the centers are located.Measurements of translucency may be performed using transmission spectrophotometers,reflection spectrophotometers, light meters, or colorimeters. Measurements oftranslucency of dental porcelains and human enamel are published in the dental literature(Brodbelt et al, 1980; Brodbelt et al, 1981; OBrien et al, 1985; Spitzer and ten Bosch,1975).GlossSurface gloss is the optical property that produces a lustrous appearance. Contrast gloss,or luster, is the proportion of specular reflection to diffuse reflection (Fig 3-15). Anotherconsideration for gloss is the amount of collimated incident light that is specularlyreflected. In specular reflection, the angle of incidence is equal to the angle of reflectance.When the incident beam is scattered by the object, there is a decrease in gloss as a largerportion of the incident beam is diffuse-scattered.Gloss is an important appearance property of dental restorative materials. A high surfacegloss is usually associated with smooth surfaces. In resin composite, surface glossdecreases with increasing surface roughness. Differences in gloss between multiple
restorations or between restorations and teeth can be easily detected even in colors thatare matched. In addition, high gloss reduces the effect of a color difference, because thecolor of the reflected light is more prominent. In a restorative material, high gloss alsolightens the color appearance.Fig 3-15 Schematic diagram of diffuse and specular reflection. (a) High gloss; (b) lowgloss. (From OBrien et al, 1984. Reprinted with permission.)FluorescenceFluorescence is the emission of light by an object at wavelengths different from those ofthe incident light. The emission ceases immediately upon removal of the incident light.Natural teeth fluoresce in the blue region when illuminated by ultraviolet light. Dentalporcelains are also fluorescent under ultraviolet light. The quality of the fluorescencedepends on the brand of porcelain, some of which fluoresce in colors different from thoseof natural teeth.Double Layer Effects on EstheticsThe color of a tooth is strongly influenced by the thickness of the enamel and the color ofthe underlying dentin. Similar considerations apply to restorations that are of layeredstructure. Examples are porcelain restorations that are composed of body porcelain overan inner opaque porcelain (Fig 3-16) and resin composites over more opaque resins. Inthese layered structures, esthetic appearances are no longer simple considerations of thefactors previously described but also involve diffuse reflectance and the relation betweenthe translucency and thickness of the outer layer and the color and reflectance of the innerlayer. The outer translucent layer acts as a light-scattering filter over the inner layer (Fig3-17). As the thickness of the outer layer increases, the effect of the inner layer isdiminished. Similar situations also exist when the translucency of the outer layerdecreases. Considerations of models of diffuse reflectance in dental porcelain systemsusing the Kubelka-Munk equation have shown excellent agreement betweenexperimentally observed and theoretically calculated color parameters (OBrien et al,1985; Ragain and Johnston, 2001).
Fig 3-16 Optical considerations for a porcelain-fused-to-metal restoration. (FromOBrien et al, 1985. Reprinted with permission.)Fig 3-17 Double layer effect. (From OBrien, 1985. Modified with permission.)
Dental Shade GuidesShade guides are used in determining the color of natural teeth so that artificial substituterestorations will possess similar color and esthetics. Preferred properties in a shade guideinclude logical arrangements and adequate distribution in color space, matching withnatural teeth, inherent consistency among shade guides, and matching between shadeguides and the dental materials such as porcelains and resin composites or denture teeth.Not all these properties are met by the shade guides currently available. Furthermore, notall shade guides are fabricated from the dental materials to which they will be matched.Most shade guides use a designation to denote the shade and color. The same designationmay not be comparable among brands. The distribution of shades within a shade guide isnot necessarily evenly partitioned in color space. Some attempts have been made to use amore logical approach and an even distribution in shade guides, but only a limitednumber follow this approach. Recently a new shade guide (Vita 3D Guide, Vita) has beenintroduced that is based on hue, value, and chroma in a logical arrangement.Shade Matching in the Dental OperatoryShade matching is a complex situation. It is important to remember the triadic interactionsof illuminant, object, and observer described previously. Considerations should alsoinclude metamerism, gloss, translucency, and fluorescence. Recognition of the factorsinfluencing shade match improve the result of the match.The most important factor in shade matching is the illuminant. This is the lighting in thedental operatory used in shade matching. A color-corrected light source with a colortemperature of 5,500 K and a color-rendering index of 90 or above is recommended. Ifpossible, the shade matching should also be checked under a different light condition, forexample, a warm white fluorescent light. In cases where the patients may have specificrequirements, such as extensive activity under certain lighting conditions, shade-matchingchecks under those conditions are also recommended. The color environment of thedental operatory is another important factor in shade matching. A neutral, light graybackground color reduces modification of color perception.Some recommendations in shade matching are as follows:1. Shade match under lights of similar spectral distribution and intensity, both in thedental operatory and the laboratory. Lighting conditions should be similar to daylight. Adental ring light is one such option (Fig 3-18).
Fig 3-18 Ring light to simulate daylight for shade matching (EFOS).2. Consider the effects of translucency and position. A high translucency and a moredistal position in the natural dentition cause a darker gray appearance.3. Use the manufacturers shade guide for fabricating the restoration.4. Follow the manufacturers recommendations for preparing the surface of the tooth forshade matching. A diffuse-reflection condition is usually used.5. Remove the individual shade tab from the guide and hold it close to the tooth for shadematching.6. The surface texture of the restoration should match that of the remaining dentition asclosely as possible.Communication of Shade-Matching Information to the LaboratoryThe shade tab used for shade matching should be transmitted to the laboratory and shouldbe specifically for the material to be used to fabricate the restoration. The type of lightingused for shade matching should be included in the communication to decrease the effectof metamerism. The prescription should accurately transmit the shade information as wellas any characterization. An example of a map indicating the approximate shade, its depth,and information about its location is shown in Fig 3-19.
Fig 3-19 Illustration of a map supplied to a ceramist to communicate color. (FromSeluk and La Londe, 1985. Reprinted with permission.)The sequential steps in the overall transmission of shade-matching information and thefinal clinical acceptance of the fabricated restoration have been described by OBrien(1987). A schematic illustration is shown in Fig 3-20. The source spectrum is the colorand translucency information of the tooth to which the fabricated restoration is to bematched. The shade taking is the encoding process. The information is decoded in thedental laboratory. The simulation is the fabricated restoration, which is then delivered tothe dentist observer for evaluation and acceptance. If necessary, additional correction datato enhance the matching are communicated back for further simulation until the finalsimulation is reached. This is the fabricated restoration with necessary corrections toattain a clinically acceptable degree of shade matching to adjacent teeth.
Fig 3-20 Schematic illustration of transmission of shade-matching information.Glossaryblack object An object that reflects no incident color lights.chroma Color intensity.color content Relative intensity at each wavelength.color fatigue Decrease in response to one color due to constant stimulus.colorimeter A device used to measure the amount of light reflected at selected colors.color reflectance Relative amount of each color reflected.color system A three-dimensional system for defining color.edge effect Lateral scattering of a light beam upon entering a translucent material; causesan error in color measurement.fluorescence Glow of an object when illuminated.gloss Shininess; relative amount of light reflected.hue Commonly called color (eg, blue, yellow). It is associated with wavelength.isomeric pair Two objects that match color under different light sources.metameric pair Two objects that exhibit metamerism.metamerism Change in color matching of two objects under different light sources.opacityHigh opacity is associated with low intensity of transmitted light.
reflected color Color reflected by an object.refractive indexRefractive index of dental porcelain is 1.5. Refractive index of tin dioxide (an opacifier)is 2.0.spectrophotometer A device used to measure the amount of light reflected at eachwavelength.translucency Amount of light transmitted; the rest of the light is scattered.value Lightness or darkness of a color; a measurement of the amount of gray.white object An object that reflects all incident color lights.Discussion Questions1. How would a dental clinic need to be changed in order to be a better environment forcolor matching?2. Why is it not necessary that a dental restoration match adjacent tooth structure exactly?About how far off in color can it be?3. Why is it necessary to send the selected shade guide sample to the dental laboratoryrather than just the shade guide number?4. Besides color, which other appearance properties are important in creating an estheticrestoration?Study Questions(See Appendix E for answers.)1. Name the coordinates required to define a color in a color system.2. A porcelain crown may appear gray and nonvital; which variable is involved?3. Why does a green object appear black in blue light?4. What factors affect color appearance?5. How does translucency affect color appearance?6. What does gloss do to color appearance?7. What is metamerism?8. How does metamerism affect the appearance of dental restorations?
9. Why do dental porcelains appear different under different lighting environments?Recommended ReadingAmerican Dental Association (1981). Council on Dental Materials, Instruments andEquipment. How to improve shade matching in the dental operatory. J Am Dent Assoc102:209-210.Bergen SF, McCasland J (1977). Dental operatory lighting and tooth color discrimination.J Am Dent Assoc 94:130-134.Billmeyer FW Jr, Saltzman M (1960). Principles of Color Technology. New York:Interscience.Brodbelt RHW, OBrien WJ, Fan PL (1980). Translucency of dental porcelains. J DentRes 59:70-75.Brodbelt RHW, OBrien WJ, Fan PL, Frazier-Dib JG, Yu R (1981). Translucency ofhuman dental enamel. J Dent Res 60: 1749-1753.Cook WD, Chong MP (1985). Color stability and visual perception of dimethacrylatebased dental composite resins. Biomaterials 6:257-264.Cook WD, Vryonis P (1985). Spectral distributions of dental colour-matching lamps.Aust Dent J 30:15-21.Dennison JB, Powers JM, Koran A (1978). Color of dental restorative resins. J Dent Res57:557-562.Dickson G, Forziati AF, Lawson MS, Schoonover IC (1956). Fluorescence of teeth: ameans of investigating their structure. J Am Dent Assoc 45:661-667.Ecker GA, Moser JB, Wozniak WT, Brinsden GJ (1985). Effect of repeated firing onfluorescence of porcelain-fused-to-metal porcelains. J Prosthet Dent 54:207-214.Hall JB, Hefferen JJ, Olsen H (1978). Study of fluorescence characteristics of extractedhuman teeth by the use of a clinical fluorometer. J Dent Res 49:1431-1436.Johnston WM, OBrien WJ, Tien TY (1986). The determination of optical absorption andscattering in translucent porcelain. Color Res Application 11:125-130.Johnston WM, OBrien WJ, Tien TY (1986). Concentration additivity of Kubelka-Munkoptical coefficients of porcelain mixtures. Color Res Application 11:131-137.Jorgenson MW, Goodkind RJ (1979). Spectrophotometric study of five porcelain shadesrelative to the dimensions of color, porcelain thickness and repeated firings. J ProsthetDent 42:96-105.Judd DB, Wyszecki G (1975). Color in Business, Science and Industry. New York: JohnWiley & Sons.
McPhee ER. Light and color in dentistry (1978). I. Nature and perception. J Mich DentAssoc 60:565-572.McPhee ER (1985). Extrinsic coloration of ceramometal restorations. Dent Clin NorthAm 29:645-666.Miller L (1987). Organizing color in dentistry. J Am Dent Assoc (special issue):26E-40E.Miyagawa Y, Powers JM, OBrien WJ (1981). Optical properties of direct restorativematerials. J Dent Res 60:890-894.OBrien WJ (1985). Double layer effect and other optical phenomena related to esthetics.Dent Clin North Am 29:667-672.OBrien WJ (1985). Research in esthetics related to ceramic systems. Ceramic Eng Sci6:57-65.OBrien WJ (1987). Optical phenomena at interfaces. IADR Symposium on Biomaterialsand Interfaces, Chicago.OBrien WJ (1988). Fraunhofer diffraction of light by human enamel. J Dent Res 67:484-486.OBrien WJ, Boenke KM, Groh CL (1991). Coverage errors of two shade guides. Int JProsthodont 4:45-50.OBrien WJ, Groh CL, Boenke KM (1989). A one-dimensional color order system fordental shade guides. Dent Mater 5:371-374.OBrien WJ, Groh CL, Boenke KM (1990). A new, small-color-difference equation fordental shades. J Dent Res 69:1762-1764.OBrien WJ, Johnston WM, Fanian F (1985). Double-layer color effects in porcelainsystems. J Dent Res 64:940-943.OBrien WJ, Johnston WM, Fanian F, Lambert S (1984). The surface roughness and glossof composites. J Dent Res 63:685-688.OBrien WJ, Kay K-S, Boenke KM, Groh CL (1991). Sources of color variation on firingporcelain. Dent Mater 7:170-173.OBrien WJ, Nelson D, Lorey RE (1983). The assessment of chroma sensitivity toporcelain pigments. J Prosthet Dent 49:63-66.Peplinski DR, Wozniak WT, Moser JB (1980). Spectral studies of new luminophors fordental porcelain. J Dent Res 59:1501-1506.Powers JM, Dennison JB, Koran A (1978). Color sensitivity of restorative resins underaccelerated aging. J Dent Res 57:964-970.Powers JM, Dennison JB, Lepeak PJ (1978). Parameters that affect the color of directrestorative resins. J Dent Res 57:876-880.
Powers JM, Fan PL, Raptis CN (1980). Color stability of new composite restorativematerials under accelerated aging. J Dent Res 59:2071-2074.Powers JM, Yeh CL, Miyagawa Y (1983). Optical properties of composites of selectedshades of white light. J Oral Rehabil 10:319-324.Preston JD (1985). Current status of shade selection and color matching. Quintessence Int16:47-58.Preston JD, Ward LC, Bobrick M (1978). Light and lighting in the dental office. DentClin North Am 22:431-451.Ragain JC Jr, Johnston WM (2001). Accuracy of Kubelka-Munk reflectance theoryapplied to human dentin and enamel. J Dent Res 80:449-452.Seghi RR, Johnston WM, OBrien WJ (1986). Spectrophotometric analysis of colordifferences between porcelain systems. J Prosthet Dent 56:35-40.Seluk LW, La Londe TD (1985). Esthetics and communication with a custom shadeguide. Dent Clin North Am 29:741-751.Shotwell JL, Johnston WM, Swarts RG (1986). Color comparison of denture teeth andshade guides. J Prosthet Dent 56:31-34.Spitzer D, ten Bosch JJ (1975). The absorption and scattering of light in bovine andhuman enamel. Calcif Tissue Res 17:129-137.Spitzer D, ten Bosch JJ (1976). The total luminescence of bovine and human dentalenamel. Calcif Tissue Res 20:201-208.Sproull RC (1973). Color matching in dentistry. I. The three-dimensional nature of color.J Prosthet Dent 29:416-424.Sproull RC (1973). Color matching in dentistry. II. Practical applications of theorganization of color. J Prosthet Dent 29:556-566.Sproull RC (1974). Color matching in dentistry. III. Color control. J Prosthet Dent31:146-154.Stanford WB, Fan PL, Wozniak WT, Stanford JW (1985). Effect of finishing on colorand gloss of composites with different fillers. J Am Dent Assoc 110:211-213.Woolsey GD, Johnston WM, OBrien WJ (1981). Masking power of dental opaqueporcelains. J Dent Res 63:936-939.Wozniak WT, Fan PL, McGill SB, Stanford JW (1985). Color comparisons of compositeresins of various shade designations. Dent Mater 1:121-123.Wozniak WT, Moore BK (1978). Luminescence spectra of dental porcelain. J Dent Res57:971-974.
Stone, high-strength, high-expansion Suprastone (Kerr/Sybron) (ISO Type 5) The term gypsum products can be extended to include gypsum-bonded investments, used as mold materials for casting dental gold alloys, because calcium sulfate hemihydrate is an essential component, forming the bond in the set material. These materials will be dealt with separately later in this chapter. Fig 4-1 Classification of gypsum products. Plaster and Stone Both plaster and stone are the result of partial dehydration of gypsum, which produces calcium sulfate hemihydrate (CaSO41/2H2O). Differences in properties result from differences in the physical nature of the powders, which in turn are a result of differences in manufacturing methods. Chemistry In the temperature range 20C to 700C, which is of importance in the dental manipulation of gypsum products, three phase transformations occur in the calcium sulfate-water system. The first two represent the two stages in the dehydration of gypsum, and these are followed by a further transformation into anhydrous calcium sulfate:
It is not possible to give unequivocal temperatures for these transformations; theranges given summarize the results of several different determinations.For the first transformation, from dihydrate to hemihydrate, the temperature limitswere determined by weight loss measurements on specimens heated isothermally indry air for 2.5 years (Andrews, 1951) and would represent an equilibrium value.Thermogravimetric measurements of the temperature for the second transformation,calcium sulfate hemihydrate to hexagonal calcium sulfate, have involved isothermalheating for periods only up to a maximum of 22 days (Khalil et al, 1971; Weiser et al,1936), so the true equilibrium temperature for this transformation is probably a littlelower than shown. Gay (1965a,b) has identified hexagonal calcium sulfate by x-raydiffraction in specimens of hemihydrate heated in the range of 75C to 105C.Hexagonal calcium sulfate is unstable below about 80C, and, if cooled to lowertemperatures and exposed to the environment, it rapidly rehydrates to form thehemihydrate. The temperature range given for the third transformation, hexagonal toorthorhombic calcium sulfate, is based on measurements made on specimens heated ata rate of 5 K/min (Earnshaw and Mori, 1985), so again the true equilibriumtemperature for this transformation would be lower than shown here. Orthorhombiccalcium sulfate is the stable anhydrous form in this system and exists as the mineralinsoluble anhydrite.Theoretically, hemihydrate is the stable hydrous form of calcium sulfate only in theapproximate temperature range of 45C to 90C. It exists as a metastable phase underdry conditions at lower temperatures, including ambient, although it has been shownthat hydration can occur if particles are exposed to the atmosphere under conditionswhere the water vapor pressure is high (Torrance and Darvell, 1990).ManufactureIntroductionFrom the transformation temperatures given in the previous section, it can be seen thatcalcium sulfate hemihydrate would be produced by heating gypsum to temperatures inthe range of 45C to 90C. However, at these temperatures the reaction is slow; evenat 90C, substantially complete conversion takes about 12 hours (Khalil et al, 1971).Therefore, in commercial processes temperatures higher than this are used for shortertimes. The stable phase at these higher temperatures is hexagonal calcium sulfate, sothe initial product of calcination is partly or very largely this anhydrous form.
However, on cooling to temperatures below 80C and exposure to the atmosphere, thehexagonal calcium sulfate rehydrates to form the hemihydrate.Plaster of ParisThis is the traditional hemihydrate plaster produced by the dry calcination of groundgypsum in open containers (pans, kettles, or rotary kilns) at temperatures in the range120C to 180C. In the absence of liquid water, there is no opportunity forreorganization of crystal morphology, so although the crystal structure of the finalproduct after exposure to air is that of calcium sulfate hemihydrate, the powderparticles retain the rough irregular shape of the original ground gypsum. Loss of waterunder dry conditions leaves parallel channels in these particles (Fig 4-2), sohemihydrate plasters produced by dry calcination are powders with a low apparentdensity, a high relative surface area, and a poor packing ability.Fig 4-2 Particles of plaster. (Original magnification 400.)Medium- and high-strength plasters (stones)Plasters giving a stronger set mass are manufactured by wet calcination. Heresufficient liquid water is present to allow through-solution conversion, sorecrystallization produces dense prismatic crystals of hexagonal calcium sulfate.These rehydrate to the hemihydrate on cooling in air, but this secondary conversioncannot be accompanied by recrystallization. The final powder particles arepseudomorphic, having the monoclinic crystal structure of hemihydrate, butretaining the hexagonal crystal habit of the anhydrous calcium sulfate precursor (Fig4-3).
Fig 4-3 Crystals of wet-calcined gypsum plaster before grinding. (Scanning electronmicrograph, original magnification 3,000.)Hemihydrate powders produced by wet calcination therefore have a higher apparentdensity and a smaller relative surface area than those resulting from dry calcination. Acontrolled amount of grinding rounds off the crystals and produces a proportion offines, both factors improving the packing ability of the powder and further increasingthe apparent density. Particles of a typical dental stone are shown in Fig 4-4.
Fig 4-4 Particles of high-strength stone. (Original magnification 400.)Medium-strength plastersThese are typified by Hydrocal (United States Gypsum), which is the basis of manyordinary dental stones. It is produced by autoclaving lump gypsum in superheatedsteam, at a pressure of 117 kPa, giving a temperature of 123C, for 5 to 7 hours. Afterdrying at 100C or higher and grinding, a hemihydrate powder is produced that givesa set mass considerably stronger than that produced by dry-calcined materials.High-strength plastersModifications to the wet process yield hemihydrate powders giving even stronger setproducts. These are typified by Densite (Georgia-Pacific) and Crystacal (BritishGypsum). Here wet calcination takes place in the presence of crystal habit modifiers,producing crystals that are shorter and thicker than those resulting from autoclaving insteam. After controlled grinding, these powders have even higher apparent densitiesand yield even stronger set masses than Hydrocal-type stones: they form the basis ofmost dental die stones. Densite is produced by boiling lump gypsum in a 30% calciumchloride solution, and Crystacal is produced by autoclaving finely ground gypsum inthe presence of small amounts ( 1%) of sodium succinate.Apparent densityThe apparent density of a powder is the reciprocal of its bulkiness and so gives ameasure of its packing ability. The low apparent density of hemihydrate powdersproduced by dry calcination is caused in part by the rough irregular shapes of theindividual particles (see Fig 4-2). A more important factor, however, is a highadhesion of particles to their neighbors, caused by a high surface free energy resultingfrom crystal imperfections and adsorption of gases during calcination (Gregg, 1965).This adhesiveness of particles makes it likely that they will stick together at firstcontact, establishing bridges in the powder and creating a structure with many voids
and a low apparent density. In contrast, powder particles produced by wet calcinationare smooth and dense (see Fig 4-4). They show less crystallographic strain andtherefore have a lower surface free energy. As a result, they have a better packingability and a higher apparent density.The Setting ProcessThe setting reactionWhen the hemihydrate powder is mixed with water in the correct proportions, it formsa thick slurry. The hemihydrate is sparingly soluble in water (6.5 g/L at 20C), soonly a small amount can dissolve. Initially, therefore, the mix is a two-phasesuspension of hemihydrate particles in a saturated aqueous solution. The stablehydrate at temperatures below 40C is the dihydrate (gypsum), which is even lesssoluble (2.4 g/L at 20C) than the hemihydrate. The aqueous phase is thereforesupersaturated with respect to the dihydrate, which crystallizes out at suitablenucleation centers in the suspension. These gypsum crystals normally are acicular inhabit and often radiate out from nucleation centers in the form of spheruliticaggregates.These nucleation centers may be impurities (eg, residual gypsum particles), particlesof gypsum added as seeds to accelerate setting, or strained areas on undissolvedhemihydrate particles. The consequent depletion of calcium and sulfate ions in theaqueous phase allows more hemihydrate to go into solution and, in turn, to precipitateout as gypsum. The setting process is therefore one of heterogeneously nucleatedrecrystallization, characterized by a continuous solution of hemihydrate, diffusion ofcalcium and sulfate ions to nucleation centers, and the precipitation of microscopicgypsum crystals. The setting reaction is the reverse of the first stage of dehydrationand so is exothermic. It is represented by the following equation:Water requirementThe differing water requirements of plaster, stone, and high-strength stone aremainly the result of differences in the apparent density of the powder. The factors thatpromote adhesiveness of the particles in the dry powder persist when they aresuspended in water (Ridge, 1961). For this reason dry-calcined plaster, with its lowapparent density, produces a flocculated suspension and needs a relatively highproportion of mixing water to give a mix of workable viscosity. Water/powder(W/P) ratios of 0.5 to 0.6 are usual. Hemihydrate powders produced by wetcalcination, because of their higher apparent densities, require less mixing water;typical W/P ratios are 0.30 to 0.33 for ordinary dental stones and 0.18 to 0.23 forhigh-strength stones.In setting, 100 g of hemihydrate combines with 18.6 g of water. Therefore, at thecompletion of the reaction in normal mixes there is always some excess unreactedwater (as a saturated solution of calcium sulfate) remaining in the set mass. Thisresidual water weakens the cast. It can be removed by low-temperature drying butleaves microscopic porosity that weakens the dry cast. Both wet and dry strengths of
the set material depend on the relative amount of unreacted water remaining aftersetting, and so on the W/P ratio of the original mix. The relative amount of residualwater is least in high-strength stone, which therefore gives the strongest set mass.Stages in settingThe setting process is continuous from the beginning of mixing until the settingreaction is complete, by which time the material has reached its full wet strength.However, important physical changes can be recognized during this process. Initiallythere is a continuous aqueous phase present, and the mix is a viscous liquid,exhibiting pseudoplasticity so that it flows readily under vibration; in this stage themix has a glossy surface giving specular reflections. As the setting reaction proceeds,gypsum crystals continue to grow at the expense of the aqueous phase, and theviscosity of the mix increases. When the clumps of growing gypsum crystals interact,the mix becomes plastic; it will not flow under vibration but can readily be molded.At this time the glossy surface disappears as the aqueous phase is drawn into poresformed when the growing gypsum crystals thrust apart. Continued crystal growthconverts the plastic mass into a rigid solid, weak and friable at first but gainingstrength as the relative amount of solid phase increases.These four stages may be designated (1) fluid, (2) plastic, (3) friable, and (4) carvable.Volume changes during settingThe setting reaction causes a decrease in the true volume of the reactants, and undersuitable conditions this contraction can be observed early in the setting process, whenthe mix is still fluid. However, once the mix begins to attain rigidity (marked by theloss of surface gloss) an isotropic expansion is observed, resulting from growthpressure of the gypsum crystals that are forming. There is therefore a decrease inapparent density of the mix during the latter stages of setting, accompanied by theformation of microscopic voids separating individual crystals in the aggregate.The initial contraction is unlikely to affect the important dimensions of a gypsum cast,because in the still-fluid mix it will occur mainly in a vertical direction. Gravity willkeep the mix adapted to the anatomical portion of an impression. The expansion thatis observed after the mix attains rigidity takes place in all directions and will affect thedimensions of the cast. The point at which the initial contraction ceases is used as zeroin laboratory measurements of effective setting expansion.Rate of the setting reactionWithin wide limits, the rate of hydration during setting is independent of the W/Pratio (Lautenschlager et al, 1969). However, the rate at which the associated physicalchanges described earlier occur is highly dependent on the W/P ratio of the mix,because these changes result from interaction of clumps of gypsum crystals growingfrom nucleation centers in the slurry. Thick mixes (low W/P ratios) harden morequickly because available nucleation centers are concentrated in a smaller volume;interaction of the growing solid phase occurs earlier and is more effective inpromoting expansion.
The effect of additivesMany salts and colloids are known to alter the setting characteristics of hemihydrateplasters by their effect on the rate of the setting reaction. They have been used in theformulation of dental plasters and stones for many years, mainly on an empiricalbasis, because their modes of action are not always completely understood.Finely powdered gypsum is an efficient accelerator, which acts by providing seeds forheterogeneous nucleation. In low concentrations soluble sulfates and chlorides areaccelerators, apparently acting by increasing the rate of solution of the hemihydrate.However, salts of relatively low solubility, such as sodium chloride and sodiumsulfate, act as retarders in higher concentrations, because as setting proceeds theamount of free water in the mix decreases and the concentration of the additiveincreases. When its limit of solubility is exceeded, the salt precipitates on nuclei ofcrystallization, thus poisoning them. Ace-tates, borates, citrates, and tartrates areretarders, which may act by nuclei poisoning, by reducing the rate of solution ofhemihydrate, or by inhibiting the growth of dihydrate crystals. Reaction of someadditives with hemihydrate can occur; soluble tartrates and citrates precipitate calciumtartrate and citrate, respectively. Colloids are effective retarders, presumably acting bynuclei poisoning.Many accelerators and retarders reduce the setting expansion, sometimes by changingthe crystal habit of growing gypsum crystals from acicular to a more compact formand inhibiting spherulite formation (Koslowski and Ludwig, 1984); both factorsreduce the effect of the crystals growth pressure. This is accompanied by a reductionin the strength of the set material.The Microstructure of Cast GypsumIntroductionThe set material consists of a tangled aggregate of monoclinic gypsum crystals,usually acicular in shape, with lengths in the range of 5 to 20 um. The aggregateexhibits two distinct types of inherent porosity on a microscopic scale:1. Microporosity caused by the presence of residual unreacted water. These voids areroughly spherical and occur between clumps of gypsum crystals.2. Microporosity resulting from growth of gypsum crystals. These voids areassociated with setting expansion and are smaller than the first type; they appear asangular spaces between individual crystals in the aggregate.The effect of W/P ratioThe relative amounts of both types of porosity are affected by the W/P ratio of themix, but in opposite ways:1. A low W/P ratio (thick mix) leaves less residual water in the set mass and sodecreases the amount of the first type of porosity.
2. A low W/P ratio increases the effect of crystal growth during setting, becauseavailable nucleation centers are concentrated in a smaller total volume of mix;interaction of growing gypsum crystals occurs earlier and is more effective so theamount of the second type of porosity is increased.3. At any W/P ratio, the total proportion of inherent porosity in the set mass is the sumof these two types. The effect of the first type predominates, so for any given plasteror stone there is always a decrease in the total inherent porosity of the set mass (ie, anincrease in apparent density) as the W/P ratio of the mix is reduced. Inherent porosityrepresents about 40% of the total cast volume at a W/P ratio of 0.50 and about 20% ata W/P ratio of 0.25 (Lautenschlager and Corbin, 1969).Typical microstructures of casts made from plaster mixed in a W/P ratio of 0.50 andhigh-strength stone mixed in a W/P ratio of 0.25 are shown in Fig 4-5. The secondtype of microporosity described here (resulting from crystal growth) can be seen inboth micrographs, while the first type (resulting from residual water) shows clearly inthe micrograph of set plaster, where the voids occur between spherulitic clumps ofgypsum crystals. The higher apparent density of the set high-strength stone is obvious.Fig 4-5 Fracture surface of cast gypsum. (Scanning electron micrographs, originalmagnification 3,000.) (A) Plaster, W/P = 0.50; (B) high-strength stone, W/P = 0.25.(From Bever, 1986. Reprinted with permission.)
PropertiesRate of settingManipulation timeRecognition of the physical changes occurring in the mix during setting is importantin the manipulation of plaster and stone.1. When casting (eg, pouring casts or dies), manipulation must be completed beforethe mix loses fluidity. The change is marked by the disappearance of the glossysurface from the mix.2. When molding (eg, taking impressions or jaw registrations, articulating casts,flasking wax pattern dentures), manipulation must be completed before the mix losesplasticity and enters the friable stage. There is no recognized objective method ofmeasuring this time.Setting timeAn arbitrary setting time (initial set) can be determined by using suitablepenetrometers (eg, Gillmore or Vicat initial needles; both give approximately thesame initial setting time). Measured in this way, the initial set is a guide to the timewhen the rigid material is strong enough to handle and, in particular, when it can becarved or trimmed to the final shape.If a dental manufacturer specifies a setting time, it will be a Gillmore or Vicat initialset. Both the setting reaction and the increase in strength continue for some time afterthis initial set. Gillmore and Vicat final needles may be used to establish a finalsetting time, but this is not usual in dental technology.Control of rate of setting1. The use of additives. In formulating dental products, manufacturers adjust the rateof setting of raw hemihydrates by adding accelerators and retarders, often as abalanced mixture. Typical accelerators are potassium sulfate and potassium sodiumtartrate ("Rochelle salts"). Typical retarders are sodium citrate and sodium tetraboratedecahydrate (borax). The action of accelerators and retarders has already beendiscussed.2. W/P ratio. It has already been pointed out that changing the W/P ratio has a markedeffect on the rate at which the physical changes associated with setting of the mixoccur. These changes take place more rapidly as the W/P ratio is reduced.Manipulation and setting times are thus directly proportional to W/P ratio.Setting expansionTypical values for setting expansion for the five types of dental gypsum plaster aregiven in Table 4-2. These are the results of laboratory measurements on five widelyused materials, setting in air.
Table 4-2 Linear setting expansions of typical dental gypsum products(setting in air)Type W/P ratio Setting expansion (%)Impression plaster 0.60 0.13Plaster 0.50 0.30Stone 0.30 0.15Stone, high-strength, low-expansion 0.20 0.10Stone, high-strength, high-expansion 0.19 0.26The observed expansion that occurs when dental plaster or stone sets is a volumetricone. In dental testing a value is determined for linear setting expansion, and theassumption is made that the expansion is isotropic. This assumption is not alwaysjustified; if restraint is imposed in some directions but not others (eg, by a rigidimpression), setting expansion can be far from isotropic.Effect of immersionGypsum products exposed to additional water while setting (eg, by immersion) showa greater expansion than when setting in air, a phenomenon commonly (butinaccurately) called hygroscopic expansion. When expansion begins, externallyavailable water is drawn into pores forming in the setting mass, and this maintains acontinuous aqueous phase in which crystal growth takes place freely. Under dryconditions this additional water is not available, and as expansion occurs the aqueousphase in the mix is reduced to a film over the growing gypsum crystals. Surfacetension forces in this liquid film restrain further crystal growth, thereby reducing theobserved setting expansion of the mix (Mahler and Ady, 1960). Thus the so-calledhygroscopic expansion is simply an enhanced setting expansion that occurs in thepresence of additional water.Control of setting expansion1. Use of additives. A low setting expansion is desirable in applications wheredimensional accuracy is important (eg, in impression taking and pouring workingcasts and dies). Many accelerators and retarders of setting also reduce settingexpansion. Manufacturers can reduce setting expansion and at the same time controlsetting time by adding a balanced blend of accelerator and retarder to the rawhemihydrate. Typical combinations are potassium sulfate-borax and potassiumsodium tartrate- sodium citrate.These additives also reduce the strength of the set material. This is not a disadvantagein impression plasters, but in stones, strength as well as dimensional accuracy isimportant; formulation of the latter materials therefore involves striking a compromisebetween a desirable reduction in setting expansion and an undesirable reduction instrength.Normally die stones in particular are formulated to have a low setting expansion. Astheir name indicates, they are used to make cast gypsum dies on which restorationssuch as inlays, crowns, and fixed partial dentures are constructed by the indirectmethod, and they are required to reproduce the prepared teeth with high dimensional
accuracy. Such materials constitute the ISO Type 4 high-strength, low-expansionstones, which have a setting expansion less than 0.15%. These would be used wherethe investment expansion is sufficient to compensate completely for the castingshrinkage of the alloy. There has now been introduced another category of die stone:ISO Type 5, high-strength, high-expansion, with a setting expansion in the range of0.16% to 0.30%. The higher expansion results from a lower concentration ofmodifying additives, so these materials also generally achieve higher strengths whenset. They are intended for use in casting techniques when investment expansion alonemay not be high enough to compensate fully for alloy shrinkage. Here the settingexpansion of the die stone is intended to contribute to the total mold expansion byproducing an oversized pattern (Fusayama, 1964), but it is important that theimpression be soft and flexible enough for isotropic setting expansion to occur. In animpression made from a stiff elastomeric material in a closely fitting rigid tray, settingexpansion will be likely to occur preferentially in a vertical direction, producing adistorted die.2. W/P ratio. For any given gypsum product, reducing the relative amount of aqueousphase in the mix allows more effective interaction of growing gypsum crystals duringsetting, thus increasing the setting expansion. Setting expansion is therefore inverselyproportional to the W/P ratio. Because of their lower water requirement, the rawhemihydrates used to produce stones and die stones have a higher inherent settingexpansion in normal mixes than does plaster. This effect is masked, however, by theadditives used in their formulation (Fig 4-6).Fig 4-6 Linear setting expansion in air and in water of various types of gypsumproducts. (A) Plaster (W/P = 0.50); (B) unmodified stone (Hydrocal B, W/P = 0.32);(C) a commercial stone based on Hydrocal (W/P = 0.32); (D) unmodified high-strength stone (Densite K5, W/P = 0.24); (E) a commercial high-strength stone basedon Densite (W/P = 0.24).
StrengthCast gypsum is a brittle material and so is weaker in tension than in compression.Materials with the highest compressive strengths are the most brittle, and their tensilestrengths are proportionally lower. For set plaster, the tensile strength is about 20% ofthe compressive strength; for set high-strength stone, it is about 10%. Since fractureof cast gypsum typically occurs in tension, tensile strength is a better guide to fractureresistance. However, compressive strength gives a better indication of surfacehardness. Values for tensile and compressive strengths of five typical dental gypsumplasters are shown in Table 4-3. Table 4-3 Strength properties of typical dental gypsum products* Tensile strength Compressive strength (MPa) (MPa)Type W/P Wet Dry Wet Dry ratioImpression plaster 0.60 1.3 5.9 Plaster 0.50 2.3 4.1 12.4 24.9Stone 0.30 3.5 7.6 25.5 63.5Stone, high-strength, 0.20 6.1 10.6 58.4 126.4low-expansionStone, high-strength, 0.19 6.2 12.6 76.4 145.2high-expansion*The materials tested were the same as those in Table 4-2.1. The effect of W/P ratio. In general, strength properties are inversely related to W/Pratio and so to the total amount of inherent porosity (Fig 4-7). Therefore whenmaximum strength is required, a given material should be mixed in as low a W/P ratioas practicable. The limiting factor is the viscosity of the mix, because it increases withdecreasing W/P ratio and can become so high that the ability to pour sound casts isprejudiced.In high-strength stones mixed even in normal W/P ratios, there is little water presentin excess of the theoretical W/P ratio (0.186) required for complete conversion ofhemihydrate to dihydrate. Since the setting reaction depends on diffusion of ions, itmay not proceed to completion in standard mixes; in fact, Donnison et al (1960) haveshown that in normal mixes the hydration may be up to 3% short of completion andthat the proportion of residual hemihydrate increases as the W/P ratio decreases.Residual hemihydrate particles are often seen in micrographs of set high-strengthstone. The content of unreacted hemihydrate becomes much greater in very thickmixes, but as Fig 4-7 shows, this does not adversely affect the strength until the W/Pratio is well below that theoretically needed for complete hydration. Such thick mixeswould be impossible to manipulate successfully in most dental applications.With any plaster or stone, using a low W/P ratio to obtain maximum strengthproperties also gives an increased setting expansion, which must be accepted. But in
applications where dimensional accuracy is more important than strength (eg,impressions), higher W/P ratios can be used.Fig 4-7 The effect of W/P ratio on the wet tensile strength of a high-strength stone.(From Selby, 1979.)2. The effect of drying. Removal of all uncombined water from cast gypsum by low-temperature drying approximately doubles strength properties (see Table 4-3), butthere is no strength increase until the last 2% of free water is removed. This strengthincrease on drying is reversible; soaking a dry cast in water reduces its strength to theoriginal level.Gypsum is stable only below about 40C. Drying at higher temperatures must becarefully controlled; loss of water of crystallization occurs rapidly at 100C or higherand causes shrinkage and a reduction in strength.SolubilityBecause gypsum is sparingly soluble in water, long-term immersion iscontraindicated. If dried gypsum casts have to be soaked, it is better to use a saturatedsolution of calcium sulfate.Disinfection of Gypsum CastsTo prevent cross-infection, the practice of disinfecting impressions is becomingincreasingly common. However, prolonged immersion in disinfectant solutions cancause unacceptably large dimensional changes in hydrocolloid (Bergman et al, 1985;Olsson et al, 1987) and polyether (Johnson et al, 1988) impressions. Moreover, duringsubsequent clinical procedures, casts or dies can become reinfected with pathogenicorganisms, which can then be transferred to technical staff. As an alternative, the
addition of disinfectants to the mixing water when casts are poured has beeninvestigated; 5% phenol (McGill et al, 1988) and 2% glutaraldehyde (Ivanovski et al,1995) have proved to be effective and did not adversely affect the properties of the setmaterial. However, both are known tissue irritants. Dental stones that contain adisinfectant are available (Donovan and Chee, 1989; Schutt, 1989). Alternatively,casts and dies may be treated by immersion in a disinfecting solution after eachclinical stage.Autoclave sterilization of casts has been suggested (Whyte and Brockhurst, 1996).Some loss of strength and surface hardness and an increase in dimensions occur, but itis claimed that under carefully controlled conditions the casts retain adequateproperties for ordinary laboratory use.Gypsum-Bonded InvestmentsIntroductionGypsum-bonded investments are the mold materials most commonly employed in thecasting of dental gold alloys with liquidus temperatures no higher than 1,080C,which are normally used for gold inlays, crowns, and fixed and removable partialdentures. Because of their tendency to decompose at high temperatures, theseinvestments are not suitable for casting high-melting gold alloys, palladium alloys(used for copings in alloy-ceramic restorations), or most base- metal alloys, such asnickel-chromium and cobalt-chromium. Gypsum-bonded investments are classifiedby the International Standards Organization (1990) as:Type 1: Thermal expansion type, for casting inlays and crownsType 2: Hygroscopic expansion type, for casting inlays and crownsType 3: For casting complete and partial denture basesThis classification is illustrated in Fig 4-8, and typical materials are listed in Table 4-4. Some materials, classified by their manufacturers as "universal," are claimed to besuitable for casting all gold-alloy restorations.Fig 4-8 Classification of gypsum-bonded investments.
Table 4-4 Typical gypsum-bonded investments Type ExampleInlay investment, thermal expansion (ISO Cristobalite Inlay (Kerr/Sybron) Type 1)Inlay investment, thermal expansion, rapid Cristoquick (GC) heat (ISO Type 1)Inlay investment, hygroscopic expansion Beauty-Cast (Whip Mix) (ISO Type 2)Denture investment (ISO Type 3) R&R Gray (Dentsply/Ransom and Randolph) Composition All gypsum-bonded investment powders consist basically of a refractory filler and a binder. There may also be small amounts (less than 5%) of important modifying agents present. Refractory The refractory component is either cristobalite or quartz (or occasionally a mixture of the two), usually present in the range of 55% to 75%. Both of these components are polymorphs of silica (SiO2). Binder In the investment powder, the binder is calcium sulfate hemihydrate, either plaster or stone. When the investment sets, the silica is unaffected; the hemihydrate binder combines with water to form dihydrate (gypsum) as in the setting of other gypsum products. The setting reaction is therefore the same as that shown in the equation given previously. The set investment consists of fine particles of silica embedded in an interlocking aggregate of smaller acicular gypsum crystals (Fig 4-9). The continuous porosity characteristic of cast gypsum provides the necessary mold venting to assist in the production of sound castings.
Fig 4-9 Microstructure of a set gypsum-bonded investment (Kerr Cristobalite Inlay;W/P = 0.38). The large particles are cristobalite; the small acicular crystals aregypsum formed during setting. (Scanning electron micrograph of fracture surface,original magnification 3,000.)Modifying agentsSmall amounts of modifying agents are added to many commercial gypsum-bondedinvestments. These may be accelerators or retarders to control the rate of setting,reducing agents such as powdered graphite or copper to protect embedded gold alloycomponents in "casting-on" techniques, or additives to increase the thermal expansionof the investment. Typical additives of the last type are boric acid and soluble halidesalts, particularly those of alkali or alkaline earth metals.Effect of composition on setting and thermal behaviorRefractoryAlthough silica is referred to as the refractory component, cast gypsum itself issufficiently heat-resistant to be used as a mold material, because it can be heated totemperatures as high as 1,000C without decomposing (Gutt and Smith, 1967). Infact, adding silica reduces its heat resistance, because in such mixtures at temperaturesabove 900C, the following reaction occurs:At high temperatures, the sulfur trioxide liberated by this reaction causes rapidcorrosion of the casting.Crystalline silica is used in dental investments not to improve their heat resistance butto control dimensional changes on heating. When heated, cast gypsum shows amarked contraction, and because both quartz and cristobalite have high expansionswhen heated, they offset the shrinkage of the binder and can provide a positive
thermal expansion if this is needed.Silica exists in 22 different condensed phases. Five of these are amorphous, and 17are crystalline; the latter are the polymorphs of silica. Of this group, only one phase,low-temperature quartz, is thermodynamically stable at normal temperature andpressure. Two more, tridymite S-1 and low-temperature cristobalite, exist undernormal atmospheric conditions as metastable (but actually long-lived) phases.Only two polymorphs of silica are of importance in dental investments: quartz andcristobalite. Quartz is a common mineral; cristobalite occurs naturally as a raremineral but is normally manufactured by prolonged heating of quartz at hightemperatures to induce the appropriate slow inversion. Both quartz and cristobaliteexist in low-temperature () and high-temperature () phases, and in both materialsthe change between low- and high-temperature phases is rapid and readily reversibleon cooling. This change is known as the high-low inversion.In both quartz and cristobalite the high-temperature phase is less dense than the low,so the inversion is accompanied by an isothermal expansion. This is added tothe normal thermal expansion to give a large overall expansion at high temperatures.As in all crystalline materials, single crystals of quartz and cristobalite showanisotropy of physical properties, including their coefficients of thermal expansion.However, in dental investments they are used as a fine powder with randomorientation of individual particles, so in the aggregate they behave isotropically, andproperties such as the coefficient of thermal expansion have a uniform average value.Typical linear thermal expansion curves for powdered quartz and cristobalite areshown in Fig 4-10. Specimens were made by densely compacting the powders intoaggregates with a minimum amount of binder in the interstices, so the thermalexpansion of the specimens was essentially that of the silica component in dentalinvestments.The temperature of the inversion of cristobalite varies according to the source ofthe sample and its previous thermal history; in the manufactured cristobalite used indental investments it is about 250C (Fig 4-10, curve A). The inversion gives anisothermal expansion of about 1.3%, and the total expansion at 700C is about 2.2%.Dental investments designed to have a high thermal expansion usually containcristobalite as the refractory.
Fig 4-10 The linear thermal expansion of cristobalite (curve A) and quartz (curve B).The specimens were aggregates of fine powders, united with a minimum amount ofbinder; their thermal behavior was thus similar to that of the refractory component ofdental casting investments. Cristobalite undergoes inversion at about 250C, quartz at573C.Quartz (Fig 4-10, curve B) undergoes its inversion at 573C, producing anisothermal expansion of about 0.7%. The high-temperature form has a negativecoefficient of thermal expansion, and the overall total expansion at 700C is about1.6%.BinderWhen the set investment is heated, the cast gypsum binder shows a markedcontraction, which occurs in several stages. In the early stages of heating, acontraction accompanies loss of water of crystallization, as the dihydrate reverts tohemihydrate and then to hexagonal calcium sulfate. A large contraction thenaccompanies its transformation, which occurs in the approximate temperaturerange of 300C to 400C. A further large contraction begins at about 650C, which isprobably the result of densification by sintering. The total linear contraction of castgypsum prepared from plaster (W/P = 0.50) and heated to 700C can be as high as3%; the corresponding shrinkage for cast gypsum prepared from a high-strength stone(W/P = 0.25) is about 1%. The latter is usually preferred as a binder in gypsum-bonded investments, not only because of its lower shrinkage on heating but becauseits superior strength when set allows a higher concentration of silica to be used in theinvestment, thereby reducing still further the effect of binder contraction.Effects of varying compositionWithin practical limits, increasing the proportion of silica in the investment powder
increases the manipulation time (given by the time of loss of fluidity) and the initialsetting time (Fig 4-11),Fig 4-11 The effect of silica content on the manipulation time (curve A) and settingtime (curve B) of experimental investments. Manipulation time was determined by thetime of loss of gloss, which indicates loss of fluidity; setting time by the Vicat initialset. The investments were mixtures of cristobalite and a high-strength stone, and allspecimens were mixed in a W/P ratio of 0.40.the setting expansion, both in air and in water, and the thermal expansion (Fig 4-12)
Fig 4-12 The effect of silica content on the setting expansion in air (curve A), thesetting expansion in water (curve B), and the thermal expansion (curve C) ofexperimental investments (compositions and W/P ratio as in Fig 4-11). Settingexpansions were recorded 2 hours after mixing, and thermal expansions after heatingto 700C.and reduces the compressive strength (Fig 4-13). The rate of the setting reaction itselfis unchanged; the increases in observed manipulation and setting times occur becausethe particles of refractory filler interfere with the interlocking of growing gypsumcrystals, making this less effective in developing a solid structure. The compressivestrength of the set investment is reduced for the same reason. Setting expansion isincreased when interlocking of growing gypsum crystals is inhibited by the refractoryparticles, because more of the crystal growth is directed outward. Thermal expansionis increased because, at any temperature, it is given by summing the bindercontraction and the refractory expansion; increasing the proportion of the expandingcomponent increases the observed expansion.
Fig 4-13 The effect of silica content on the compressive strength of experimentalinvestments (compositions and W/P ratio as in Fig 4-11). Tests were made on wetspecimens, 2 hours after mixing.Effects of modifying agentsImportant modifying agents are those added to some commercial investments toincrease their thermal expansion. These include boric acid and soluble halide salts ofalkali or alkaline earth metals. All of them act mainly by reducing the two largecontractions of the gypsum binder that occur on heating to temperatures above 300C.Boric acid, when heated above 150C, forms a viscous liquid with a compositionintermediate between metaboric acid and boron oxide; this viscous liquid impedes theevaporation of the last traces of water, delaying the transformation of calciumsulfate (Mori, 1986). The presence of the viscous liquid phase also reduces the high-temperature contraction that results from sintering, because it stabilizes the originalcontacts formed between the gypsum crystals and silica during setting (Mori, 1982).The presence of halide anions greatly reduces the first major shrinkage andcompletely eliminates the second. The reason for this is not yet understood. If alkalimetal or alkaline earth cations are also present (eg, as halide salts), the effect of thehalide anion is nullified at temperatures above 650C and a rapid contraction occurs;this is probably the result of accelerated sintering. This large high-temperatureshrinkage of the binder is not observed in gypsum-bonded investments containingalkali metal or alkaline earth halides, because at a concentration of 50% or more ofsilica the silica particles in the set investment form a continuous "skeleton" that resistsoverall shrinkage.The presence of modifiers added to increase the thermal expansion also affects thestrength changes of the investment that occur on heating, again because of theireffects on the calcium sulfate binder.On heating, gypsum-bonded investments without these additives show a rapid
increase in compressive strength of about 100% in the range of 100C to 175C; thisis the result of drying and is analogous to that occurring in cast gypsum. Between175C and 225C there is an equally rapid decrease in compressive strength,attributable to the dehydration reaction dihydrate hemihydrate, bringing thestrength back to about that of the original wet specimens. Relatively minor strengthfluctuations occur during subsequent heating to higher temperatures, attributable to(1) further phase changes in the binder, (2) the inversion in the refractory, and(3) sintering of the binder (Ohno et al, 1982). Investments of this type, heated totemperatures in the range of 670C to 700C, show compressive strength changesranging from +10% to -40%, compared with the wet strength at ambient temperatures.Investments containing boric acid, when heated to the same temperatures, showincreases in compressive strength ranging from +40% to +50%, probably the result ofthe effect of the viscous liquid phase stabilizing contacts between calcium sulfate andsilica particles. Investments containing halides of alkali metals and alkaline earths (eg,sodium, barium, and strontium chlorides) show a marked strength decrease on heatingto 700C, ranging from -50% to -85%. This is probably the result of the increasedsintering contraction of the binder at temperatures over 650C. The silica skeletonresists shrinkage of the investment as a whole, so the high sintering contraction occursindependently in the binder, reducing the strength of its bond with the silica particles.PropertiesParticle size of the powderThe particle size affects the smoothness of the mold cavity surface (and thus of thecasting) and also the inherent porosity of the mold (and thus the venting of the moldcavity). Only the particle size of the refractory filler is of practical importance. It isthe major constituent and remains unchanged in the set investment. The gypsumcrystals formed during setting of the binder are much smaller than the silica particles(see Fig 4-9).Excessive surface roughness of the casting can interfere with its fit; a refractory with afine particle size ensures a smooth mold surface and a smooth casting. In gypsum-bonded investments, venting of the mold cavity is normally provided by thecontinuous porosity inherent in the set material. This is at a maximum when packingof the silica particles is least dense, which in turn is achieved by ensuring that theparticle size is uniform.Therefore, the refractory powder used in making the investment should have auniform, fine particle size. A particle size of no more than 75 um is usual.Rate of settingThe same physical changes that occur during the setting of gypsum plasters can alsobe recognized when gypsum-bonded investments set.Manipulation time Investing the wax pattern or pouring the investment cast must becompleted while the mix is still fluid. As with gypsum plasters, loss of fluidity is
indicated by the disappearance of the glossy surface from the mix.Setting time This is usually given as a Gillmore or Vicat initial set. It indicates whenthe investment is strong enough for the sprue base and sprue former to be removed.Preferably mold heating should be delayed until setting expansion is complete(usually between 1 and 2 hours from the start of mixing).ExpansionInlay investments currently available have total expansions, measured underlaboratory conditions, in the range of 1.5% to 2.5%. Denture investments gainincreased strength by having a higher content of hemihydrate binder, at the expense ofthe refractory component, so their total expansions are less; the lower figure for theexpansion range is about 1.3%. It is, however, by no means certain that such figuresshow the expansion of the mold cavity that can be expected under practicalconditions.Modern methods of casting small restorations can be classified into two groups:1. In hygroscopic expansion techniques, all or most of the mold expansion is gainedwhen the investment sets; the setting expansion is greatly increased by exposure toadditional water. Thermal expansion of the investment is low.2. In thermal expansion techniques, both setting and thermal expansion contributeimportantly to mold expansion.Setting expansion1. Setting expansion in air. Linear setting expansions of most inlay investments,measured under dry conditions, are in the range of 0.1% to 0.6%.2. Setting expansion in water (hygroscopic setting expansion). Inlay investments showa much greater setting expansion if exposed to additional water during setting (eg, byimmersion in a water bath). The phenomenon is the same as that described forgypsum plasters, but the effect on setting expansion is much greater because of thepresence of the refractory particles (see Fig 4-12). If no constraint is imposed, thelinear setting expansion of inlay investments can be as high as 4% (Earnshaw, 1969a).But even a small restraining force causes a large reduction, and when measured underusual laboratory conditions, the hygroscopic setting expansion of most inlayinvestments is in the range of 0.3% to 2.0%. Investments specifically designed for usein hygroscopic expansion techniques have setting expansions, when immersed inwater, of at least 1.3%.3. The effect of the casting ring liner. In most casting techniques the investment moldsets and is heated in a casting ring made of heat-resistant alloy, which has a muchlower thermal expansion than the investment mold. The need for a soft ring liner, toeliminate or at least reduce restraint to investment expansion by the ring, was firstrecognized by Souder (Hollenback, 1962), who advocated the use of asbestos tape toprovide the necessary cushioning. Since asbestos readily absorbs water, the liner wasprewetted to prevent its absorbing water from the unset investment mix.
The technique of lining a casting ring with wet asbestos was first described in 1930 byTaylor and coworkers, and from then until recent times, the use of a wet asbestos ringliner has been a standard procedure. This makes additional water available to thesetting investment and causes an increased setting expansion. Even when theinvestment mold sets in air, as in thermal expansion techniques, some hygroscopicsetting expansion occurs. Investments used in thermal expansion techniques have arelatively high silica content, so the increase in setting expansion produced byexposure to water is high (see Fig 4-12). Because this high setting expansion isuncontrollable and likely to be anisotropic, techniques have been developed in whicha dry, waterproofed asbestos ring liner is used (Fusayama, 1959, 1964) or the use ofthe rigid casting ring with its liner is avoided (Finger and Jorgensen, 1980).Attention has been drawn to the danger that asbestos fibers in casting-ring liners couldcause asbestosis or mesothelioma (Priest and Horner, 1980). It is claimed that theacceptable threshold limit for asbestos fibers in air can be considerably exceededwhen castings are removed from asbestos-lined casting rings (Yli-Urpo et al, 1982).For this reason, and because of the increasing unavailability of asbestos products,asbestos as a casting-ring liner has been almost completely replaced by alternativematerials. There are two types: (1) cellulose, which readily absorbs water and, likeasbestos, must be prewetted, and (2) ceramic materials which at atmospheric pressurewill not absorb water and are normally used dry. The ceramic materials are madefrom fibers of an aluminosilicate glass derived from kaolin; these are formed intosheets by means of standard paper-making techniques (Barnard, 1981). The majorcomponents in the glass are alumina (47% to 65%) and silica (38% to 50%), whichmakes the material highly heat-resistant. On the other hand, the cellulose materialsburn if heated in air, and at a burnout temperature of 700C they disappear completelyfrom the casting ring. However, if liners are kept short of both ends of the ring, theinvestment mold is retained in place during casting.Cellulose liners have a water uptake similar to asbestos and a similar effect on thesetting expansion of the investment.Although ceramic liners absorb negligible amounts of water when immersed atatmospheric pressure, they absorb it readily under vacuum. This occurs duringvacuum investing; since the previously dry liners obtain the water from theinvestment mix, the W/P ratio of the unset investment is greatly reduced. Thecombination of a low W/P ratio and a wet liner considerably increases theinvestments setting expansion; the total expansion is higher than when prewettedasbestos or cellulose liners are used with normal W/P ratios.Thermal expansion After it has set, the investment mold is heated to therecommended temperature for casting. This is necessary to dry the investment, to meltand burn out the wax pattern, to oxidize residual carbon from the mold, and to preventpremature freezing of thin sections when the alloy is cast. Heating also causes thermalexpansion of the mold and therefore of the mold cavity.1. Hygroscopic expansion techniques. With these techniques, the mold is heated toabout 480C, at which temperature its thermal expansion is relatively low (Fig 4-14).
Investments for use in these techniques are based on a quartz refractory that does notundergo inversion until heated to 573C (see Fig 4-10).Fig 4-14 Setting and thermal expansion of a typical investment of the hygroscopicexpansion type (Whip Mix Beauty-Cast, W/P = 0.30). The specimen was immersed inroom-temperature water during setting and then heated to 480C. This investment isbased on quartz and contains a halide, which gives it a small positive thermalexpansion, uniform over a range of about 150C. The dashed continuation of thecurve shows the effect of heating the investment to 700C.A mold temperature as low as 480C has the advantage of ensuring a fine grainstructure in the solidified casting, though this is not an important consideration if thealloy contains grain-refining elements. It has the disadvantage that carbon remainingfrom burnout of the wax pattern is oxidized very slowly. Excessive carbon depositsinterfere with venting of the mold cavity, so prolonged heating at the castingtemperature (preferably 1 hour) is needed to ensure that casting defects caused byinadequate venting ("back-pressure porosity") do not occur.2. Thermal expansion techniques. With thermal expansion techniques, the mold isusually heated to about 700C in order to gain maximum mold expansion. A highermold temperature should not be used or breakdown of the calcium sulfate binder canoccur in the presence of carbon, thereby liberating sulfur dioxide. The carbon may bepresent as graphite added to the original investment powder as a reducing agent ormay simply be carbon residue from burnout of the wax pattern. The reaction, whichinvolves reduction of the calcium sulfate binder, takes place in two stages:
The sulfur dioxide formed by the second reaction causes sulfide formation on thegold-alloy casting, resulting in discoloration and embrittlement of the alloy (OBrienand Nielsen, 1959).Investments for thermal expansion techniques may contain either cristobalite or quartzas the refractory; occasionally a mixture of both is used. Cristobalite investments havethe advantage that thermal expansion is fairly constant over the temperature range of400C to 700C, but have the disadvantage that the large expansion at 250C,resulting from the inversion of cristobalite, can cause mold cracking if heatingis not carefully controlled (Fig 4-15, curve A). It should be slow in the temperaturerange of 230C to 270C while the inversion of cristobalite is occurring throughoutthe mold.Quartz has a lower thermal expansion than cristobalite (see Fig 4-10), so most quartzinvestments for use in thermal expansion techniques contain additives to increasetheir thermal expansion. The expansion on heating is more gradual, so control ofheating rate is not as important, but maximum expansion is available only in thetemperature range of 600C to 700C (Fig 4-15, curve B).Fig 4-15 Setting and thermal expansion of two typical investments of the thermalexpansion type (curve A: Kerr Cristobalite Inlay, W/P = 0.38; curve B: R&R Gray,W/P = 0.25). With both materials the specimens were surrounded by a wet ring linerwhile setting and were then heated to 700C. The former material is an inlayinvestment based on cristobalite. The latter material is described as a universalinvestment but is most commonly used for casting dentures and is based on quartz,with the addition of sodium chloride to increase its thermal expansion.
At a burnout temperature of 700C, residual carbon is oxidized rapidly, so venting ofthe mold cavity is not a problem.3. The effect of a wet liner. In thermal expansion techniques, if a wet ring liner isused, not only the setting expansion but also the subsequent thermal expansion can beaffected. Once the investment has set, the extra water it absorbed from the liner hasthe same effect as if it had been added during mixing (ie, an increased W/P ratio).Therefore, the thermal expansion may be reduced.The same considerations apply to denture investments. The investment cast forms partof the final mold, and its expansion is the major factor determining the accuracy of thecasting. It sets in contact with a duplicating impression, usually an aqueous gel,which, like a wet ring liner, makes free water available to the setting investment withthe same effects as those already described.Control of expansion1. Composition. The manufacturer adjusts investment expansion by the choice ofrefractory and binder and sometimes by the use of suitable additives.2. W/P ratio. Decreasing the W/P ratio increases both setting expansion (in air orwater) and thermal expansion. The W/P ratio must be carefully controlled forreproducible mold expansion. Changes in expansion can most easily be effected bychanging the W/P ratio (Fig 4-16).Fig 4-16 The effect of changing the W/P ratio on the setting, thermal, and totalexpansions of a typical investment of the thermal expansion type, set against a dryceramic liner without vacuum investing, and then heated to 700C.
3. Period of exposure to water. In hygroscopic expansion techniques, additionalcontrol can be obtained by varying the length of time the setting investment isexposed to an aqueous environment. This may be achieved by reducing the time forwhich the setting investment is immersed in a water bath, or by adding controlledamounts of water to the top of the investment mix in the ring instead of immersing it.In the latter case, if only a small volume of water is added, it will be completelyabsorbed by the investment before setting is complete, and subsequent expansion willbe reduced. Varying the amount of added water varies the setting expansionproportionally.StrengthThe mold must be strong enough to withstand stresses at ambient temperatures (eg,during removal of the sprue former) and when heated to the recommended moldtemperature for casting (eg, during rapid entry of molten alloy). Strength properties ofinvestments are usually determined by testing in compression. Inlay investments havewet compressive strengths mostly in the range of 2 to 6 MPa. Because of the need tomake a working cast, denture investments have higher compressive strengths whenset, mostly in the range 9 to 14 MPa. In both investment types, changes in thecompressive strength on heating to the recommended casting temperature varyaccording to the presence of additives to control investment thermal expansion.Unless it is known whether an additive is present in an investment, and if so what it is,it is impossible to predict strength at the casting temperature from measurementsmade at ordinary ambient temperatures. Little information is available on thecompressive strength of gypsum-bonded investments at the casting temperature (hotstrength). In one study on a limited number of materials (Earnshaw, 1969b), it wasfound that the hot strength of four investments without additives was in the range of1.8 to 9.4 MPa; for three investments containing boric acid it was 6.3 to 13.3 MPa;and for three investments containing sodium chloride it was 3.1 to 5.2 MPa.Rapid-heat investmentsAlthough it was stated earlier that investments based on a cristobalite refractoryrequire slow heating while the inversion is occurring, some "rapid-heat"investments have been introduced, which are placed immediately after setting into afurnace preheated to 700C. At least some of these contain cristobalite as therefractory. The recommended technique is to place the mold, 30 minutes after thepattern is invested, into the preheated furnace for an additional 30 minutes; the castingis then made. A setting and thermal expansion curve for a typical example is shown inFig 4-17.
Fig 4-17 Setting and thermal expansion of a rapid-heat investment of the thermalexpansion type (GC Cristoquick, W/P = 0.33). As the manufacturer instructed, theinvestment was allowed to set against a dry ceramic liner for 30 minutes, then wasimmediately transferred to a furnace preheated to 700C.Little information is available on these materials. It can be seen in Fig 4-17 thatsetting expansion is still occurring rapidly at 30 minutes; measured under ordinaryconditions, it is not complete until 2 hours after mixing and measures 1.1%. The rapidrate of expansion at 30 minutes means that precise timing of placement of the mold inthe furnace is critical if reproducible mold expansion is to occur.Such a drastic heating program could be expected to cause severe thermal cracking inan ordinary cristobalite investment. Measurements on a mold in a lined inlay ringshowed that the periphery of the investment mass reached 250C within 6 minutes ofentering the hot furnace, while the center was at only 110C. The center of the molddid not reach 250C until 4 minutes later. Both periphery and center had reached amaximum of 690C within the 30-minute heating period.The indicated temperatures shown in Fig 4-17 were recorded by a thermocouplewhose hot junction was embedded in the center of a specimen that had about the samethickness as an inlay mold. The expansion caused by the inversion of cristobalite,shown on the graph as beginning at 110C and finishing at 170C, obviously tookplace when enough of the outer parts of the specimen had reached 250C to produce avolume change.These rapid-heat investments save laboratory time and simplify the casting procedure,as the furnace is maintained at 700C instead of being repeatedly heated and cooled.Despite the curtailed setting expansion, the investments total expansion under theseconditions was 1.95%, more than enough to compensate for the casting shrinkage ofordinary dental gold alloys.
Casting accuracyIn all casting procedures, after the molten metal or alloy has filled the mold, avolumetric contraction occurs in the liquid and then in the solid casting as it cools. Inaddition, with almost all metals and alloys there is a volumetric contraction duringsolidification.In dental casting, thermal contraction of the liquid alloy, and its solidificationcontraction, do not affect the dimensions of the casting because, under the influenceof the casting force, continued feeding of liquid alloy occurs from the excess in thesprue and button. Interruption to the flow of liquid during solidification, which maybe caused by premature freezing of an incorrectly designed sprue, will not cause anoverall contraction of the casting, but will lead to localized shrinkage porosity.Therefore, thermal contraction of the solidified casting, as it cools from solidus toambient temperature, remains as the sole cause of the observed casting shrinkage.Although this is a volumetric contraction, in dental technology dimensional changesare usually studied on a linear basis. It is assumed that these changes occurisotropicallyan assumption that is frequently unjustified.The fact that the observed casting shrinkage is thermal contraction of the solid alloycan be confirmed, at least for pure gold, by comparing measured values for its linearcasting shrinkage with a value calculated from its coefficient of linear thermalexpansion () and the temperature difference between its freezing temperature andambient.Results of direct measurements of the linear casting shrinkage of gold are shown inTable 4-5. A theoretical value can be calculated as follows:If 20C is taken as an average ambient temperature, the solidified gold cools through1,044 K. Total linear contraction per unit length is given by 1,044 16.7 10-6 =0.0174, which converts to 1.74%.Alloying gold will alter the value for and for solidus temperature. Calculationssimilar to that given previously have been made on a group of 12 high-noble-metalcasting alloys, and the calculated linear casting shrinkages varied from 1.65% to1.80% (Finger and Jorgensen, 1980). Thus an average value of 1.7% would apply togold and high-gold alloys. Table 4-5 Measured values for the linear casting shrinkage of pure goldReference Specimens (mm) Linear casting shrinkage (%)*Hollenback and Skinner Cylindrical rod (5.6 25) 1.67 0.02 (8)(1946)Earnshaw (1960) Cylindrical rod (6.3 60) 1.74 0.03 (6)
Nakai et al (1980) Rectangular prism (3 5 1.73 0.04 (9) 20)*Values are shown as mean and standard deviation, with number of tests inparentheses.It is conventionally assumed that compensation for this casting shrinkage is providedby mold expansion. Calculations of available compensation, however, must be basedon measurements of investment expansion made under conditions that reproducethose obtained in the casting ring (Earnshaw, 1988).Another factor that must be considered is the effect of the ring liner on investmentexpansion. Absorbent liners (asbestos and cellulose) vary in thickness, water uptake,and compressibility when wet. In thermal expansion techniques, some may not havesufficient compressibility to accommodate all of the increased setting expansionprovided by the availability of extra water, so that restriction of expansion could occurin a diametral direction in the ring (Morey and Earnshaw, 1992). Thus they affect to avarying degree the available mold expansion. Ceramic liners also vary in thicknessand compressibility, and if vacuum investing is used, they vary in the amount of waterthey absorb from the investment mix. Again they affect mold expansion in the ring toa varying degree (Earnshaw and Morey, 1992).The choice of casting-ring liner can thus affect, often to a significant extent, thedimensional accuracy of the casting. Figure 4-18 shows the relative inaccuracyproduced in full-crown castings made in a high-gold alloy with a gypsum-bondedcristobalite investment of the thermal expansion type, used with vacuum investing.The only variation in technique was the casting-ring liner used. All the liners werewater absorbent, and all were prewetted under controlled conditions. Three wereasbestos, and three cellulose.Fig 4-18 The effect of different prewetted ring liners on the relative inaccuracy ofgold-alloy full-crown castings. The castings were made with a cristobalite inlayinvestment of the thermal expansion type used with vacuum investing. C = control
castings made without a liner; GA, KA, and SH = castings made with asbestos liners;and AU, BE, and WM = castings made with cellulose liners. The height of each barshows the mean of at least 10 castings, while the narrow superimposed bar shows thestandard deviation.Figure 4-19 shows the results of similar experiments made with five different dryceramic liners used with and without vacuum investing. These two graphs show thegreat variation in casting inaccuracy produced when the same investment is used withdifferent casting-ring liners. This variation in inaccuracy is often unpredictable; inthese experiments, only when the ceramic liners were used with vacuum investingwas there any correlation between measured liner properties and casting inaccuracy.Fig 4-19 The effect of different dry ceramic ring liners on the relative inaccuracy ofgold-alloy full-crown castings. Conditions were the same as in Fig 4-18, except thatcastings were made with and without vacuum investing. C = control castings madewithout a liner; DK, GC, and KF = castings made with ceramic liners supplied fordental use; and K1 and K2 = castings made with liners cut from commercialinsulating material of the same type, supplied in sheets nominally 1 mm and 2 mmthick.Although with gypsum-bonded investments mold expansion is the major factoraffecting relative casting inaccuracy, mold strength at the casting temperature mustalso be considered. The average value of 1.7% for alloy thermal contractionrepresents the inherent casting shrinkage of the alloythe shrinkage that would occurin a casting that was free to contract without constraint. Under practical conditions thecasting is enclosed in a mold, and in all but the simplest castings its shape allowssome interlocking between investment and mold. In the early stages of cooling themold has a lower rate of thermal contraction than the casting; the thermal contractionof a typical high-gold alloy, cooling from its solidus temperature to 500C, would be
0.74%, while for a typical cristobalite inlay investment, cooling from 700C to 500C,it would be 0.20%. If the investment has a high hot strength, alloy thermal contractionwill be opposed by the mold; the degree of constraint will depend on the casting shapeand is usually directional. At temperatures near its solidus the alloy is weak andplastic, and mold constraint can cause anisotropic thermal contraction. When the alloyhas cooled enough to attain rigidity, a strong mold can cause plastic deformation byhot-working the alloy. Both factors cause anisotropic contraction and distortion of thecasting.A constant pattern of distortion of gold-alloy mesio-occluso-distal inlays has beenreported (Teteruck and Mumford, 1966) and can be attributed to directional restraintof alloy shrinkage by the mold (Earnshaw, 1969b). The gypsum-bonded investmentused in Teteruck and Mumfords experiments had a compressive strength at 700C inthe range of 4 to 6 MPa.Therefore, although with gypsum-bonded investments the total investment expansionthat occurs in the casting ring is the major factor affecting the casting inaccuracy, thehot strength of the mold must be considered. For the casting to reproduce accuratelythe size and shape of the original pattern, the investment expansion must compensatefully for the thermal contraction of the solid alloy, the ring and ring liner must allowthe potential expansion of the investment to be achieved isotropically, and theinvestment at the burnout temperature must not be so strong that it restricts theshrinkage of the alloy in any direction. On the other hand, it should not be so weakthat it may fracture during casting. A safe minimum compressive strength at 700C is1.8 MPa, and this allows substantially isotropic alloy contraction (Morey andEarnshaw, 1995).Storage of Gypsum ProductsWhen hemihydrate powders are exposed to the atmosphere, water vapor is adsorbed;the extent to which this occurs depends on the prevailing water vapor pressure(Torrance and Darvell, 1990). If sufficient water is adsorbed to form a liquid film, andif this becomes thick enough to function as a solvent, the setting reaction begins onthe surface of the powder particles, causing deterioration of the material. Gypsumcrystals are formed that act as nucleation centers when the powder is mixed withwater, and accelerate the setting rate. But if exposure of the powder continues, surfacehydration will form a layer of gypsum on each particle, hindering the access of waterto the hemihydrate, and the subsequent setting rate is retarded. If exposure continuesover a long period, eventually the material will not set properly, because insufficientunreacted hemihydrate remains to form a coherent set mass. This is equally likely tooccur in gypsum-bonded investments and will have the same effects.A long-standing recommendation to store gypsum products at relative humidities notgreater than 70% (Farmer and Skinner, 1942) appears satisfactory only attemperatures of 25C or lower, but of uncertain validity at higher temperatures. Toavoid deterioration, especially at high temperatures and high relative humidities, bulkgypsum products should be stored in closed bins, in a cool dry area of the laboratory."Topping up" of bins should not be done over old stock. Packaging of small quantitiesof powder, in waterproof containers, is a preferable method of storage in the
laboratory. Many die stones and gypsum-bonded investments are now supplied bytheir manufacturers packaged in this way.Glossaryacicular (of a crystal) Slender, needlelike.apparent density (of a powder) The mass of a sample divided by the volume itoccupies, measured at a specified degree of compaction. The measured volumeincludes all interstitial spaces and porosities, so powders with a poor packing abilityshow a low apparent density.calcination Prolonged heating of a substance at some temperature below its meltingtemperature.crystal habit (crystalline form) The external geometric shape of a crystal.crystal structure The regular three-dimensional arrangement of atoms within acrystal. This internal atomic arrangement is characteristic of a particular crystallinesolid, but may or may not be the same as the external shape of individual crystals.inversion A temperature-dependent change from one polymorphic form to another.Rapid (high-low) inversions involve only an alteration in bond angles within thecrystal structure (shear or displacive transformation). This change requires only asmall activation energy (excess energy required for the change to occur), so it occursrapidly on heating to the critical temperature and is rapidly reversible on cooling. Anexample is the inversion of quartz or cristobalite. Slow inversions involvebreaking of interatomic bonds and atomic diffusion to form a new crystal structure(reconstructive transformation). In a ceramic material in which a significant amountof the interatomic bonding is covalent, such as crystalline silica (Jastrzebski, 1976;Sosman, 1965), such a transformation involves a high activation energy, so prolongedhigh-temperature heating is needed for complete conversion. Because thetransformation is so sluggish, the new high-temperature phase is retained duringcooling to ambient temperature, where in most materials the rate of atomic diffusionis extremely slow. The high-temperature form therefore persists indefinitely as ametastable phase. An example is the quartz cristobalite inversion.isotropic Occurring equally in all directions. (Antonym: anisotropic.)nucleation center In an aqueous solution, a region where spontaneous, orderlydeposition of ions or molecules forms nuclei that continue to grow, beginning theprocess of crystallization. Normally this process involves heterogeneous nucleation,where nucleation centers are provided by the deposition of ions or molecules onexisting solid surfaces, such as solid particles (seeds) already present in the solution.nuclei poisoning The inactivation of nuclei of crystallization by the deposition offoreign material on their surfaces.polymorphism The existence of an element or chemical compound in more than twodifferent crystalline forms.
pseudomorphic A crystalline material whose crystal habit differs from the normalshape that would be dictated by its crystal structure.pseudoplasticity The behavior of non-Newtonian fluids in which the rate of shearincreases more than in proportion to the shearing stress (shear-thinning liquids). Thickmixes of plaster or stone are typical examples; they appear to be very viscous when atrest but flow readily when subjected to a shear stress (eg, stirring or vibration).refractory Capable of resisting high temperatures.relative surface area (of a powder) The total surface area of a given mass.specular (of reflections) Mirrorlike.spherulite A spherical aggregation of needle-shaped crystals radiating out from acommon center.water/powder (W/P) ratio The mixing proportions of plaster or stone, expressed as adecimal fraction. If 100 g of plaster is to be mixed with 50 g of water, the W/P ratio is0.50.water requirement The amount of water that must be added to a given mass ofplaster or stone to produce a mix of suitable viscosity.Discussion Questions1. How many different applications do gypsum products have in dentistry, as well asother fields?2. Why are storage conditions and shelf life important considerations in the use ofgypsum products? Why do these present special problems for the dental services oflarge organizations such as the armed forces?3. Why is it essential to follow directions to achieve the higher strengths possible withimproved die stones?4. What are the main methods of reducing bubbles in gypsum casts and molds?Study Questions(See Appendix E for answers.)1. What differences in chemical composition are there in the powders of plaster,stone, and die stone?2. What physical differences are there in the powders of plaster, stone, and die stone?How are these differences related to the methods of manufacture of the powders?3. Give typical W/P ratios for plaster, stone, and die stone. Why are these different?
For each type, assuming that the setting reaction goes to completion, what percentageof the mass of the set material would consist of free water?4. What chemical and physical changes accompany the setting of gypsum products?5. What is the difference between the microstructures of gypsum casts made fromplaster and stone? What is the cause of this difference, and what is its effect onstrength properties?6. What is meant by the setting time of gypsum products? What is the practicalsignificance of (a) the loss of surface gloss, (b) the Gillmore initial set, and (c) theVicat initial set?7. Explain how the manufacturer of a dental gypsum product adjusts its rate ofsetting.8. For a given gypsum product, what is the effect of increasing the W/P ratio on therate of setting? Explain.9. Theoretically, the setting of gypsum products should be accompanied by avolumetric contraction. Why is a setting expansion observed in practice?10. Why do gypsum products show a greater setting expansion in water than in air?11. What is the practical significance of the setting expansion of dental gypsumproducts?12. Give typical values for the linear setting expansion in air of impression plaster,plaster, stone, and low-expansion and high-expansion die stones.13. Explain how the manufacturer of a gypsum product controls its setting expansion.14. What practical limits are placed on the extent of this control?15. For a given gypsum product, what is the effect of increasing the W/P ratio onsetting expansion? Explain.16. What is the practical significance of the tensile strength and the compressivestrength of dental gypsum products?17. For a given gypsum product, what is the effect of increasing the W/P ratio ontensile strength and compressive strength? Explain.18. What is the effect of drying on the tensile strength and the compressive strength ofcast gypsum? Explain.19. What constituents are likely to be present in a gypsum-bonded investmentpowder? Give the function of each.20. Within normal limits, what effect does increasing the proportion of refractory
filler in an investment have on (a) rate of setting, (b) setting expansion in air, (c)setting expansion in water, (d) thermal expansion, and (e) compressive strength?21. How does the investment set?22. What is the practical significance of microscopic porosity formed in theinvestment mass during setting?23. What are the requirements for the particle size of an investment powder? Givereasons.24. Why is the particle size of the refractory filler more important than that of thebinder?25. What is the most important property of an investment? Why?26. What is a hygroscopic expansion technique?27. What is a thermal expansion technique?28. In hygroscopic expansion techniques, why is prolonged heating of the mold at theburnout temperature necessary?29. How can the user of a dental investment discover whether it contains cristobaliteor quartz as a refractory? What is the practical importance of this information?30. Why is control of the heating rate more important with a cristobalite investmentthan with a quartz investment?31. Why is an accurate furnace pyrometer more important with a quartz investmentthan with a cristobalite investment?32. Why should gypsum-bonded investments not be heated above 700C?33. In thermal expansion techniques, what is the effect of a wet liner on theinvestments setting expansion?34. What is the effect of increasing the W/P ratio on (a) the investments settingexpansion in air, (b) its setting expansion in water, and (c) its thermal expansion.35. In hygroscopic expansion techniques, how can mold expansion be controlled bythe user?36. In thermal expansion techniques, how can mold expansion be controlled by theuser?37. What is the practical significance of the compressive strength of the investment atthe casting temperature?38. How should gypsum products be stored in a dental laboratory? How can incorrect
storage conditions affect these materials?Recommended ReadingAndrews H (1951). The production, properties and uses of calcium sulphate plasters.London: Building Research Congress, Division 2, Part F, 135.Anusavice K (1996). Phillips Science of Dental Materials, ed 10. Philadelphia:Saunders, 196-198.Asgar K (1972). Casting alloys in dentistry. In: Dickson G, Cassel JM (eds). DentalMaterials Research. Washington, DC: National Bureau of Standards, SP 354, 63.Asgar K, Mahler DB, Peyton FA (1955). Hygroscopic technique for inlay castingusing controlled water additions. J Prosthet Dent 5:711.Barnard G (1981). Recent developments in using ceramic fibres in reducingatmospheres. Metals Australasia 13:10.Beretka J, Crook DN, King GA, Middleton LW (1980). Applications of by-productgypsum in the plaster industry. Melbourne: Eighth Australian Chemical EngineeringConference, August.Bergman B, Bergman M, Olsson S (1985). Alginate impression materials,dimensional stability and surface detail sharpness following treatment withdisinfectant solutions. Swed Dent J 9:255.Bever MB (ed) (1986). Encyclopedia of Materials Science and Engineering.Elmsford, NY: Pergamon Press, 1098.Buchanan AS, Worner HK (1945). Changes in the composition and settingcharacteristics of plaster of Paris on exposure to high humidity atmosphere. J DentRes 24:65.Collins PF (1935). Dental Investment Composition and Process. US Patent:2,006,733.Collins PF (1941a). Dental Investment Composition. U.S. Patent: 2,247,571.Collins PF (1941b). Dental Investment Composition. US Patent: 2,247,572.Collins PF (1941c). Dental Investment Composition. US Patent: 2,247,573.Combe EC (1974). Recent developments in model and die materials. In: vonFraunhofer JA (ed). Scientific Aspects of Dental Materials. London: Butterworths,402-415.Combe EC, Smith DC (1965). The effects of some organic acids and salts on thesetting of gypsum plaster. II. Tartrates. J Appl Chem 15:367.
Combe EC, Smith DC (1966). The effects of some organic acids and salts on thesetting of gypsum plaster. III. Citrates. J Appl Chem 16:73.Combe EC, Smith DC (1968). Studies on the preparation of calcium sulphatehemihydrate by an autoclave process. J Appl Chem 18:307.Craig RG (ed) (1997). Restorative Dental Materials, ed 10. St Louis: Mosby-YearBook, 347.Donnison JA, Chong MP, Docking AR (1960). Calorimetric study of the hygrosopicsetting of calcined gypsum. Aust Dent J 5:269.Donovan T, Chee WWL (1989). Preliminary investigation of a disinfected gypsumdie stone. Int J Prosthodont 2:245.Dootz ER, Craig RG, Peyton FA (1965). Influence of investments and duplicatingprocedures on the accuracy of partial denture castings. J Prosthet Dent 15:679.Earnshaw R (1960). Further measurements of the casting shrinkage of dental cobalt-chromium alloys. Br Dent J 109:238.Earnshaw R (1964). The effect of restrictive stress on the setting expansion ofgypsum-bonded investments. Aust Dent J 9:169.Earnshaw R (1969a) The effect of restrictive stress on the hygroscopic settingexpansion of gypsum-bonded investments. Aust Dent J 14:22.Earnshaw R (1969b). The compressive strength of gypsum-bonded investments athigh temperatures. Aust Dent J 14:264.Earnshaw R (1976). Effects of additives on the thermal expansion of cast gypsum. JDent Res 55:518.Earnshaw R (1988). The effect of casting ring liners on the potential expansion of agypsum-bonded investment. J Dent Res 67:1366.Earnshaw R, Marks BI (1964). The measurement of setting time of gypsum products.Aust Dent J 9:17.Earnshaw R, Morey EF (1992). The fit of gold-alloy full-crown castings made withceramic casting ring liners. J Dent Res 71:1865.Earnshaw R, Mori T (1985). Contraction of cast gypsum between 200C and 500C. JDent Res 64:658.Eberl JJ, Ingram AR (1949). Process for making high-strength plaster of Paris. IndEng Chem 41:106.Fairhurst CW (1960). Compressive properties of dental gypsum. J Dent Res 39:812.
Farmer GJ, Skinner EW (1942). Effect of relative humidity on the setting time ofplaster of Paris. Northwestern Univ Bull 43:12.Finger W, Jorgensen KD (1980). An improved dental casting investment. Scand JDent Res 88:278.Finger W, Jorgensen KD, Ono T (1980). Strength properties of some gypsum-bondedinvestments. Scand J Dent Res 88:155.Fusayama T (1959). Factors and technique of precision casting. J Prosthet Dent 9:468,486.Fusayama T (1964). Synthetic study on precision casting. Bull Tokyo Med Dent Univ11:165.Gay P (1965a). Some crystallographic studies in the system CaSO4 - CaSO42H2O. I.The polymorphism of anhydrous CaSO4. Mineral Mag 35:347.Gay P (1965b). Some crystallographic studies in the system CaSO4 - CaSO42H2O. II.The hydrous forms. Mineral Mag 35:354.Gibson CS, Johnson RN (1932). Investigations of the setting of plaster of Paris. J SocChem Ind (Transactions) 51:25.Greener EH, Harcourt JK, Lautenschlager EP (1972). Materials Science in Dentistry.Baltimore: Williams & Wilkins, 276.Gregg SJ (1965). The Surface Chemistry of Solids, ed 2. London: Chapman and Hall,232.Gutt WH, Smith MA (1967). The form of calcium sulphate. Trans Br Ceram Soc66:337.Haddon CL (1944). Gypsum plaster products. Chem Ind 22:190.Haddon CL, Cafferata BJ (1944). Improvements in the manufacture of plaster ofParis. British Patent 563,019.Harcourt JK, Lautenschlager EP (1970). Accelerated and retarded dental plastersetting investigated by X-ray diffraction. J Dent Res 49:502.Hoggatt GA (1952). Method of producing gypsum plaster. US Patent:2,616,789.Hollenback GM (1962). A brief history of the cast restoration. J South Calif StateDent Assoc 30:8.Hollenback GM, Skinner EW (1946). Shrinkage during casting of gold and goldalloys. J Am Dent Assoc 33:1391.International Standards Organization (1990). International Standard 7490, Dental
Gypsum-bonded Casting Investments for Gold Alloys. Geneva, 1.International Standards Organization (1998). International Standard 6873, DentalGypsum Products. Geneva, 1.Ivanovski S, Savage NW, Brockhurst PJ, Bird P (1995). Disinfection of dental stonecasts: antimicrobial effects and physical property alterations. Dent Mater 11:19.Jastrzebski ZD (1976). The Nature and Properties of Engineering Materials, ed 2.New York: John Wiley & Sons, 59.Johnson GH, Drennon DG, Powell GL (1988). Accuracy of elastomeric impressionsdisinfected by immersion. J Am Dent Assoc 116:525.Jorgensen KD, Posner AS (1959). Study of the setting of plaster. J Dent Res 38:491.Khalil AA, Hussein AT, Gad GM (1971). On the thermochemistry of gypsum. J ApplChem Biotechnol 21:314.Kingery WD, Bower HK, Uhlmann DR (1976). Introduction to Ceramics, ed 2. NewYork: John Wiley & Sons, 81-87.Koslowski T, Ludwig U (1984). Retardation of gypsum plasters with citric acid:mechanism and properties. In: Kuntze RA (ed). The Chemistry and Technology ofGypsum ASTM STP861. Philadelphia: American Society for Testing and Materials,97-104.Lager GA, Armbruster T, Rotella FJ, Jorgensen JD, Flinks DG (1984). Acrystallographic study of the low-temperature dehydration products of gypsum. AmMineral 69:910.Lautenschlager EP, Corbin F (1969). Investigation on the expansion of dental stone. JDent Res 48:206.Lautenschlager EP, Harcourt JK, Ploszaj LC (1969). Setting reactions of gypsummaterials investigated by X-ray diffraction. J Dent Res 48:43.Mahler DB, Ady AB (1960). An explanation for the hygroscopic setting expansion ofdental gypsum products. J Dent Res 39:578.Matsuya S, Yamane M (1981). Decomposition of gypsum-bonded investments. JDent Res 60:1418.McGill S, Narea EM, Suchak AJ, Stanford JW (1988). The effect of disinfectingsolutions on alginate and gypsum materials. J Dent Res 67:281.Moore TE (1933). Method of making dental castings and composition employed insaid method. US Patent:1,924,874.Morey EF, Earnshaw R (1992). The fit of gold-alloy full-crown castings made with
pre-wetted casting ring liners. J Dent Res 71:1858.Morey EF, Earnshaw R (1995). The effect of potential investment expansion and hotstrength on the fit of full-crown castings made with a gypsum-bonded investment.Dent Mater 11:312.Mori T (1982). The effect of boric acid on the thermal behavior of cast gypsum. DentMater J 1:73.Mori T (1985). Transformation of CaSO4(III) to CaSO4(II) in gypsum-bondedinvestments. J Dent Res 64:658.Mori T (1986). Thermal behavior of the gypsum binder in dental casting investments.J Dent Res 65:877.Mori T, Yamane M (1982). Fractography of cast gypsum. Aust Dent J 27:30.Nakai A, Nakamura Y, Seki S-I, Kakuta K, Kawashima J-I (1980). Measurement ofcasting shrinkage with U-type tungsten die. J Jap Dent Apparat Mat 21:122.Neiman R (1941). Investment. US Patent:2,247,395.Neiman R, Ernst RC, Steinbock EA (1943a). Investment composition. USPatent:2,313,085.Neiman R, Ernst RC, Steinbock EA (1943b). Investment composition. USPatent:2,313,086.OBrien WJ, Nielsen JP (1959). Decomposition of gypsum investment in the presenceof carbon. J Dent Res 38:541.Offutt JS, Lambe CM (1947). Plasters and gypsum cements for the ceramic industry.Am Ceram Soc Bull 26:29.Ohno H, Nakano S, Miyakawa O, Watanabe K, Shiokawa N (1982). Effects of phasetransformations of silicas and calcium sulfates on the compressive strength ofgypsum-bonded investments at high temperatures. J Dent Res 61:1077.Olsson S, Bergman B, Bergman M (1987). Agar impression materials, dimensionalstability and surface detail sharpness following treatment with disinfectant solutions.Swed Dent J 11:169.Pomes CD, Slack GL, Wise MW (1950). Surface roughness of dental castings. J AmDent Assoc 41:545.Priest G, Horner, JA (1980). Fibrous ceramic aluminium silicate as an alternative toasbestos liners. J Prosthet Dent 44:51.Randel WS, Dailey MC (1933). High strength calcined gypsum and process ofmanufacture of same. US Patent: 1,901,051.
Ridge MJ (1959). Acceleration of the set of gypsum plaster. Aust J Appl Sci 10:218.Ridge MJ (1960). Mechanism of setting of gypsum plaster. Rev Pure Appl Chem10:243.Ridge MJ (1961). Factors determining the water requirement of gypsum plaster. JAppl Chem 11:287.Ridge MJ (1972). The hydration of calcium sulphate hemihydrate. Proc Royal AustralChem Inst 39:55.Ridge MJ, Beretka J (1969). Calcium sulphate hemihydrate and its hydration. RevPure Appl Chem 19:17.Russell JJ (1960). The effect of moisture content on the compressive strength of smallcubes of some cast gypsum plasters. Zement-Kalk-Gips 13:345.Schutt RW (1989). Bactericidal effect of a disinfectant dental stone on irreversiblehydrocolloid impressions and stone casts. J Prosthet Dent 62:605.Selby A (1979). The Relationship Between the Viscosity of the Mix and the TensileStrength of Cast Gypsum [thesis]. Sydney: University of Sydney.Sodeau WH, Gibson CS (1927). The use of plaster of Paris as an impression material.Br Dent J 48:70.Sosman RB (1965). The Phases of Silica. New Brunswick: Rutgers University Press,32, 36-42.Souder W, Paffenbarger GC (1942). Physical Properties of Dental Materials.Washington, DC: National Bureau of Standards, C433, 80-93.Suffert LW, Mahler DB (1955). Reproducibility of gold castings made by present daydental casting technics. J Am Dent Assoc 50:1.Sweeney WT, Taylor DB (1950). Dimensional changes in dental stone and plaster. JDent Res 29:749.Taylor NO, Paffenbarger GC, Sweeney WT (1930). Dental inlay casting investments:physical properties and a specification. J Am Dent Assoc 17:2266.Teteruck WR, Mumford G (1966). The fit of certain dental casting alloys usingdifferent investing materials and techniques. J Prosthet Dent 16:910.Torrance A, Darvell BW (1990). Effect of humidity on calcium sulphate hemihydrate.Aust Dent J 35:230.Weinstein LJ (1929). Composition for dental moulds. US Patent: 1,708,436.
Weiser HB, Milligan WD, Eckholm WC (1936). The mechanism of dehydration ofcalcium sulfate hemihydrate. J Am Chem Soc 58:1261.Whyte MP, Brockhurst PJ (1996). The effect of steam sterilisation on the propertiesof set dental gypsum models. Aust Dent J 41:128.Worner HK (1942). Dental plasters. Part I. Aust J Dent 46:1.Yli-Urpo A, Oilo G, Syverud M (1982). The effect of asbestos-alternatives on theaccuracy of cast veneer crowns. Swed Dent J 6:127.
Chapter 5. Surface Phenomena and Adhesion to Tooth StructureIntroductionSurface phenomena include surface tension, wetting, adsorption, capillary action, andadhesion. Applications include capillary penetration around restorations, dentures,and teeth, and adhesion to tooth structure by sealants and restorative materials.Surface EnergyIntroductionAtoms and molecules at the surfaces of liquids and solids possess more energy(surface energy) than do those in the interior. In the case of liquids, this energy iscalled surface tension. As illustrated in Fig 5-1,Fig 5-1 Distribution of vacancies (open circles) within isolated capillary liquid. Morevacancies are present at the surface (a) as compared to the bulk (b). Fewer vacanciesare found at the liquid-solid interface (c). (From OBrien, 1970. Modified withpermission.)the molecules at the surface are farther apart due to loss of molecules by evaporation.From Fig 5-2 it can be seen that this greater average separation leads to a netattraction between molecules and a higher energy of attraction. This results in asurface contractile force or surface tension, which causes the liquid to form drops andto exhibit a surface skin that resists extension or penetration.
Fig 5-2 Relations between intermolecular forces, intermolecular energies, anddistance as affected by distance (rij) between molecules. Departure from equilibriumdistance rij causes repulsion or attraction. (From OBrien, 1970. Reprinted withpermission.)The surface energies of several substances are given in Table 5-1. It can be seen thatthe surface energies of oxides and metals are greater than those of liquids. In general,the higher the bond strength of a substance, the greater the surface energy. Sincemetallic bonds are much stronger than the van der Waals bonds of liquids, metalshave higher surface energies. The units of surface energy are ergs/cm2, but the surfacetension of liquids is often expressed in the equivalent units of dynes/cm. The totalsurface energy of a system is the product of the surface energy of the material and thetotal area. Therefore, a high total surface energy exists if a material is finely divided(powder or colloid) to provide a large surface area, especially if the material has ahigh surface energy per unit area (eg, metals or ionic crystals). Table 5-1 Surface energies of various substancesSubstance Surface energy Temperature 2 (erg/cm ) (C)Water 72 20Benzene 29 20Olive oil 36 20Saliva 56 23NaCl crystal 300 25Dental porcelain 365 1,000Copper, solid 1,430 1,080Silver, solid 1,140 750
SinteringSintering is a densification process in which finely divided particles are heated incontact. The firing of porcelain is a sintering process used for forming denture teethand porcelain-fused-to-metal crowns. The driving force for this process is thereduction of total surface area and, thus, total surface energy.WettingWetting is defined in terms of the degree of spreading of a liquid drop on a solidsurface. The contact angle (), formed by the liquid surface and the interfaceseparating the liquid and solid, is used as a measure of the degree of wetting (Fig 5-3).Fig 5-3 Wetting. Low contact angle indicates good wetting (left); high contact angleindicates poor wetting (right). (From OBrien and Ryge, 1965b. Reprinted withpermission.)A 0-degree contact angle indicates complete wetting, and low values correspond togood wetting. Values above 90 degrees indicate poor wetting. Table 5-2 gives contactangles for several systems. Table 5-2 Contact angles of liquids on solidsSolid Liquid Contact angle (degrees)Amalgam alloy Water 80Silicate cement Water 10Acrylic Water 75Teflon Water 110Ag3Sn Mercury 140Gold alloys Porcelain enamel 40-50Nickel alloys Porcelain enamel 80-100Hydron Water 0Etched enamel Pit and fissure sealants 0
Good wetting promotes capillary penetration and adhesion and indicates strongattraction between the liquid and solid surface molecules. Good wetting is importantin soldering and is a factor in better denture retention. A more natural appearance isachieved if restorative materials are wetted by a thin film of saliva. Hydrophobicsubstances are those that exhibit high contact angles with water (eg, Teflon, siliconecoatings) (Figs 5-4 and 5-5).Fig 5-4 Hydrophobic film of fluorinated polymer on enamel giving high contactangle. (From OBrien, 1973a.)
Fig 5-5 Poor wetting shown by porcelain enamel drops on nongold alloy at 1,040C.The furnace thermocouple is seen above the drops. (From OBrien and Ryge, 1965a.Reprinted with permission.)AdsorptionTo reduce surface energy, atoms and molecules that are mobile will concentrate athigh energy surfaces. For example, finely divided charcoal will adsorb quantities ofseveral gases; detergent (or soap) molecules will concentrate at the surface of water,leading to a large reduction in surface energy. Adsorption is strongest when there islarge energy saving (high surface energy material and large surface area) and slowsdown as the surface is covered.Adsorption occurs only at the surface, whereas absorption involves penetration anduptake by the interior of the material (as in swelling of hydrocolloid impressionmaterials in water). Gold foil adsorbs gases readily and must be degassed before use.ColloidsIntroductionColloids contain material that is present in particles larger than ordinary atoms ormolecules but still invisible to the unaided eye (ie, 10 to 10,000 A). There are threetypes of colloidal systems.Insoluble dispersed particlesThese are called lyophobic, since the materials are insoluble in a liquid medium (eg,sulfur in water). The fine particles acquire electrical charges that keep them insuspension. Table 5-3 gives a classification of the types of lyophobic systems. As oneexample of such a system, colloidal gold is used to form a gold coating on alloys to bebonded to porcelain. Although lyophobic systems may last for many years, they areunstable and can be precipitated by electrical methods (smokes) or gravity(emulsions). Table 5-3 Classification of lyophobic colloids
Dispersed phase Continuous phase TypeSolid Liquid SolSolid Gas Aerosol (smoke)Liquid Liquid EmulsionLiquid Gas Aerosol (fog)Gas Liquid FoamGas Solid FoamLarge moleculesThese systems are true solutions in which the dispersed molecules are of colloidaldimension. They are stable, but the large size of the macromolecules present gives thesolutions properties similar to those of lyophobic systems.Dental materials consisting of such solutions include agar and alginate hydrocolloidimpression materials. These materials aggregate to form gels, due to van der Waalsbonding between the long chain molecules. Gels undergo imbibition and syneresis(absorption and exudation of solvent) with resulting swelling and shrinkage,respectively. This behavior is responsible for the dimensional instability of theseimpression materials. As with other colloidal systems, the liquid state is called the solstate.Association colloidsThese are aggregates of smaller molecules that achieve colloidal size. Surface activeagents, such as soaps and detergents, are examples. Each molecule consists of a long-chain hydrocarbon with a small charged polar group at one end (eg, sodiumpalmitate). The aggregates formed by these molecules, called micelles, often arespherical; in aqueous systems, the hydrocarbon ends gather in the center of themicelle and the polar groups are exposed on the outside. This system is useful incleaning because grease and other organic films are dissolved in the interior of themicelles and held in suspension.Capillary PenetrationIntroductionThe surface energy of a liquid creates pressure that drives the liquid into crevices,narrow spaces, and thin tubes. Saliva penetration around restorations (leakage) andaround teeth are important examples. Capillary penetration of saliva is also partiallyresponsible for denture retention.Capillary riseIf a glass tube is immersed in a liquid (Fig 5-6(a)), the capillary rise, h, is given by theformula:
where is the surface tension, is the contact angle, r is the tube radius, d is theliquids density, and g is the gravitational constant, 980 dynes/g. If the contact angle isless than 90 degrees, as in water-glass and saliva-enamel systems, elevation of theliquid occurs. However, if the contact angle exceeds 90 degrees (eg, mercury on glassor water on Teflon), depression takes place and pressure must be applied to force theliquid into the space (Fig 5-6(b)). If the capillary liquid is not connected with areservoir of liquid, isolated capillaries (isocaps) are formed (Fig 5-7). The liquids inisocaps exert adhesive force on the walls of the capillary, which can be strong for thinlayers. This capillary adhesion is a factor in denture retention.Fig 5-6 Effect of contact angle on capillary penetration: (a) capillary elevation withconcave meniscus (low contact angle); (b) capillary depression with convex meniscus(high contact angle). P is the capillary pressure. (From OBrien et al, 1968. Modifiedwith permission.)Fig 5-7 (a) Capillary liquid in contact with a reservoir. (b, c) Isolated capillaries.(From OBrien and Fan, 1975. Modified with permission.)
To increase the penetration of saliva around acrylic dentures, surface coatings of silicaare applied to reduce the contact angle. The main factor here, however, ismaintenance of a small gap distance (ie, close adaptation between denture andmucosa), as shown in Fig 5-8.Fig 5-8 Capillary space between denture and mucosa.Penetration coefficientThe rate of movement of a liquid into a capillary space is related to the surface tension(), contact angle (), and viscosity (), as given by the penetration coefficient (PC):Therefore, a liquid with low viscosity, high surface tension, and low contact angle (ie,good wetting) will penetrate faster than one with the opposite combination ofproperties. This is important in adhesives such as pit and fissure sealants, which mustpenetrate into surface roughness and crevices quickly for good bonding.AdhesionIntroductionAdhesion is the attachment of materials in contact that resists the forces of separation.Adhesive phenomena are critical in many areas of dental materials, including thebonding of porcelains to metals and the adhesion of resins to tooth structure. Severaltypes of adhesive bonds may be identified according to the classifications in Fig 5-9.Mechanical adhesion depends on mechanical interlocking of the two phases and mayinclude microscopic attachments, as in the case of resin bonding to etched enamel orhoop stresses of a porcelain around a metal core. Chemical adhesion relies onchemical bonding between two phases. Diffusion bonding results when one phase
penetrates by diffusion into the surface of a second phase and forms a hybrid layer,which is a composite of the two materials.Fig 5-9 Classification of bonding mechanisms.Several factors affect the strength of an adhesive bond:1. Cleanliness. The surfaces to be attached should be free of debris andcontamination.2. Penetration of surface. Liquid adhesives (eg, sealants and bonding agents) mustpenetrate into crevices created by acid etching of enamel and dentin. The penetrationcoefficient of the liquid was discussed in the preceding section.3. Chemical reactions. The formation of strong chemical bonds across an interfacewill increase the number of attachment sites. This is believed to occur betweenporcelain enamels and the oxides of tin, indium, and iron formed on the surfaces ofalloys containing high proportions of precious metals. On the other hand, a weakcompound may be formed by a chemical reaction, resulting in a weak boundary layer(eg, certain oxides) rather than attachment sites.4. Shrinkage of adhesive. Liquid adhesives solidify by processes such as solventevaporation and polymerization, and shrinkage results. The adhesive may then pullaway from the substrate, or stresses may be created that weaken the bond. Shrinkageis toward the center of the adhesive mass (Fig 5-10). However, shrinkage in light-cured systems occurs toward the light source.
Fig 5-10 Shrinkage of adhesive toward center of mass during curing: (a) film, (b)crowns, (c) filling. A = adhesive. (From Lee, 1973.)5. Thermal stresses. If the adhesive and substrate have different thermal expansioncoefficients, changes in temperature will produce stresses in the bond. For example,porcelain enamels are bonded to alloys at high temperatures and then cooled to roomtemperature. Close matching of the thermal expansion coefficients of porcelainenamel and alloy is required to minimize stresses.6. Corrosive environment. The presence of water or corrosive liquid or vapor willoften lead to deterioration of an adhesive bond. For example, acrylic resins willinitially adhere to clean unetched tooth enamel, but the bond deteriorates upon storagein water.Adhesion to enamelEnamel is highly mineralized tissue composed of hydroxyapatite (about 96%), water(about 4%), and collagen (about 1%). Treatment with 35% to 50% phosphoric acidresults in selective demineralization of exposed enamel rod ends, leaving a surfacewith increased area and high energy (Fig 5-11).
Fig 5-11 Microstructure of enamel etched with phosphoric acid. (Originalmagnification 4,100.) High surface energy permits efficient wetting by the hydrophobic resin, whichpenetrates to form tags (Fig 5-12) and provides bond strength through mechanicalinterlocking. Contamination of the dry, etched surface by saliva or water, orincomplete removal of the etching agent or dissolved minerals, adversely affects thelong-term stability of the bond. The acid-etch technique produces shear bondstrengths during laboratory testing of 20 to 22 MPa, on average above those producedat the composite-enamel interface by shrinkage due to polymerization (~18 MPa).
Fig 5-12 Attachment sites of polymer tags (T) in etched enamel (E).Acid etching of enamel is a widely accepted clinical procedure and has increased thelife of resin composite restorations by decreasing the possibility of marginal staining,secondary caries, and postoperative sensitivity due to sealing of the enamel margins.The acid-etch technique allows the use of a more conservative cavity preparation and,to a certain extent, restores fracture resistance to the bonded structure.Adhesion to dentinHuman dentin is composed of hydroxyapatite (45%), water (25%), and organic matrix(30%). Bonding to dentin is routinely achieved by etching and the diffusion ofhydrophilic primers, followed by application of bonding resins. Composite restorativematerials are then bonded to the resin layer; the resin-dentin interface has laboratorybond strengths of 22 to 35 MPa.The stages of conditioning and resin impregnation are illustrated in Fig 5-13. In thefirst stage, the conditioning dissolves the smear layer of debris on the den-tinalsurface and in tubules, partially decalcifies the dentin to an optimum depth of around5 um, and opens dentinal tubules. In the second stage, hydrophilic primer couplingagents such as 2-hydroxyethyl methacrylate (HEMA), 4-methyloxyethyl trimellitateanhydride (4-META), and glutaraldehyde are applied and penetrate into both thetubules and the decalcified intertubular dentin. The primer stabilizes collagen andfacilitates the penetration of the bonding resins, which are bisphenol glycidylmethacrylate (bis-GMA) or urethane dimethacrylate (UDMA) monomers that areapplied and polymerized.
Fig 5-13 Schematic representation of the resin-dentin interdiffusion zone at (top) theconditioning phase and (bottom) the resin-impregnation phase. (From Van Meerbeek,1993. Reprinted with permission.)There are two main types of conditioner components in current use. First there are thestrong acids (phosphoric and citric acids). These acids nonselectively attack the dentinand the smear layer and expose the tubules (Fig 5-14). Other acids (10% maleic acid)are used to dissolve both inorganic and organic tissues, but they are less aggressive.The second type of conditioner is weak acids (eg, polyacrylic acid), which are used todissolve only the smear layer without demineralizing dentin.
Fig 5-14 Dentin after deep etching with 20% phosphoric acid for 2 minutes. (Originalmagnification 5,000.)The layer of resin penetration is known as the hybrid zone and may extend from 1 to5 um deep (Fig 5-15). If there is a layer of decalcified dentin below the hybrid zone, itacts to weaken the bond due to the resin being absent. This can be avoided by limitingthe depth of etching with shorter etching times or less concentrated acids. Excessivedrying of the dentin layer before primer application is not desirable, because it leadsto collapse of the surface collagen layer and reduces primer diffusion. Lateralpenetration into peritubular dentin may also take place from resin that has penetratedfirst into the tubules. Figure 5-16 shows a scanning electron micrograph (SEM) of afractured hybrid layer with tags that have been plucked from the tubules during bondtesting. Resin tags in tubules are not strongly anchored due to polymerizationshrinkage and dentinal fluid.Fig 5-15 Cross-sectional view of resin-etched bovine dentin interface showing resin(R), the hybrid zone (H), and demineralized dentin (DD). (From Wang andNakabayashi, 1991. Reprinted with permission.)
Fig 5-16 Scanning electron micrograph of a fractured resin-dentin interface showingresin tags plucked from tubules. DD = demineralized dentin. (From Wang andNakabayashi, 1991. Reprinted with permission.)Bond-strength values of materials to enamel and dentin are given in Table 5-4. Thelaboratory bond-strength values to dentin vary significantly more than those reportedfor enamel. Therefore, bonding to dentin is less reliable. Table 5-4 Tensile bond strengths obtained between various restorativematerials and tooth substance*Bonding couple Bond strength (MPa)Acid-etched enamel + resin (eg, bis-GMA) 16-20Enamel + glass ionomer 5Dentin + glass ionomer 1-3Dentin + glass ionomer (light cured) 3-11Enamel + NPG-GMA 2-5Dentin + 4-META 2Dentin + mordant ion + 4-META 18Dentin + phosphate esters of bis-GMA 3-5Acid-etched enamel + phosphate esters of bis-GMA 20Dentin + maleic acid/HEMA + HEMA/bis-GMA 18Acid-etched enamel + HEMA/bis-GMA 23Dentin + isocyanate 4Dentin + glutaraldehyde/HEMA 18*Derived from McCabe (1990).
A major difference between commercial products is the number of components thatneed to be applied in sequence. Several multicomponent products contain an etchant(conditioning agent), primer, and bonding resin. According to CRA (2000), there arefour types of dentin adhesive products:Type 1: Etchant applied and rinsed off to remove smear layer; primer and adhesiveapplied separatelyType 2: Etchant applied and rinsed off to remove smear layer; primer and adhesiveapplied in a single solutionType 3: Self-etching primer applied to dissolve smear layer and not rinsed off;adhesive applied separatelyType 4: Self-etching primer and adhesive applied as a single solution to dissolve thesmear layerSingle-component products (Fig 5-17) include a gel etchant and a one-bottlecomponent that contains the primer and resin (bis-GMA). This appears to be thedirection for future developments since it is simpler than the multicomponent"chemistry sets."Fig 5-17 A one-step dentin adhesive. A combination of the two components containsetchant, primer, and initiators. (One-Up Bond F; courtesy of J. Morita.)
Glossaryacid-etch technique The method of etching enamel with an acid to produce aroughened surface for resin bonding.adhesion Surface attachment of two materials (as opposed to cohesion, which is thebonding within a single material).capillary penetration Movement of a liquid into a crevice or tube because ofcapillary pressure.colloid Material in which a constituent in a finely divided state that is invisible to theeye but capable of scattering light is suspended. Although colloids are not truesolutions, many have long-term stability.contact angle Angle formed between the surface of a liquid drop and the solid surfaceon which it rests. Usually designated by the Greek letter and used as a measure ofwetting.hybrid zone A layer of dentin that contains resin. Produced by etching and resindiffusion.hydrophobic Water-repellent; showing a high contact angle.isocaps Isolated capillary bridges formed between solid surfaces.lyophobic colloid An unstable colloid made from insoluble dispersed material in finesuspension.micelles Aggregated molecules formed in association colloids.penetration coefficient Combination of the properties of viscosity, surface tension,and contact angle that promotes rapid capillary penetration.sintering Densification process in which solid particles are fused together, usually athigh temperatures.surface energy Extra energy that atoms or molecules on the surface of a substancehave over those in the interior. The units are erg/cm2.surface tension The surface energy of a liquid.wetting The spreading of a liquid drop on the surface of a solid.Discussion Questions1. Why is wetting by an adhesive so important for bonding to tooth structure or anyother material?2. Why is the strength of enamel and dentin a limiting factor in the adhesive bond
strength?3. What is the essential role that hydrophilic primer coupling agents play in theformation of the hybrid layer?4. How could the geometry of a restoration affect the final bond strength to toothstructure?Study Questions(See Appendix E for answers.)1. Why does surface tension exist in liquids?2. How does wetting affect capillary penetration of a liquid?3. How do absorption and adsorption differ?4. Name three colloidal systems of importance to dental materials.5. Which properties affect the penetration rate of liquids into capillaries?6. In terms of innovation, would the bonding of restorative materials to dentin byetching and forming a hybrid layer be classified as a major, medium, or minor productimprovement?Recommended ReadingAdamson AW (1960). Physical Chemistry of Surfaces. New York: IntersciencePublishers.Asmussen E (1985). Clinical relevance of physical, chemical and bonding propertiesof composite resins. Oper Dent 10:61-73.Asmussen E, Antonucci JM, Bowen RL (1988). Adhesion to dentin by means ofGluma resin. Scand J Dent Res 96:584-589.Asmussen E, Munksgaard EC (1988). Bonding of restorative resins to dentine: statusof dentine adhesives and impact on cavity design and filling techniques. Int Dent J38:97-104.Baran G, OBrien WJ (1977). The wetting of silver-tin phases by mercury in air. J AmDent Assoc 94:898-900.Bayne SC, et al (1991). Contributing co-variables in clinical trials. Am J Dent 4:247-250.Berry EA III, von der Lehr WN, Herring HK (1987). Dentin surface treatments for theremoval of the smear layer: an SEM study. J Am Dent Assoc 115:65-67.
Bowen RL (1988). Bonding agents and adhesives: reactor response. Adv Dent Res2:155-157.Bowen RL, Cobb EN, Rapson JE (1982). Adhesive bonding of various materials tohard tooth tissues: improvement in bond strength to dentin. J Dent Res 61:1070-1076.Bowen RL, Eichmiller FC, Marjenhof WA (1991). Glass-ceramic inserts anticipatedfor megafilled composite restorations. J Am Dent Assoc 122:71-75.Brannstrom M (1984). Smear layer: pathological and treatment considerations. OperDent Suppl 3:35-42.Bryant RW, Mahler DB (1986). Modulus of elasticity in bonding of composite andamalgams. J Prosthet Dent 56:243-248.Clinical Research Associates (2000). CRA Newsletter (Nov).Douglas WH (1989). Clinical status of dentine bonding agents. J Dent 17:209-215.Duke ES, Lindemuth J (1990). Polymeric adhesion to dentin: contrasting substrates.Am J Dent 3:264-270.Duke ES, Lindemuth J (1991). Variability of clinical dentin substrates. Am J Dent4:241-246.Duncanson MG Jr, Miranda FJ, Probst RT (1986). Resin dentin bondingagentsrationale and results. Quintessence Int 17:625-629.el-Kalla IH, Garcia-Godoy F (1997). Saliva contamination and bond strength ofsingle-bottle adhesives to enamel and dentin. Am J Dent 10:83-87.Fan PI (1987). Dentin bonding systems: an update. J Am Dent Assoc 114:91-95.Fan PI, OBrien WJ (1974). Penetrativity of sealants. J Dent Res 54:262-264.Fan PI, OBrien WJ (1975). Strain resulting from adhesive action of water in capillarybridges. Nature, Aug 21.Gaberolglio R, Brannstrom M (1976). Scanning electron microscopic investigation ofhuman dentinal tubules. Arch Oral Biol 21:355-362.Glantz PO (1969). On wettability and adhesiveness. Odontol Rev 20(suppl 17).Heymann HO, et al (1991). Examining tooth flexure effects of dentinal adhesives inclass V cervical lesions. J Am Dent Assoc 116(2):179-183.Jorgensen KD, Asmussen E, Shimokobe H (1975). Enamel damage caused bycontracting restorative resins. Scand J Dent Res 83:120-122.Jorgensen KD, et al (1976). Deformation of cavities and resin fillings in loaded teeth.
J Dent Res 84:46-50.Lambrechts P, et al (1987). Evaluation of clinical performance for posteriorcomposite resins and dentine adhesives. Oper Dent 12:53-78.Lee H (1973). Adhesion of polymeric materials to tooth structure. In: Moskowitz H(ed). Proc Symposium on Adhesive Dental Materials. New York: New YorkUniversity.Lewis AF, Natarajan RT (1975). The attachment site theory of adhesive joint strength.In: Lee LH (ed). Adhesion Science and Technology. Part B. New York: PlenumPress, 563-575.McCabe JF (1990). Applied Dental Materials. London: Blackwell.McGuckin RS, et al (1991). Shear bond strength of Scotchbond in vivo. Dent Mater7(1):50-53.Morin DL, et al (1984). Cusp reinforcement by the acid-etch technique. J Dent Res63:1075-1078.Morin DL, et al (1988). Biophysical stress analysis of restored teeth: experimentalstrain measurement. Dent Mater 4:41-48.Nakabayashi N, Pashley DH (1998). Hybridization of Dental Hard Tissue. Chicago:Quintessence.OBrien WJ (1967). Capillary Penetration of Liquids Between Solids [doctoraldissertation]. Ann Arbor: University of Michigan.OBrien WJ (1970). Surface energy of liquid isolated in narrow capillaries. SurfaceSci 19:387.OBrien WJ (1973a). Capillary effects on adhesion. In: Moskowitz H (ed). ProcSymposium on Adhesive Dental Materials. New York: New York University.OBrien WJ (1973b). Capillary action around dental structures. J Dent Res 52:533-549.OBrien WJ (1976). Effects of capillary penetration and negative pressure at sites ofcaries susceptibility. In: Stiles HM, et al (eds). Microbial Aspects of Dental Caries.Washington, DC: Information Retrieval.OBrien WJ, Craig RG, Peyton FA (1968). Capillary penetration around ahydrophobic filling material. J Prosthet Dent 19:399-405.OBrien WJ, Fan PL (1975). Capillary adhesion. In: Lee LH (ed). Adhesion Scienceand Technology. Part B. New York: Plenum Press, 621-633.OBrien WJ, Ryge G (1965a). Contact angles of drops of enamel on metals. J Prosthet
Dent 15:1094-1100.OBrien WJ, Ryge G (1965b). Wettability of poly(methyl methacrylate) treated withsilicone tetrachloride. J Prosthet Dent 15:304-308.Pashley DH (1984). Smear layer: physiological consideration. Oper Dent Suppl 3:13-29.Pashley DH (1991). Dentin bonding: overview of the substrate with respect to theadhesive material. J Esthet Dent 3(2):46-50.Pashley DH (1991). In vitro simulations of in vivo bonding conditions. Am J Dent4:237-240.Pashley DH, et al (1978). Regional resistances to fluid flow in human dentine in vitro.Arch Oral Biol 23:807-810.Pashley DH, Carvalho RM, Sano H, et al (1999). The microtensile bond test: areview. J Adhes Dent 1:299-309.Perdigao J (1995). An Ultra-Morphological Study of Human Dentin Exposed toAdhesive Systems [thesis]. Leuven, Belgium: University of Leuven.Selna LG, et al (1975). Finite element analysis of dental structures: axisymmetric andplane stress idealizations. J Biomed Mater Res 9:237-244.Shahverdi S, Canay S, Sahin E, Bilge A (1998). Effects of different surface treatmentmethods on the bond strength of composite resin to porcelain. J Oral Rehabil 25:699-705.Tao L, et al (1988). Effect of different types of smear layers on dentin and enamelshear bond strengths. Dent Mater 4:208-216.Tate WH, You C, Powers JM (1999). Bond strengths of compomers to dentin usingacidic primers. Am J Dent 12:235-242.Thresher RW, Saito GE (1973). The stress analysis of human teeth. J Biomech 6:443-449.Van Meerbeek B, et al (1992). Factors affecting adhesion to mineralized tissues. OperDent Suppl 5:111-124.Van Meerbeek B, et al (1993). Comparative SEM and TEM examination of theultrastructure of the resin-dentin interdiffusion zone. J Dent Res 72:495.Wang T, Nakabayashi N (1991). Effect of 2-(Methacryloxy) ethyl phenyl hydrogenphosphate on adhesion to dentin. J Dent Res 70(1):59-66.Yettram AL, et al (1976). Finite element stress analysis of the crowns of normal andrestored teeth. J Dent Res 55:1004-1011.
Yoshii E (1997). Cytotoxic effects of acrylates and methacrylates: relationships ofmonomer structures and cytotoxicity. J Biomed Mater Res 37:517-524.Ziemiecki TL, et al (1987). Clinical evaluation of cervical composite resinrestorations placed without retention. Oper Dent 12:27-33. Chapter 6. Polymers and PolymerizationIntroductionPolymers have a major role in most areas of dentistry. Their distinctive propertiesallow a range of clinical applications not possible with other types of materials. Themost widely used impression materials (alginates, polyethers, polysulfides, andsilicones) are polymers. A polymeric matrix with a particulate ceramic filler is themost commonly used anterior esthetic restorative material. Additional applicationsinclude denture teeth, cements, dies, provisional crowns, endodontic fillings, tissueconditioners, and pit and fissure sealants. However, the primary use of polymers interms of quantity is in the construction of complete dentures and the tissue-bearingportions of partial dentures. This chapter introduces concepts related to polymercomposition and properties and concludes with a discussion of those polymerscurrently used in the construction of complete and partial dentures, liners, and tissueconditioners.PolymersCompositionA polymer is a molecule that is made up of many units (poly = many; mer = unit).The oligomer is a short polymer composed of two, three, or four mer units. A mer isthe simplest repeating chemical unit of which the polymer is composed, and is oftenthe basis for naming the material. Thus, polystyrene is a polymer composed of styreneunits.Monomers (mono = single) are the molecules that unite to form a polymer, and theprocess by which this occurs is termed polymerization. If monomers of two or moredifferent types are joined, copolymers are formed. Copolymers may be either random(mers do not appear in specific order) or block (large numbers of one type of merappear arranged in sequence). Atoms along the length of any polymer are joinedthrough strong, primary covalent bonds.Molecular weightThe degree of polymerization is defined as the total number of mers in a polymermolecule. The molecular weight of a polymer molecule is the sum of the molecularweights of the mers of which it is made. Typical polymer molecules may becomposed of thousands to millions of mers. Often, a distribution of molecular sizes ispresent in a material, and the reported molecular weight is the average molecularweight. The particular distribution is the result of conditions present during
polymerization. Variations in conditions have a pronounced effect on the properties ofthe final material.Spatial structureThere are three basic spatial structures of polymers: linear, branched, and cross-linked(Fig 6-1). Linear and branched molecules are discrete but are bonded to one anotherthrough weak, physical bonds. Upon heating, the weak bonds break and the ability ofthe chains to then slide past one another results in a softened material. Upon cooling,the bonds reform and hardening occurs. Materials that are able to undergo this processare termed thermoplastic. Examples include polystyrene, polyvinyl acrylics, andpoly(methyl methacrylate) (PMMA).Fig 6-1 Polymer chains. (a) A linear chain; (b) a branched chain; (c) copolymerchains, linear (upper) and branched (lower); (d) cross-linking chains.Cross-linking results in the formation of a network structure of covalently bondedatoms; primary linkages occur between chains, and the polymer actually becomes asingle giant macromolecule. The spatial structure that allows chain sliding uponheating is not present in cross-linked materials. Cross-linked polymers therefore donot undergo softening upon heating and are termed thermosets. Typical examples aresilicones, cis-polyisoprene, bisphenol A-diacrylate, and cross-linked poly(methylmethacrylate).Properties
Many factors affect the properties of polymers, including the chemical composition ofthe chain, its degree of polymerization, and the number of branches and/or cross-linksbetween polymer chains. In general, longer chains and a higher molecular weightresult in the polymers increased strength, hardness, stiffness, and resistance to creepalong with increased brittleness (Fig 6-2). Resin composites, for example, have ahighly cross-linked matrix, in which a large number of strong covalent linkagesbetween chains transforms the molecules into a rigid, very high-molecular-weightmaterial. The resulting increased strength and stiffness contribute to the ability of thismaterial to withstand occlusal stresses during function.Fig 6-2 Relation between strength and polymer molecular weight. (From Mark,1962.)In contrast, elastomeric impression materials are composed primarily of individualcoiled chains with just a few cross-links. This type of molecular structure permits thelarge-scale uncoiling and recoiling of chains that give these materials high flexibility.The amount of crystallinity present in a polymer affects properties. Materials that arehighly crystalline have atoms with a very regular arrangement in space and arestronger, stiffer, and absorb less water than do noncrystalline materials. Few dentalpolymers are crystalline. Most are amorphous, meaning that the atoms of which theyare composed have irregular arrangements in space. Amorphous polymers are oftencalled glassy polymers.Small plasticizer molecules, when added to a stiff uncross-linked polymer, reduce itsrigidity. When small molecules surround large ones, the large molecules are able tomove more easily. A plasticizer therefore lowers the glass-transition temperature(Tg) of the polymer, so a material that is normally rigid at a particular temperaturemay become more flexible. The glass-transition temperature is the temperature atwhich a polymer ceases to be glassy and brittle and becomes rubberlike. Thetemperature of a polymer, as shown in Fig 6-3, has a strong effect on its strengthproperties.
Fig 6-3 Effect of temperature on the tensile properties of a polymer. The temperaturebelow which brittle failure occurs is called the glass-transition temperature. (FromBerry and Bueche, 1962.)Finally, during polymerization a volumetric decrease occurs, resulting in shrinkage(up to 21% for unfilled acrylic resins, 6% for denture resins, 1% to 3% for resincomposites) and the production of internal stresses. A change in shape, often calledwarpage, may occur when the polymer is reheated. Additionally, polymers havevarying abilities to absorb water. A small amount of expansion may occur during thisprocess.PolymerizationIntroductionMost polymerization reactions are of two types: addition polymerization, in whichno by-product is formed, and condensation polymerization, in which a low-molecular-weight by-product such as water or alcohol is formed. Materials that set byaddition polymerization include poly(methyl methacrylate), used in the constructionof dentures, and bis-GMA, a common component of the matrix of resin composites.Materials that set by the condensation mechanism include polysulfide rubber andsome silicone rubber impression materials.The three stages in the free-radical addition polymerization reaction are described inthe following subsections. They may be accelerated by heat, light, or small amountsof peroxides.
InitiationThe initiation step involves the production of free radicals, which will encourage apolymer chain to begin growing (Fig 6-4). Free-radical molecules have chemicalgroups with unshared electrons. In chemically activated systems, free radicals aregenerally produced by the reaction of an organic peroxide initiator and an amineaccelerator. In light-activated systems, the scission of camphorquinone results in theproduction of two molecules with one unshared electron each. Whatever the means ofproduction, the free radicals attack the double bonds of available monomer molecules,resulting in the shift of the unshared electron to the end of the monomer and theformation of activated monomer molecules.Fig 6-4 Three stages of addition polymerization of methyl methacrylate.
PropagationActivated monomers attack the double bonds of additional available monomers,resulting in the rapid addition of monomer molecules to the free radical. This secondstage, propagation, continues as the chain grows in length.TerminationTermination of the growing free radical may occur by several mechanisms and canresult in the formation of branches and cross-links.Small amounts of inhibitors, such as hydroquinone, may be added to the monomer toincrease storage life. Hydroquinones react with free radicals, thereby decreasing therate of initiation.Denture Base PolymersIntroductionThe polymeric denture base can consist of either a simple stiff base on which theteeth are arranged, or a sandwich of stiff base and a resilient liner to provide greaterretention and comfort. When the tissue underlying a loose denture is traumatized dueto the constant motion of the hard plastic over the mucosa, a viscoelastic gel known asa tissue conditioner can be molded onto the fitting surface of the denture in situ sothe tissue can heal and an accurate impression of the untraumatized fitting surface canbe taken prior to making a new, better-fitting denture. A classification is shown in Fig6-5.Fig 6-5 A classification of denture bases, liners, and tissue conditioners.
Advances in denture design have been mediated by the materials available at the time. In the 1800s the art of hand carving ivory and wooden denture bases resulted in dentures retained by mechanical devices such as springs. Goodyears invention of vulcanized rubber, vulcanite, in 1839 provided not only a thermoplastic material that could be molded accurately, but also one that did not biodegrade and was strong enough to withstand masticatory forces for many years. Vulcanites intrinsic dark color and opacity meant that the translucency and reflectivity of living mucosa was impossible to mimic. With the commercial availability of man-made polymers in the early 1930s came an opportunity to apply some of the optically brilliant polymers to dentistry. It was the need for custom fit that delayed their use, however, since polymerization of the free monomer, with its inherent massive volume shrinkage, did not lend itself easily to the vulcanizing techniques used at the time. It was the adoption of the dough technique first described in the mid-thirties that made the use of acrylics in dentistry possible. In the dough technique, a liquid component (monomer) is mixed with a powder component (polymer). The monomer wets the polymer to a dough-like consistency, which is packed into the mold prior to polymerization. Adoption of the new denture bases was rapid in America. However, in Europe, change was forced upon the profession by rubber shortages during World War II. By the end of the war the use of vulcanite for dentures had almost ceased. After the war, resins developed for aircraft production and the burgeoning plastics industry were offered for use as denture base materials, but the simplicity of the dough technique and the lifelike results have sustained acrylics as the market leader to the present day. Table 6-1 gives a comparison of current denture base materials. Table 6-1 A comparison of denture base materials Material Advantages Disadvantages Ideal propertiesHeat cured Good appearance Free-monomer content Good appearance High glass-transition or formaldehyde can High flexural strength temperature cause sensitization High impact resistance Ease of fabrication Low impact strength High stiffness Low capital costs Flexural strength low Long fatigue life Good surface finish enough to penalize High craze resistance poor denture design High creep resistance Fatigue life too short High radiopacity RadiolucencyHeat cured, Improved impact Reduced stiffness Low free-monomer rubber strength content reinforced Good adhesion with teeth and linersHeat cured, fiberHigh stiffness Carbon and Kevlar Low solubility reinforced Very high impact fibers: Low water uptake strength Poor color Dimensional stability Good fatigue life Poor surface Dimensional accuracy Polypropylene fibers:
Good translucency Good surface finishAutocured Easy to deflask No cheaper over long Dimensional accuracy term Capable of higher Increased creep flexural strength than Increased free-monomer heat cured content Color instability Reduced stiffness Tooth adhesion failureInjection Dimensional accuracy High capital costs molded Low free-monomer Difficult mold design content problems Polycarbonate and Less craze resistance nylon Less creep resistance Good impact strengthLight activated No methacrylate Decreased elastic monomer modulus Decreased polymerization shrinkage Possible improved fit compared to conventional material Requires little equipment Time savings Composition and manufacture Heat-cured acrylic The bulk of denture base acrylic is supplied these days in the form of a free-running powder and a liquid. Originally the powder was produced by grinding blocks of PMMA. However, it was soon found that smoother, more consistent doughs resulted from the use of a spherical bead polymer. By suspending monomer liquid in water with the aid of either a surfactant or water-soluble polymer, the rate of polymerization can be well controlled by the cooling action of the surrounding water. The additives required to make the beads dough easily are fortunately very soluble in monomer globules and relatively insoluble in water. The globules can be thermally polymerized without a catalyst; however, benzoyl peroxide is usually added, partly to act as a catalyst in the polymerization of the beads, and partly so the beads become the source of the peroxy free radical during the polymerization of the dough in the dental flask (Fig 6-6).
Fig 6-6 Scanning electron micrograph of poly(methyl methacrylate) beads.To assist dough formation, a plasticizer is also incorporated into the bead polymer.For many years this was an external plasticizer, that is, one that resided between thepolymer chains rather than being chemically attached to them. Any inert, nontoxicorganic molecule will suffice; dibutylphthalate was used for many years. Today,internal plasticizers are used instead, containing various methacrylate or acrylatemonomers. They locally soften the bead and allow the monomer to diffuse morerapidly into the bead during the dough stage. Pigment can be added to the bead eitherduring polymerization or after, by ball milling. By this method, the manufacturerproduces a PMMA bead mixture having a fairly wide molecular weight distributionwith an average molecular weight on the order of 1 million. The all-importantdoughing characteristics of the bead are governed by particle size distribution,molecular weight distribution, and plasticizer content. The highest molecular weightdistributions and lowest plasticizer content are favored, because they result in betterphysical and mechanical properties in the cured denture base.The monomer used to form the dough is largely the same as that used to make themethyl methacrylate beads. Methyl methacrylate quickly diffuses into the polymerbeads on contact, causing them to swell, and extracting some low-molecular-weightpolymer into the monomer trapped in the interstices between the beads. As the beadsswell, entanglements occur between the juxtaposed beads, and the bead-monomermixture becomes a cohesive gel. The beads never dissolve completely (Fig 6-7),although the monomer infiltrates well into the core of each bead. In the swollen state,benzoyl peroxide can diffuse from the bead into the interstices, where later it willinitiate the curing of the dough. In addition, cross-linking agent molecules, capable ofdiffusing into the beads, are present in the monomer phase.
Fig 6-7 The fracture surface of heat-cured denture base acrylic resin showing that thebead structure remains and that cracks pass through, rather than around, beads duringfracture.The cross-linking agent confers two useful properties on the cured gel. It reduces thedenture bases solubility to organic solvents, and it reduces the tendency of thedenture base to craze (form precracks) under stress. However, cross-linking agentsalso are very important from a practical point of view because they help to keep thedenture-making apparatus simple. For a monomer to be converted to a solid polymer,the polymer chain produced must achieve a certain minimal length. Polymers havingmolecular weights below 5,000 are liquid and viscous; resilient polymers need toachieve a minimum molecular weight of about 150,000. Without a cross-linking agentthe flask would have to be airtight and the monomer flushed with nitrogen to achievethe molecular weight required without being inhibited by air. Free-monomer levelswould then be unacceptably high, and the denture would have a lower stiffness leveland a greater tendency to creep. The cross-linking agent accelerates the increase in thecuring systems molecular weight and combats the effects of oxygen inhibition.However, excessive levels of cross-linking agent in the monomer result in denturebases that are brittle. The most common cross-linking agents are dimethacrylates,either ethylene glycol dimethacrylate or 1,4-butylene glycol dimethacrylate.High-impact acrylicHigh-impact acrylic denture base is also made by the heat-cured dough method;impact resistance arises from the incorporation of a rubber phase into the beads duringtheir suspension polymerization. Certain rubbers will dissolve in methyl methacrylatemonomer, notably copolymers of butadiene with styrene and/or methyl methacrylate.The rubber remains soluble in the monomer globule until the polymer content of theglobule becomes too high and the rubber begins to precipitate out. The nature of thisprecipitation is complicated by the fact that some of the growing chains of PMMAmay have become grafted to the butadiene rubber. This results in what is known as aphase inversion, resulting in dispersion throughout the bead of tiny islands of rubber
containing small inclusions of rubber/PMMA graft copolymer (Fig 6-8). Why theseinclusions improve the impact strength of the cured denture base will be discussedlater. There are, however, many patents that describe the formation of the beads, anddentistry uses examples that are either beads with uniformly distributed rubberinclusions, or beads that have a core of rubber-included polymer covered by an outershell of conventional polymer to give a more conventional dough formation. Beadsthat have no shell often gel very quickly and may entrap air as a result. The monomerused to get high-impact beads differs from conventional monomers in that it containseither very little or no cross-linking agent. Fortunately, the inclusion of rubber doeshave a craze-inhibiting effect, as will be explained later.Fig 6-8 Electron micrograph of high-impact denture base showing the size and shapeof the polystyrene-butadiene rubber inversion phase.Autopolymerizing denture baseThe autopolymerizing, or pour-type, denture base is chemically similar to the heat-cured denture base except that a reducing agent is added to the monomer. Thereducing agent is usually a tertiary aromatic amine, although barbituric acidderivatives also have been used. The reducing agent reacts with the benzoyl peroxideat room temperature to produce peroxy free radicals, which initiate the polymerizationof the monomer in the denture base. There is wide variation among manufacturers inthe molecular weights of the polymers in the beads. Some have average molecular
weights as low as 190,000. Cross-linker concentrations vary greatly in the monomerliquid, from 0% to 9%; interestingly, excess cross-linker is associated with high creep.The size, molecular weight, and plasticizer content are balanced to give a highpenetration of monomer into the bead without too early an increase in viscosity of themix to allow pouring of the acrylic into the mold and good wetting of the plastic teeth.This compromise is difficult to achieve and often results in high residual free-monomer contents and low cross-link densities. Manufacturers attempts to achievethe best compromise result in the wide ranges of molecular weights and cross-linkerconcentrations found in materials, which inevitably result in large differences inphysical and mechanical properties between the various products, especially wherecreep is concerned.Injection-molded plasticInjection-molded plastics have the advantage of consistent molecular weight, but thedisadvantage of capital equipment costs, low craze resistance, and difficultiesassociated with attachment of teeth to the denture base. The plastics still offered foruse as injection-molded denture base acrylic are polycarbonate and nylon. Theyrepresent a very small fraction of the market, although they offer a real alternative tometal dentures for patients sensitized to conventional methacrylate or to nickel orcobalt.Acrylic. Acrylic is supplied as granules of low-molecular-weight (MW = 150,000)linear PMMA, with narrow molecular weight range and only a small amount ofresidual free monomer. Note there is no cross-linking, as this would increase the meltviscosity during molding. Plasticization is low and often results in stiffnesses slightlyin excess of conventional heat-cured denture base, despite the low molecular weight.Polycarbonate. This tough plastic is supplied as granules but is not suited to injectioninto damp molds. It has a high melt viscosity and may depolymerize explosively ifoverheated in the presence of water. Again, absence of cross-linking results in poorsolvent resistance and craze resistance. The high melt viscosity exacerbates problemsof tooth attachment.Nylon or polyamides. This is a family of condensation polymers that result from thereaction of a diacid with a diamine to give a variety of polyamides whose physicaland mechanical properties depend on the linking groups between the acid or aminegroups. The first dental use of nylon was not a success because of the excessive waterabsorption of the type chosen, which resulted in excessive creep and somebiodegradation. More recent work on glass-reinforced nylons with much lower waterabsorptions (eg, nylon 66) has produced more encouraging results. These nylons areeither filled with specially coated glass beads or chopped glass fibers. The glass fibersincrease the stiffness of the nylon to about that of a conventional heat-cured denturebase from a stiffness of half that when only glass-bead reinforcement is used. Glass-fiber reinforcement should be used with care, and patients should be warned not toabrade the fitting surface so as to avoid exposing irritation-causing fibers.Light-activated materialsIn recent years, a light-activated system has come on the market and is now used for
many prosthetic applications. This material consists of a urethane dimethacrylatematrix with an acrylic copolymer and has a microfine silica filler. It is supplied inpremixed sheet or rope form. A baseplate is made by adapting the material to a castand polymerizing in a light chamber at 400 to 500 nm. Teeth are added to the basewith additional material followed by a second light exposure. The system eliminatesthe need for flasks, wax, boil-out tanks, packing presses, and heat-processing unitsrequired for the construction of conventional dentures. The manufacturer claims asignificant time savings in both the dental office and the laboratory.Fabrication and its effect on physical and mechanical propertiesWhen fabricating a denture base from polymersby whatever meanscertainphysical and mechanical properties of the final polymer are important. The curedpolymer should be stiff enough to hold the teeth in occlusion during mastication andto minimize uneven loading of the mucosa underlying the denture. The polymershould not creep under masticatory loads if good occlusion is to be maintained. Thepolymer must have sufficient strength and resilience to withstand not only normalmasticatory forces, but sudden high stress caused by impact forces. The materialshould not deteriorate in the aqueous oral environment, and crazes should not formdue to attack by solvents present in food, drinks, or medicaments. The cured polymershould be biologically inert and slow to foul when in contact with oral flora.During fabrication of a denture the physical and mechanical properties mentionedhere can be influenced by cure conditions and choice of materials. Each cure cycle orfabrication technique is a compromise that attempts to optimize the properties thoughtimportant for a given application. For an allergic patient, low free-monomer contentmay be thought more important than stiffness. For a patient requiring a soft lining,stiffness is very important if the reduced cross-sectional area of the denture is not tocause stability or loading problems.Heat-cured denture baseIn the previous discussion of heat-cured denture base acrylic, the mechanism ofdoughing was described. When manipulating the dough prior to packing, the operatoris aware of various stages of gelation: the initial melting of the beads with themonomer; the sandy stage; the formation of first entanglements as the outer layers ofthe bead swell; and, when the dough is pulled, the formation of stringy threads thatcan be drawn out as low-molecular-weight components dissolve into and thicken theinterstitial monomer. In the last stage, the dough becomes elastic as monomerpenetration reaches the core of the beads, plasticizing them and lowering their glass-transition temperature from an initial 125C to well below room temperature; thebeads have become rubber. Curing the dough before the monomer has diffused to thecore of the beads may result in reduced flexural strength and a tendency for cracks topropagate along lines of weakness between the cross-linked interstitial phase and thelinear, more pliable beads. Allowing the monomer and cross-linker to diffuse to thecenter of the beads results in a more homogeneous distribution of stress, and theformation of a tough, three-dimensional network within the existing amorphous beadpolymer to form what is known as an interpenetrating polymer network (IPN) (seeFig 6-7).
The curing cycle is designed to raise the temperature to a point at which (1) sufficientbenzoyl peroxy radicals are produced to overcome the scavenging effect of oxygen,and (2) polymer chains form by free-radical addition polymerization. Too rapid a risein temperature produces large numbers of radicalsa radical avalancheand, as aresult, many growing polymer chains. These chains collide either with other radicalsor with polymer chains, producing an increase in branching and cross-linking of theinterstitial polymer. This in turn reduces toughness. The polymerization reaction itselfis exothermic; if the rate of reaction is too high, heat builds up in the dough until theboiling point of the monomer is exceeded. Porosity of the final denture base results,with a subsequent loss of strength and esthetics and an increase in the possibility offouling.Slow cures result in much tougher denture bases, producing fewer cross-links andbranches, and having a higher overall molecular weight between cross-links becausefewer polymer chains grew at any one time. Free-monomer content is often loweralso, because the steadier rise in internal viscosity of the curing polymer allows themonomer easier access to the growing free radicals. The cross-linker is morecompletely polymerized in heat-cured systems; this results in significantly lowercreep values due to removal of the plasticizing effect of unreacted pendant cross-linker groups.The shrinkage that occurs when a liquid monomer is converted to a solid polymer canbe largely compensated for by keeping the curing dough under compression. Thereare, however, hybrid systems that deliberately start the polymerization of the doughon one side of the mold, while forcing uncured dough into the mold on the oppositeside. As curing progresses across the mold, the mold space is kept filled, with aresulting improvement in dimensional accuracy. The advantage of this system is thatthere is less tendency to raise the bite by overpacking the mold with dough, which canoccur with conventional flasks.Heat-cured systems have one great advantage over autopolymerized and injection-molding methods: an increased rate of monomer diffusion at the higher temperature.This is most beneficial when acrylic teeth are used, for it leads to better wetting of theteeth by the dough and the formation of chemical welds between the teeth and denturebase. Conversely, an increased temperature of cure can also result in the annealing ofstresses that build up in the structure due to polymerization shrinkage. If this stress isnot released, it can act as the foci for crazes or distortions caused by overzealouscleaning regimes.Autopolymerizing acrylicThe pour technique for dentures, originally developed during the 1960s, has lost muchof its popularity because of problems that stem from incorrect processing. In thistechnique, the acrylic is mixed to a liquid consistency, then poured into a sprued moldthat consists largely of reversible hydrocolloid. The fitting surface of the moldconsists of the plaster model itself; the acrylic teeth occupy their positions in the agarmold in the same way they do in a conventional plaster mold.The pour-type mold itself has design weaknesses. The gelatinous agar cannot grip the
teeth as easily as the rock-hard plaster, and hence there is a greater tendency for theteeth to be displaced during the pouring of the acrylic. Prior to being placed in themold, the teeth themselves have been part of the wax-up; any wax remaining on theteeth will prevent the monomer from wetting their surfaces. This problem is far lesscommon when solution and diffusion of the wax can occur at the elevatedtemperatures of the heat-curing process.The use of a hydroflask to produce an increased atmospheric pressure around themold has two main advantages: (1) Most important, porosity caused by monomerboiling is prevented by the simple expedient of raising its boiling point; and (2) airincluded during mixing is compressed, raising the density of the cured resin andimproving its transverse strength. However, the technician can do little to reduce free-monomer content to achieve high toughness, because this is built into the formulationwhen the manufacturer chooses the powder/liquid ratio, the cross-linker content, andthe accelerator/catalyst ratio. In general, the creep of these products is greater thanthat of heat-cured acrylics.Injection moldingThe technician has little leeway when using injection-molded plastics. The moldshould be dry to prevent the generation of steam during molding. Patience is requiredto ensure the melt has reached the right temperature and cools sufficiently aftermolding. Inadequate spruing will lead to underfilled molds, as can underheating themelt; overheating the melt can cause explosions, especially when polycarbonate isinjected into moist molds.Injection moldings rely almost totally on mechanical forces to retain the teeth. Lowmelt temperatures will cause strong forces to be put on the teeth during the injectionphase and may dislodge some molars, even from plaster molds.Depolymerization or oxidation from overheating the melt can result in porosity, lossof strength, color changes, and increased fouling.Light-activated materialsLight-activated materials compare well to conventional heat-cured materials in termsof impact strength and hardness, but have a considerably lower elastic modulus. Adenture constructed of light-cured material would therefore be expected to deformelastically to a greater extent than a heat-cured denture under the forces ofmastication. However, transverse strengtha measure of the load required to fracturea thin strip of material in the transverse directionis just slightly lower than that ofthe conventional material.As a consequence of the higher-molecular-weight oligomers used in light-curedsystems, polymerization shrinkage is smaller, about 3%, rather than the 6% shrinkagefound in conventional systems. One study showed that denture bases processed byvisible light fit better than conventional or quick heat-cured resins. Ideally, a total lackof polymerization shrinkage would allow the best fit.Since light-activated materials contain no methyl methacrylate monomer, they may be
considered for use in those patients who have demonstrated a sensitivity. Theformulation of light-activated denture bases contains a copolymer of urethanedimethacrylate and an acrylic resin along with silica fillers. Blue light is used topolymerize thin sheets of the plastic raw material in a light chamber.Future improvements in polymeric denture basesThe properties of polymeric denture bases that are closest to being offered asimproved features of commercial products are radiopacity, impact strength, andstiffness.Radiopacity in denture bases would be a desirable attribute. Denture wearers, be theymotorists, members of the security forces, or athletes, can endure seriouscomplications from relatively minor traumatic incidents if their denture fractures anda portion of it either is ingested into the lungs or intestines or, in more seriousincidents, is driven through the skull into the brain pan. Fragments of radiolucentdenture base are difficult to find even when sophisticated ultrasound techniques areused, and their presence is often suspected only after a secondary infection sets in.The use of radiopaque salts and fillers often reduces esthetic properties and strength,and organometallic components have often proved too toxic for use. Bromine-containing organics can give good esthetics but often lack the heat stability necessaryfor heat processing or have to be added in such high quantities that the bulky brominegroups overplasticize the resulting acrylic denture base, causing creep, wateradsorption, and stiffness problems. However, by phase-separating a bromo-polymeradditive within the bead phase, it has been shown that sufficiently high glass-transition temperatures of 110C and stiffnesses of 2.0 GPa (290,000 psi) can beachieved, while at the same time preserving esthetic properties and achieving highlevels of radiopacity.High-impact denture base materials can be prepared using inversion-phase separatedpolymer beads. However, a 50% improvement in impact strength (2.1 J/m) could beachieved, in combination with good esthetics and radiopacity, by the formation of athree-phase bead consisting of (1) PMMA, (2) styrene/butadiene rubber, and (3) thepoly(2,3-dibromopropyl methacrylate). Processing conditions must be well controlled.The availability and quality of high-modulus fibers is improving quickly, as is thevariety of materials from which the fibers are made. Early experiments with glassfibers resulted in failure because of the irritating nature of the fibers that protrudedfrom the finished surfaces. Carbon fibers had no such irritant effects and greatlyincreased impact strength and flexural stiffness of the denture base for little materialexpense. However, the carbon fibers are black, so their use must be restricted to thelingual aspects of a denture. Kevlar fibers (poly-p-phenylene terephthalamide) havestiffnesses of 90 GPa (13 million psi), are straw-colored, and are not easy to pack.They can, however, greatly enhance the mechanical properties of the denture. As withcarbon fibers, they are disappointing esthetically and need to be restricted to lingualaspects of the denture, although they can be extended to the midline of the teethwithout being noticeable. This is an advantage, for if this were done with carbonfibers it would create a black shadow beneath the teeth in the plastic gum work.
Incorporation of the fibers into dentures produces conventional dentures that can withstand uncommonly rigorous treatment. When the fibers are combined with bis- GMA, the flexural strength is such that they do not break in the conventional three- point flexural test apparatus, yet they have Youngs moduli of 30 GPa (4 million psi), a figure comparable with ceramics. Lingual bars for partial dentures could be made using such materials, and, perhaps, with some changes in partial denture design, much less obtrusive polymeric partial dentures could be fabricated with only the clasps being made of metal. Permanent Soft Lining Materials Introduction Permanent soft lining materials are resilient polymers used to replace the fitting surface of a hard plastic denture, either because the patient cannot tolerate a hard fitting surface or to improve retention of the denture. Because the lining is soft, its dimensional stability is important, as are its durability and resistance to fouling. However, because by definition soft lining materials are above their glass-transition temperature when in the mouth, such physical phenomena as water absorption, osmotic presence of soluble components, and biodegradability play a greater role in the clinical success of a liner than they do in the glassy polymers used as denture bases. Acrylics and silicones are the two main families of polymers used commercially as soft liners, though other rubbers have been used in limited clinical experiments. Table 6-2 gives a comparison of soft lining materials. Table 6-2 A comparison of soft liners and tissue conditioners Material Advantages Disadvantages Ideal properties Soft linersAcrylic High peel strength to Poor resilience High resilience acrylic denture base Loses plasticizer in Unaffected by High rupture strength time aqueous environment Some can be polished Some buckle in water and cleansers if cooled Good bond to denture Reasonable resistance base to damage by denture Good abrasion cleansers resistanceSilicone (RTV) Resilience Low tear strength Biocompatible Low bond strength to Antifouling properties dentures Good dimensional Attacked by cleansers stability Buckle in water Poor abrasion resistanceSilicone heat curedResilience Low tear strength Adequate bond Poor abrasion strength to acrylic resistance More resistant to
aqueous environment and cleansers than RTVTissue Rheological and Low cohesive Flow under constant conditioners viscoelastic strength force properties almost Affected by cleansers Resilient at high rates ideal Alcohol can sting of deformation Can be applied inflamed mucosa Remain viscous for chairside several days Dentures fit well Have a high tack to Can record freeway aid retention to space denture base Acrylic soft liners The acrylics consist of either highly plasticized intrinsically glassy polymers or soft acrylics that have a natural glass-transition temperature at least 25C less than that of the mouth. The plasticizer used to soften the acrylic can either be unbound to the acrylic and hence free to diffuse out during use, resulting in a loss of resilience, or it can be reacted into the cured matrix of the acrylic. The latter method is preferred because it should increase the clinical life of the soft liner; unfortunately, in practice, such acrylics are hard to formulate. The reactive plasticizer often has a much lower rate of polymerization than the acrylic monomer. The result is a form of phase separation that leads to an uneven uptake of water by the soft liner. Water accumulates in the plasticizer-rich phase, and soluble im-purities in the polymer create an osmotic pressure that causes it to swell and distort. Therefore, although such internally plasticized acrylics have been produced commercially, they have often been withdrawn after distortion problems have been noted in practice, often due to insufficient curing of very finely balanced formulations. The plasticized acrylics are based on copolymer beads consisting mainly of ethyl methacrylate; both n- and isobutyl methacrylate can be used, as can 2-ethoxyethyl methacrylate. However, the latter monomer is used mainly in the liquid component. The beads are copolymerized with acrylates, which, in general, have much lower glass-transition temperatures than their methacrylate homologues, but unfortunately have very unpleasant odors. So that the beads are free-flowing, the bead polymers have glass-transition temperatures slightly above room temperature. The monomer usually contains the plasticizer, which is a large phthalate ester. The monomer must swell sufficiently for the plasticizer to enter the beads. The plasticizer is then trapped inside the beads as the monomer polymerizes and the mean free path between the polymer chains decreases. The monomer can be methyl methacrylate, although its Tg, even when plasticized, is rather high; n- or isobutyl methacrylate is preferred because it has a much lower Tg when polymerized. Some manufacturers use isobutyl methacrylate to produce a balance of properties such that in ice water the liner can be polished like denture base acrylic, while the liner remains resilient in the mouth.
Water can, of course, be used as the plasticizer in hydrophilic liners. This was theprinciple behind the hydroxyethyl methacrylate soft liners. However, the water is notpresent when the denture is fabricated, and its uptake leads to a swelling of the liner,which must be compensated for. Water-swollen liners also allow ions into theirmatrices, which can subsequently crystallize and thus harden the lining as well ascause osmotic pressure effects, as in the polymerizable plasticizers.Silicone soft linersThe silicones used as soft liners can be divided into two types: room-temperaturevulcanizing (RTV) and heat curing. The resilience of silicones makes them at firstseem to be the ideal soft lining materials. However, silicones have poor tear strength,no intrinsic adhesion to acrylic denture base, and, if not properly cured, a tendency toosmotic pressure effects. The RTV silicones greatest drawback is their lack ofadhesion, which is especially a problem around the edges of the attachment betweenacrylic and silicone. Heat-cured silicones have in their formulation a siloxanemethacrylate that can polymerize into the curing denture base and into the heat-curedaddition silicone. The RTV silicones use a condensation cross-linking system basedon organo-tin derivatives such as those used in impression rubbers. Their degree ofcross-linking is lower and their serviceability is low as a result, with frequent reportsin the literature of swelling and buckling during use and excessive sensitivity todenture cleansers. The rupture strength of some RTV silicones is known to deteriorateconsiderably when exposed to water for long periods. The heat-cured siliconesachieve a greater degree of cross-linking and have much longer clinical lifetimes.Temporary Soft Liners and Functional Impression MaterialsTemporary soft liners, or tissue conditioners, need only survive in the mouth for a fewweeksalthough some are so well formulated as to remain resilient and in place formany months. However, it is their viscoelastic properties that are important,specifically their ability to flow under masticatory and linguistic forces, spreading theload on the mucosa evenly. When first mixed they flow easily, recording such voidsas mean freespace. They soon become highly viscous, however, and thereafter onlyrespond to persistent forces, such as changes in the shape of the mucosa beneath thedenture. In this way swollen mucosa traumatized by ill- fitting dentures can recoverwhile the denture, with its tissue conditioner lining, adapts to any lack of fit driven bymasticatory forces.The materials used for the temporary soft liners were many when the technique wasfirst developed, and included many nontoxic, puttylike materials, such as plasticineand chewing gum. Modern materials are exclusively acrylic gels. An acrylic gel canbe made by mixing swellable acrylic beads with alcohol. Poly(methyl methacrylate) isunsuitable for this purpose, although poly(ethyl methacrylate) or its copolymers withacrylates have proved most popular. To maintain the softness of the gel in the mouth,plasticizer is added to the alcohol, which diffuses into the polymer beads and lowerstheir glass-transition temperature to well below that of the mouth. The beads are madeof low-molecular-weight polymer and have a high tack when swollen. This has theadvantage of increasing the cohesive strength of the gel and causing it to be wellretained by the denture base acrylic.
There is no polymerization or curing reaction involved in the setting of the gel, justthe entanglement of outer polymer chains of juxtaposed beads. The rate of gelling isincreased by lowering the molecular weight of the bead, reducing its size, orincreasing the amount of acrylate in its copolymers. The alcohol content of the liquidalso can be used to control the rate of gelling, as can the size of the plasticizermolecule; the more alcohol used, the faster the rate of gelling. However, because thealcohol diffuses out of the gel and is only partially replaced by water, high-alcohol-content gels tend to harden much faster than others. Practitioners should be aware ofthe alcohol content of these products, first because they sting when initially inserted,and second because they give false positive results if the patient is given abreathalyzer test.Glossaryaddition polymerization A polymerization process involving free radicals in whichno by-product is formed as the chain grows.condensation polymerization A polymerization process in which a by-product, suchas water or alcohol, is formed as the chain grows.copolymer A polymer consisting of two or more types of mers, or units, joinedtogether.crazing Minute surface cracks on polymers; precursors to crack growth andsubsequent failure of the material.cross-linking agent A monomer having two or more groups per molecule capable ofpolymerization. When polymerized, each active group is capable of incorporation in agrowing polymer chain, causing either a loop in the chain or a cross-link between twochains.degree of polymerization The total number of mers in one polymer molecule.denture base Materials used to contact the oral tissues and support artificial teeth.glass-transition temperature (Tg) (softening temperature) The temperature atwhich the polymer ceases to be a glass (ie, fractures in a brittle manner) and becomesa rubber or leather (ie, tends to permanently deform under a load too small to causefracture).glassy polymer An amorphous polymer that behaves as a brittle solid.hydrophilic liner A soft liner that is readily wet by water.interpenetrating polymer network (IPN) A combination of two polymers innetwork form, at least one of which is synthesized and/or polymerized in theimmediate presence of the other. An IPN can be distinguished from simple polymerblends, blocks, and grafts in two ways: (1) An IPN swells but does not dissolve insolvents; and (2) creep and flow are suppressed.
monomer The basic repeating chemical molecule of a polymer (eg, polyethylene is along chain of ethylene monomer units).molecular weight The sum of the molecular weights of the mers of which thepolymer is made.oligomer A polymer made up of two, three, or four monomer units.phase inversion The inversion of the internal and external phases in an emulsion, eg,the change of an oil-in-water emulsion to a water-in-oil emulsion.plasticizer A small molecule that, when added to a polymer, lowers its glass-transition temperature and increases the rate at which solvents penetrate the polymer.polymer A molecule made up of thousands or millions of repeating units. Polymersmay be linear, branched, or cross-linked.polymerization The process by which monomers unite to form a polymer.soft lining material (soft liner) A soft polymer used as a thin layer on the tissue-bearing surface of a denture.thermoplastic A polymer that softens upon heating and rehardens upon cooling.thermoset A polymer that is not able to undergo softening upon heating.tissue conditioner A soft liner used to treat traumatized mucosa.Discussion Questions1. Why is higher impact strength an important advantage for denture base materials?2. How does the heat-curing rate affect the porosity and strength of acrylic denturebases?3. Although cross-linking can improve mechanical properties, how can it lead toproblems in the bonding between acrylic teeth and the denture base?4. Why do acrylic polymers still dominate the denture base market?Study Questions(See Appendix E for answers.)1. What are the main types of denture base materials used?2. What are the ideal properties of a denture base material?3. What are the advantages and disadvantages of heat-cured acrylic denture basematerials?
4. What are the advantages and disadvantages of auto-cured denture base materials?5. What are the advantages and disadvantages of rubber-reinforced denture basematerials?6. What are the advantages and disadvantages of fiber-reinforced denture basematerials?7. What are the advantages and disadvantages of injection-molded denture bases?8. What are the advantages and disadvantages of light-activated denture basematerials?9. What are the materials currently being used as soft liners?10. What are the advantages and disadvantages of RTV silicones?11. What are the advantages and disadvantages of heat-cured silicones?12. What are the advantages and disadvantages of acrylic soft liners?13. What are the ideal properties of tissue conditioners?Recommended ReadingAnderson GC, Schulte JK, Arnold TG (1988). Dimensional stability of injection andconventional processing of denture base acrylic resin. J Prosthet Dent 60(3):394-398.Bafile M, Graser GN, Myers ML, Li EKH (1991). Porosity of denture resin cured bymicrowave energy. J Prosthet Dent 66:269-274.Berry JP, Bueche AM (1962). Ultimate strength of polymers. In: Weiss P (ed).Adhesion and Cohesion. Amsterdam: Elsevier, 20.Cunningham JL, Benington IC (1999). An investigation of the variables which mayaffect the bond between plastic teeth and denture base resin. J Dent 27:129-135.Davy KWM, Causton BE (1982). Radio-opaque denture base: a new acryliccopolymer. J Dent 10:253-264.Eichold WA, Woefel JB (1990). Denture base acrylic resins: friend or foe? CompendContin Educ Dent 11:720-725.Goll G, Smith DE, Plein JB (1983). The effect of denture cleansers on temporary softliners. J Prosthet Dent 50:466-472.Khan Z, von Fraunhofer JA, Razavi R (1987). The staining characteristics, transversestrength, and microhardness of a visible light-cured denture base material. J ProsthetDent 57:384-386.
MacGregor AR, Graham J, Stafford GD, Huggett B (1984). Recent experience withdenture polymers. J Dent 12:146-157.Mack PJ (1989). Denture soft linings: materials available. Aust Dent J 34:517-521.Mark FF (1962). Future trends for improvement of cohesive and adhesive strength ofpolymers. In: Weiss P (ed). Adhesion and Cohesion. Amsterdam: Elsevier, 241.Qudah S, Harrison A, Huggett R (1990). Soft lining materials in prosthetic dentistry: areview. Int J Prosthodont 3:477-483.Ruyter IE (1982). Methacrylate-based polymeric dental materials: conversion andrelated properties. Acta Odontol Scand 40:359-376.Ruyter IE, Svendsen SA (1980). Flexural properties of denture base polymers. JProsthet Dent 43:95-104.Schmidt WF, Smith DE (1983). A six-year retrospective study of Molloplast-B-lineddentures. Part 1. Patient response. J Prosthet Dent 50(3):308-313.Smith LT, Powers JM (1992). Relative fit of new denture resins polymerized by heat,light and microwave energy. Am J Dent 5(3):140-142.Smith LT, Powers JM, Ladd D (1992). Mechanical properties of new denture resinspolymerized by visible light, heat and microwave energy. Int J Prosthodont 5:315-320.Takamata T, Setcos JC (1989). Resin denture bases: review of accuracy and methodsof polymerization. Int J Prosthodont 2:555-562.Wright PS (1976). Soft lining materials: their status and prospects. J Dent 4:247-256. Chapter 7. Impression MaterialsIntroductionImpression materials are used to make replicas of oral structures. All impressionmaterials must be in a plastic or fluid state while the replica is being made. Physicalchange, chemical reaction, or polymerization convert these fluid materials into eitherelastic or nonelastic (ie, plastic or brittle) negative replicas of the soft and/or hardtissues of the mouth. A model or cast material (eg, high-strength stone) is pouredinto the impression and, upon setting, produces a positive impression of the tissues ofinterest. Nonelastic materials include impression plaster, impression compound, andzinc oxide-eugenol. Elastic materials in current use are agar hydrocolloid, alginate,polysulfide, condensation silicone, addition silicone, and polyether. These materialswill be discussed separately. A classification key is shown in Fig 7-1.
Fig 7-1 A classification key of impression materials.The American Dental Associations (ADAs) Council on Dental Materials,Instruments, and Equipment is responsible for developing and disseminatingspecifications for dental materials, instruments, and equipment. The AmericanNational Standards Institute (ANSI) has made the Council the AdministrativeSecretariat of the American National Standards Committee MD156 for DentalMaterials, Instruments, and Equipment. Specifications relating to dental impressionmaterials can be found in published documents listed in Table 7-1. Table 7-1 ADA/ANSI specifications for dental impression materialsMaterial ADA/ANSI Specification No.Dental impression compound 3Zinc oxide-eugenol impression paste 16Dental agar impression material 11Alginate impression material 18Nonaqueous, elastomeric impression material 19Dental duplicating material 20Dental gypsum products 25
Nonelastic MaterialsImpression plasterPlaster of Paris is seldom used as impression material now that elastomeric materialsare available, but it can be used as a "wash" (a thin lining material placed over astiffer base material or tray) material for edentulous impressions. The maincomponent of impression plaster is calcium sulfate hemihydrate, which reacts withwater to form calcium sulfate dihydrate. Manufacturers incorporate additives to adjustthe setting time and setting expansion. The water/powder (W/P) ratio recommendedby the manufacturer should be measured out carefully. The powder should besprinkled into the water, allowed to sit for 30 seconds to wet the powder, and thenmixed for the minimum time necessary to obtain a homogeneous mix. Impressionplaster is rigid and will break rather than bend. The plaster must be stored in anairtight container because it will absorb water from the air and its setting time will beadversely affected.Dental impression compound (Types I and II)There are two types of dental compound as defined by the ADA. Type I is used forimpression taking, and Type II is used for tray preparation. Although dentalcompound has fallen into disuse, it can be used for full-crown impressions (Type I),impressions of partially or completely edentulous jaws (Type I), and impression traysin which a final impression is taken with another material (Type II). Compoundcannot be used to record undercuts since it is not elastic. Impression compound isavailable in either cakes or sticks in various colors from a number of manufacturers(Jelenko, Kerr, Mizzy, and Moyco).CompositionDental compound contains several ingredients. Natural resins, which comprise about40% of the formulation, make the compound thermoplastic. Shellac is often used.Waxes (about 7%) also produce thermoplastic properties. Stearic acid (about 3%) actsas a lubricant and plasticizer. Fillers and inorganic pigments account for theremaining 50% of the formulation. Diatomaceous earth, soapstone, and talc areexamples of commonly used fillers.Thermal and mechanical propertiesDental compound is thermoplastic; it is used warm (45C) and then cooled to oraltemperature (37C), at which it is fairly rigid. The setting mechanism is therefore areversible physical process rather than a chemical reaction. Dental compound islimited by its thermal properties. Type I materials have a flow of at least 85% at 45Cand less than 6% at 37C. Type II materials flow about 70% at 45C but less than 2%at 37C. Both types become quite plastic with only an 8C rise in temperature. Thethermal conductivity of dental impression compounds is very low. These materialsdo not conduct heat very well and therefore require heat soaking to attain a uniformtemperature throughout the mass. When heated or cooled, they soften or hardenquickly on the outside, but time is needed for the temperature to become uniformthroughout the entire mass. If the impression is removed from the mouth before it has
cooled completely, severe distortion may occur. Since these materials contain resinsand waxes, they have high thermal expansion and contraction coefficients.Contraction from oral temperature to room temperature may be as high as 0.3%.Therefore, the dimensions of the resulting impression could be significantly differentthan those of the mouth. Since compound has such a high viscosity, it is difficult torecord details.ManipulationThe correct use of compound as an impression material requires considerablejudgment in handling. Compound is softened by heating over a flame or in a waterbath. Care must be taken to prevent volatilizing ingredients over a direct flame.Kneading in water also may cause changes in composition and flow properties. Theaim, therefore, is a thorough heating without excessive temperatures or long periodsof storage in water. A room-temperature water spray is used to cool the impression inthe mouth. Cooling must be continued until the entire mass is rigid to reduce plasticflow. Care must also be taken to prevent overheating and burning of tissues. Also,cooling water should not be too cold, in order to prevent thermal shock.To ease separation of the die stone, the impression should first be softened byimmersion in warm water.AdvantagesDental impression compound is compatible with die and model materials and is easilyelectroplated to form accurate and abrasion-resistant dies.DisadvantagesThe handling of dental impression compound is very technique sensitive. If it is notprepared properly, volatiles can be lost on heating, or low-molecular-weightingredients can be lost during immersion in a water bath. Also, excessive wetkneading can incorporate water into the mix and change the flow properties of thecompound. Due to a high coefficient of thermal expansion, the dimensions of theimpression are not likely to be the same as the dimensions in the mouth. Thesematerials are nonelastic and may distort on removal from the mouth. The casts shouldbe poured within 1 hour.Troubleshooting1. Distortion. If the material is not completely cooled, the inner portions of theimpression will still be soft when the impression is removed, resulting in distortion.Also, if water has been incorporated as the result of wet kneading, the material couldhave excessive flow at mouth temperature, producing distortion during removal fromthe mouth. If the tray used to carry the compound to the mouth is too flexible,distortion can result. It is important to select a tray that is strong and rigid. A delay inpreparing the stone cast also may cause distortion. The cast should be poured as soonas possible after the impression has been removed from the mouth.2. Compound is too brittle or grainy. Prolonged immersion in the water bath will
cause low-molecular- weight components to leach out.DisinfectionDental impression compound can be disinfected by immersion in sodiumhypochlorite, iodophors, or phenolic glutaraldehydes. The manufacturersrecommendations for proper disinfection should be followed.Zinc oxide-eugenolZinc oxide-eugenols main use as an impression material is for dentures on edentulousridges with minor or no undercuts. It can also be used as a wash impression overcompound in a tray or in a custom acrylic tray. Zinc oxide-eugenol is also used as abite registration material.CompositionThis material is commercially available in a powder and liquid form and as twopastes. One paste, called the base or catalyst paste, contains zinc oxide (ZnO), oil, andhydrogenated rosin. The second paste, the accelerator, contains about 12% to 15%eugenol, oils, rosin, and a filler such as talc or Kaolin. These two pastes havecontrasting colors so it can be determined when the pastes are thoroughly mixed.These materials are supplied as a soft- or hard-set type. Equal lengths of the twopastes, or properly proportioned amounts of the powder and liquid, are mixed with astiff spatula on a special oil-resistant paper pad or a glass slab. The mixed material isplaced in a preliminary impression made from tray compound or tray acrylic. Thesetting time is shortened by increases in temperature and/or humidity. The set materialdoes not adhere to set dental plaster or stone.Zinc oxide, in the presence of moisture, reacts with eugenol to form zinc eugenolate,which acts as a matrix holding together the unreacted zinc oxide:
The setting reaction is accelerated by the presence of water, high humidity, or heat. Adimensional change of only about 0.1% shrinkage accompanies the setting.Impression materials are classified as hard- and soft-set according to the ANSI/ADAspecification. The hard-set material sets faster (in about 10 minutes, compared to 15minutes for the soft-set material), although the hard- and soft-set materials both beginto set in about 5 minutes. The hard-set material is more fluid before setting than thesoft-set material; after setting, it is harder and more brittle.Noneugenol pastes containing carboxylic acids (eg, lauric or ortho-ethoxybenzoicacid) in place of eugenol are available to avoid the stinging and burning sensationexperienced by some patients.Mechanical propertiesThe hardness of zinc oxide-eugenol impression materials is determined using a Krebspenetrometer with a load of 100 g for 10 seconds. The hardness for Type I (hard-set)materials should be no greater than 0.5 mm and the hardness for Type II (soft-set)materials should be between 0.8 and 1.5 mm.The shrinkage of these materials during the hardening process is approximately 0.1%.Subsequently, no additional dimensional change should occur.ManipulationThese materials are usually mixed on a mixing pad with a spatula. Equal lengths ofbase and catalyst are extruded on the mixing pad. The components are mixedthoroughly with a stiff stainless steel spatula. Adequate mixing time is 45 to 60seconds, after which the mix should appear streak-free. The pastes have an initial settime of 3 to 5 minutes, with the setting time decreasing as the temperature and/orhumidity increases. The model or cast should only be made from gypsum-type plasteror stone. After the stone has set, the impression is immersed in warm water (60C) toease its removal from the cast.The spatula may be cleaned by warming or by wiping with available solvents.AdvantagesThe advantages of zinc oxide-eugenol include high accuracy of soft tissueimpressions due to its low viscosity. The material is stable after setting, has goodsurface detail reproduction, and is inexpensive. It also adheres well to dentalimpression compound.DisadvantagesThe Disadvantages of this material are messiness and a variable setting time due totemperature and humidity. Eugenol is irritating to soft tissues. This material isnonelastic and may fracture if undercuts are present.Troubleshooting
1. Inadequate working or setting time. This could result from excessive humidityand/or temperature. An increase in either of these variables results in decreasedworking and setting time. It is important to select a material that provides the requiredsetting time.2. Distortion. If the tray warps on standing, the impression will also become distorted.It is important to select a stable tray material.3. Loss of detail. If there is loss of detail, the impression material may not becompatible with the stone used to prepare the cast, and/or there may be adhesionbetween the impression and the stone.DisinfectionZinc oxide-eugenol impressions can be disinfected by immersion in 2%glutaraldehyde or 1:213 iodophor solutions at room temperature. The manufacturersrecommendations for proper disinfection should be followed.Elastic MaterialsAgar (reversible) hydrocolloidAgar hydrocolloids have been largely replaced by rubber impression materials butare still used for full-mouth impressions without deep undercuts, quadrantimpressions without deep undercuts, and single impressions (less frequently). Theycan be used for fixed partial denture impressions because of their high accuracy.CompositionAgar hydrocolloids are available in both tray and syringe consistencies. The materialis supplied as a gel in plastic tubes and contains agar (12% to 15%) as a gelling agent,borax (0.2%) to improve strength, potassium sulfate (1% to 2%) to provide goodsurfaces on gypsum models or dies, alkylbenzoates (0.1%) as preservatives, andcoloring and flavoring agents (traces) for ease of "reading" the impression andesthetics. The balance of the formulation (~85%) is water. The syringe consistency isprepared by increasing the water content and decreasing the agar content.The material, supplied as a solid gel, can be converted to a sol (liquid) by heating;cooling a sol causes it to become a gel:The gel-to-sol and sol-to-gel transformations are dependent on time and temperature.The liquefaction and gelation temperatures are different (the latter being lower), andthe effect is called hysteresis. A typical value of the gelation temperature is 43C(109F).
Mechanical propertiesThe mechanical properties of agar hydrocolloids are given in Table 7-2. They arehighly elastic (98.8%) and sufficiently flexible (11%) to give accurate impressions ofteeth with undercuts. They are stronger when stressed quickly; therefore, rapidremoval is recommended. Table 7-2 Properties of elastomeric impression materials* Agar Alginate Polysulfide Condensation Addition Polyether silicone siliconeElastic 98.8 97.3 96.9-94.5 99.6-98.2 99.9-99.0 99.0-98.3recovery (%)Flexibility (%) 11 12 8.5-20.0 3.5-7.8 1.3-5.6 1.9-3.3Flow (%) 0.4-1.9 < 0.10 < 0.05 < 0.05Reproduction 25 75 25 25 25 25limit (um)Shrinkage, 24 0.4-0.5 0.2-1.0 0.01-0.2 0.2-0.3hours (%)Tear strength 700 380-700 2,240-7,410 2,280-4,370 1,640- 1,700-(g/cm) 5,260 4,800*See end-of-chapter glossary for definitions of terms.ManipulationAgar requires a special water bath with three chambers for heating and water-cooledtrays. The following sequence is used:1. Heat in water at 100C (212F) for 8 to 12 minutes.2. Store in water at 65C (149F).3. Place in a tray (containing cooling coils) at 65C (149F).4. Temper in 46C (115F) water for 2 minutes before taking the impression.5. After seating the tray, cool it with water at no less than 13C (55F) until gelationoccurs.6. After the impression is removed from the mouth, wash it to remove saliva, whichwill interfere with the setting of the gypsum.7. Shake off excess water and lightly blow off with air.8. Disinfect the impression.9. Pour mixed dental stone into the impression. If the impression is stored for a shorttime in 100% relative humidity, it should be washed as described in steps 6 and 7 toremove any exudate on the surface caused by syneresis (the exudation of water,accompanied by contraction) before pouring the model.
10. After the initial setting of the stone, store the gypsum model and impression in a humidor. Agar impressions become less accurate during storage, and prompt pouring of gypsum casts is necessary. Table 7-3 lists the dimensional changes that occur upon storage under different conditions. If agar impressions must be stored, the minimum changes in dimensions are found upon storage in 100% relative humidity for no longer than 1 hour. However, the gel structure can absorb water, a process called imbibition, which is usually accompanied by expansion. Table 7-3 Dimensional change of hydrocolloid impressions Storage conditions Dimensional change CausesAir Shrinkage Evaporation of water from gelH2O Expansion Imbibition and absorption of water100% relative humidity Shrinkage SyneresisInorganic salt solutions Expansion or shrinkage Depends on relationship of electrolyte in gel and in solution As the values in Table 7-4 indicate, agar materials have a long working time. Handling, however, offsets this convenience because of the need for storage tanks. Gelation, produced by circulating cool water through the special trays, also requires special equipment. Thermal shock produced by suddenly cooling the warm colloid may be painful to patients who have metallic restorations. Table 7-4 Handling properties of elastomeric impression materials* Agar Alginate Polysulfid Condensatio Additio Polyether e n silicone n silicone Preparation Boil, Powder, 2 pastes 2 pastes or 2 pastes 2 pastes temper, water paste-liquid store Handling Complicate Simple Simple Simple Simple Simple d Ease of use Technique Good Fair Fair Good Good sensitive Patient Tedious, Pleasant, Unpleasan Pleasant, Pleasant Unpleasan reaction thermal clean t, stains clean t, clean shock Ease of Very easy Very Easy Moderate Moderat Moderate removal easy e to difficult Working 7-15 2.5 5-7 3 2-4.5 2.5 time (min) Setting time 5 3.5 8-12 6-8 3-7 4.5 (min) Stability 1 h at Immediat 1 h Immediate 1 w 1 w kept
100% RH e pour pour dryWetting and Excellent Excellent Excellent Fair Fair to Goodease of goodpouringDie material Stone Stone Stone Stone Stone StoneElectroplatin No No Yes Yes Yes YesgDisinfection Poor Poor Fair Excellent Excellen Fair tComparative Low Very low Low Moderate High to Very highcost very high*See end-of-chapter glossary for definition of terms.Contact with agar retards the setting of gypsum, resulting in dies and casts with poorsurface finish. With older products, soaking the impression in a 2% potassium sulfatesolution was necessary to achieve a smooth surface finish. Most agar products nowcontain potassium sulfate, which acts as an accelerator for the gypsum settingreaction, and soaking is no longer necessary.AdvantagesAgar impression materials are inexpensive, have no unpleasant odors, and arenontoxic and nonstaining. They do not require a custom tray or adhesives, and thecomponents do not require mixing. These materials are hydrophilic and can be usedin the presence of moisture, are able to displace blood and body fluids, and are easilypoured in stone. The stone casts are easily removed from the hydrocolloidimpressions.DisadvantagesThese materials require the use of expensive equipment and must be prepared inadvance. They tear easily, must be poured immediately, are dimensionally unstable,can only be used for single casts, and cannot be electroplated. The surface of stonecasts will be weakened by compositions containing borax.TroubleshootingSometimes problems of distorted impressions or loss of detail may be encounteredwhen using agar hydrocolloids. The following are factors that could lead to distortion:1. Slow removal from the mouth. To avoid permanent deformation, the impressionshould be removed with a quick jerk.2. Removal from the mouth before the gel reaches a temperature of 37C (98.6F) orless. Above this temperature the impression material will still be plastic. The coolingrate of hydrocolloid is dependent on the temperature of water circulating through the
tray.3. Cooling water that is too cold ( 13C). Rapid cooling of the impression may causea concentration of internal stresses that may be subsequently released.4. Application of force on the tray during gelation. After the load is removed,relaxation of stresses will occur.5. Delay in pouring the cast. Waiting any length of time to pour the cast will result inshrinkage of the impression due to the loss of water.6. Instability of tray. If there is loss of detail, it may be caused by movement of thetray before gelation is complete. Failure to keep the impression stabilized will resultin a multiple impression of the oral structures.DisinfectionAgar hydrocolloids can be disinfected by immersion in sodium hypochlorite,iodophors, or phenolic glutaraldehydes. The manufacturers recommendations forproper disinfection should be followed.Alginate (irreversible) hydrocolloidAlginates are the most widely used impression materials in dentistry. They are usedfor making impressions for removable partial dentures with clasps, preliminaryimpressions for complete dentures, and orthodontic and study models. They are notaccurate enough for fixed partial denture impressions.CompositionAlginates are supplied as a powder containing sodium or potassium alginate (12% to15%) and calcium sulfate dihydrate (8% to 12%) as reactants; sodium phosphate (2%)as a retarder; a reinforcing filler (70%), such as diatomaceous earth, to control thestiffness of the set gel; potassium sulfate or alkali zinc fluorides (~10%) to providegood surfaces on gypsum dies; and coloring and flavoring agents (traces) foresthetics. The sodium phosphate content is adjusted by the manufacturer to produceeither regular- or fast-set alginates.The powder is mixed with water to obtain a paste. Two main reactions occur when thepowder reacts with water during setting. First, the sodium phosphate reacts with thecalcium sulfate to provide adequate working time:Second, after the sodium phosphate has reacted, the remaining calcium sulfate reactswith the sodium alginate to form an insoluble calcium alginate, which forms a gelwith the water:
To avoid the inhalation problems of alginate dust, some materials have beenintroduced in a dustless version in which the powder is coated with a glycol (IdenticDust Free, Cadco; Jeltrate Plus, Caulk).Some products contain a chemical disinfectant in the alginate powder due to theconcern for infection control (Coe Hydrophilic Gel, GC America; Identic Dust Free;Jeltrate Plus). Two examples of these disinfectants are didecyl-dimethyl ammoniumchloride and chlorhexidine acetate. When the quaternary ammonium compound isused, the detail reproduction and gypsum compatibility of the alginate improve.However, the impressions made from these materials should still be disinfected uponremoval from the mouth.Mechanical propertiesTable 7-2 gives an elastic recovery value of 97.3% for alginates, which indicates lesselasticity and therefore less accuracy than agar hydrocolloids and silicone andpolyether impression materials. The compressive and tear strengths increase withincreasing rates of deformation. The limit of reproduction is also lower, indicatingthat less fine detail will be obtained. Figure 7-2 compares the elasticity of alginateswith the more accurate agar materials. Alginates have a higher permanent deformationupon stretching to pass over undercuts.Fig 7-2 Illustration of agar hydrocolloids greater accuracy due to their greater degreeof recovery after deformation around undercuts. (From Roydhouse, 1962. Reprintedwith permission.)
ManipulationAlthough easy to use, care is required in handling alginate hydrocolloids. The powder,supplied in a can, should be shaken up for aeration and one scoop of powder is usedfor one measure of water. A powder scoop and a graduated cylinder for water areusually supplied with the product. With predispensed powder products, one packet ofpowder is used with the amount of water specified by the manufacturer. A lower W/Pratio increases strength, tear resistance, and consistency, and decreases working andsetting times and flexibility. Cooling the water increases the working and settingtimes. Insufficient mixing results in a grainy mix and poor recording of detail.Adequate spatulation gives a smooth, creamy mix with a minimum of voids. Oneminute of thorough mixing for the regular-set material and 45 seconds for the fast-setmaterial are generally recommended. Alginates have a relatively short working timeof about 2.5 minutes (see Table 7-4) and set about 3.5 minutes after mixing. Alginatesare as unstable as agar hydrocolloids, because both are gels, and they undergoshrinkage or expansion upon loss or gain of water. Storage in either air or waterresults in significant dimensional change; however, storage at 100% humidity resultsin the least dimensional change. Therefore, the cast should be poured soon afterremoval of the impression and cleaning (see Table 7-4). Alginates, like agar, retardthe setting of the gypsum model and die materials when in contact. Potassium sulfateis added by the manufacturer to accelerate the setting of the gypsum and to obtainsmooth model and die surfaces.An alginate tray material can be combined with an agar syringe material to prepareimpressions. These impressions take advantage of the agar hydrocolloids detailreproduction and compatibility with gypsum qualities and at the same time minimizeequipment needs. A simple heater can be used to prepare the syringe material, and thewater-cooled trays are no longer necessary. The alginate is placed in a tray, the agar issyringed around the preparation, and then the alginate is seated on top of the agar.Care must be taken to select an agar-alginate impression pair with suitable bondstrengths. It is best to select combinations recommended by the manufacturers. Bestresults are obtained when single-unit impressions are made by this technique.AdvantagesAlginate impression materials are inexpensive, easy to manipulate, pleasant tasting,able to displace blood and body fluids, hydrophilic, and easily poured in stone. Theycan be used with stock trays.DisadvantagesAlginates tear easily, must be poured immediately after removal from the mouth, havelimited detail reproduction, are dimensionally unstable, and can only be used forsingle casts. The gypsum compatibility varies with the brands of alginates and dentalstones used. They are incompatible with many epoxy resin die materials.Troubleshooting
Problems may sometimes be encountered when using alginate hydrocolloids. Thefollowing should serve as a guide for troubleshooting problems with these materials:1. Inadequate working or setting time. The temperature of the mixing water may betoo high. Generally, the temperature of the water should range between 18C and24C (65F and 75F). If the mixture is incompletely spatulated, it may beinhomogeneous and may set prematurely. Under normal conditions, adequatespatulation requires 45 to 60 seconds. If the W/P ratio is too low as the result ofincorrect dispensing, the setting time could be too fast. Improper storage of thealginate powder can result in deterioration of the material and shorter setting times.2. Distortion. If the tray moves during gelation or if the impression is removedprematurely, the result will be a distorted impression. The amount and duration ofcompression should be considered. It is important, therefore, to remove theimpression from the mouth rapidly. Since the weight of the tray can compress ordistort the alginate, the impression should not be placed face down on the benchsurface. If the impression is not poured immediately, distortion could occur.3. Tearing. If the impression tears, it is possible that the impression was removedfrom the mouth before it was adequately set. Wait 2 to 3 minutes after loss oftackiness to remove the impression for development of adequate tear strength. Also,the rate of removal from the mouth may be a factor. Since the tear strength of alginateincreases with the rate at which a stress is applied, it is desirable to rapidly remove theimpression from the mouth. In addition, thin mixes are more prone to tearing thanthose with lower W/P ratios. The presence of undercuts also can produce tearing.Blocking out these areas will place less stress on the impression material duringremoval. It is also possible that there is not enough impression material; there shouldalways be at least 3 mm of material between the tray and the oral tissues.4. Loss of detail. If there is loss of detail, the impression may have been removedfrom the mouth prematurely. Multiple impressions of the oral structure will result ifthe material is still in the plastic state when removed.5. Consistency. If the preset mix does not have the proper consistency (is either toothick or too thin), the W/P ratio is incorrect. Care must be taken to fluff the powderbefore measuring and not to overfill the powder dispenser. Vigorous spatulation andmixing for the full recommended time is required to avoid consistency problemscaused by inadequate mixing. If hot water is used, the mix may become grainy andprematurely thick.6. Dimensional change. If dimensional change is a problem, a delay in pouring theimpression might be the cause. Such delays will result in a cast that is distorted aswell as undersized, because alginate impressions lose water when stored in air.7. Porosity. If the impression is porous, this could result from whipping air into themix during spatulation. After the powder has been wetted by the water, the alginateshould be mixed so as to squeeze the material between the spatula blade and the sideof the rubber bowl.8. Poor stone surface. If the set gypsum remains in contact with the alginate for too
long a period of time, the quality of the stone surface will suffer.DisinfectionAlginate hydrocolloids can be disinfected by immersion in sodium hypochlorite oriodophors. The manufacturers recommendations for proper disinfection should befollowed.Polysulfide rubber (mercaptan)Polysulfide rubbers are widely used for fixed partial denture application, due to theirhigh accuracy and relatively low cost. These materials are useful for multipleimpressions when extra time is needed. The polysulfides are supplied in tubes of basepaste and catalyst paste, which are mixed together. Polysulfides are available in low,medium, and high viscosities.CompositionThe base paste contains the polysulfide polymer, fillers, and plasticizers. Low-molecular-weight (~4,000 MW) polysulfide polymer, having both terminal andpendant (near the center of the polymer) mercaptan groups (-SH), is used:The content of the reinforcing fillers (eg, zinc oxide, titanium dioxide, zinc sulfide,and silica) varies from 12% to 50% depending on the consistency (light, regular, orheavy). The fillers and plasticizers control the stiffness of the paste. The accelerator orcatalyst paste contains lead dioxide (30%), hydrated copper oxide or organicperoxide, as a catalyst; sulfur (1% to 4%) as a promoter; and dibutyl phthalate or othernonreactive oils (17%) to form a paste. The balance of the catalyst paste is inorganicfillers used to adjust the consistency and reactivity. Those materials containing anorganic peroxide may have decreased dimensional stability due to evaporation of theperoxide.The lead dioxide catalyzes the condensation of the terminal and pendant -SH with -SH groups on other molecules, resulting in chain lengthening and cross-linking. In theprocess the material changes from a paste to a rubber. The reaction is accelerated byincreases in temperature and by the presence of moisture.
Note that this is a condensation polymerization with water as a by-product.Mechanical propertiesThe values for the mechanical properties of these materials are summarized in Table7-2. For elastic recovery, the polysulfides have values of about 96%, slightly lowerthan those for the other rubber impression materials (eg, silicone and polyether).Values for flow range from 0.4% to 1.9%, indicating a tendency to distort uponstorage. The flow tends to be highest for the light-bodied and least for the heavy-bodied materials. Light-bodied polysulfides have flexibilities of about 16%; regular-bodied polysulfides have values of about 14%; and heavy-bodied polysulfides havevalues of about 10%. This is an advantage over the stiffer addition silicones andpolyethers because removal from undercut areas is easier. Polysulfides have thehighest tear strength of the rubber materials, which allows their use in deepsubgingival areas where removal is difficult.ManipulationThese materials are mixed on a mixing pad with a spatula. Equal lengths of base andcatalyst are extruded on a disposable mixing pad. The components are mixedthoroughly with a stiff tapered spatula. The catalyst is dark and the base is white sothorough mixing is readily observed by lack of streaks in the mix. Adequate mixingtime is 45 to 60 seconds. The working time is about 5 to 7 minutes (see Table 7-4),which is adequate considering the mixing times. Both working and setting times areshortened by higher temperatures and humidity. A value of 0.45% is given forshrinkage after 24 hours. Although this is less than that of the condensation silicones,the cast or die should be poured within 1 hour of taking the impression. Sincepolysulfides take longer to set than silicones, they require more chair time. They stainclothing permanently. They can be electroplated; some products can be silverplated,but copperplating is not recommended.AdvantagesAdvantages of polysulfides include a long working time, good tear strength, goodflow before setting, good reproduction of surface detail, high flexibility for easierremoval around undercuts, and lower cost compared to silicones and polyethers.Disadvantages
Disadvantages of these materials include the need to use custom-made rather thanstock trays due to a greater chance of distortion, a bad odor, a tendency to run downthe patients throat due to lower viscosity, and the lead dioxide materials that stainclothing. Polysulfides must be poured within 1 hour and cannot be repoured.TroubleshootingSometimes problems may be encountered when using polysulfide rubber impressionmaterials:1. Inadequate working time. This could result from excessive humidity and/ortemperature. An increase in either of these variables results in decreased working andsetting times. An improper base-to-catalyst ratio could also produce inadequateworking time (too much catalyst will reduce working time).2. Distortion. A number of factors cause distortion, one of which is too much load.Because recovery after deformation is dependent on the amount and duration ofloading, the impression should not be placed face down on the laboratory bench.Improper removal from the mouth could also cause distortion of the impression;removal should be rapid because permanent deformation is a function of duration ofstress. If a bubble is located just below the surface adjacent to a preparation (internalporosity), the impression may distort.3. Loss of detail. Premature removal from the mouth may be a cause of this. Removalprior to sufficient polymerization or before the material is sufficiently elastic willresult in inaccurate registration of detail. This may also be the result of incompletemixing; failure to incorporate all the catalyst into the base will result in incompletepolymerization of portions of the surface. Movement of the tray prior to the time ofremoval could also cause loss of detail. The impression tray should be held firmlyuntil the elastic stage is attained.4. Surface bubbles or voids. These could be caused by the incorporation of air into themix. The impression material should always be mixed carefully with only the flatsurface of the blade. If the material is partially polymerized prior to insertion in themouth, voids may occur in the impression.DisinfectionPolysulfide impressions can be disinfected by immersion in sodium hypochlorite,iodophors, complex phenolics, glutaraldehydes, or phenolic glutaraldehydes. Themanufacturers recommendations for proper disinfection should be followed.Condensation silicone rubberCondensation silicone rubber impression materials are used mainly for fixed partialdenture impressions. They are ideal for single-unit inlays. These materials aresupplied either as two-paste or paste-liquid catalyst systems. Condensation siliconesare available in low, medium, high, and very high (putty) viscosities.Composition
The base paste usually contains a moderately high-molecular-weightpoly(dimethylsiloxane) with terminal hydroxy groups (-OH), an orthoalkylsilicate forcross-linking, and inorganic filler. A paste will contain 30% to 40% filler, whereas aputty will contain as much as 75%. The catalyst paste or liquid usually contains ametal organic ester, such as tin octoate or dibutyl tin dilaurate, and an oily diluent. Athickening agent is used when making catalyst pastes. Sometimes a catalyst willcontain both the orthoalkylsilicate and the metal organic ester:The metal organic ester catalyzes the reaction. One part of the polymerizationinvolves chain extension by condensation of the terminal -OH group in a siloxane.The other part consists of cross-linking between chains by the orthoalkylsilicatemolecules:A volatile alcohol is formed as a by-product.Mechanical propertiesAccepted values for the mechanical properties of these materials are given in Table 7-2. An average value of 99% for elastic recovery is excellent. The flow of silicones islow; most values are less than 0.1%, indicating that less distortion is likely to becaused by light pressure on standing. The silicones are stiffer than polysulfides, asindicated by lower flexibility values in Table 7-2. The shrinkage in 24 hours rangesfrom 0.2% to 1.0%. About half the shrinkage takes place in the first hour, and it isgreater than for polysulfides or polyethers. Polymerization and evaporation of thealcohol formed in the reaction are responsible for this high shrinkage. Accuracy isgreatly improved by first taking an impression with a highly filled silicone putty and,
after setting, taking a second impression with a light-bodied silicone. Thus, the finaltotal shrinkage is lower.ManipulationThe manipulation of condensation silicones is the same as for polysulfides, exceptthat the silicone material may be supplied as a base paste plus a liquid catalyst. Whenit is supplied in this form, one drop per inch of extruded base paste is usuallyrecommended. The setting time (6 to 8 minutes) is less than that of the polysulfides,which offers some advantage in chair time savings. Electroplating is possible.Because of the high polymerization shrinkage, the cast or die must be poured as soonas possible. Higher temperatures and humidity shorten the setting time.AdvantagesCondensation silicones are clean, pleasant materials for the patient. They are highlyelastic, and the setting time can be controlled with the amount of accelerator. The useof a putty-wash system improves accuracy and eliminates the need for a custom tray.DisadvantagesThese materials tend to be inaccurate due to shrinkage on standing and should bepoured within 1 hour. They are very hydrophobic, require a very dry field, and aredifficult to pour in stone.Troubleshooting1. Inadequate working time. This could result from excessive humidity and/ortemperature. Although not as critical as polysulfide rubber, the setting times ofsilicone impression materials are influenced by temperature and humidity. Increasesin these conditions tend to shorten both working and setting times. An improper base-to-catalyst ratio could also produce inadequate working time. Insufficient catalyst willresult in prolonged setting times. Failure to polymerize in the predicted time mayresult from deterioration during storage.2. Distortion. This may result from incorrect separation from impressed structures.Failure to remove the impression in a rapid, jerking motion may cause the impressionto become permanently deformed. An impression can also become distorted if there isinadequate support of the impression after removal from the mouth. It may undergopermanent deformation if allowed to rest face down on the bench. Excessive delay inpouring the cast (30 minutes or more) also may result in dimensional changes.Possible shrinkage may result from continued polymerization and vaporization ofvolatiles in the silicone rubber. This shrinkage can be compensated for by use of thedouble impression technique. A preliminary impression is made with a very high-viscosity material (putty), providing space for the final impression, which is madewith a low-viscosity material using the preliminary impression as the tray.3. Loss of detail. Premature removal of the impression from the mouth could causeloss of detail. Failure to allow the impression material to set adequately will result inplastic deformation. Loss of detail also can be caused by incomplete mixing. Failure
to adequately incorporate all the catalyst into the base will result in incompletepolymerization. Loss of detail can also result from movement of the tray after theimpression has been seated. Failure to maintain the tray in a stable position will resultin a blurred impression.DisinfectionCondensation silicone impressions can be disinfected by immersion in sodiumhypochlorite, iodophors, complex phenolics, glutaraldehydes, or phenolicglutaraldehydes. The manufacturers recommendations for proper disinfection shouldbe followed.Addition (vinyl) siliconesAddition silicones represent an advance in accuracy over condensation silicones.This has been achieved by a change in polymerization reactions to an addition typeand the elimination of an alcohol by-product that evaporates, causing shrinkage.These materials are available as two-paste systems in four viscositieslight, medium,heavy, and puttyand a range of colors, allowing monitoring of the degree of mixing.Due to their high accuracy, these materials are suitable for fixed and removable partialdenture impressions. They are rigid after setting and expensive, and therefore are notused for routine study models. Hydrophilic materials have been introduced thatreportedly contain surfactants to improve the wetting characteristics compared tounmodified silicones. Monophase materials have been formulated with sufficientshear thinning to be used as both low-viscosity and high-viscosity materials.CompositionThese materials are based on silicone prepolymers with vinyl and hydrogen sidegroups, which can polymerize by addition polymerization. They are therefore calledvinyl or addition silicones. The setting reaction is produced by mixing one pastecontaining the vinyl-poly(dimethylsiloxane) prepolymer with a second paste thatcontains a siloxane prepolymer with hydrogen side groups. A platinum catalyst,chloroplatinic acid, is present in one of the pastes and starts the additionpolymerization reaction as follows:Other reactions also occur that may release hydrogen gas, which on rare occasion canproduce porosity. Some manufacturers include hydrogen absorbers in theirformulations to eliminate this problem. Since no volatile by-products are produced inthe reaction, addition silicones have a much greater dimensional stability thancondensation silicones. Some manufacturers include a retarder for extending theworking and setting times.
Mechanical propertiesThe working and setting times of addition silicones are faster than polysulfides; aretarder is often supplied to extend the working time. Addition silicones haveexcellent elasticity and show very low dimensional shrinkage upon storage (see Table7-2). Therefore, addition silicones can be safely poured up later or sent to a dentallaboratory. Addition silicones do have greater rigidity, however, and therefore it isdifficult to remove the impression around undercuts, as indicated by the lowerflexibility value. The tear strength of addition silicones is similar to that ofcondensation silicones, but less than that of polysulfides.ManipulationAddition silicones are as pleasant to handle as condensation silicones. Because thereis the possibility of hydrogen release upon setting, finely divided palladium is addedto some products to absorb the hydrogen and prevent bubbles from forming on stonedie surfaces. If a product does not contain a hydrogen absorber, an hour should passbefore pouring dies, and the impression should stand overnight before epoxy dies arepoured. Addition silicones can be electroplated with both copper and silver.Automatic mixers that provide quick, bubble-free mixes are available with severalproducts (Fig 7-3).Fig 7-3 Automatic mixers, which provide quick, bubble-free mixes, are available withmany addition silicone impression materials.AdvantagesAddition silicones are highly accurate and have high dimensional stability after
setting. Recovery from deformation on removal is excellent. The material stays in thetray of reclined patients, does not stain clothing, has pleasant colors and scents, maybe used with stock or custom trays, and can be copper- or silverplated. The materialsmay be poured 1 week after taking the impression, and multiple pours are possible.DisadvantagesThe Disadvantages are that the material is expensivetwice the cost of polysulfides;is more rigid than condensation silicones and difficult to remove around undercuts;has a moderate tear strength, making removal from gingival retraction areassomewhat risky; and may release hydrogen gas on setting, producing bubbles on diesurfaces if an absorber is not in the product. Hydrophobic materials are difficult toelectroplate and to pour in stone. Also, sulfur in latex gloves and rubber dams caninhibit polymerization.Troubleshooting1. Inadequate working time. This can result from excessive temperature. As thetemperature increases, the working and setting times decrease. If the impressionmaterial does not set, the catalyst may have been contaminated. The platinum-containing catalyst becomes inactive after contacting certain substances, such as tin orsulfur compounds. If addition silicones are combined with condensation silicones, thematerial will not set. Components from these two systems are not compatible andcannot be mixed together.2. Loss of detail. This could occur if unmodified addition silicones are used. Thesehydrophobic materials cannot displace any moisture or hemorrhage that is notremoved prior to placement of the impression material.3. Porosity. The stone surface may appear porous if hydrogen gas is evolved. If this isthe case, it is recommended that the pouring of dies be delayed for at least 1 hour.4. Distortion. This may occur if the polysiloxane adhesive does not provide adequateretention. Mechanical retention may be required in combination with the adhesive.DisinfectionAddition silicone impressions can be disinfected by immersion in sodiumhypochlorite, iodophors, complex phenolics, glutaraldehydes, or phenolic glutaralde-hydes. The manufacturers recommendations for proper disinfection should befollowed.Polyether rubberPolyether rubbers are used for accurate impressions of a few prepared teeth withoutsevere undercuts. Their high stiffness and short working time restricts their use toimpressions of a few teeth. Polyethers are available in low-, medium-, and high-viscosity materials.
CompositionPolyethers are supplied as two-paste systems. The base paste contains low-molecular-weight polyether with ethylene-imine terminal groups:along with fillers, such as colloidal silica, and plasticizers:The catalyst paste contains an aromatic sulfonic acid ester plus a thickening agent toform a paste along with fillers:When the base paste is mixed with the catalyst paste, ionic polymerization occurs byring opening of the ethylene-imine group and chain extension. The reaction convertsthe paste to a rubber as follows:Mechanical propertiesPolyethers are similar to addition silicones in properties. The early polyethers hadshort working and setting times and low flexibilities. Thinners were available toincrease the working time and flexibility without any significant loss of other physicalor mechanical properties. However, more recent formulations have a working time of2.5 minutes and a setting time of 4.5 minutes (see Table 7-4). Shrinkage values of0.3% in 24 hours place the polyethers at the upper end of the range for accuracy, butinferior to some addition silicones. Because this rubber absorbs water and changesdimensions, storage in water is not recommended. Elastic recovery values average98.5%, between those for polysulfides and addition silicones (see Table 7-2). The
flow of polyethers is very low and contributes to accuracy. The flexibility also is low(ie, the stiffness is high). This quality causes some problems on removal of theimpression from the mouth or the die from the impression. More rubber between thetray and the impression area is recommended to relieve this problem. Polyethers havelow tear strength values.ManipulationThe manipulation of polyethers is similar to that of polysulfides and silicones. Equallengths of base and catalyst paste are mixed vigorously and rapidly (30 to 45seconds), because the working time is short. They are easy to mix. The impressionscan be readily silverplated to produce accurate dies. Precautions should be taken tomix the material thoroughly and to avoid contact of the catalyst with the skin ormucosa because tissue reactions have been observed.A handheld gun-type mixer that provides quick, bubble-free mixes is available for oneproduct (Permadyne Garant, ESPE). Also, an automatic mixing device (Pentamix,ESPE) (Fig 7-4) has been introduced for use with a polyether packaged in polybags(Impregum Penta).Fig 7-4 The Pentamix 2 is used for mixing PENTA polyether impression materials(ESPE).AdvantagesAdvantages of polyethers include pleasant handling and ease of mixing. Thesematerials are more accurate than polysulfide or condensation silicone impressionmaterials. They have good surface detail reproduction and are easily poured in stone.If kept dry, they will be dimensionally stable for up to 1 week.DisadvantagesDisadvantages include high cost, short working and setting times, and high stiffnessafter setting, which limit their use. Their bitter taste is objectionable to some patients.
Storage of polyether impressions is critical, as they will distort if stored in water orhigh humidity. They cannot be left in disinfectant solutions for long periods.Troubleshooting1. Inadequate working time. This can result from excessive temperature. An increasein temperature will decrease the working and setting times. An improper base-to-catalyst ratio (too much catalyst) will decrease the working time.2. Tearing. The rigidity of this material may result in tearing upon removal of theimpression from the mouth or of the die from the impression. Tearing may occur ifthe rubber thickness is inadequate (at least 4 mm).3. Distortion. The impression may distort due to moisture absorption and/orplasticizer extraction. These phenomena may result in dimensional change whenimpressions are stored in high-humidity environments or are exposed to water. Theuse of the thinner may increase the water absorption. Delay in impression placementmay cause distortion. The onset of setting will result in the formation of elasticproperties, which will cause deformation upon removal from the mouth.4. Loss of detail. This can be caused by incomplete mixing. Failure to obtain ahomogeneous mix will result in incomplete polymerization. If problems areencountered with multiple dies, it may be the result of gingival tearing and/orswelling. The rigidity and the relatively low tear strength of the polyethers may resultin progressive deterioration at the gingival margin of the impression. The impressionmay absorb enough moisture from the gypsum that multiple pours could produceswelling.DisinfectionPolyether impressions can be disinfected by immersion in sodium hypochlorite. Themanufacturers recommendations for proper disinfection should be followed.Dental Duplicating MaterialsDental duplicating materials are used to prepare duplicate casts for prostheticappliances and orthodontic models. These materials are used to make an impressionof the original dental cast. Agar hydrocolloid duplicating materials are used mostfrequently. Their composition has a higher water content than agar hydrocolloidimpression materials, and subsequently, a lower agar content. Therefore, thecompressive strengths for duplicating materials is generally lower than those ofimpression materials. Advantages of the reversible materials are that they can bereused a number of times and may be stored in the liquid state for use as needed.Disadvantages include the fact that immediate pours are necessary and degradation ofthe material will be accelerated by contamination. A classification key is shown in Fig7-5.
Fig 7-5 A classification key of dental duplicating materials.Clinical Decision Scenarios for Dental Impression MaterialsThis section presents one approach for choosing impression materials for specificsituations. This approach is based on consideration of the advantages andDisadvantages of each material and takes into account the different practitionerrequirements, such as skill level, cost factors, and so on, as applicable.Each scenario includes (1) a description of the situation; (2) a list of the criticalfactors; (3) a list of the advantages and Disadvantages of each material prioritizedusing the following codes: * = of minor importance, ** = important, *** = veryimportant; and (4) an analysis of the situation and the decision reached.Materials Polysulfides vs addition silicones in a dental school clinicDescription A dental school instructor has been asked to determine whichimpression material will be used in the undergraduate crown-and-bridge clinics. Thereis a fixed budget that, typical of universities, dictates the use of inexpensive materials.The students are slow and unskilled at their stage of training, so a material allowinglong working time is desirable. In addition, the students have not yet developed theirgingival retraction techniques to the point that they have a wide sulcus into which toinject their syringe material. Because of this, a material with a high tear strength isdesirable so the gingival area will not tear off from the main part of the impressionand remain in the sulcus upon removal of the tray. After review of the materialsavailable, all are rejected except for the polysulfides (mercaptans) and the additionsilicones (polyvinyl siloxanes).Critical Factors Low cost, long working time, high tear strength
PolysulfidesAdvantages*** Longer working time*** Lower cost*** Good tear resistance * High flexibility (easy to remove from undercuts)*** Good accuracyDisadvantages * Disagreeable odor and taste * Can stain clothing * Low dimensional stability (should be poured within 1 hour) * Longer setting timeAddition siliconesAdvantages * Good dimensional stability (can be mailed unpoured) * Short setting time*** Very accurate * Easy to mix and clean up * No disagreeable odor or taste * Rigid materialDisadvantages*** High cost * Low flexibility (harder to remove from undercuts)*** Shorter working time*** Lower tear resistance (may tear off in deep subgingival areas)
* Some emit hydrogen gas (pouring must be delayed)Analysis/Decision Since the factors identified as important were low cost, high tearstrength, and long working time, all advantages or Disadvantages pertaining to theseproperties are marked ***, as is the property of good accuracy. This is essential in anyimpression material used for crown-and-bridge procedures. Because accuracy is anadvantage of both materials, it cancels out and is not a deciding factor.In this example, the factors the dentist is interested in are advantages for thepolysulfides, but not for the addition silicones. This makes the choice easythepolysulfides are selected.The next step is to conduct a trial of the chosen material to see if this decision is wellfounded. For example, one half of the class takes impressions with polysulfide, andthe other half uses the material previously used. If the polysulfide works well in thehands of students and is less expensive than the addition silicone, the trial confirmsthe decision.Materials Polysulfides vs addition silicones in a busy practiceDescription An experienced clinician in a busy practice has been using agarhydrocolloid in water-cooled trays but has heard that the new elastomeric impressionmaterials have become more dimensionally stable than they were originally. She isinterested in trying either a polysulfide or an addition silicone. She has alwaysobtained very good impressions with the agar hydrocolloid material but has neverliked having to interrupt her busy schedule to pour the impressions right away. Shefeels that her time could be better used if a technician could set the dowel pins andpour the impression, but she has not felt that her practice is large enough to justify anin-office laboratory technician. She has likewise been unable to send the agarhydrocolloid impressions to a laboratory for pouring because of the materialsproperties.The clinician realizes that to use a polysulfide material, she should use custom traysdue to the lack of dimensional stability of the material. However, she does not like totake the dental assistant away from chairside for the time required to make a traybecause she lowers productivity by doing so. She would prefer a material withsufficient dimensional stability that it could be used in a disposable stock plastic tray.She is also looking for a material that will set much faster than the agar so she candecrease chair time for a crown impression.Critical Factors Low cost, short setting time, good dimensional stabilityPolysulfidesAdvantages * Longer working time
*** Lower cost * Good tear resistance * High flexibility (easy to remove from undercuts)*** Good accuracyDisadvantages * Disagreeable odor and taste * Can stain clothing*** Low dimensional stability (should be poured within 1 hour)*** Longer setting timeAddition siliconesAdvantages*** Good dimensional stability (can be mailed unpoured)*** Short setting time*** Very accurate * Easy to mix and clean up * No disagreeable odor or taste * Rigid materialDisadvantages*** High cost * Low flexibility (harder to remove from undercuts)** Shorter working time * Lower tear resistance (may tear off in deep subgingival areas) * Some emit hydrogen gas (pouring must be delayed)Analysis/Decision Here the decision is less obvious than in the previous example.The addition silicone seems to offer much of what the dentist desires, but it coststwice as much as the polysulfide. In this case, the decision might be in favor of thepolysulfide due to the significant cost difference. After the trial period, however, the
dentist confirmed her suspicion that the polysulfide was not stable enough to usestock trays and it took 15 to 30 minutes for either her or her assistant to fabricate thecustom trays. She also found that that use of "putty" material to line the stock traygreatly reduced the cost of the addition silicone. In addition, she found that placingdowel pins and pouring up the polysulfide took another 15 to 30 minutes of someonestime. The amount of time lost from chairside production more than offset the highercost of the addition silicones, whose properties allowed her to use stock trays and tomail the impressions to her laboratory. Seeing this in her trial, the dentist reconsideredand changed to the addition silicone, which satisfied her needs.Materials Polysulfides vs addition silicones for "triple tray"Description The dentist has been using the polysulfides and is quite content butwishes to try a new impression technique that is gaining great favor among his peers.This method uses what is known as a "triple tray" and has the advantage for the singlecrown of obtaining the working impression, the opposing impression, and the biterelation all at the same time. This could significantly cut down the amount of timeneeded for each patient. The dentist finds, however, that the sides of the flimsy plastictrays sometimes spread apart when the dental arches impinge on them as the patientbites into position. The tray then attempts to spring back from this distortion when itis removed from the mouth. The recovery from the spreading requires that he use amaterial with sufficient rigidity that it can maintain its shape against this elasticrecovery of the tray. If not, the tray recovery may distort the impression and result in anonfitting crown.Critical Factors Low flexibility, good dimensional stabilityPolysulfidesAdvantages * Longer working time * Lower cost * Good tear resistance*** Good accuracyDisadvantages*** High flexibility (easy to remove from undercuts) * Disagreeable odor and taste * Can stain clothing*** Low dimensional stability (should be poured within 1 hour)
* Longer setting timeAddition siliconesAdvantages*** Good dimensional stability (can be mailed unpoured) * Short setting time*** Very accurate * Easy to mix and clean up * No disagreeable odor or taste*** Rigid materialDisadvantages * High cost*** Low flexibility (hard to remove from undercuts) * Shorter working time * Lower tear resistance (may tear off in deep subgingival areas) * Some emit hydrogen gas (pouring must be delayed)Analysis/Decision In this case, the trial period showed that the addition silicone wasthe only feasible choice. The need for rigidity in the impression material for the tripletray is important enough that it becomes the deciding factor. Although other factors,such as accuracy, are important, unless the material is rigid enough to hold its shape,these other properties are meaningless.Materials Polysulfides vs addition silicones for full-arch impressionDescription In this situation, the dentist is a prosthodontist in an established specialtypractice. He has a dental laboratory in his office and employs two dental laboratorytechnicians. He therefore has the capability of having custom trays made in his officeand the impressions poured right away. Most of his patients have been referred fromdentists who do the easier cases themselves. Consequently, his patients usuallyalready have multiple crowns or fixed partial dentures in different areas of the mouth.He feels that full-arch impressions are better because in the more extensive cases heneeds the accuracy in bite relations that can only come from full-arch registration. Hehas heard that addition silicones are very accurate and that they have better
dimensional stability than the material he has been using. This appeals to him for"pickup" impressions where a rigid material and better dimensional stability greatlyenhance the probability of success. On the other hand, he is concerned that thestiffness of the addition silicone will make the removal of full-arch impressions fromthe mouth much more difficult. He is also concerned that the stiffness may pose agreater risk of inadvertently removing crowns or fixed partial dentures that hispatients already have in other areas of the mouth.Critical Factors Good accuracy, high flexibility, good dimensional stabilityPolysulfidesAdvantages * Longer working time * Lower cost * Good tear resistance*** High flexibility (easy to remove from undercuts)*** Good accuracyDisadvantages * Disagreeable odor and taste * Can stain clothing*** Low dimensional stability (should be poured within 1 hour) * Longer setting timeAddition siliconesAdvantages*** Good dimensional stability * Short setting time*** Very accurate * Easy to mix and clean up * No disagreeable odor or taste*** Rigid material
Disadvantages * High cost*** Low flexibility (harder to remove from undercuts) * Shorter working time * Lower tear resistance (may tear off in deep subgingival areas) * Some emit hydrogen gas (pouring must be delayed)Analysis/Decision The high flexibility listed under the advantages of polysulfides isoffset by the rigidity listed as an advantage under addition silicones. He found that therigidity was desirable for pickup impressions, but the flexibility was desirable forregular impressions. He decided to try the addition silicone and found that it did,indeed, give very accurate and dimensionally stable impressions. His pickupimpressions were better than they had ever been. However, in normal situations therigidity of the material made removal of the full-arch impressions much moredifficult. Some crowns and fixed partial dentures on which he was not working cameoff in the impression material due to its rigidity. He found, however, that he couldcompensate for this rigidity by filling the impression tray only partially full in theareas where he only needed the occlusal registration and filling it full in the area ofthe preparations.Glossaryaddition silicone A silicone polymer resulting from the free-radical polymerization ofvinyl groups by a platinum catalyst.agar An ingredient in agar impression material. It is usually extracted from seaweedas a polysaccharide.alginate Alginate impression material containing salts of alginic acid.cast material Material used to form casts (models or dies) from impressions.condensation (in polymerization) In a condensation polymerization (eg, to formsilicone impression materials), two molecules unite and one small molecule (eg, H2O,ROH) is released as a by-product.~Si-OH + R-O-Si~ ROH + ~Si-O-Si~condensation silicone A silicone polymer resulting from the condensation of terminal-OH groups by orthoalkylsilicates and releasing alcohol as a by-product.elastic recovery The amount of rebound after a cylinder of material is strained 10%for 30 seconds.
electroplate The process of depositing metal from solution onto the surface of animpression using an electric current.eugenol Oil of cloves. As a derivative of phenol, eugenol reacts as an acid with zincoxide.flexibility The amount of strain produced when a sample is stressed between 100 and1,000 g/cm2. A flexible material shows a higher value of flexibility than a stiffmaterial.flow The amount of shortening of a cylinder when placed under a light load for 15minutes.gel A colloid system in which the solid (eg, agar) and liquid (eg, water) arecontinuous phases. A gel is usually flexible.hydrocolloid A colloid system in which the liquid phase is water. Agar impressionmaterial is a hydrocolloid (agar + water).hydrophilic Having a strong affinity for water; can be readily wetted by water.hydrophobic Resistant to wetting by water.hysteresis The phenomenon of a gels having a liquefaction temperature differentfrom the solidification temperature of the sol.imbibition The taking up of fluid by a colloidal system, resulting in swelling.plasticizer A material that is added to increase flow.polyether The polymer resulting from the ionic polymerization with ring opening ofthe ethylene-imine group and chain extension.polysulfide The polymer resulting from the condensation of terminal mercaptangroups catalyzed by lead dioxide or other catalysts.silicone rubber A polymer resulting from the formation of silicon-oxygen-siliconbonds (-Si-O-Si-). Silicone impression material is a silicone rubber.sol A colloid system in which the solid phase is dispersed in the liquid phase. A solusually has fluid properties.syneresis The exudation of a liquid film on the surface of a gel.terminal group A chemical group at the end of a molecule (eg, -SH).thermal conductivity The quantity of heat passing through a body 1 cm thick with across section of 1 cm2 when the temperature difference between the hot and cold sidesof the body is 1C.
thermoplastic The property of softening on heating and hardening on cooling.working time Duration from the start of mixing to the time when a test rod leaves apermanent indentation in the material upon withdrawal.Discussion Questions1. Why are there so many impression materials in dentistry at the present time?2. How could the movement of soft tissues during impression taking affect theaccuracy of the final impression?3. Since elastic impression materials are viscoelastic, wouldnt immediate pouring of agypsum cast result in inaccuracy?4. Why is it essential to sterilize an impression before sending it to a laboratory, andhow is this done?5. Why is the impression tray an important factor in obtaining a good impression?Study Questions(See Appendix E for answers.)1. What components are present in dental compound, and what is the purpose ofeach?2. What term describes the quality of dental compound that allows it to be repeatedlysoftened on heating and hardened on cooling?3. What is the principal difference between the properties of impression and tray-typecompounds?4. What precautions should be taken when heating dental compound?5. What importance does low thermal conductivity have on the clinical handling ofdental impression compound?6. What factors affect the flow of impression compound?7. What are the reactive ingredients in a zinc oxide-eugenol material?8. What is responsible for the setting of zinc oxide-eugenol impression paste?9. What factors affect the setting time of zinc oxide-eugenol?10. What are the functions of the various components in agar hydrocolloid?11. What is meant by hysteresis in agar hydrocolloid?
12. What kinds of dimensional changes occur when an agar impression is stored inair, water, 100% relative humidity, or potassium sulfate solution?13. What is the function of each of the components in alginate powder?14. What factors affect the setting time of alginates?15. What reaction is responsible for providing the working time of alginate, and whatother reaction is responsible for the setting of alginate?16. Why are alginate impression materials called irreversible hydrocolloids?17. What effect does the water/powder ratio of alginates have on their properties?18. What effect does spatulation of alginates have on their properties?19. What effect does water temperature have on the working and setting times ofalginates?20. How do the properties of alginate impression materials compare with those of agarimpression materials?21. Describe the setting reactions for polysulfide, silicone, and polyether rubberimpression materials.22. What effect do proportioning and temperature have on the working and settingtimes of the three rubber impression materials?23. What impression material may be used if you wish to use either a gypsum die, asilverplated die, or a copperplated die?24. Compare the elastic recoveries of polysulfide, silicone, and polyether impressionmaterials. How does elastic recovery affect clinical usage?25. Compare the flexibilities of polysulfide, silicone, and polyether impressionmaterials.26. How would you disinfect your impression prior to sending it to the laboratory?27. List the advantages of each of the following recent advances in impressionmaterials: (a) addition silicones with hydrophilic properties; (b) single-viscosity, ormonophase, addition silicones; (c) automatic mixers for addition silicones andpolyethers.Recommended ReadingAlbers HF (1990). Impressions: A Text for Selection of Materials and Techniques.Santa Rosa, CA: Alto Books.
American Dental Association (1993). Clinical Products in Dentistry: a DesktopReference. Chicago: ADA.Anderson JN (1960). Flow and elasticity in alginates. Dent Progr 1:63-74.Anusavice KJ (1988). Dental impression materials: reactor response. Adv Dent Res2:65-70.Braden M (1966). Characterization of the setting process in dental polysulfiderubbers. J Dent Res 45:1065-1071.Braden M, Causton B, Clarke RL (1972). A polyether impression rubber. J Dent Res51:889-896.Braden M, Elliot JC (1966). Characterization of the setting process of silicone dentalrubbers. J Dent Res 45:1016-1023.Buchan S, Peggie RW (1966). Role of ingredients in alginate impression compounds.J Dent Res 45:1120-1129.Chee WW, Donovan TE (1992). Polyvinyl siloxane impression materials: a review ofproperties and techniques. J Prosthet Dent 68:728-732.Chong JA, Chong MP, Docking AR (1965). The surface of gypsum cast in alginateimpressions. Dent Pract 16:107-109.Council on Dental Materials and Devices (1977). Status report on polyetherimpression materials. J Am Dent Assoc 95:126-130.Council on Dental Materials, Instruments, and Devices (1990). Vinyl polysiloxaneimpression materials: a status report. J Am Dent Assoc 120:595-596, 598, 600.Council on Dental Materials, Instruments, and Devices (1991a). Disinfection ofimpressions. J Am Dent Assoc 122(8):110.Council on Dental Materials, Instruments, and Devices (1991b). Retarding the settingof vinyl polysiloxane impressions. J Am Dent Assoc 122(8):114.Council on Dental Materials, Instruments, and Devices; Council on DentalTherapeutics; Council on Dental Research; Council on Dental Practice (1992).Infection control recommendations for the dental office and the dental laboratory. JAm Dent Assoc 123(Suppl):1-8.Craig RG (1977). A review of properties of rubber impression materials. J Mich DentAssoc 59:254-261.Craig RG (1985). Evaluation of an automatic mixing system for an addition siliconeimpression material. J Am Dent Assoc 110:213-215.Craig RG (1988). Review of dental impression materials. Adv Dent Res 2:51-64.
Craig RG, OBrien WJ, Powers JM (1996). Dental MaterialsProperties andManipulation, ed 6. St. Louis: Mosby.Craig RG, Sun Z (1994). Trends in elastomeric impression materials. Oper Dent19:138-145.Craig RG, Urquiola NJ, Liu CC (1990). Comparison of commercial elastomericimpression materials. Oper Dent 15:94-104.Farah JM, Powers JM (eds) (1992). Impressions and accessories. The Dental Advisor9(4):1-8.Fish SF, Braden M (1964). Characterization of the setting process in alginateimpression materials. J Dent Res 43:107-117.Harris WT Jr (1969). Water temperature and accuracy of alginate impressions. JProsthet Dent 21:613-617.Johnson GH, Craig RG (1986). Accuracy and bond strength of combinationagar/alginate hydrocolloid impression materials. J Prosthet Dent 55:1-6.Kahn RL, Donovan TE, Chee WW (1989). Interaction of gloves and rubber dam witha poly(vinyl siloxane) impression material: a screening test. Int J Prosthodont 2:342-346.Kim K-N, Craig RG, Koran A III (1992). Viscosity of monophase addition siliconesas a function of shear rate. J Prosthet Dent 67:794-798.Lautenschlager EP, Miyamoto P, Hilton R (1972). Elastic recovery of polysulfidebase impressions. J Dent Res 51:773-779.MacPherson GW, Craig RG, Peyton FA (1967). Mechanical properties ofhydrocolloid and rubber impression materials. J Dent Res 46:714-721.Marker VA (1989). Dental impression materials. In: Okabe T, Takahashi S (eds).Transactions International Congress on Dental Materials [Honolulu, HI, 1-4 Nov1989]. Honolulu, HI: 114-138.Merchant VA (1992). Update on disinfection of impressions, prostheses, and casts. JCalif Dent Assoc 20:31-35.McCabe JF, Wilson HJ (1978). Addition curing silicone rubber impression materials:an appraisal of the physical properties. Br Dent J 145:17-20.McLean JW (1961). Physical properties influencing the accuracy of silicone andthiokol impression materials. Br Dent J 110:85-91.Myers GE, Peyton FA (1959). Clinical and physical studies of the silicone rubberimpression materials. J Prosthet Dent 9:315-324.
Myers GE, Peyton FA (1961). Physical properties of the zinc oxide-eugenolimpression pastes. J Dent Res 40:39-48.Myers GE, Stockman DG (1960). Factors that affect the accuracy and dimensionalstability of the mercaptan rubber base impression materials. J Prosthet Dent 10:525-535.Naylor WP, Evans DB (1991). An overview of impression materials and techniquesfor fixed prosthodontics. In: Hardin JF (ed). Clarks Clinical Dentistry, vol 4.Hagerstown, MD: Harper and Row.Pratten DH, Craig RG (1989). Wettability of a hydrophilic addition siliconeimpression material. J Prosthet Dent 61:197-202.Pratten DH, Novetsky M (1991). Detail reproduction of soft tissue: a comparison ofimpression materials. J Prosthet Dent 65:188-191.Rosenblum MA, Asgar K, Leinfelder KF (1985). Dental prosthetic materials. In:Reese JA, Valega TM (eds). Restorative Dental Materials, vol I. London:Quintessence, 158-168.Roydhouse RH (1962). Materials in Dentistry. Chicago: Year Book MedicalPublishers.Smith DC, Wilson HJ (1965). Further studies on alginate impression materials. DentPract 15:380-382.Stackhouse JA Jr (1970). The accuracy of stone dies made from rubber impressionmaterials. J Prosthet Dent 24:377-386.Stackhouse JA Jr (1980). Electrodeposition in dentistry: a review of the literature. JProsthet Dent 44:259-263.Stackhouse JA Jr (1981a). Impression materials and electrodeposits. Part I.Impression materials. J Prosthet Dent 45:44-48.Stackhouse JA Jr (1981b). Impression materials and electrodeposits. Part II.Electrodeposits. J Prosthet Dent 45:146-151.Stannard JG, Sadighi-Nouri M (1986). Retarders for polyvinylsiloxane impressionmaterials: evaluation and recommendations. J Prosthet Dent 55:7-10.Wilson HJ (1966a). Some properties of alginate impression materials relevant toclinical practice. Br Dent J 121:463-467.Wilson HJ (1966b). Elastomeric impression materials. I. The setting material. Br DentJ 121:277-283, 1966.Wilson HJ, Smith DC (1963). Alginate impression materials. Br Dent J 114:20-26.
Chapter 8. Polymeric Restorative MaterialsIntroductionThe first material developed for use as a direct esthetic restorative was silicatecement. Introduced in the late 1800s, the cement was prepared from an alumina-silicaglass and a phosphoric acid liquid. Highly soluble in oral fluids, silicate deterioratedrapidly, yet remained the favored material until the early 1950s. Dissolution,discoloration, loss of translucency, and lack of adequate mechanical propertiescontributed to its eventual replacement. Its main advantage was the slow release offluoride from the glass phase.Self-curing unfilled acrylic resins were introduced around 1945 as a substitute forsilicate cement and were in moderate use in the 1950s. These materials were related todenture base resins and were much less soluble and more color stable than silicates.They were easy to use, polishable, and had good initial esthetics. Their main problemswere high shrinkage upon polymerization, large thermal dimensional change, eventualdiscoloration, and a high wear rate.Resin composites, a combination of hard, inorganic filler particles bonded to softdimethacrylate polymer, were introduced in the 1960s. As a consequence of thebonded filler phase, these materials had much better mechanical properties than didunfilled resins, approaching the properties of dentin and enamel. Originally intendedfor use in anterior Class 3, 4, and 5 restorations where esthetics are important,improvements have included light curing, bonding to tooth structure, and reducedwear. Continued development in wear resistance, dentin bonding, and reducedpolymerization shrinkage has led to their increased use in posterior restorations.ClassificationA composite is a material composed of two or more distinct phases. Resin compositesfor dental use were formulated to combine the esthetics and ease of use of apolymerizable resin base with the improved properties to be gained from the additionof a ceramic filler. Resin composites are often classified according to the size of theceramic filler particle (Fig 8-1 and Tables 8-1 and 8-2).Fig 8-1 The microstructure of resin composite materials.
Table 8-1 Average properties of resin composites Property Microfilled Microhybrid Inorganic filler content (vol %) 20-55 60-70 Thermal conductivity Insulator Insulator Coefficient of thermal expansion 50-68 20-40 -6 (/C 10 ) Hardness (Knoop) 22-36 50-60 Water sorption (mg/cm2) 1.2-2.2 0.5-0.7 Compressive strength (MPa) 225-300 300-350 Tensile strength (MPa) 25-35 35-60 Youngs modulus (GPa) 3-5 7-14 Polymerization shrinkage (%) 2-4 1.5-1.7 Table 8-2 Clinical characteristics and selection of resin composites Microfilled Microhybrid Fine particleFiller size 0.01-0.12 um 0.01-3.0 um 0.5-3.0 umAppearance Optical properties Good gloss, luster, Opaque appearance similar to enamel and smoothnessPolishability Highly polishable Polishable Semi polishableUsage Non-stress-bearing Anterior and posterior Core buildups, esthetic restorations* restorations conservative posterior restorations *Only heavily filled microfilled materials may be used for posterior restorations. Fine-particle resin composites contain ground glass or quartz particles 0.5 to 3.0 um in diameter, which occupy 60% to 77% of the composite by volume. Since the filler has a density greater than that of the polymer matrix, the fraction of the filler by weight is higher, about 70% to 90%. Particles present may be of uniform diameter or have a distribution of diameters, in which case smaller particles fit in the spaces between larger particles, and packing is more efficient. Microfilled resin composites contain spherical colloidal silica particles 0.01 to 0.12 um in diameter. Colloidal silica is produced by vapor-phase hydrolysis of silicon compounds resulting in an average surface area of 200 m2/g, which greatly increases the viscosity of the polymer matrix upon incorporation. Filler loading in these composites is therefore limited to about 20% to 55% by volume or 35% to 60% by weight, and low-molecular-weight organic diluents of low viscosity are often added to give the composite a workable clinical consistency. Filler content may be increased and properties improved by grinding a polymerized microfilled composite into particles 10 to 20 um in diameter and subsequently using these reinforced particles as filler along with colloidal silica. Heavily filled microfilled composites have a filler content of 32% to 66% by volume or about 40% to 80% by weight (Fig 8-2).
Fig 8-2 A microfilled light-cured composite restorative material in compules.Hybrid (or blend) resin composites have a combination of colloidal and fineparticles as filler. The colloidal particles fill the matrix between fine particles,resulting in a filler content of around 60% to 65% by volume. Hybrids (Figs 8-3a and8-3b) currently dominate the market.Fig 8-3a A well-established hybrid composite.Microhybrid resin composites, the generic term for advanced composites, are acombination of a microfilled and fine-particle composite and are so called because oftheir small-diameter (0.4 to 1.0 um) filler particles. They were recently introduced asall-purpose "universal" composites offering both esthetics and superior wearresistance for use in anterior and posterior applications (Fig 8-3b).
Fig 8-3b Microhybrid composite with low average particle size (0.4 um).Composition and ReactionFiller compositionFiller particles are of inorganic composition. In addition to quartz, fine-sized particlesmay be composed of barium or lithium aluminum silicate glasses; borosilicate glass;or barium, strontium, or zinc glasses. Particles in microfilled composites are colloidalsilica.Composites may be made radiopaque by incorporating elements of high atomicweight, such as barium, strontium, zirconium, or ytterbium, into the filler particle.Organic matrixThe organic polymer matrix in currently available composites is most commonly anaromatic or urethane diacrylate oligomer such as bisphenol A-glycidyl methacrylate(bis-GMA) or urethane-dimethacrylate (UDMA), represented by the simplifiedformula:where R may be any of a number of organic groups, such as methyl-, hydroxyl-,phenyl-, carboxyl-, and amide-.The oligomers have in common reactive double bonds at each end of the molecule,which are able to undergo addition polymerization in the presence of free radicals.The oligomer molecules are highly viscous and require the addition of low-molecular-weight diluent monomers, usually triethylene glycol dimethacrylate (TEGMA), so aclinically workable consistency may be maintained upon the incorporation of the
filler.Coupling agentsA bond between filler particle and matrix in the set composite is achieved by use of anorganic silicon compound, or silane coupling agent. The silane molecule has reactivegroups at both its ends and is coated on the filler particle surface by the manufacturerbefore mixing with the oligomer. During polymerization, double bonds on the silanemolecule also react with the polymer matrix. A bond between filler and matrix allowsthe distribution of stresses generated under function. The net result is a material withstrength properties greater than those of the particulate filler or the matrix separately.Bonding also enhances the retention of the filler particle during abrasive action at thecomposite surface. As a result, hard filler particles, in addition to soft matrix, arepresent to engage in abrasive wear with opposing enamel, for example, greatlyimproving the wear resistance of the material.Initiators and acceleratorsPolymerization of composites may be achieved by chemical means (self-cure) or byvisible-light activation. Dual cure is a combination of light and chemical curing. Inchemically activated systems, an organic peroxide initiator (or catalyst), upon reactingwith a tertiary amine accelerator, produces free radicals that attack the double bondsof oligomer molecules and begin the process of addition polymerization.Initiation of polymerization in light-activated systems depends on the scission of theinitiator molecule, often camphorquinone, by visible light of appropriate wavelength.In the presence of an aliphatic amine accelerator, free radicals are produced andpolymerization begins. For both systems, the following general reaction occurs:Since dimethacrylate oligomers as well as dimethacrylate diluent monomers havereactive double bonds at each end of the molecules, polymerization results in a highlycross-linked polymer.Other ingredientsInorganic oxide pigments are added to composites in small amounts to provide arange of standard shades. Most often, four shades, ranging from yellow to gray, aresupplied. In response to consumer interest, manufacturers now offer an extendedrange of 16 or 25 shades, as well as shade selections from the Bioform and Vitaceramic shade guides. Most manufacturers offer modifiers such as highly pigmentedtints for mixing with standard shades, as well as opaquers and glazes.Polymerization inhibitors and stabilizers are added to the composite to lengthen shelf
life.Composite Product SystemsComposites are packaged as a two-paste system supplied in two jars, or as a single-paste system supplied in a syringe or in compules. An enamel acid etchant, alongwith a dentin bonding agent, may also be supplied by the manufacturer.Chemically cured composites supplied as two pastes are typically used as resincements or for core applications. Each jar contains dimethacrylate and filler; one jaralso contains the peroxide initiator, and the other contains the amine accelerator. Theinitiator and the accelerator are kept separate until mixing. A few composites areoffered as two-paste, dual-curing systems. Setting begins after the catalyst and baseare mixed and can be accelerated by light curing.Todays composites designed for restorative applications are supplied as single pastesin opaque, disposable syringes or in color-coded compules for use with a syringe.Light-activated composites are currently the most widely used systems available.Commercially available curing units transmit light from a halogen lamp to the toothsurface by way of a curved quartz rod, a liquid-filled transmission tube, or a bundle offlexible quartz fibers attached to a fiber-optic handpiece. Ultraviolet light is generallyfiltered out at the light source.The initiator present in most photocuring monomers is camphorquinone, which issensitive to light with the spectrum shown in Fig 8-4. To initiate polymerization,curing lights must emit light within this spectrum, which is in the blue range. Filteredhalogen lights produce a broad range of wavelengths within the camphorquinonespectrum and are the standard.Other lights that have higher intensities for faster polymerization have beenintroduced. These include plasma arc lamps (PAC) and argon laser lights (Fig 8-4).Although more intense, not all PAC and laser lights have the broad spectrum of thehalogen lamps. It is important to match the spectrum of a PAC light to the productbeing used. The PA 430 has been found to be more effective for certain resin prFig 8-4 Spectra of curing lights including halogen (HAL), plasma arc (PA), and argonlaser, along with absorption spectrum needed for initiation with camphorquinone.
oducts. Lasers are still in the development stage due to their narrow spectrum.Halogen curing lights are available with continuous operation and programmedcycles. One program is called a stepping function, which cycles the light on and off toreduce possible overheating of the tooth.As with ultraviolet light used in early curing units, blue light has the potential to causeretinal damage. Figure 8-5 shows a curing light for composite materials. Protectiveeyewear during operation of curing units is also available and recommended.Fig 8-5 Halogen blue curing light with variable cycles.PropertiesSetting timeComposite systems that are chemically activated have setting times ranging from 3 to5 minutes from the start of mixing. The setting time is determined at the time ofmanufacture by control of the concentrations of initiator and accelerator. However,studies show that even after a curing time of 24 hours, polymerization is incompleteand 25% to 45% of double bonds remain unreacted.The setting time and the depth of cure of light-initiated materials depend on theintensity and penetration of the light beam. Polymerization is approximately 75%complete at 10 minutes after exposure to blue light, and curing continues for a periodof at least 24 hours. At 24 hours, up to 30% of double bonds still remain unreacted.Polymerization shrinkage
The occurrence of shrinkage during polymerization creates stresses (~18 MPa) at thetooth-composite interface that may exceed the strength of any bond betweencomposite and enamel or dentin. Bond failure at the interface allows an influx of oralfluids and greatly contributes to the possibility of marginal staining, secondary caries,and postoperative sensitivity. In addition, stresses at the tooth-composite interfacemay exceed the tensile strength of enamel perpendicular to the enamel rods, resultingin fractures through the enamel along the interface.Shrinkage is a direct function of the volume fraction of polymer matrix in thecomposite, and thus occurs to a larger degree in microfilled composites than in fine-particle composites or hybrids. Microfilled composites typically show settingcontractions of 2% to 4% as compared to 1.0% to 1.7% for fine-particle composites(see Table 8-1).The shrinkage problem can be partially overcome in two ways. First, incrementaladdition and polymerization of thin layers of a light-initiated material will result indecreased total setting contraction as opposed to bulk curing a single thick layer.However, although this method does result in lower stresses at the tooth-compositeinterface, studies show that marginal gaps may occur nonetheless.A second approach involves the preparation of a composite inlay either directly in themouth or indirectly as a laboratory procedure. In the latter procedure the inlay is heatprocessed (see Fig 8-6), allowing the degree of polymerization to approach 100%, andthen cemented in the mouth with a thin layer of resin cement. The bulk of the resincomposite cement layer needed is small, producing a very small amount of shrinkageand low interfacial stresses. Long-term studies are still underway, and compositeinlays produced in this way are expected to show improved durability and increasedwear resistance due to enhanced physical properties.Fig 8-6 Composite laboratory curing unit (Targis Power; courtesy of Ivoclar NorthAmerica).
Thermal propertiesThe organic polymer matrix has low thermal conductivity, and composites thereforeprovide good thermal insulation for the dental pulp. Thermal conductivities of allcomposites closely match those of enamel and dentin and are much lower than that ofdental amalgam.As a consequence of the weak physical bonds by which individual polymer moleculesare held together, polymers have a marked tendency to expand and contract inresponse to temperature changes. In contrast, the highly inorganic content of toothstructure is affected to a much smaller degree. Dimensional changes in the compositeresulting from thermal cycling in the mouth produce further strain on the bond at thetooth-composite interface, increasing the possibility of marginal percolation. Thiseffect occurs to a larger extent with resin-rich microfilled composites than with fine-particle materials or hybrids.Water sorption and solubilityThe polymer matrix is able to absorb water, which is accompanied by some swellingof the composite, but this is not sufficient to counteract polymerization shrinkage. Theuptake of water by composites has been correlated with decreases in surface hardnessand wear resistance. As a result of their larger volume fraction of matrix, microfilledcomposites have higher water sorption values and therefore a greater potential fordiscoloration by water-soluble stains.Solubility of resin composites ranges from 1.5% to 2.0% of the original materialweight. The major detected leachable components in water include residual oligomeror monomer; therefore, incomplete polymerization of the composite results inmarkedly increased solubility. Additional leachable molecules include degradationproducts of various composite components and may include formaldehyde, benzoicacid, and methacrylic acid. The largest part of the dissolution occurs within the firstfew hours of placement.Elements from filler particles dissolve in water to varying degrees and are detected inquantities as high as 180 umol/g. Boron and silicon are the main elements, butbarium, strontium, and lead, other additives to glass particles, also leach out. Thepresence of silicon in solution may indicate degradation of the surface treatment ofthe filler.Alcohol is a solvent of bis-GMA and acidulated fluoride gels increase the rate ofdissolution of filler particles. Therefore, alcohol-free rinses and neutral fluorideproducts should be used.Color stabilityDarkening and a color shift to yellow or gray has often been noted in self-curingsystems and has been attributed to the presence of the tertiary amine accelerator,which produces colored products upon oxidation. Photo-initiated systems do notcontain a tertiary amine and have shown considerably improved color stability overlong periods of time.
Under accelerated aging conditions in a weathering chamber, erosion of the resinmatrix and exposure of filler particles of microfilled composites resulted in alightening of the color of the material. Color stability of microfilled composites,however, was affected by erosion only to a small degree.RadiopacityA degree of radiopacity slightly exceeding that of enamel may be useful in diagnosis.Radiopacity may be conferred by incorporating elements of high atomic number, suchas barium, strontium, and zirconium, into the filler. The relative number of theseatoms is still small, however, and the materials are much less radiopaque than isamalgam. Many composites currently available have some degree of radiopacity, andseveral for posterior use have radiopacities greater than that of enamel.Mechanical propertiesThe higher compressive and tensile strengths of fine-particle and hybrid composites,as compared to microfilled composites, reflect the higher volume fraction of the high-strength filler component. Note that for all materials compressive strengths are severaltimes higher than tensile strengths, reflecting the somewhat brittle behavior ofcomposites. More highly filled composites have tensile strengths near that of dentinand compressive strengths similar to or higher than that of dentin (Table 8-3). Somehighly filled composites have compressive strengths greater than that of enamel. Table 8-3 Mechanical properties of enamel and dentin Compressive Tensile Youngs Hardness number strength (MPa) strength (MPa) modulus (GPa) (Knoop, Vickers)Enamel 384 10.3 84.1 343 (408)Dentin 297 51.7 18.5 68 (60)The elastic (Youngs) modulus is a measure of a materials stiffness. A material withlow elastic modulus deflects under stress. As a group, composites have elastic modulithat are only a fraction of that of enamel. Fine-particle materials, however, havemoduli similar to that of dentin. Under high loads, such as occur in posterior teethduring mastication, deflection of the restoration strains the tooth-composite bond.Deflection additionally places considerable tensile stresses on adjacent cusps.The lower filler content of microfilled composites results in elastic moduli of onequarter to one half that of the more highly filled fine-particle composites, and aretherefore recommended for cervical (Class 5) restorations since deflection couldreduce stresses at the tooth-composite interface.Microindentation hardness of composites is directly related to volume fraction of thehard, inorganic filler component. Hardness is also related to the degree ofpolymerization. In laboratory experiments, composites that underwent a secondaryheat treatment to increase the degree of polymerization showed higher Knoophardness values than did composites that were light cured only.
As a group, the hardness of composites is a fraction of that of enamel but is similar toor higher than that of dentin.WearWear in composites is a complex phenomenon that depends on several intrinsic andextrinsic factors. The large amount of data collected for various available compositesis confusing, at least in part because measuring techniques have not beenstandardized. In vivo wear has not been shown to correlate well with any singlematerial property. In addition, the appearance of wear patterns in restorations of longduration is complicated by the presence of erosion, a degradative uniform loss ofmaterial across the composite surface; several wear mechanisms are shown in Fig 8-7.Nevertheless, a number of factors that contribute to wear have been identified.Fig 8-7 Several possible wear mechanisms for dental composites. (F = filler particle;M = matrix.) (From OBrien and Yee, 1980. Modified with permission.)Filler content, particle size, and hardnessIncreased filler volume results in decreased wear. Laboratory studies demonstrate agreater loss of material volume during abrasive action for microfilled as compared tomore highly filled fine-particle composites. A higher filler volume results in a higherfracture toughness, as shown in Fig 8-8.
Fig 8-8 The effect of filler volume fraction on fracture toughness, KIC. (Courtesy of J.Ferracane.)Keeping volume fraction constant, wear resistance is increased by decreasing the sizeof the filler particle. Large, hard particles transmit considerable stress to the matrix,possibly resulting in microcracking and subsequent loss of material (Fig 8-9). Bycontrast, a reduced load per particle results when a large number of small particles ispresent per unit volume.Fig 8-9 Worn surface of a composite restoration showing a protruding hard quartzfiller particle with an adjacent microcrack. (SEM, original magnification 1,000.)(From OBrien and Yee, 1980. Reprinted with permission.)It has been reported that wear of composites with filler particles smaller than 1.0 umoccurs at a constant rate with time. Wear of composites with particles larger than 1.0um is greatest in the year after placement, declining thereafter.The incorporation of softer filler particles with hardness characteristics similar to thatof enamel appears to result in decreased wear. It is thought that soft particles are morecapable than hard particles of absorbing energy generated during the masticatoryprocess, thereby transmitting lower stresses to the matrix. Scanning electronmicrographs of a material with hard quartz particles and another with soft glass
particles are shown in Figs 8-9 and 8-10. Note the difference in the shapes of theparticles that project from the occlusal surface.Fig 8-10 Worn surface of a composite with a soft glass filler. (SEM, originalmagnification 2,500.)Interestingly, the presence of filler particles with hardness values greater than that ofenamel has been shown to increase the roughness of opposing enamel over time.Tooth position in the archIn general, the more distally located the restoration, the higher the rate of wear.PorosityInternal porosity, particularly in stress-bearing areas, increases wear. It has beenproposed that porosities concentrate stresses in the matrix and, under loading,contribute to the formation of microcracks. In addition, voids, produced during thespatulation process or during incorporation of filler during manufacture, are air-filled.An air-inhibited layer of incompletely polymerized matrix may exist at the voidsurface. Light-initiated systems requiring no spatulation have demonstrated higherwear resistance than self-curing systems.Degree of polymerizationStrength properties of polymers are directly related to molecular size. Duringpolymerization, molecular size increases enormously. The enhanced wear resistancefound in some studies of heat-processed composite inlays is thought to be related totheir higher degree of polymerization.Coupling agentThe absence of a silane coupling agent at the matrix-filler interface reduces wearresistance by about half.Method of finishing
Wear resistance decreases with the use of carbide or diamond finishing burs. Theiruse is thought to weaken the surface through the formation of microcracks or todegrade the matrix through the generation of heat. It has been reported that treatmentof the surface after occlusal adjustment and subsequent curing with a low-viscosityunfilled resin decreases wear by about 50%.Wear resistance of composites developed for posterior use has improved steadily overrecent years.Depth of curePolymerization in both chemically and light-activated composites is incomplete.Degrees of conversion are reported to be in the range of 60% to 75%. The number ofunreacted double bonds at 24 hours is higher in light-activated than in chemicallyactivated systems and results from a number of factors affecting depth of cure.Light intensity at the surface and time of exposure are critical. The tip of the lightsource should be held within 3 to 4 mm of the surface in order to cure a light shade ofmaterial to a depth of 2.0 to 2.5 mm using a standard exposure time of 40 seconds. Alonger exposure time will increase the degree of polymerization at all depths and is anecessity when using darker shades or more opaque materials. A reduction inthickness of the increment to be cured is a more reliable way of achievingpolymerization than is an increase in exposure time. In addition, hardness of the topsurface of a cured restoration is not a good indication of the extent of polymerizationat the bottom surface.Depth of cure is also influenced by the wavelength of light and the concentration ofthe activator-initiator system. The refractive indices of the resin and filler, as well asthe size, shape, and number of filler particles, are important to the dispersion of thelight beam. The small, highly numerous colloidal-sized particles of microfilledcomposites scatter incident light very efficiently, necessitating a longer exposure timeto obtain adequate polymerization.Chemically activated systems are considered to have an infinite depth of cure.BiocompatibilityHistological studies of the effect of residual monomer molecules on pulp tissue haveshown a moderate degree of cytotoxicity, even in low concentrations. Recent in vivobiocompatibility studies, however, show that resin composites, whether completely orincompletely cured, cause little irritation to the pulp if an adequate marginal seal ispresent. It has been proposed that a significant degree of sensitivity after theplacement of a restoration is a consequence of microbial invasion from the oralenvironment and not of toxicity of the material itself. A second possibility is thatpostoperative sensitivity may be a consequence of debonding between dentin and thecomposite at the cavity floor, causing a pumping action of dentinal fluid duringchewing (percolation), possibly expressing irritants or bacterial toxins into dentinaltubules.
Until the precise mechanisms involved are understood, pulpal protection isrecommended in deep parts of the cavity preparation.ManipulationPlacementEugenol inhibits the polymerization of resin composites. Therefore, liners, bases, andinterim restorations containing eugenol are not recommended. The use of cavityvarnish is not recommended under composite restorations, because monomers presentin the composite may solubilize and disrupt the integrity of the varnish film. Also,varnish will prevent bonding.Following cavity preparation and prior to placement of the composite, a sealingprocedure of some type is indicated. If any dentin bonding agent is to be used, the useof a rubber dam is indicated because moisture in exhaled air may interfere withbonding. The dentin is first conditioned according to the manufacturers directions.Deep preparations may require the placement of a glass-ionomer or resin-modifiedglass-ionomer liner or base over the dentin. Very deep cavities require pulpalprotection in the form of a thin layer of a calcium hydroxide product on the dentinover the pulp.Enamel and dentin are treated strictly according to manufacturers directionsdepending on the bonding agent used. Generally, enamel and dentin are etched for 15seconds using a 35% to 50% phosphoric acid solution or acid gel. High-viscosity geletchants have the advantage of ease of control of the application to enamel walls. Thepreparation is thoroughly washed with water for at least 15 seconds to remove allresidue. The surface is gently air-dried, at which point the enamel should have anopaque, white appearance. Any contamination by saliva after this step requires re-etching to clean the surface thoroughly.A dentin bonding agent is applied to the clean enamel and dentin according to themanufacturers directions. The bonding resin should be air-blown gently to ensure athin film application. Dentin bonding agents work as well on enamel as do enamelbonding agents. While components of bonding systems should not be interchanged,any composite can be used with most bonding agents.A transparent matrix band is sometimes placed for the purpose of contouring therestoration.Two-paste systemTo ensure uniform distribution of filler particles in the matrix, each paste should bestirred periodically with disposable plastic mixing sticks, taking care to avoid cross-contamination that will cause polymerization of the pastes in the jars. Less particlesettling and an increase in shelf life results if the pastes are refrigerated.Equal amounts of the two pastes are dispensed onto a mixing pad with a disposabletwo-bladed plastic spatula. One blade of the spatula should be used to dispense one
paste, and the other blade, the second paste. When needed, the two pastes are mixedthoroughly, requiring 20 to 30 seconds. Care should be taken to avoid theincorporation of air during mixing. Metal spatulas are not recommended for mixing,because filler particles are capable of abrading metal and small amounts of metal maybe incorporated into the composite, resulting in discoloration.Two-paste composites have a working time from the start of mixing of 1 to 1.5minutes and a setting time of 3 to 5 minutes. The mixed material is inserted in one oftwo ways, depending on the viscosity of the particular product. Viscous material isbest placed with plastic instruments that do not adhere to the unset material. A smallamount of bonding resin on the tip of the plastic instrument will prevent sticking. Ifthe viscosity is low enough, the material may be injected into the cavity preparationfrom a syringe. A syringe placement tends to minimize the incorporation of voids intothe restoration.The cavity preparation is slightly overfilled. At 3.5 to 4 minutes after the start ofmixing, the matrix band, if used, is removed. After an additional 2 to 6 minutes, thecomposite surface is sufficiently hard for finishing to begin.Single-paste systemThe shelf life of composites supplied as single pastes and stored in a cool, dryenvironment is about 1 year.The composite is best placed in small layers to minimize polymerization shrinkage.Shrinkage per layer placed is less if the tooth-composite bonding area per layerthickness is large. Each layer should be light cured for at least 40 seconds. Aftercuring, a tacky, air-inhibited layer is present, through which the subsequent layerbonds.Microfilled composites require longer exposure times than do fine-particle compositesbecause their colloidal-sized filler particles scatter blue light more efficiently.FinishingComposites are finished and polished in order to establish a functional occlusalrelationship and a contour that is physiologically in harmony with supporting tissues.In addition, proper contour and high gloss give the restoration the appearance of anatural tooth structure. Early composites had large, hard quartz particles. Polishingpreferentially removed the resin matrix, leaving filler particles exposed and giving thesurface a dull appearance. In addition, quartz has a hardness about 2.5 times that ofenamel and is difficult to polish compared to glasses, which have hardnesscharacteristics similar to that of enamel.Particles smaller than about 0.05 um cannot be detected visually and allow polishingto a high luster. Fine-particle composites have no microfilled particles, are consideredto be only semipolishable, and tend to have a rather opaque appearance. Thecolloidal-sized filler particles of microfilled materials scatter light efficiently, givingthese restorations a pleasing esthetic appearance. Hybrid composites are polishable,but are not as translucent as microfilled composites.
Common prophylaxis pastes are very abrasive to composites and should not be usedfor polishing.The composite surface may be contoured with a plastic matrix strip, but some grossreduction is often required. Finishing begins with coarse abrasives, such as 9- and 12-bladed finishing burs and fine diamonds, and progresses to 16- and 30-bladedfinishing burs, ultrafine diamonds, and medium-grit abrasive points, disks, and strips.Polishing is accomplished with aluminum oxide polishing paste on a rubber cup atlow speed.A postocclusal adjustment cure of 40 seconds further hardens the surface. It isrecommended that this step be followed by re-etching and the application and curingof a low-viscosity unfilled resin. The resin penetrates microcracks on the finishedsurface, further reducing wear.Pitting has been observed on the surface of microfilled-particle-reinforced compositesafter polishing. The pits are thought to occur at the junction of the new resin and theprepolymerized resin/filler, resulting in an increased susceptibility to chipping.A properly placed anterior composite restoration has an expected clinical life of 7 to10 years. Posterior restorations are generally serviceable for less than that. The majorreasons for replacing any composite include deterioration of esthetics, interfacialstaining, wear, microleakage, and secondary caries.Material SelectionIntroductionA variety of materials are available for use as direct esthetic dental restorations: resincomposites, compomers, hybrid ionomers, and glass ionomers. Each has a resincomponent, except the traditional glass ionomer. The unique characteristics of each ofthese materials make them desirable for a range of applications. Choosing the mostsuitable material requires matching a materials desired properties and manipulation toapplication for use. The continuum of resin composite to glass-ionomer estheticrestorative materials is illustrated in Fig 8-11 and their uses are presented in Table 8-4.
Fig 8-11 Continuum of glass-ionomer and composite restorative materials. (After Albers, 1996). Table 8-4 Direct esthetic materials and their uses Restorative material ApplicationFlowable resin composite Restorations following air abrasion Small Class 3 and 5 restorations Liner/base under packable compositeHybrid and microhybrid resin Anterior restorations composite Posterior restorationsMicrofilled resin composite Areas of esthetic concern Anterior restorationsPackable resin composite Class 1 and 2 restorationsPolyacid-modified resin Class 3 and 5 restorations composite (compomer) Cervical erosion or abrasion lesions Class 1 and 2 restorations in pediatric patients Sandwich technique for Class 2 restorationsGlass ionomer High caries-risk patients Cervical erosion or abrasion lesions Class 5 restorations where esthetics is not a concernResin-modified glass ionomer Class 3 and 5 restorations (hybrid ionomer) Cervical erosion or abrasion lesions Class 1 restorations in pediatric patients Sandwich technique or Class 2 restorations Liners, bases, and luting cements Resin composites Composites are the most commonly used direct esthetic restorative material today. They offer excellent esthetics, strength, and wear resistance but have little or no fluoride release. Microfilled composites are used for anterior applications, and hybrid composites are recommended for posterior applications; however, the difference between posterior and anterior composites has become less distinct due to the development of the microhybrid composites.
Composites can also be selected based on their handling characteristics. Packablecomposites have been termed an alternative to amalgam (Fig 8-12).Fig 8-12 A packable composite material. An interlocking particle network allows thepackable handling properties.They differ from anterior and posterior composites in that they have higher fillerloading (greater than 80% by weight and 66% to 70% by volume) with either fibers,porous filler particles, irregular filler particles, or viscosity modifiers. They arerecommended for use in Class 1 and 2 cavity preparations. Because of the high depthof cure and lower polymerization shrinkage of packable composites, a bulk-filltechnique may be possible. A low-viscosity (flowable) material (Fig 8-13) can beused as a liner to fill irregular internal surfaces and proximal boxes before placing thepackable composite. Flowable composites or compomers will wet and adapt to thetooth surface, sealing it and possibly reducing postoperative sensitivity.Fig 8-13 A flowable composite with a filler load of about 60% by weight and averageparticle size of 0.6 um.
CompomersCompomers, or polyacid-modified composites (Fig 8-14), contain monomersmodified by polyacid groups with fluoride-releasing silicate glasses. The propertiesand clinical characteristics of compomers are directly related to their composition ofcomposite and glass ionomer. Compomers release fluoride by a mechanism similar toglass and hybrid ionomers, but the amount of release and its duration are lower.Additionally, compomers do not recharge from fluoride treatments or brushing withfluoride dentifrices as much as do glass and hybrid ionomers. Like composites,compomers require a bonding agent to bond to tooth structure. Single-bottle bondingagents that contain acidic primers have been used with some compomers. Acidicprimers will bond to both enamel and dentin without the need for phosphoric acidetching. However, studies have shown the bond strength of compomers to teeth isimproved with additional etching with phosphoric acid. Compomers set by light-activated polymerization and by an acid-base reaction with water absorbed from thetooth. They are packaged as single-paste formulations in compules and syringes.Compomers are recommended for cervical lesions, Class 3 and 5 restorations inadults, primary teeth, Class 1 and 2 restorations in children, sandwich technique forClass 2 restorations, and with medium-caries-risk patients.Fig 8-14 A compomer with fluoride-silicate glass, colloidal silica, dimethacrylateresin, and hydrophilic polymer.Resin-modified glass ionomersResin-modified glass ionomers, or hybrid ionomers, contain fluoride-releasing glassand polyacid monomers. They set by an acid-base reaction and both chemical andlight-cured free-radical reactions. They are recommended for cervical lesions, Class 3and 5 restorations in adults, primary teeth, Class 1 restorations in children, sandwichtechnique for Class 2 restorations, and with high-caries-risk patients. Because of theresin content, these restorations are more esthetic and stronger than glass ionomers.
Hybrid ionomers are packaged in powder-liquid form or are pre-encapsulated to bemixed in an amalgamator. The use of a bonding agent prior to placement is notrecommended because it decreases fluoride release. Hybrid ionomers naturally bondto tooth structure once the tooth is conditioned with polyacrylic acid or a primer. Seealso chapter 9 for the use of hybrid ionomers as cements. A comparison of theproperties of several of these materials is given in Table 8-5. Table 8-5 Mechanical properties of glass ionomer and resin compositecombinations*Materials class Flexural Flexural Compressive Diametral Shear Shrinkage strength modulus strength tensile bond (% vol) (MPa) (GPa) (MPa) strength strength (MPa) (MPa)Conventional 25 8 180-200 22-25 3-5 3glass ionomerResin- 35-70 4 170-200 35-40 8-14 3.5modified glassionomerCompomer 97 6-8 210-245 45-47 14 4.5Fluoride- 85 8 40 24 3releasing resincompositeFlowable resin 111-167 4-8 20-22 5compositeResin 140 18 350 65-75 24-28 3composite*From Burgess et al (1996). Used with permission from The Compendium ofContinuing Education in Dentistry.Pit and Fissure SealantsThese sealants are mainly fluid resins that are applied to posterior occlusal surfaces ofcaries-prone teeth to seal pits and fissures from bacterial action. The principalmonomer used is bis-GMA, which may be lightly filled with ceramic filler particles toimprove wear resistance. Prior to application of the fluid monomer, the tooth enamelis etched with phosphoric acid. Upon application of the fluid resin, it penetrates intothe pits and fissures by capillary action. There also is penetration into themicrostructure of the etched enamel to form "tags" that lead to micromechanicalaction. Deep penetration is promoted by a high penetration coefficient (PC) whichresults from low viscosity, high surface tension, and low contact angle, that is, goodwetting (chapter 5). Figure 8-15 shows the penetration of a sealant into a fissure.
Fig 8-15 The penetration of a sealant into a fissure. (a) Depth of sealant penetration;(b) total depth.Sealants have been found to be effective in several studies. Long-term studies haveshown around 50% decay reductions in sealed teeth compared with controls. About90% of sealants are at least partially present in 5-year studies. Also, partial loss orwear of a sealant does not prevent its preventive action in deep fissures. Onedisadvantage to using sealants is that they may trap food debris and bacteria that couldlead to continued caries action. Studies have shown that although some food debris isusually trapped under sealants, the bacteria become dormant if they are isolated.Fluoride-containing sealants are also available.Clinical Decision Scenarios for Restorative MaterialsThis section presents a formal approach to choosing restorative materials for specificsituations. Each scenario uses the same format as that presented in chapter 7.Advantages and Disadvantages of each material are prioritized using the followingcodes: * = of minor importance, ** = important, *** = very important.Situation Light-cured vs chemically cured composite materials for anterior Class 3restorationsDescription A patient has a small proximal caries lesion on the mesial surface of amaxillary permanent central incisor. He desires an esthetic restoration. The dentist hasboth visible light-cured composite material and chemically cured material in hisarmamentarium.Critical Factor EstheticsLight cureAdvantages*** Good esthetics** Better color stability
Less porosity More working timeDisadvantages Less complete cure Curing light neededChemical cureAdvantages*** Good esthetics * More complete cure Curing light not neededDisadvantages More porosity** Poorer color stability Less working timeAnalysis/Decision Although either material would be satisfactory, the greater colorstability provides the determining factor in this instance and leads to selection of thelight-cured material. The greater working time of light-cured material is convenientbut not necessary to a dentist experienced in the use of the chemically cured material.The higher porosity of the chemically cured materialinduced by the need to mix thepaste and catalystas well as the activators and accelerators needed in the chemicalcure, probably contribute to the lower color stability.Situation Resin composite vs amalgam for coresDescription A patient comes to the office complaining of a broken tooth. Uponexamination, the dentist finds that the lingual cusps of the mandibular right permanentfirst molar have fractured at the gingival line. The tooth already has a large mesio-occlusodistal (MOD) amalgam in it, and the facial cusps are not sturdy. The patient isleaving for a winter vacation to Florida in 10 days and hopes to have the toothrepaired before then. The treatment plan is to prepare a pin-retained core buildup andthen a full gold crown. The dentist has both amalgam and a composite core materialavailable.
Critical Factor TimeAmalgamAdvantages Greater strength Long clinical historyDisadvantages*** 24-hour set No bond to toothResin compositeAdvantages*** Immediate set Bonds to tooth Can be prepared immediatelyDisadvantages Lesser strengthAnalysis/Decision Although this may seem like an abbreviated list, these areessentially the main considerations. While the strength of the amalgam is thought tobe greater in these applications, composites have served well if properly done. Thedeciding factor is often that the composite can be placed and prepared for the crownimmediately, whereas it is recommended that the amalgam be allowed to set 24 hoursbefore preparation. Thus, the composite may be placed and the tooth prepared in oneappointment. If amalgam had been the material of choice, a second appointmentwould have been necessary for the crown preparation. This was the deciding factorthat made the dentist choose the composite in this instance.Materials Microfilled resin composite vs hybrid composite for direct veneerDescription A recent college graduate requests an improvement in the appearance ofher maxillary lateral incisors, which are slightly crowded, and she wants it donebefore a job interview in 2 weeks. She is advised that orthodontic treatment would bea more permanent solution, but it would take 1 or 2 years. Due to urgency, the dentistagrees to place direct veneers using either a microfilled or hybrid composite material.
Critical Factors Appearance, strong bond to enamel, strengthHybrid compositeAdvantages Ease of placement * Stronger than microfilled composite** More wear resistance Lower expansion and contraction*** Strong bond to enamelDisadvantages*** Less natural appearance * Less smooth finishMicrofilled compositeAdvantages Ease of placement*** More natural appearance * Smoother finish*** Strong bond to enamelDisadvantages** Less wear resistance * Weaker than hybrid Higher expansion and contractionAnalysis/Decision Given that the microfilled composite material has a smoother andmore natural appearance, the dentist chose to use this material. No tooth removal wasnecessary. The lateral incisors were isolated, cleaned with pumice, and enamel etched,then natural-looking restorations were created. The patient was delighted with theresults. The dentist explained to the patient that these restorations may need to beresurfaced/polished on a regular basis and replaced every 4 or 5 years due to wear.
Glossaryacid etch Selective etching of portions of the enamel rods with phosphoric acid,resulting in both high surface area and increased surface energy. Resin is able to flowinto the enamel substructure and upon polymerization provides a mechanical bond tothe enamel.compomer (polyacid-modified resin composites) A blend of resin composite andglass ionomer; requires a bonding agent to bond to tooth.coupling agent A chemical attached to the filler surface for the purpose of creating abond with the resin matrix upon polymerization. The presence of a coupling agentimproves several properties of the composite, including strength and wear resistance.cross-linked polymer A polymer with a three-dimensional network structure.dentin bonding agent Low-viscosity resin used for adhesion to enamel and/or dentin.dimethacrylate A methacrylate monomer with reactive, or polymerizable, groups ateach end.fine-particle resin composites Composites containing fine-sized filler particles (0.5to 3.0 um). Less polishable than microfilled composites.hybrid ionomer A resin-modified glass ionomer that sets by an acid-base reactionand resin polymerization. The powder is similar to glass ionomer and the liquidcontains monomers, polyacids, and water.hybrid (blend) resin composites Composites containing colloidal silica (0.01 to 0.12um) in addition to fine-sized particles.microfilled resin composites Composites containing colloidal silica as filler. Mostpolishable and translucent of the resin composites.microhybrid resin composite Composites containing filler particles in the range of0.4 to 1.0 um; a blend of hybrid and microfilled composites.monomer A single molecule with double or triple bonds that are capable of unitingthe monomers into oligomers or polymers.oligomer A short polymer made up of two to four monomer units.packable composites A composite with a higher filler content than traditional resincomposites with either fibers, porous filler particles, irregular filler particles, orviscosity modifiers.polymer A macromolecule formed by the linkage of monomers or oligomers.polymerization The process by which a polymer is formed from monomers or
oligomers.resin composite A physical mixture of silicate glass particles (filler) with an acrylicmonomer (matrix phase) that is polymerized during application. A material havingtwo or more distinct components and with properties different from those of theindividual components.Discussion Questions1. Why are these materials called "polymeric restorative materials" when they usuallycontain mostly ceramic phases?2. How have composites overcome many of the problems of unfilled resin restorativematerials?3. How well are composite materials competing against dental amalgam?4. Although microfilled composite materials have inferior mechanical properties, theycontinue to be widely used. Why?Study Questions(See Appendix E for answers.)1. What is the general composition of resin composite restorative materials?2. What are the applications for resin composite restorative materials?3. How long do composite restorations last?4. What are the advantages of fine-particle composites?5. What are the advantages of microfilled composites?6. What is a hybrid, or blend, composite?7. What is polymerization shrinkage, and why is it a problem?8. Which restorative materials release fluoride? List them in order of amount released.9. What is the material of choice for cervical restorations?Recommended ReadingAbdulrahman A-D, Wennberg A (1993). Biocompatibility of dentin bonding agents.Endod Dent Traumatol 9:1-7.Albers HF (1996). Tooth-Colored Restoratives, ed 8. Santa Rosa: Alto Books.Armstrong SR, Seol J, Boyer DB (1999). Fracture toughness of direct tooth-colored
restorative materials [abstract 811]. J Dent Res 78:207.Asmussen E (1982). Factors affecting the quantity of remaining double bonds inrestorative resin polymers. Scand J Dent Res 90:490-496.Attin T, Vataschki M, Hellwig E (1996). Properties of resin-modified glass-ionomerrestorative materials and two polyacid-modified resin composite materials.Quintessence Int 27:203-209.Barkmeier WW, Blake SM, Wilwerding TM, Latta MA (1999). In-vitro wearassessment of compomer restoratives [abstract 1652]. J Dent Res 78:312.Bayne SC, Thompson JY, Swift EJ Jr, Stamatiades P, Wilkerson M (1998). Acharacterization of first-generation flowable composites. J Am Dent Assoc 129:567-577.Burgess JO, et al (1996). Directly placed esthetic restorative materials. CompendContin Educ Dent 17:8,731-748.Christensen GJ (1998). Condensable restorative resins. Clin Res AssociatesNewsletter 22(7):1.Christensen GJ (1999). Sorting out the confusing array of resin-based composites indentistry. J Am Dent Assoc 130:275-277.Craig RG (1993). Restorative Dental Materials, ed 9. St Louis: Mosby.Czerner A, Weller M, Lohbauer U, Ebert J, Frankenberger J (2000). Wear resistanceof flowable composites as pit and fissure sealants [abstract 1087]. J Dent Res 79:279.Dhuru V, Benhamuerlaine M (2000). Water sorption of selected tooth color materials[abstract 1100]. J Dent Res 79:281.Eick JD, Robinson SJ, Byerley TJ, Chappelow CC (1993). Adhesives andnonshrinking dental resins of the future. Quintessence Int 24:632-640.Eliades G, Palaghias G, Vougiouklakis G (1990). Surface reactions of adhesives ondentin. Dent Mater 6:208-216.El-Kalla IH, Garcia-Godoy F (1999). Mechanical properties of compomer restorativematerials. Oper Dent 24:2-8.Farah JW, Powers JM (1991). Anterior and posterior composites. Dental Advisor8(4):1-8.Farah JW, Powers JM (1999). Fluoride-releasing restorative materials. Dental Advisor15:1.Fortin D, Vargas MA (2000). The spectrum of composites: new techniques andmaterials. J Am Dent Assoc 131(suppl):26S-30S.
Iazetti G, Burgess JO, Tavares C (1999). Mechanical properties of fluoride-releasingmaterials [abstract 417]. J Dent Res 78:158.Kelsey WP, Latta MA, Barkmeier WW (1999). Physical properties of high density,composite restorative materials [abstract 810]. J Dent Res 78:207.Kerby R, Berlin J, Knobloch L (1999). Fracture toughness of posterior condensablecomposites [abstract 415]. J Dent Res 78:157.Kerby R, Lee J, Knobloch L, Seghi R (1999). Hardness and degree of conversion ofposterior condensable composite resin [abstract 414]. J Dent Res 78:157.Latta MA, Randall CJ (1999). Physical properties of compomer restorative materials[abstract 412]. J Dent Res 78:157.Lohbauer U, Schoch M, Frankenburger R, Braem MJA, Kramer N (1999). Flexuralstrength characterization of resin composites by Weibull analysis [abstract 805]. JDent Res 78:206.MacGregor KM, Cobb DS, Denehy GE (2000). Physical properties of new packablecomposites vs. a conventional hybrid [abstract 1777]. J Dent Res 79:366.MacGregor KM, Cobb DS, Vargas MA (1999). Physical properties of condensableversus conventional composites [abstract 411]. J Dent Res 78:157.Manhart J, Chen HY, Draegert U, Kunzelmann KH, Hickel R (2000). Vickershardness and depth of cure of light-cured packable composite resins [abstract 1807]. JDent Res 79:369.McKinney JE, Wu W (1985). Chemical softening and wear of dental composites. JDent Res 64:1326-1331.Minato D, Ruse ND, Feduik D (1999). Fracture toughness of a hybrid, a microfill, anda compomer using NTP test [abstract 2343]. J Dent Res 78:398.Musa A, Pearson GJ, Gelbier M (1996). In vitro investigation of fluoride ion releasefrom four resin-modified glass polyalkenoate cements. Biomaterials 17:1019-1023.Nguyen D, Angeletakis C, Shellard E (2000). A new high polish retentionmicrohybrid composite [abstract 1081]. J Dent Res 79:279.OBrien WJ, Yee JJ (1980). Microstructure of posterior restorations of compositeresins after clinical wear. Oper Dent 5(3):90-94.Pearson GJ, Longman CM (1989). Water sorption and solubility of resin-basedmaterials following inadequate polymerization by a visible-light curing system. J OralRehabil 16:57-61.Powers JM, Fan PL, Raptis CN (1980). Color stability of new composite restorative
materials under accelerated aging. J Dent Res 59:2071-2074.Product Information Sheet. Compoglass F physical proprties. Ivoclar North America.Roeder LB, Tate WH, Powers JM (1999). Surface roughness of polished condensablecomposites [abstract 3024]. J Dent Res 78:483.Ruddle DE, Thompson JY, Stamatiades PJ, et al (1999). Mechanical properties andwear behavior of condensable composites [abstract 407]. J Dent Res 78:156.Ruse ND (1999). What is a compomer? J Can Dent Assoc 65: 500-504.Ruyter IE, Oysaed H (1987). Composites for use in posterior teeth: composition andconversion. J Biomed Mater Res 21:11-23.Transactions of the Academy of Dental Materials (1998). Proceedings of Conferenceon Critical Reviews of Restorative Quandaries, vol 12.Van Meerbeek B, Braem M, Lambrechts P, Vanherle G (1993). Two-year clinicalevaluation of two dentine-adhesive systems in cervical lesions. J Dent 21(4):195-202.Van Meerbeek B, Lambrechts P, Inokoshi S, Braem M, Vanherle G (1992). Factorsaffecting adhesion to mineralized tissues. Oper Dent 5 (Suppl):111-124.Wendt SL Jr, Leinfelder KF (1992). Clinical evaluation of a heat-treated resincomposite inlay: 3-year results. Am J Dent 5:258-262.Willems G, Lambrechts P, Braem M, Vanherle G (1993). Composite resins in the 21stcentury. Quintessence Int 24:641-658.Willems G, Lambrechts P, Braem M, Vanherle G (1993). Three-year follow-up offive posterior composites; in vivo wear. J Dent 21:74-78.Winkler MM, Xu X, Burgess JO (2000). In vitro contact wear of 8 posterior resincomposites [abstract 1082]. J Dent Res 79:279.Zidan O, Gomez-Marin O, Tsuchiya T (1987). A comparative study of the effects ofdentinal bonding agents and application techniques on marginal gaps in Class Vcavities. J Dent Res 66:716-721.
Chapter 9. Dental CementsIntroductionAlthough dental cements are used only in small quantities, they are perhaps the mostimportant materials in clinical dentistry because of their application as (1) lutingagents to bond preformed restorations and orthodontic attachments in or on the tooth,(2) cavity liners and bases to protect the pulp and foundations and anchors forrestorations, and (3) restorative materials. This multiplicity of applications requiresmore than one type of cement because no one material has yet been developed thatcan fulfill the varying requirements.Over the last two decades, the emphasis has been on materials for luting in view ofthe increased use of fixed partial dentures. More recently, with the advent of glass-ionomer cements, interest in restorative applications has revived also. These differentapplications require different physical properties and appropriate clinical manipulativecharacteristics, and so, in response to the changing situation, new internationalstandards are being developed (International Standards Organization [ISO]), as arevarious national standards (American National Standards Institute/American DentalAssociation [ANSI/ ADA]) based on performance criteria rather than specificcomposition.For acceptable performance in luting and restorative applications, the cement musthave adequate resistance to dissolution in the oral environment. It must also developan adequately strong bond through mechanical interlocking and adhesion. Highstrength in tension, shear, and compression is required, as is good fracture toughnessto resist stresses at the restoration-tooth interface. Good manipulation properties, suchas adequate working and setting times, are essential for successful use. Themanipulation, including dispensation of the ingredients, should allow for some marginof error in practice. The material must be biologically acceptable.Most cements are powder-liquid materials that may be dispensed and mixed manuallyor predispensed in capsules that are mixed mechanically. Some recent materials arecomposed of two pastes. Cements set by chemical reaction between the ingredients(often an acid-base reaction) or involve polymerization of a monomeric component.In the early 20th century zinc oxide-phosphoric acid, zinc oxide-eugenol (clove oil85%), and silicate glass-phosphoric acid cements were discovered. These zincphosphate, zinc eugenate, and silicate cements were widely used until the 1970s,when new cements began to be developed.The introduction of new types of cements was prompted by the emphasis on improvedbiocompatibility and bonding to the tooth that began to develop 20 years ago. Newinformation on pulpal histopathology resulting from particular clinical techniques andmaterials, as well as the demonstration of marginal leakage involving penetration ofbacteria to the dentin interface and a reduction in retention of restorations, led to therealization that new materials possessing good wetting and bonding to enamel anddentin and low toxicity were needed.These concepts were the basis of the development of cements based on polyacrylic
acid: first the zinc polyacrylate (polycarboxylate) cements, then the glass-ionomercements, and more recently the resin cements and hybrid ionomer cements. The newercements have gradually become established as alternatives to zinc phosphate cementbecause of their minimal effects on pulp, similar strength and solubilitycharacteristics, and adhesive properties.The advent of the acrylic resins led to the development of poly(methyl methacrylate)in the mid-1950s. These materials had limitations such as lack of adhesion, leakage,and toxicity that terminated their use for routine cementation. In the last 15 years,polymerizable bis-GMA and other dimethacrylate monomer cements have becomeavailable in various forms for attachment of cast restorations and orthodontic bracketsto enamel. More recently, similar systems containing (potentially) adhesivemonomers have been marketed for fixed partial denture cementation.The cements based on the reaction between calcium hydroxide and a liquid salicylatealso originated 25 years ago. They were primarily fluid, two-paste materials intendedfor the lining of deep cavities that had actual or potential exposure, thus providing anantibacterial sealing action to facilitate the formation of reparative dentin. Thesusceptibility to acid erosion of the original formulations, both through marginalleakage of restorations and exposure to phosphoric acid during acid-etch techniques,has resulted in more resistant compositions and, quite recently, to a light-cured, resin-based material.As a result of the research of the last 15 years, cements of five basic types areavailable, classified according to the matrix-forming species, as shown in Fig 9-1 andTable 9-1:1. Phosphate bonded2. Phenolate bonded3. Polycarboxylate bonded4. Dimethylacrylate bonded5. Polycarboxylate and dimethylacrylate combinations
Fig 9-1 Classification of dental cements according to bonding mechanism. Table 9-1 Classification of dental cements Type (matrix bond) Class of cement FormulationsPhosphate Zinc phosphate Zinc phosphate Zinc phosphate fluoride Zinc phosphate copper oxide/salts Zinc phosphate silver salts Zinc silicophosphate Zinc silicophosphate Zinc silicophosphate mercury saltsPhenolate Zinc oxide-eugenol Zinc oxide-eugenol Zinc oxide-eugenol polymer Zinc oxide-eugenol EBA/alumina Calcium hydroxide Calcium hydroxide salicylate salicylatePolycarboxylate Zinc polycarboxylate Zinc polycarboxylate Zinc polycarboxylate fluoride Glass ionomer Calcium aluminum polyalkenoate Calcium aluminum polyalkenoate- polymethacrylateResin Acrylic Poly(methyl methacrylate) Dimethacrylate Dimethacrylate unfilled Dimethacrylate filled Adhesive 4-METAResin-modified glass Hybrid ionomers Self cured Light cured ionomers Numerous brands of each type are available, and there is some overlap between properties. Since clinical and in vivo evaluation of cements is still very limited, the predictive value of laboratory data for assessment of clinical performance requires knowledgeable interpretation, especially because generalizations on specific types of
cement cannot be made on the basis of the behavior of one or two brands. The applications of the different types of cements are given in Table 9-2. Examples of current widely used brands of permanent luting cements are given in Table 9-3. Typical properties of luting cements are given in Table 9-4. Table 9-2 Selection of dental cements Application Cement typeLuting inlays, crown posts, multiretainers, fixed Glass-ionomer cement, hybrid partial denture in or on: ionomers, resinNonvital teeth or teeth with advanced pulpal Zinc phosphate recession and average retentionVital teeth with average retention, average pulpalZinc polycarboxylate recession, thin dentin, especially for single units and small-span fixed partial denturesMultiretainer splints on vital teeth with above- Zinc oxide-eugenol polymer average retention, minimal dentin thickness; hypersensitive patientsProvisional cementation Zinc oxide-eugenol polymer Zinc polycarboxylate (thin mix)Provisional cementation and stabilization of old, Dimethacrylate resin composite loose restorations; fixation of facings and acid- etched cast restorationsBase/liner in:Cavity with remaining dentin greater than about Glass-ionomer cement, resin ionomer 0.5 mm Zinc polycarboxylate Zinc phosphate (low-acid type)Cavity with minimal dentin or exposure Calcium hydroxide salicylate Zinc oxide-eugenol polymer Table 9-3 "Permanent" luting cements Product Type Manufacturer Fuji Plus Hybrid ionomer GC America Vitremer Luting Hybrid ionomer 3M/Espe Flecks Extraordinary Zinc phosphate Mizzy Fuji I Glass ionomer GC America Fynal Zinc oxide-eugenol L.D. Caulk Hy-Bond Polycarboxylate Zinc carboxylate Shofu Dental Cement Hy-Bond Zinc Phosphate Cement Zinc phosphate Shofu Dental Ketac-Cem Glass ionomer 3M/Espe Advance Hybrid ionomer L.D. Caulk Modern Tenacin Zinc phosphate L.D. Caulk Super EBA Zinc oxide-eugenol Bosworth Tylok Plus Zinc carboxylate L.D. Caulk Zinc Cement Improved Zinc phosphate Mission White Dental
Phosphate-Based CementsZinc phosphate cementApplicationsBecause of their long history, these materials have the widest range of applications,from the cementation (luting) of fixed cast alloy and porcelain restorations andorthodontic bands (Table 9-3) to their use as a cavity liner or base to protect pulp frommechanical, thermal, or electrical stimuli.Composition and settingThe powder is mainly zinc oxide with up to 10% magnesium oxide and small amountsof pigments. It is fired at high temperature ( 1,000C) for several hours to reduce itsreactivity. The liquid is an aqueous solution of phosphoric acid containing 45% to64% H3PO4 and 30% to 55% water. The liquid also contains 2% to 3% aluminum and0% to 9% zinc. Aluminum is essential to the cement-forming reaction, whereas zinc isa moderator of the reaction between powder and liquid, allowing adequate workingtime and permitting a sufficient quantity of powder to be added for optimumproperties in the cement.Some zinc phosphate cements have modified compositions. One material, widely usedas a cavity liner, has 8% aluminum and only 25% H3PO4 in the liquid and a powderthat contains calcium hydroxide. Others may contain fluoride and have as much as10% stannous fluoride.The amorphous zinc phosphate formed binds together the unreacted zinc oxide andother components of the cement. The set cement consists of a cored structure ofresidual zinc oxide particles in a phosphate matrix:ManipulationThe measurement of components and the timing of mixing are essential to consistentsuccess. The mixing slab must be thoroughly dried before use. The powder is added tothe liquid in small portions to achieve the desired consistency. Dissipation of the heatof reaction by mixing over a large area on a cooled slab will allow a greaterincorporation of powder in a given amount of liquid. The cement must be undisturbeduntil the end of the setting time. The cement liquid is kept sealed with a stopper toprevent changes in the water content. Cloudy liquid should be discarded. Increasingthe powder/liquid ratio gives a more viscous mix, shorter setting time, higher strength,lower solubility, and less free acidity. Use of a chilled (5C) thick glass slab slows theinitial reaction and allows incorporation of more powder, giving superior properties inthe set cement.Properties
The long persistence of zinc phosphates in clinical practice indicates that reasonableperformance is obtained. Although the properties are far from ideal, they are usuallyregarded as a standard against which to compare newer cements (see Table 9-4). Theprincipal reasons for their satisfactory performance under routine conditions are thatthey can be easily manipulated and that they set sharply to a relatively strong massfrom a fluid consistency. Table 9-4 Properties of dental luting cements Strength (MPa)Material Film Setting Solubility Compressive Tensile Modulus thickness time (wt%) of (mm) (min) elasticity (GPa)Zinc phosphate 25-35 5-14 0.2 max 80-100 5-7 13Zinc oxide-eugenol Unmodified 25-35 2-10 1.5 2-25 1-2 Polymer 35-45 7-9 1 35-55 5-8 2-3reinforced EBA-alumina 40-60 7-13 1 55-70 3-6 3-6Zinc 20-25 6-9 0.06 55-85 8-12 5-6polycarboxylateGlass ionomer 25-35 6-9 1 90-140 6-7 7-8Polymer based 20-60 3-7 0.05 70-200 25-40 4-6For a given brand of material, the properties are a function of the powder/liquid ratio.For a given cementing consistency, the higher the powder/liquid ratio, the better thestrength properties and the lower the solubility and free acidity.At room temperature (21C to 23C) the working time for most brands at lutingconsistency is 3 to 6 minutes; the setting time is 5 to 14 minutes. Extended workingtimes and shorter setting times can be achieved by use of a cold mixing slab, whichpermits up to an approximate 50% increase in the amount of powder, improving bothstrength and resistance to dissolution.The cement must have the ability to wet the tooth and restoration, flow into theirregularities on the surfaces it is joining, and fill in and seal the gaps between therestoration and the tooth. The minimum value of film thickness is a function ofpowder particle size, powder/liquid ratio, and mix viscosity. As measured by ISO andANSI/ADA specifications, acceptable cements give film thicknesses of less than 25um. In practice, the cement fills in the inaccuracies between the restoration and thetooth and allows most castings to seat satisfactorily. Unless escapeways or vents areprovided with full crowns, separation of powder and liquid may occur, with marginaldefects in the cement film.At the recommended powder/liquid ratio (2.5 to 3.5 g/mL), the compressive strengthof the set zinc phosphate cement is 80 to 110 MPa (11,000 to 16,000 psi) after 24
hours. The minimum strength for adequate retention of restorations is about 60 MPa(8,500 psi). The strength is strongly and almost linearly dependent on powder/liquidratio. The tensile strength is much lower than the compressive strength, 5 to 7 MPa(700 to 900 psi), and the cement shows brittle characteristics. The modulus ofelasticity (stiffness) is about 13 GPa (1.8 106 psi).According to the standard method, the solubility and disintegration in distilled waterafter 23 hours may range from 0.04% to 3.3% for inferior material. The standard limitis 0.2%. The fluoride-containing cements give a figure of about 0.7% to 1.0% becauseof the leaching of fluoride. The solubility in organic acid solutions, such as lactic orcitric acid, is 20 to 30 times higher. These data are only a rough guide to solubilityunder oral conditions. The comparative evaluation of cement solubility under clinicalconditions has shown significant loss but conflicting results. Dissolution contributesto marginal leakage around restorations and bacterial penetration. This may befacilitated by dimensional change. The cement has been found to contract about 0.5%linearly, giving rise to slits at the tooth-cement and cement-restoration interfaces.Biologic effectsThe freshly mixed zinc phosphate is highly acidic with a pH of between 1 and 2 aftermixing. Even after setting 1 hour, the pH may still be below 4. After 24 hours, the pHis usually 6 to 7. Pain on cementation is due not only to the free acidity of the mix butalso to osmotic movement of fluid through the dentinal tubules. Hydraulic pressuredeveloped during seating of the restoration may also contribute to pulpal damage.Prolonged pulpal irritation, especially in deep cavities that necessitate some form ofpulpal protection, may be associated with the extended duration of the set materialslow pH. This is minimized by a high powder/liquid ratio and rapid setting. Onematerial that has a low acid content and incorporates calcium hydroxide has littleeffect on pulp when used as a liner. Very thin mixes will also lead to etching of theenamel.Advantages and DisadvantagesThe main advantages of zinc phosphate cements are that they can be mixed easily andthat they set sharply to a relatively strong mass from a fluid consistency. Unless themix is extremely thin (for instance, with a very low powder/liquid ratio), the setcement has a strength that is adequate for clinical service, so manipulation is lesscritical than with other cements.However, zinc phosphates distinct Disadvantages include pulpal irritation, lack ofantibacterial action, brittleness, lack of adhesion, and solubility in oral fluids.Modified zinc phosphate cementsCopper and silver cementsBlack copper cements contain cupric oxide (CuO); red copper cements containcuprous oxide (Cu2O). Others may contain cuprous iodide or silicate. Since a muchlower powder/liquid ratio is necessary to obtain satisfactory manipulationcharacteristics with these cements, the mix is highly acidic, resulting in much greater
pulpal irritation. Their solubility is higher and their strength is lower than zincphosphate cements. Their bacteriostatic or anticariogenic properties seem to be slight.Silver cements generally contain a small percentage of a salt such as silver phosphate.Their advantages over zinc phosphate cement have not been substantiated.Fluoride cementsStannous fluoride (1% to 3%) is present in some orthodontic cements. These materialshave a higher solubility and lower strength than zinc phosphate cement due todissolution of the fluoride-containing material. Fluoride uptake by enamel from suchcements results in reduced enamel solubility and potentially anticariogenic effects.Silicophosphate cementsThese materials have been available for many years as a combination of zincphosphate and silicate cements. The presence of the silicate glass provides a degree oftranslucency, improved strength, and fluoride release.ApplicationsTheir principal applications have been for the cementation of fixed restorations andorthodontic bands (Type I), as a provisional posterior restorative material (Type II),and as a dual-purpose material (Type III).Composition and settingThe powder in these materials consists of a blend of 10% to 20% zinc oxide (zincphosphate cement powder) and silicate glass (silicate cement powder) mechanicallymixed or fused and reground. The silicate glass usually contains 12% to 25% fluoride.Some materials have been labeled "germicidal" because of the presence of smallamounts of mercury or silver compounds. The liquid is a concentratedorthophosphoric acid solution containing about 45% water and 2% to 5% aluminumand zinc salts.The setting reaction has not been fully investigated, but may be represented asfollows:The set cement consists of unreacted glass and zinc oxide particles bonded togetherby the aluminosilico-phosphate gel matrix.ManipulationThe mixing is analogous to that for a phosphate cement; a nonabradable spatula and acooled mixing slab should be used. The filling mix should be glossy, with puttylikeconsistency.Properties
At cementing consistency, the setting time is 5 to 7 minutes; working time is about 4minutes and may be increased by using a cold mixing slab.These cements generally have shorter working times and a coarser grain size, leadingto a higher film thickness than with zinc phosphate cements. One material is improvedin these respects, and film thickness is adequate for cementation of cast gold andporcelain restorations.The compressive strength of the set cement is in the range from 140 to 170 MPa(20,000 to 25,000 psi); the tensile strength is considerably lower at 7 MPa (1,000 psi)(see Table 9-4). The toughness and abrasion resistance are higher than those ofphosphate cements.The solubility in distilled water after 7 days is about 1% by weight. Solubility inorganic acids and in the mouth is less than for phosphate cements. Fluoride is leachedout and may contribute to anticariogenic action. The durability in bonding orthodonticbands to teeth is greater, and less decalcification is observed.The glass content gives considerably greater translucency than phosphate cements,making silicophosphate cements useful for cementation of porcelain restorations.Biologic effectsBecause of the acidity of the mix and the prolonged low pH (4 to 5) after setting,pulpal protection is necessary on all vital teeth. Fluoride and other ions are leachedout from the set cement by oral fluids, resulting in increased enamel fluoride andprobable anticariogenic action.Advantages and DisadvantagesSilicophosphate cements have better strength, toughness, and abrasion resistanceproperties than zinc phosphate cements, and show considerable fluoride release,translucency, and, under clinical conditions, lower solubility and better bonding.Disadvantages include an initial pH and total acidity that are greater than those forzinc phosphate cements. Pulpal sensitivity may be of longer duration, and pulpalprotection is essential. Manipulation is more critical than with zinc phosphatecements.Phenolate-Based CementsIntroductionThere are three main types of cement under this classification:1. The simple zinc oxide-eugenol combination that may contain setting accelerators
2. The reinforced zinc oxide-eugenol materials3. The ortho-ethoxybenzoic acid (EBA) cementsCements have also been formulated using other phenolic liquids, but these have seenlittle use except for those containing calcium hydroxide and a salicylate.Zinc oxide-eugenol cementsApplicationsThe basic combination of zinc oxide and eugenol finds its principal applications in theprovisional cementation of crowns and fixed partial dentures, in the provisionalrestoration of teeth, and as a cavity liner in deep cavity preparations.Composition and settingThe powder is essentially pure zinc oxide (United States Pharmacopeia [USP] orequivalent, arsenic free). Commercial materials may contain small amounts of fillers,such as silica. About 1% of zinc salts, such as acetate or sulfate, may be present toaccelerate the setting. The liquid is purified eugenol or, in some commercialmaterials, oil of cloves (85% eugenol). One percent or less of alcohol or acetic acidmay be present to accelerate setting together with small amounts of water, which isessential to the setting reaction.A chemical reaction occurs between zinc oxide and eugenol, with the formation ofzinc eugenolate (eugenate):The precise mechanism is not fully understood, but the set mass contains residual zincoxide particles bonded by a matrix of zinc eugenolate and some free eugenol. Water isessential to the reaction, which is accelerated also by zinc ions. The reaction isreversible because the zinc eugenolate is easily hydrolyzed by moisture to eugenoland zinc hydroxide. Thus, the cement disintegrates rapidly when exposed to oralconditions. The rate of reaction between the zinc oxide and the eugenol is dependenton the nature, source, reactivity, and moisture content of the zinc oxide and on thepurity and moisture content of the eugenol.ManipulationThe zinc oxide is slowly wetted by the eugenol; therefore, prolonged and vigorousspatulation is required, especially for a thick mix. A powder/liquid ratio of 3:1 or 4:1must be used for maximum strength.PropertiesThe working time is long because moisture is required for setting. Variable results areobtained with different samples of zinc oxide, depending on their mode of preparation
and reactivity. For a given oxide, set time is controlled by moisture availability,accelerators, and the powder/liquid ratio. Mixes of cementing consistency set veryslowly unless accelerators are used and/or a drop of water is added. Commercialmaterials set in the range of 2 to 10 minutes, resulting in adequate strengths at 10minutes for amalgam restorations to be placed (see Table 9-4).The particle size of the zinc oxide and the viscosity of the mix govern the filmthickness. Use of a fluid mix gives values of about 40 um.Because of the weak nature of the binding agent, the compressive strength is low, inthe range of 7 to 40 MPa (1,000 to 6,000 psi). The tensile strength is very low also.The solubility is high, about 1.5% by weight in distilled water after 24 hours. Eugenolis extracted from the set cement by the hydrolytic decomposition of the zinceugenolate/eugenate. The cement disintegrates rapidly when exposed to oralconditions.Biologic effectThe presence of eugenol in the set cement under clinical conditions appears to lead toan anodyne and obtundent effect on the pulp in deep cavities. When exposed directlyto oral conditions, the material maintains good sealing characteristics despite avolumetric shrinkage of 0.9% and a thermal expansion of 35 10-6/C. The sealingcapacity and antibacterial action appear to facilitate pulpal healing; however, when indirect contact with connective tissue, the material is an irritant. Reparative dentinformation in exposed pulp is variable. Eugenol is a potential allergen.Advantages and DisadvantagesThe main advantage of these materials is their bland and obtundent effect on thepulpal tissues, together with their good sealing ability and resistance to marginalpenetration.Disadvantages include low strength and abrasion resistance, solubility anddisintegration in oral fluids, and little anticariogenic action.Reinforced zinc oxide-eugenol cementsApplicationsThese materials have been used as cementing agents for crowns and fixed partialdentures, cavity liners and base materials, and provisional restorative materials.Composition and settingThe powder consists of zinc oxide with 10% to 40% finely divided natural orsynthetic resins (eg, colophony [pine resin], poly[methyl methacrylate], polystyrene,or polycarbonate) together with accelerators. The liquid is eugenol, which may alsocontain dissolved resins as mentioned earlier and accelerators such as acetic acid, aswell as antimicrobial agents such as thymol or 8-hydroxyquinoline.
The setting reaction is similar to zinc oxide-eugenol cements. Acidic resins such ascolophony (abietic acid) may react with the zinc oxide, strengthening the matrix.ManipulationMore powder is required for a cementing mix than with other cements. The properratio must be adhered to for adequate strength properties. Measures are provided forsome commercial materials. The mixing pad or slab should be thoroughly dry. Thepowder is mixed into the liquid in small portions with vigorous spatulation until thecorrect amount has been incorporated. Adequate time should be allowed for settingwithout disturbance of the cement. Both powder and liquid containers should be keptclosed and stored under dry conditions.PropertiesThese cements may have a long working time because moisture is needed for setting.Some commercial materials contain moisture and, therefore, have working and settingtimes in the same range as zinc phosphate cements, that is, 7 to 9 minutes in oralconditions. Setting time is also lengthened by reducing the powder/liquid ratio.At cementing consistency, values of film thickness from 35 to 75 um have beenobtained with commercial materials (see Table 9-4). Clinical trials have shownsatisfactory performance in seating castings for cements with the lowest values.These materials have compressive strengths in the range from 35 to 55 MPa (5,000 to8,000 psi). The tensile strength is 5 to 8 MPa (700 to 1,000 psi) (see Table 9-4). Thestrength is adequate as a lining material and for luting single restorations and retainerswith good retention form. The modulus of elasticity is 2 to 3 GPa (300,000 to 400,000psi). The mechanical properties of these cements are reduced by immersion in water,which results in loss of eugenol, although this appears to be slower than with simplezinc oxide-eugenol materials. This tendency seems less pronounced with the polymer-reinforced materials.Because of the presence of the resin, the solubility of these cements appears to besomewhat lower than that of zinc oxide-eugenol materials.Biologic effectsPolymer-reinforced zinc oxide-eugenol cements have biologic effects similar to basicmaterials, although there is some variation in inflammatory reaction in connectivetissue with the brand of material. There may be softening and discoloration of someresin restorative materials.Advantages and DisadvantagesThe main advantages of these materials are the minimal biologic effects, good initialsealing properties, and adequate strength for final cementation of restorations.The principal Disadvantages are the lower strength, higher solubility, and higher
disintegration compared to zinc phosphate cements; hydrolytic instability; and thesoftening and discoloration of some resin restorative materials.EBA and other chelate cementsTo further improve on the basic zinc oxide-eugenol system, many researchers haveinvestigated mixtures of zinc and other oxides with various liquid chelating agents.The only system that has received extensive commercial exploitation for luting andlining is that containing ortho-ethoxybenzoic acid.**Noneugenol cements have also been developed in which fatty acids or low-odorphenolic derivatives are used to overcome the smell and taste of eugenol.ApplicationsThese materials have been used for the cementation of inlays, crowns, and fixedpartial dentures, for provisional restorations, and as base or lining materials.Composition and settingIn EBA materials the powder is mainly zinc oxide containing 20% to 30% aluminumoxide or other mineral fillers. Polymeric reinforcing agents, such as poly(methylmethacrylate), may also be present. The liquid consists of 50% to 66% ethoxybenzoicacid with the remainder eugenol.The setting mechanism has not been fully elucidated. It appears to involve chelate saltformation between the EBA, eugenol, and zinc oxide. The setting is accelerated by thesame factors that are operative for zinc oxide-eugenol cements.ManipulationIn general, the manipulation is similar to that of reinforced zinc oxide-eugenolcements. The cement mixes readily to a very fluid consistency even at a highpowder/liquid ratio. In order to obtain optimal properties, it is important to use as higha powder/liquid ratio as possible; this is about 3.5 g/mL for cementation and 5 to 6g/mL for liners or bases. Vigorous spatulation is required for about 2 minutes toincorporate all the required powder. The correct mix flows readily under pressurebecause of the long working time. Adequate setting time in the mouth should beallowed. Several days may be required to reach maximum strength.PropertiesThe working time at room temperature is long because of the dependence onmoisture. The setting time ranges between 7 and 13 minutes under oral conditions(see Table 9-4).The film thickness appears to be in the range of 40 to 70 um for the different brandsand seems adequate for permanent cementation of restorations at the lower level.At cementing consistency, the compressive strength of these materials is in the range
of 55 to 70 MPa (8,000 to 10,000 psi); higher values, similar to those of zincphosphate cements, can be obtained by increasing the powder/liquid ratio. The tensilestrength is considerably lower, about 3 to 6 MPa (500 to 900 psi). The modulus ofelasticity is about 5 GPa (700,000 psi). The EBA cements show viscoelasticproperties with very low strength and large plastic deformation at slow (0.1 mm/min)rates of deformation and at oral temperature (37C). This may explain why theretention values for crowns and orthodontic bands are considerably below thoseobtained using zinc phosphate cements.The solubility is similar to that of the polymer-reinforced zinc oxide-eugenolmaterials in distilled water, although loss of eugenol also occurs. The resistance tosolubility in organic acids appears to be greater than that of the zinc phosphatecements. When exposed to moisture, greater oral dissolution occurs than for othercements. However, a clinical survey by Silvey and Myers (1978) of the performanceof an EBA-alumina cement over 3 years showed only very slightly worse results thanfor zinc phosphate and polycarboxylate cements. Oral breakdown may thus depend onthe precise brand and manipulation.Biologic effectsThe biologic properties of these materials appear to be similar to those of zinc oxide-eugenol materials.Advantages and DisadvantagesThe principal advantages of EBA cements are their easy mixing, long working time,good flow characteristics, and low irritation to pulp. Strength and film thickness canbe comparable to those of zinc phosphate cements (see Table 9-4).The main Disadvantages are the critical proportioning, hydrolytic breakdown in oralfluids, liability to plastic deformation, and poorer retention than zinc phosphatecements. These materials seem best suited for luting restorations with good fit andretention where there is no undue stress and as cavity bases.Calcium hydroxide chelate cementsThe value of calcium hydroxide as a pulp-capping material that facilitates theformation of reparative dentin has long been recognized. This action appears to belargely attributable to its alkaline pH and consequent antibacterial and protein-lyzingeffect. Although a number of aqueous paste materials based on calcium hydroxide areavailable, they are not easy to manipulate and the dried films tend to crack. In theearly 1960s, phenolate-type cements based on the setting reaction between calciumhydroxide and other oxides and salicylate esters were introduced.ApplicationsThese materials are used as liners in deep cavity preparations.Composition and setting
These materials are usually formulated as two pastes: One paste contains calciumhydroxide, zinc oxide, and zinc salts in ethylene toluene sulphonamide; the othercontains calcium sulfate, titanium dioxide, and calcium tungstate (a radiopacifyingagent) in a liquid disalicylate ester of butane-1,3-diol. The calcium hydroxide isintended to be in excess to produce an alkaline pH that will effect an antibacterial andremineralization action. There is some variation among the materials in this respect.At least one material contains fluoride.Calcium and zinc oxide react with the salicylate ester to form a chelate similar to thezinc oxide- eugenol reaction. Likewise the reaction is greatly accelerated by moistureand accelerators.ManipulationEqual lengths of the two pastes are mixed to a uniform color.PropertiesWorking time may be 3 to 5 minutes, depending on the availability of moisture. In themouth, setting is rapid, about 1 or 2 minutes.The compressive strength at 7 minutes is about 6 MPa (900 psi), and the tensilestrength 1.5 MPa (200 psi); at 1 hour the corresponding values are about 10 MPa(1,500 psi) and 1.5 MPa (200 psi); and at 24 hours the values are 14 to 20 MPa (2,000to 3,000 psi) and 1.7 to 2 MPa (250 to 300 psi). Thin films become resistant to 8 MPa(1,100 psi) penetration force in 90 seconds. At 37C plastic flow without fractureoccurs.The solubility in 50% phosphoric acid during acid-etching procedures is significant.These cements seem to be subject to hydrolytic breakdown. When continued marginalleakage takes place, complete dissolution of the linings of these materials can occur.Biologic effectsThese cements appear to exert a strong antibacterial action when free calciumhydroxide is available and to assist in remineralization of carious dentin. Theyfacilitate the formation of dentin bridges when used for pulp capping on exposures.Their effect on exposed pulp is superior to that of zinc oxide-eugenol materials. Thesematerials can also exert a pulpal protective action by neutralizing and preventing thepassage of acid and by acting as a barrier to the penetration of other agents such asmethyl methacrylate.Advantages and DisadvantagesThe advantages of these materials include their easy manipulation, rapid hardening inthin layers, good sealing characteristics, and beneficial effects on carious dentin andexposed pulp.Their Disadvantages are that they show low strength even when fully set, exhibitplastic deformation, are weakened by exposure to moisture, and will dissolve under
acidic conditions and if marginal leakage occurs. The data on physical properties andclinical experience suggest that further improvements in these materials are requiredbefore they can be utilized as the sole liner in deep cavity preparations.More recently polymerizable resin compositions containing calcium hydroxide havebeen introduced as alternatives to these materials.Polycarboxylate (Carboxylate)- Based CementsZinc polycarboxylate cementsThe polycarboxylate cements were developed in the late 1960s as adhesive dentalcements that would combine the strength properties of the phosphate system with thebiologic acceptability of the zinc oxide- eugenol materials.ApplicationsZinc polycarboxylates are used for the cementation of cast alloy and porcelainrestorations and orthodontic bands, as cavity liners or base materials, and asprovisional restorative materials.Composition and settingThe powder in these cements is zinc oxide with, in some cases, 1% to 5% tin ormagnesium oxide; 10% to 40% aluminum oxide or other reinforcing filler may bepresent in some brands. A small percentage of stannous or other fluoride may also beincluded to improve mechanical properties and provide leachable fluoride. The liquidis approximately a 40% aqueous solution of polyacrylic acid or an acrylic acidcopolymer with other organic acids, such as itaconic acid. The molecular weight ofthe polymer is generally in the range of 30,000 to 50,000, which accounts for theviscous nature of the solution. In some brands of the material the polyacrylic acidcomponent is dried and added to the powder. In a brand that is encapsulated the liquidis a weak solution of NaH2PO4, which both reduces the viscosity of the polyacrylicacid and retards the setting of the cement. In other brands water is simply added to thepowdered ingredients.The zinc oxide reacts with the polyacrylic acid, forming a cross-linked structure ofzinc polyacrylate. The set cement consists of the residual zinc oxide particles bondedtogether by this amorphous gel-like matrix:ManipulationThe material should be carefully proportioned and the freshly dispensed componentsmixed rapidly in 30 to 40 seconds. The mix should be used while it is still glossy,before the onset of cobwebbing. The correct cementing mix is more viscous than azinc phosphate mix, but because of its different rheology it flows adequately underpressure. The water mix materials are more fluid initially (Fig 9-2). The interior ofrestorations and tooth surfaces should be clean and free of saliva. The powder and
liquid should be stored under cool conditions and kept sealed with a stopper.Prolonged or cold storage may cause the liquid to gel; to reverse this, it must bewarmed to 50C. Loss of moisture from the liquid will lead to thickening.Fig 9-2 Typical consistency for water mix polycarboxylate and glass-ionomercements. The mix is comparable to zinc phosphate cements.PropertiesThe rate of setting is affected by the powder/liquid ratio, the reactivity of the zincoxide, the particle size, the presence of additives, and the molecular weight andconcentration of the polyacrylic acid. At luting consistency the recommendedpowder/liquid ratio for most materials is about 1.5:1 by weight. The working time is2.5 to 3.5 minutes at room temperature, and the setting time is 6 to 9 minutes at 37C;the water mix materials tend to give slightly longer setting times. As with othercements, working time can be substantially increased by mixing the material on a coldslab and by refrigerating the powder. The liquid should not be chilled, as thisencourages gelation due to hydrogen bonding.The freshly mixed cement shows shear thinning. Contrary to the subjectiveimpression that the correct mix for a zinc polycarboxylate cement is much thickerthan that of a luting zinc phosphate mix, under pressure they flow out to the samedegree to a film thickness of 25 to 35 um. In fact, the zinc phosphate mix tends tothicken more quickly than the zinc polycarboxylate mix. One of the most commonerrors made with the polycarboxylate cements is to make a mix that appears to be asfluid as a zinc phosphate mix; this will result in a low powder/liquid ratio withconsequent poor properties in the cement. Measuring devices for these materials willensure correct proportions.At cementing consistency, the compressive strength of these materials is in the range
of 55 to 85 MPa (8,000 to 12,000 psi), and the tensile strength is 8 to 12 MPa (1,100to 1,700 psi) (see Table 9-4). Strength increases with the powder/liquid ratio, reachinga maximum at about 2:1 by weight, and it is increased also by additives such asalumina and stannous fluoride. In general these cements have somewhat lowercompressive strengths than zinc phosphate cements but are significantly stronger intension. The cement gains strength rapidly after the initial setting period; the strengthat 1 hour is about 80% of the 24-hour value. The modulus of elasticity is about 6 GPa(850,000 psi).In distilled water, the solubility ranges from less than 0.1% to 0.6%. The latter highvalue relates particularly to cements that contain stannous fluoride. However, as in thezinc phosphate system, the solubility is appreciably higher in acids such as lactic andcitric acid. In vivo solubility is similar to or less than that for zinc phosphate cements.Bonding to clean enamel and dentin surfaces can occur through calciumcomplexation. In practice, adhesion to dentin may be limited because of debris andcontamination. The material also sticks to clean stainless steel, amalgam, chromium-cobalt, and other alloys. Bond strength is related to the strength of the cement.Biologic effectsThe effect of zinc polycarboxylate cements on pulp is comparable to or less than thatof zinc oxide-eugenol. The formation of reparative dentin in exposed pulp is variable.The generally good biocompatibility appears to be primarily due to the low intrinsictoxicity and also to (1) the rapid rise of the cement pH toward neutrality; (2)localization of the polyacrylic acid and limitation of diffusion by its molecular sizeand ion binding to dentinal fluid and proteins; and (3) the minimal movement of fluidin the dentinal tubules in response to the cement. The presence of stannous fluoridedoes not appear to affect the mild response. The fluoride-containing cements releasefluoride, which is taken up by neighboring enamel and which presumably will exertanticariogenic effects.Advantages and DisadvantagesThe main advantages of these materials are the low irritation, adhesion to toothsubstance and alloys, easy manipulation, strength, solubility, and film thicknessproperties comparable to those of zinc phosphate cements.The Disadvantages are the need for accurate proportioning for optimal properties andthus more critical manipulation, the lower compressive strength and greaterviscoelasticity than zinc phosphate cements, the short working time of somematerials, and the need for clean surfaces to utilize the adhesion potential.Polymer-Based CementsIntroductionThe majority of the materials in this group are polymethacrylates of two types: (1)materials based on methyl methacrylate and (2) materials based on aromatic
dimethacrylates of the bis-GMA type. The closely related cyanoacrylate monomers,notably ethyl and isobutyl, have found some limited use for the attachment of facingsand for pin cementation. However, the hydrolytic stability and biologic effects in thissituation are suspect and little use is made of them.Acrylic resin cementsApplicationsAcrylic resin cements are used for the cementation of restorations, facings, andprovisional crowns.Composition and settingThe powder in these materials is a finely divided methyl methacrylate polymer orcopolymer containing benzoyl peroxide as the initiator. Mineral filler and pigmentsmay also be present. The liquid is a methyl methacrylate monomer containing anamine accelerator.The monomer dissolves and softens the polymer particles and concurrentlypolymerizes through the action of free radicals from the peroxide-amine interaction.The set mass consists of the new polymer matrix uniting the undissolved but swollenoriginal polymer granules.ManipulationThe liquid is added to the powder with minimal spatulation to avoid an incorporationof air. The mix must be used immediately because working time is short. Excessmaterial must be removed at the final set, hard stage and not when the material isrubbery, otherwise marginal deficiencies will be created.PropertiesThe properties of these materials are comparable to those of the cold-curing acrylicresin filling materials. They are stronger and less soluble than other types of cementbut display low rigidity and viscoelastic properties. They have no effective bond totooth structure in the presence of moisture; thus they permit marginal leakage,although they may show better bonding than other cements to resin facings andpolycarbonate crowns.Biologic effectsAs with acrylic resin filling materials, marked pulpal reaction may occur and pulpalprotection is necessary.Advantages and DisadvantagesThe advantages of these materials include relatively high strength and toughness andlow solubility.
Disadvantages include a short working time, deleterious effects on pulp, and difficultyin removal of excess cement from margins.Adhesive resin cementsAdhesive acrylic materials have been formulated by adding an adhesion promoter, 4-methyloxy ethyl trimelletic anhydride (4-META), to the methyl methacrylatemonomer as well as an additional polymerization initiator, tributyl boron, which isalso believed to aid chemical bonding to dentin. Such materials have been developedas cements for metal fixed partial dentures especially of base metal (Superbond,Parkell) and for bonding amalgam to dentin and composites (Amalgambond, Parkell).In vitro tests have shown high bond strengths for the luting cement to oxidized,etched, or silica-coated casting alloy surfaces. Shear bond strength to amalgam issignificantly less than the bond strength to dentin, which is comparable to other dentinbonding systems in the region of 20 MPa. Since these materials have only low (10%) filler content, the physical properties are typical of acrylic resins, that is,moderate strength with high deformation under load. Although the materials havebeen widely used for cementation of fixed partial dentures, there is little clinical dataon longevity, and the cements are said to be technique sensitive.Dimethacrylate cementsDimethacrylate cements are usually based on the bis-GMA system: They arecombinations of an aromatic dimethacrylate with other monomers containing variousamounts of ceramic filler. They are basically similar to composite restorativematerials.ApplicationsDimethacrylate cements are used for bonding crowns (usually porcelain), fixed partialdentures, inlays, veneers, and indirect resin restorations.Composition and settingThese cements are classified according to the following methods of curing:1. Chemically (or auto-) cured: These are usually paste-paste systems and are used tocement metal and opaque ceramic core (eg, Procera, In-Ceram) restorations (Fig 9-3).
Fig 9-3 Chemically cured resin cement for use under opaque restorations (Panavia 21,Kurarary/J. Morita).2. Dual cured: These cements start curing with light and continue with chemicalcuring. The chemical cure will polymerize more thoroughly than light curing alone(Fig 9-4). These are used to cement translucent restorations (eg, porcelain, indirectresin restorations).Fig 9-4 Dual-cured resin cement in syringe form for use when light may not penetrateenough for complete curing (Dual Cement, Vivadent).
3. Light cured/dual cured: These can be used for light curing only or can be dualcured when dual-cure catalysts are added to the light-cure base. These products areused for both light-cure applications (eg, thin porcelain veneers) and dual-cureapplications (Fig 9-5).Fig 9-5 Light-cured/dual-cured cements may be cured with light or with addition ofdual-cure catalyst, which will allow setting to continue after light is turned off(Variolink II, Vivadent).In the powder-liquid materials, the powder is generally a finely divided borosilicate orsilica glass together with fine polymer powder and an organic peroxide initiator. Theliquid is a mixture of bis-GMA and/or other dimethacrylate monomers containing anamine promoter for polymerization. Some materials contain monomers withpotentially adhesive groups, such as phosphate or carboxyl, similar to dentin bondingmaterials. The two-paste materials are of similar overall composition but with themonomers and fillers combined into two pastes. In light-cured and dual-curedmaterials, light-sensitive polymerization systems such as diketones (eg,camphorquinone) and amine promoters are present, respectively, in the two cementcomponents in addition to the chemical-initiator systems.On mixing the components, polymerization of the monomers occurs, leading to ahighly cross-linked resin composite structure.ManipulationCorrect proportioning of powder and liquid components using measures is important.Paste materials are usually proportioned 1:1 (equal lengths). Rapid, thorough mixing,minimizing air inclusion, until uniform is critical.Properties
As with resin composite restorative materials, monomer conversion is incomplete,even under optimum cure conditions, and thus manipulation is critical to optimumphysical properties. For light- and dual-cured materials, the maximum light exposureis desirable. Maximum properties are generally reached about 10 minutes afterpolymerization; only small changes occur over the ensuing 24 hours.Since polymerization systems vary and filler contents range between 20% and 80%for the various products, physical properties vary widely (see Table 9-4) and thesolubility of a specific material for a particular clinical application should be checkedindividually. Compressive strengths have been reported to range between 100 and 200MPa (14,000 and 28,000 psi), and diametral tensile strengths from 20 to 50 MPa(3,000 to 7,000 psi) with corresponding differences in microhardness. These valuesare considerably higher than traditional cements, and therefore high values can beobtained for retention of well-fitting crowns. However, optimum luting performanceis very dependent on fluidity, seating capability, and film thickness. Many resincements tend to show unacceptably high values for film thickness. Recently, toimprove wetting of the tooth, preparation, seating, and bond strength, some resincements have been used with dentin bonding primers, thus increasing the clinicalcomplexity of the system. Although these materials have been used widely inadhesive techniques, especially for ceramic restorations, there are comparatively fewclinical reports of their longevity. Aside from failures induced by material andtechnique shortcomings during the critical clinical manipulation, studies indicate thatresin cement bonds will most likely fail through cyclic fatigue stresses. Some studieson etched metal restorations cemented with chemically cured cements have indicateda median survival time of about 8 years.Biologic effectsThe materials themselves appear to pose few problems, although some patientsexperience objectionable odors. Cases of allergy among dental personnel haveoccurred, especially where reactive dentin bonding systems have been used. Skincontact should be avoided.Pulpal pathology may be due to poor seating, polymerization contraction, andconsequent microleakage. All systems show some microleakage that may contributeto tooth sensitivity and clinical failure. Microleakage appears to occur least withsystems employing dentin bonding agents, but there are no long-term studies on thisaspect.Advantages and DisadvantagesThe advantages of these cements include high strength; low oral solubility; and highmicromechanical (and possible chemical) bonding to prepared enamel, dentin, alloys,and ceramic surfaces.Disadvantages include the need for a meticulous and critical technique, more difficultsealing and higher film thickness than traditional cements, possible leakage and pulpalsensitivity, and difficulty in removal of excess cement.
Glass-Ionomer CementsIntroductionThese materials were formulated in the 1970s by bringing together the silicate andpolyacrylate systems. The use of an acid-reactive glass powder together withpolyacrylic acid solution leads to a translucent, stronger cement that can be used forluting and restorative materials.ApplicationsGlass-ionomer cements are used for the cementation of cast-alloy and porcelainrestorations and orthodontic bands, as cavity liners or base materials, and asrestorative materials, especially for erosion lesions. They are being replaced by hybridionomer cements, which allow better handling.Composition and settingThe powder in these materials is finely ground calcium aluminum fluorosilicate glasswith a particle size around 40 um for the filling materials and less than 25 um for theluting materials. One brand (Zionomer Liner, Den-Mat) also contains zinc oxide.Silver powder is fused into the glass in Ketac-Silver (3M/ESPE) for improvedphysical properties. The liquid is a 50% aqueous solution of a polyacrylic-itaconicacid or other polycarboxylic acid copolymer that contains about 5% tartaric acid.Some other materials contain 10% to 20% added silver, silver alloy, or stainless steel.In some materials the solid copolymer is added to the powder, and the solutioncontains tartaric acid; in others, all the ingredients are in the powder, and the liquid iswater.On mixing, the polyacrylic and tartaric acids react with the glass, leaching calciumand aluminum ions from the surface, which cross-link the polyacid molecules into agel. The tartaric acid serves to increase working time and gives a sharp setting byforming metal ion complexes. Differences in composition between brands affect thehardening rate and properties. Some recent evidence suggests that a polysilicatematrix may also form within the polygel over time.ManipulationThe material should be carefully proportioned and the freshly dispensed componentsmixed rapidly in 30 to 40 seconds. Some brands are encapsulated, mechanicallymixed, and injected. The powder/liquid ratio for luting is about 1.3:1 for theconventional types of glass-ionomer cement. This ratio appears to be critical withthese cements to obtain optimal cementation properties. Best results are obtained bymixing the chilled powder with the liquid on a chilled slab. The correct cementingmix is fluid, similar to zinc phosphate. The lining mix is somewhat more viscous,depending on the brand. The restorative mix should have a puttylike consistency and aglossy surface. Tooth surfaces should be clean and free from saliva but notdehydrated. Restoration surfaces should be free from debris and contamination. Thecement hardens slowly and should be protected from loss or gain of moisture when set
clinically. Restoration margins or filling surfaces should be protected with a varnishor a light-curing sealant. This is less important with light-cured materials.PropertiesFor the luting materials, the setting time is in the range of 6 to 9 minutes. The liningmaterials set in 4 to 5 minutes, and the restorative materials set in 3 to 4 minutes.Materials that are light-cured set in approximately 30 seconds when exposed to avisible light source. The acid-base reaction continues slowly and properties improveover time.Film thickness is in the range of 25 to 35 um, which is adequate to seat castingssatisfactorily, although the flow properties are quite dependent on the powder/liquidratio.For the luting cements, the compressive strength increases over 24 hours to 90 to 140MPa (13,000 to 20,000 psi) depending on the brand. The tensile strength increasessimilarly to 6 to 8 MPa (900 to 1,100 psi). The compressive modulus of elasticity isabout 7 GPa (900,000 psi). The lining materials have compressive and tensilestrengths in the same range with some light-cured materials at the higher end of therange reaching 150 to 160 MPa (21,000 to 23,000 psi) in compression and 10 to 12MPa (1,400 to 1,700 psi) in tension. The light-cured materials are significantlytougher in some brands, with a lower modulus. The restorative materials range from140 to 180 MPa (20,000 to 26,000 psi) in compression and 12 to 15 MPa (1,700 to2,100 psi) in tension. The light-cured restorative materials may have strengths as highas 200 MPa in compression and 20 MPa in tension. Some silver-containing materialsare in this range, and even higher strengths have been achieved in recent materials.In general, with light-cured materials, properties are dependent on the depth of cure.The solubility of the cements in water is about 1% for a luting material, and this ishigher in lactic acid. Good resistance to dissolution is observed under oral conditions.Resistance to dissolution and disintegration is improved by varnish protection forconventional cements.Erosion of clinical restorations of conventional cements by acid phosphate fluoridepreventive-treatment solutions has been observed, making these solutionscontraindicated.Some studies show that light-cured glass-ionomer materials continue to absorb waterover several months, with swelling and reductions in strength and stiffness. Theclinical significance of this behavior is not yet clear.Glass-ionomer cements exhibit bonding to enamel, dentin, and alloys in a mannersimilar to zinc polycarboxylates. In vitro and in vivo the adhesion is variable and isaffected by surface conditions. Slight and variable marginal leakage has beenobserved. Bonding to dentin for conventional materials is not improved bypretreatment with polyacrylic acid solutions, whereas with light-cured materials it isdependent on the use of dentin primers.
Biologic effectsPulpal response to the lining and restorative materials appears generally favorable.Variable behavior has been reported for the various luting materials with instances ofpostoperative sensitivity. This has been attributed to a prolonged initially low pHcoupled with the effects of the toxic ions. This may be accentuated by dehydration ofdentin and marginal leakage of bacteria. Leaching of fluoride and uptake by adjacentenamel occurs with these cements, and this continues for at least a year withpotentially cariostatic effects. Antibacterial action has been attributed to low initialpH, leaching, release of silver and other ions, or a combination of these. Light-curedmaterials have been observed to show greater cytotoxicity.Advantages and DisadvantagesThe advantages of glass-ionomer cement materials include easy mixing, high strengthand stiffness, leachable fluoride, good resistance to acid dissolution, potentiallyadhesive characteristics, and translucency.The Disadvantages include initial slow setting and moisture sensitivity, variableadhesive characteristics, radiolucency, and possible pulpal sensitivity.Resin-modified glass-ionomer cementsApplicationsA recent addition to the spectrum of materials, these versatile cements, sometimesalso called hybrid ionomers (see Fig 8-11), have many uses: cavity liners, bases, corebuildups, and luting cements. One hybrid ionomer (Fig 9-6) is used for permanentcementation of crowns, orthodontic appliances, and core buildups.Fig 8-11 Continuum of glass-ionomer and composite restorative materials. (AfterAlbers, 1996).
Fig 9-6 A hybrid ionomer (Vitremer, 3M).Composition and settingIn hybrid ionomers, the acid-base setting reaction in glass-ionomer cements has beenmodified by the introduction of water-soluble polymers and polymerizable monomersinto the composition. The use of copolymers of acrylic acid and methacrylatemonomers in the liquid leads to materials that undergo the customary acid-basereaction on setting and can also be light cured via the methacrylate groups. This givesimproved lining and restorative materials with an immediate command set and thushigher early strength and water resistance. Some commercial materials contain apreponderance of polymeric components with minimal acid-base reaction.The classification of these materials as glass-ionomer cements is controversial. Somelight-cured restorative glass-ionomer cements are used with a dentin primer similar todentin bonding resin composite systems and thus depend on surface infiltration forbonding in addition to chemical interaction.Resin-modified glass ionomers are available in hand-mixed and predosed capsules(Fig 9-7). The resin monomers in the liquid depend on the product and include bis-GMA, hydroxyethylmethacrylate, and methacrylate-modified polyacrylates alongwith photoinitiators.
Fig 9-7 A simple hybrid ionomer luting cement for hand mixing or automix withcapsules and gun (Fuji I, GC America).ManipulationFor hand-mixed compositions, the powder should be fluffed before dispensing. Thepowder and liquid should be mixed quickly, within 30 seconds, on the pad. Thesecements have a working time of about 2.5 minutes. For luting, the cement is appliedto the undesiccated tooth to avoid possible postoperative sensitivity.PropertiesTable 9-5 gives a comparison of properties of resin-modified glass ionomers versusglass-ionomer cements. The strength properties of the two types of cements aresimilar, with considerable variations among brands. There is a major difference inflexibility, with the hybrid ionomers being twice as flexible, as indicated by lowermodulus of elasticity values. Also, many of the hybrid ionomers have been found toexpand on setting, possibly due to the absorption of water, which is more than forresin cements. Therefore, hybrid ionomers are not recommended for luting all-ceramic crowns, to avoid possible expansion stresses and crown fracture. Table 9-5 Mechanical properties of glass-ionomer and hybrid ionomercements* Glass ionomers Resin-modified glass ionomersFlexural strength (MPa) 25 35-70Flexural modulus (GPa) 8 4Compressive strength (MPa) 180-200 170-200Diametral tensile strength (MPa) 22-25 35-40
Shrinkage (% vol) 3 3.5-expansion*Data from Burgess et al (1996). Used with permission from The Compendium ofContinuing Education in Dentistry.Biologic effectsHybrid ionomers release fluoride from the glass component, which is favorable forcaries prevention. Long-term, large-scale clinical data are not available for an overallassessment of their biologic effects.Advantages and DisadvantagesTheir advantages include dual cure, fluoride release, higher flexural strength thanglass-ionomer cements, and ease of handling. Also, they are capable of bonding tocomposite materials.One problem is a possible setting expansion that may lead to cracking of all-ceramiccrowns. Therefore, resin cements, zinc phosphate, and glass-ionomer cements are stillrecommended for metal-free crowns.Selection and Use of CementsNone of the cements available is free from deficiencies in the required clinicalcharacteristics, such as biocompatibility, ease of manipulation, satisfactory sealing,retentive properties, and long-term stability. A proportion of clinical failures isinevitable, but this can be minimized by proper selection and manipulation of thecement. The following factors should be kept under review:1. Rapid uniform and reproducible dispensing of the components2. Rapid, thorough mixing3. Moisture isolation where practical4. An undisturbed setting5. Careful removal of excess6. Avoidance of excessive drying of dentinFactors within the clinicians control, such as the design and execution of thepreparation, adequate isolation, proper seating of the restoration, and finishing of themargins, are also important determinants of success as is the manipulation of thecement.These considerations may influence cement selection and use, but a governing factoris the biological state of the tooth tissue. Thus, as indicated in Table 9-2, the selection
of particular cements for specific clinical situations is limited both by the preparationand the properties of the cement.Clinical Decision Scenarios for Dental CementsThis section presents one approach for choosing dental cements for specific situations.Each of the following scenarios uses the same format as that presented in chapter 7.Advantages and Disadvantages of each material are prioritized using the followingcodes: * = of minor importance, ** = important, and *** = very important.Materials Zinc phosphate vs resin cement for crown cementationDescription A dentist has finished preparation of a full gold crown for a maxillaryleft permanent second molar and is ready to cement the crown. This is a routine crowncementation. The preparation is normal, the tooth is vital, and there is no knownpulpal pathology. The dentist may choose between a resin cement and zinc phosphatecement.Critical Factors Ease of use, cost, effectivenessZinc phosphateAdvantages*** Low cost Long clinical history High rigidity Long working time*** Easy to useDisadvantages*** No bond to tooth Slow setting time Moisture sensitivity during mixingResinAdvantages*** Bonds to tooth
Fast setting time Higher strength*** Easy to useDisadvantages*** High cost Short working time Film thickness varies widely among brands Difficult to remove excessAnalysis/Decision Comparing the properties of the two cements reveals they arebalanced in advantages and Disadvantages for this situation. The choice finally restsin the personal preference of the dentist. Since this dentist had more experience withzinc phosphate, she chose to use that material.Materials Glass ionomers vs zinc phosphate cement for crown cementationDescription An older gentlemen with a history of periodontal surgery to correct bonydefects has broken the cusps off a previously restored mandibular first molar. Thepatients plaque control is only fair, and he is taking medications that could result insome degree of "dry mouth." He has had a slightly increased level of caries activitysince the surgery and since beginning the medication. The dentist has elected torestore the tooth with a cast crown, which has now been returned from the laboratoryand is ready for cementation. The dentist has both zinc phosphate and glass-ionomerluting cements available and must decide which to use.Critical Factors Caries resistance, good sealZinc phosphateAdvantages*** Good seal** Reasonable cost** Adequate strength** Little sensitivityDisadvantages
*** No fluoride releaseGlass ionomerAdvantages*** Good seal*** Fluoride release** Adequate strength** Reasonable costDisadvantages** Occasional sensitivityAnalysis/Decision Both cements have a good seal, but only the glass ionomerreleases fluoride after cementation. Fluoride is generally accepted to reduce caries andseems to do so in individuals such as this patient. For this reason, the glass ionomerwas selected. Careful attention to instructions allowed cementation without thesensitivity sometimes experienced with glass-ionomer cements. The dentist wassatisfied with this treatment choice.Materials Glass ionomers vs zinc phosphate for bases under amalgam restorationsDescription A patient has a mandibular molar that exhibits extensive cariousdestruction. Due to the patients finances, a large, pin-retained amalgam restoration isselected. Following caries removal and preparation, it is determined that the cavityneeds a base prior to placement of the amalgam restoration. The dentist has zincphosphate and glass-ionomer cements available and must choose between them for abase material.Critical Factors Strength, modulus of elasticityZinc phosphateAdvantages*** Adequate modulus of elasticity*** Adequate strength** Ease of use** No sensitivity
Disadvantages** No fluoride releaseGlass ionomerAdvantages*** Adequate modulus of elasticity*** Adequate strength** Fluoride release** Ease of useDisadvantages** Occasional sensitivityAnalysis/Decision Since the advantages and Disadvantages were essentiallybalanced for this situation, neither cement had a clear advantage. The highlysignificant modulus of elasticity, essential for a good base, was roughly equivalent. Inthis case, the dentist chose glass ionomer because of the added advantage of fluoriderelease, which is thought to reduce recurrent decay. However, because that was not aproblem with this patient, either cement would have been an acceptable choice.Materials Zinc oxide-eugenol vs calcium hydroxide as liners under amalgamrestorationsDescription A patient in need of a slightly deep mesio-occlusodistal amalgam on amandibular left first molar was seen by the dentist. The patient reported that the lasttwo amalgams the dentist placed had been quite sensitive for several weeks followingplacement. They had finally lost their sensitivity, but the patient felt they had hurtunusually long for new restorations. Upon preparation, the dentist decided that a basewas indicated. Both calcium hydroxide and zinc oxide-eugenol base materials wereavailable.Critical Factors Strength, modulus of elasticity, reduction of sensitivityZinc oxide-eugenolAdvantages** Ease of use** Decreased sensitivity
** Low costDisadvantages*** Low strength*** Low modulus of elasticityCalcium hydroxideAdvantages** Ease of use** Stimulates secondary dentin** Low costDisadvantages*** Low strength*** Low modulus of elasticityAnalysis/Decision In this situation, again, there is no clear advantage for either base.Both have low strength and low modulus of elasticity, necessitating that they beapplied as very thin layers. The zinc oxide-eugenol has the advantage of the anodyneeugenol, which is known to reduce tooth sensitivity. The calcium hydroxide, on theother hand, will stimulate the formation of secondary dentin and thus is good if therestoration is near the pulp. This was true in the situation described, but the patientalso had a history of sensitive teeth following placement of amalgam restorations.Therefore, the dentist selected the zinc oxide-eugenol as the liner of choice. Had thecavity preparation been deeper and the pulp visible through the dentin, calciumhydroxide would have been selected due to its ability to stimulate formation ofsecondary dentin.Materials Flowable resin composite vs hybrid ionomer for Class 5 restorations inhigh-caries-risk patientDescription An older patient has recurrent caries around the margins of a few oldClass 5 amalgam restorations, probably due to poor hygiene and a mild xerostomiaresulting from a cholesterol-lowering drug. The patient requested that the replacementrestorations be more esthetic. The dentist considers flowable composites and hybridionomers.Critical Factors Ease of placement, prevention of recurrent decay, reasonableesthetics
Flowable compositeAdvantages*** Very simple placement*** Excellent esthetics * Less solubleDisadvantages*** Higher incidence of recurrent decay** Higher sensitivity to moisture contamination during placementHybrid ionomerAdvantages*** Ease of placement*** Less recurrent decay*** Reasonable esthetics** Less sensitivity to moisture during placementDisadvantages * More soluble than flowablesAnalysis/Decision Due to the patients high risk of recurrent decay, the dentistdecided to use the hybrid ionomer restorative material. She chose a dual-cure hybridionomer for its ease of use and potential to be recharged with fluoride at future visits.Materials All-purpose adhesives vs cavity varnish under amalgam restorationsDescription A patient is seen and diagnosed as needing numerous amalgamrestorations, some large. Upon preparation, the cavities turn out to be normal in sizeand depth. There is little remarkable about the patient or the restorations. The dentisthas both cavity varnish and new all-purpose adhesives to use under the amalgamrestorations. The all-purpose adhesives are reported by the manufacturer to bond theamalgam to the teeth, but the dentist knows that such claims are as yet probablyexaggerated.Critical Factors Marginal leakage, bond to tooth, cost, time required for application
VarnishAdvantages*** Low cost*** Easy placementDisadvantages*** No bond to tooth*** Mediocre sealAdhesivesAdvantages*** Superior marginal seal*** Bond to toothDisadvantages** High cost*** Complex placementAnalysis/Decision Since there is no evidence of excessively weakened cusps, thepossible bonding of the new adhesives is not significant in this case. The superior sealmakes them desirable, but their high cost and complex placement process complicatesthe choice. The dentist had been to a recent lecture on dental materials in which thespeaker claimed the new materials should be a standard of practice, so he chose toplace the adhesives. The patient reported a complete lack of postoperative sensitivityin the new restorations.Materials Dentin adhesives vs glass-ionomer liners under composite restorationsDescription A patient has several Class 5 toothbrush abrasion lesions on hismaxillary and mandibular premolars. At first, they were no problem, but over theyears they have become sensitive, and the patient wants the discomfort relieved. Thelesions are not carious but are somewhat deep. The occlusal, mesial, and distalmargins are on enamel, but the cervical margin is on cementum. The dentist decidesagainst glass-ionomer restorations because she feels a better esthetic result can beobtained with a composite material. In addition, she feels the composite will betterresist further toothbrush abrasion. She is uncertain whether to use a dentin bondingagent alone or a glass-ionomer lining cement under the cervical margin to preventleakage. She has heard that composites often leak on margins that are on cementum.
Critical Factors Marginal seal, bond strengthDentin adhesivesAdvantages** Good seal*** Adequate bond strength** Lower costDisadvantages*** Poorer marginal sealGlass ionomerAdvantages*** Better marginal seal*** Adequate bond strengthDisadvantages** Additional cost** Additional procedureAnalysis/Decision Although there are more advantages for the bonding agent, themost significant advantagebetter marginal sealfavors the glass-ionomer liner. Itadds to the cost and the time to do the procedure, but it provides a significantly betterseal. The better seal results in a superior restoration that justifies the extra cost andtime. The glass-ionomer liner was selected.Materials Hybrid ionomer vs glass ionomer for treatment of recurrent caries at goldcrown marginsDescription During a dental hygiene appointment, patient examination revealedrecurrent caries around the margins of a few gold crowns. Replacement of the crownsis not feasible due to the patients lack of funds. Normally, the dentist would use aglass-ionomer material to restore the marginal areas after the decay has beenremoved. However, he is considering the use of the newer hybrid ionomers due totheir dual-curing ability.Critical Factors Prevention of recurrent caries, ease of placement, bond to tooth
structureHybrid ionomerAdvantages*** Easy to place*** Tooth colored * Low cost*** Fluoride release** Bonds to tooth * Smoother finish** Light/dual cureDisadvantages * Less durable * Isolation is criticalGlass ionomerAdvantages*** Resonably easy to place*** Tooth colored * Low cost*** Fluoride release*** Bonds to toothDisadvantages * Less durable** More plaque retentive * Isolation is critical** Chemical cure only
Analysis/Decision Though the two materials have comparable fluoride release, thedentist chose a resin-modified glass ionomer mainly for its greater ease of use. Thehybrid ionomer can be placed and cured in less than 1 minute due to the dual-curefeature, while the traditional chemically cured glass ionomers require protection fromoral fluids for 4 to 5 minutes during setting. The dual-curing hybrid ionomer may alsorelease more fluoride because it contains more fluoride glass, which is the source offluoride ions and aids in the chemical setting reaction.Glossaryaccelerator (promoter) Substance that facilitates decomposition of an initiator.anodyne Relieves pain.chelating Ring structure reaction with metal ions.cored structure A material consisting of at least two phases, for example, as residualparticles of a component embedded in a matrix of reaction product.initiator Substance capable of decomposing into free radicals that initiatepolymerization.lute A cementlike material that also fills and seals gaps.obtundent A material that reduces irritation or has a soothing effect on tissue.rheology Science of the deformation and flow of matter.setting time Time from the beginning of mixing of the cement to the development ofa hard and rigid (usually brittle) state in the mouth.working time Time available, measured from the beginning of mixing at roomtemperature, for clinical manipulation of a cement before viscosity becomes too greatfor seating of the restoration.Discussion Questions1. Why is fluoride release so important in a cement?2. What is the source of fluoride in a glass-ionomer cement?3. What is the difference in function between a cement liner and a cement base?4. Why are polymer cements recommended for use with CAD/CAM inlays with poormarginal fits?Study Questions
(See Appendix E for answers.)1. What is the minimum compressive strength required of a dental cement foradequate retention of restorations?2. What is the structure of set zinc phosphate cement?3. How does the solubility of phosphate cements in citric or lactic acid compare withtheir solubility in water?4. What are adhesive resin cements?5. What are resin-modified glass ionomers?6. What agents accelerate the setting of zinc oxide- eugenol cements?7. Why do zinc oxide-eugenol cements have a high solubility?8. What materials can be added to zinc oxide-eugenol cements to improve theirstrength?9. What effects do zinc oxide-eugenol cements have on resin restorative materials?10. How does the composition of EBA cements differ from that of zinc oxide-eugenolcements?11. What factors affect the setting reaction of polycarboxylate cements?12. Give possible reasons for the minimal effect of polycarboxylate cements on pulp.13. What are important considerations in manipulating polycarboxylate cements?14. What are the advantages of light curing glass-ionomer cements?15. What are the major advantages of glass-ionomer cements?16. Define the two types of polymer-based cement.17. What are the principal Disadvantages of polymer-based cement?18. It has been reported that hybrid ionomers expand on setting, which could causecracking of all- ceramic crowns. This was discovered years after the cements weremarketed. Using the hierarchy of evidence, which type of study would have warneddentists about this problem?19. Although short-term pulpal studies on glass-ionomer cements gave a satisfactoryoverall biocompatibility, there were occasional signs of cytotoxicity with certainproducts. After many years of clinical use, it has been reported that, if the dentin hasbeen dehydrated by excessive drying, there is a definite chance of postoperativesensitivity when these cements are used to cement crowns. Speculate on why this
serious clinical problem was not clearly identified in the histologies of treated toothpulps that were used in the biocompatibility tests.Recommended ReadingAlbers HF (1996). Tooth-Colored Restoratives, ed 8. Santa Rosa: Alto Books.Antonucci JM, McKinney JE, Stansbury RW (1998). Resin modified glass ionomercement. US Patent: 160,856.Arfaci AH, Asgar K (1974). Bond strength of selected cementing materials.Microfilmed Paper No. 549. Delivered at the Annual Meeting of the InternationalAssociation for Dental Research, Dental Materials Group, Atlanta, GA, 21-24 Mar.Beagrie GS, Smith DC (1978). Development of a germicidal polycarboxylate cement.J Can Dent Assoc 44:409.Boyer DB, et al (1993). Analysis of debond rates of resin-bonded prostheses. J DentRes 72:1244-1248.Brannstrom M, Nyborg H (1974). Bacterial growth and pulpal changes under inlayscemented with zinc phosphate cement and Epoxylite CBA 9080. J Prosthet Dent31:556.Burgess JO, et al (1993). A comparative study of three glass ionomer base materials.Am J Dent 6:137-141.Burgess JO, Norling BK, Rawls HR, Ong JL (1996). Directly placed estheticrestorative materialsthe continuum. Compend Contin Educ Dent 17:731-732, 734,748.Burke FJT, McCaughey AD (1993). Resin luting materials: their current status. DentUpdate (April):109-115.Causton BE (1982). Primers and mineralizing solutions. In: Smith DC, Williams DF(eds). Biocompatibility of Dental Materials, vol 2. Boca Raton, FL: CRC Press, 125-144.De Freitas JF (1973). The long-term solubility of a stannous fluoride-zinc phosphatecement. Aust Dent J 18:167.Dennison JD, Powers JM (1974). A review of dental cements used for permanentretention of restorations. Part I. Composition and manipulation. J Mich Dent Assoc 56(April):116.Eames WB, Hendri K, Mohler HC (1979). Pulpal response in rhesus monkeys tocementation agents and cleaners. J Am Dent Assoc 98:40.Eames WB, ONeal SJ, Miller CB (1974). Cementation variables in the seating ofcastings. Microfilmed Paper No. 545. Delivered at the Annual Meeting of the
International Association for Dental Research, Dental Materials Group, Atlanta, GA,21-24 Mar.Eames WB, ONeal SJ, Monteiro J, et al (1978). Techniques to improve the seating ofcastings. J Am Dent Assoc 96:432.Forss H (1993). Release of fluoride and other elements from light-cured glassionomers in neutral and acidic conditions. J Dent Res 72:1257-1262.Friedl KH, Schmalz G, Hiller KA, Shams M (1997). Resin-modified glass ionomercements: fluoride release and influence on Streptococcus mutans growth. Eur J OralSci 105:81-85.Glenn JF (1982). Composition and properties of unfilled and composite resinrestorative materials. In: Smith DC, Williams DF (eds). Biocompatibility of DentalMaterials, vol 3. Boca Raton, FL: CRC Press, 97-130.Grieve AR (1969). A study of dental cements. Br Dent J 127:405-410.Grieve AR, Jones JC (1981). Marginal leakage associated with four inlay cementingmaterials. Br Dent J 151:331.Griffith JR, Cannon RWS (1974). Cementationmaterials and techniques. Aust JDent 19(2):92-99.Grobler SR, Rossouw RJ, Van Wyk Kotze TJ (1998). A comparison of fluoriderelease from various dental materials. J Dent 26: 259-265.Hatton PV, Brook JM (1993). Characterization of the ultrastructure of glass ionomer(poly-alkenoate) cement. Br Dent J 173:275-277.Hembree JH Jr, George TA, Hembree ME (1978). Film thickness of cements beneathcomplete crowns. J Prosthet Dent 39:533.Hilton TJ (1996). Cavity sealers, liners, and bases: current philosophies andindications for use. Oper Dent 21:134.Hoard RJ, Caputo AA, Contino RM, et al (1978). Intracoronal pressure during crowncementation. J Prosthet Dent 40:520.Hood JA, Childs WA, Evans DF (1981). Bond strengths of glass ionomer andpolycarboxylate cements to dentin. N Z Dent J 77:141.Jarzynka W (1978). Effect of fluorine contained in the phosphate cement "Fluostable"on tooth pulp. Czas Stomatol 31:1003.Jendresen MD (1973). New dental cements and fixed prosthodontics. J Prosthet Dent30:684.Johnson GH, Herbert AJ, Powers JM (1983). Properties of glass ionomer luting
cements. Microfilmed Paper No. 189. Delivered at the Annual Meeting of theAmerican Association for Dental Research, Dental Materials Group, Cincinnati, OH,17-20 Mar.Kent BE, Wilson AD (1973). The properties of a glass ionomer cement. Br Dent J135:322.Kidd EAM, McLean JW (1979). The cavity sealing ability of cemented cast goldrestorations. Br Dent J 147:39.Kohmura TT, Ida KA (1979). A new type of hydraulic cement. J Dent Res 58:1461.Markowitz K, et al (1992). Biologic properties of eugenol and zinc oxide-eugenol: aclinically-oriented review. Oral Surg Oral Med Oral Pathol 73:729-737.McCabe JF (1998). Resin-modified glass-ionomers. Biomaterials 19:521-527.McComb D (1982). Retention of castings with glass ionomer cement. J Prosthet Dent48:285.McLean JW (1992). The clinical use of glass ionomer cements. Dent Clin North Am36:693-711.Meyer JM, Cattani-Lorente MA, Dupuis V (1998). Compomers: between glass-ionomer cements and composites. Biomaterials 19:529-539.Miller RA, Bussell NE, Richetts CK, et al (1979). Analysis of purification of eugenol.J Dent Res 58:1394.Mitchem JC, Gronas DG (1978). Clinical evaluation of cement solubility. J ProsthetDent 40:453.Mitchem JC, Gronas DG (1981). Continued evaluation of the clinical solubility ofluting cements. J Prosthet Dent 45:289.Mount GO, Makinson OF (1978). Clinical characteristics of a glass ionomer cement.Br Dent J 145:67.Myers CL, Drake JT, Brantley WA (1978). A comparison of properties of zincphosphate cements mixed on room temperature and frozen slabs. J Prosthet Dent40:409.Nicholson JW (1998). Chemistry of glass-ionomer cements: a review. Biomaterials19:485-494.Norman RD, Swartz ML, Phillips RW, et al (1969). A comparison of the intraoraldisintegration of three dental cements. J Am Dent Assoc 78:777.Oilo G (1978). Adhesive bonding of dental luting cements: influence of surfacetreatments. Acta Odontol Scand 36:263.
Oilo G (1978). Extent of slits at the interface between luting cements and enamel,dentin and alloy. Acta Odontol Scand 36:257.Oilo G, Espevik S (1978). Stress/strain behavior of some dental luting cements. ActaOdontol Scand 36:45.Pameijer GH, Segal E, Richardson J (1981). Pulpal response to a glass ionomercement in primates. J Prosthet Dent 46:36.Peacocke LE, Jones DW, Sutow E, et al (1979). Direct tensile strength of glassionomer, polycarboxylate and phosphate cements. Microfilmed Paper No. 1212.Delivered at the Annual Meeting of the International Association for Dental Research,Dental Materials Group, New Orleans, LA, 29 Mar- 1 Apr.Peterson WG, Joos RW, Boyer LV, et al (1978). Initial response of Ca(OH)2 bases insimulated oral conditions. Microfilmed Paper No. 210. Delivered at the AnnualMeeting of the International Association for Dental Research, Dental MaterialsGroup, Washington, DC, 16-19 Mar.Powers JM, Dennison JD (1974). A review of dental cements used for permanentretention of restorations. Part II. Properties and criteria for selection. J Mich DentAssoc 56(7-8):218-225.Reisbick MH (1981). Working qualities of glass ionomer cements. J Prosthet Dent46:525.Rueggeberg FA, Caughman WF (1993). The influence of light exposure onpolymerization of dual-cure resin cements. Oper Dent 18:48-55.Silvey RG, Myers GE (1978). Clinical studies of dental cements. VII. A study ofbridge retainers luted with three different cements. J Dent Res 57:703.Smith DC (1971). Dental cements. Dent Clin North Am 15:3.Smith DC (1974). A review of the zinc polycarboxylate cements. J Can Dent Assoc37:22.Smith DC (1977). Past, present and future of dental cements. In: Craig RG (ed).Dental Materials Review, Ann Arbor: University of Michigan Press, 52-77.Smith DC (1980). Glass ionomer contents. In: Kawahara H (ed). Implantology andBiomaterials in Stomatology. Tokyo: Ishikayn Publisher, 26-54.Smith DC (1982). Composition and characteristics of dental cements. In: Smith DC,Williams DF (eds). Biocompatibility of Dental Materials, vol 2. Boca Raton, FL:CRC Press, 143-199.Smith DC (1983). Dental cements. Current status and future prospects. Dent ClinNorth Am 27:763-792.
Smith DC (1988). Dental cements. Adv Dent Res 2:131-141.Smith DC (1991). Dental cements. Curr Opin Dent 1:228-234.Suljak JP, Hatibovic-Kofman S (1996). A fluoride release-adsorption-release systemapplied to fluoride-releasing restorative materials. Quintessence Int 27:635-638.Uno S, Finger WJ, Fritz U (1996). Long term mechanical characteristics of resin-modified glass ionomer restorative materials. Dent Mater 12:64-69.Vougiouklakis G, Smith DC (1982). The bonding of cervical restorative materials todentin. J Oral Rehabil 9:231.White S, Yu Z (1993). Compressive and diametral tensile strengths of currentadhesive luting agents. J Prosthet Dent 69:568-572.White S, Yu Z (1993). Physical properties of fixed prosthodontic resin compositeluting agents. Int J Prosthodont 6:384-389.White SN, Yu Z, Kipmio V (1992). Effect of seating force on film thickness of newadhesive luting agents. J Prosthet Dent 68:476-481.Wilder AD, Boghosian AA, Bayne SC, et al (1998). Effect of powder/liquid ratio onthe clinical and laboratory performance of resin-modified glass-ionomers. J Dent26:369-377.Williams JA, Billington RW, Pearson GJ (1993). The comparative strengths ofcommercial glass-ionomer cements with and without metal additions. Br Dent J172:279-282.Wilson AD (1978). The chemistry of dental cements. Chem Soc Rev 7:265.Wilson AD (1990). Resin-modified glass-ionomer cements. Int J Prosthodont 3:425.Wilson AD, McLean JW (1988). Glass Ionomer Cements. Chicago: Quintessence.Wilson AD, Paddon JM, Crisp S (1979). The hydration of dental cements. J Dent Res58:1065.Wilson AD, Prosser HJ (1982). Alumino silicate dental cements. In: Smith DC,Williams DF (eds). Biocompatibility of Dental Materials, vol 3. Boca Raton, FL:CRC Press, 42-77.
Chapter 10. Abrasion, Polishing, and BleachingIntroductionSurface finish and appearance are important aspects of restorative dentistry. Thesurfaces of normal, healthy-looking teeth have a high gloss and an unstainedwhite/ivory color. Abrasion is a process of surface roughening that can either wearaway tooth structure destructively or be used to correct tooth shape or attain anoptimal smooth finish on the surface of a restoration. Polishing and bleaching are twodifferent approaches to whitening teeth by attacking surface stains. Polishing is anabrasive process of smoothing a rough surface and removing stains with very fineparticles. Bleaching lightens or eliminates surface stains chemically by application ofstrong peroxide solutions. This chapter deals with the basic processes of thesetechniques.AbrasionIntroductionAbrasion is the process of wear on the surface of one material by another material byscratching, gouging, chiseling, tumbling, or other mechanical means. The materialthat causes the wear is called an abrasive; the material being abraded is called thesubstrate.Grinding is the gross reduction of the surface of a substrate by the process ofabrasion; it is usually performed with large-particle-size abrasives. The surfacetexture of the substrate after a grinding procedure is usually rough to the touch andgives a diffuse reflection to incident light (Fig 10-1(b)).Many abrasives used in dentistry are particles that are bonded to a mandrel or disk foruse in a rotary handpiece. Some abrasives are used as powders (or pastes) to beapplied to the substrate using a cloth wheel, brush, or cup. The basic principlesdescribed in this chapter apply whether an abrasive is used in a bonded form or apowdered form.Fig 10-1 Schematic diagram of diffuse and specular reflection: (a) high gloss; (b) low
gloss. (From OBrien et al, 1984. Reprinted with permission.)Factors affecting rate of abrasion1. A large difference in hardness between the abrasive and substrate (eg, toothenamel, amalgam) allows the most efficient grinding to take place. Brinell and Knoophardness values are functions of a materials resistance to indentation, whereas Mohsvalues indicate one materials resistance to scratching by another (Table 10-1). Table 10-1 Hardness of dental abrasives and substrates Hardness scaleMaterial Mohs Brinell KnoopAbrasivesTalc 1Gypsum 2Chalk 3Rouge 5-6Pumice 6 450 560Tripoli 6-7Garnet 6.5-7 550Tin oxide 6-7Sand 7 650 800Cuttle 7 650 800Tool steel 800Zirconium silicate 7-7.5Tungsten carbide 9 1,200 2,100Aluminum oxide 9 1,700 1,900Silicon carbide 9-10 3,000 2,500Boron carbide 9-10 2,800Diamond 10 >3,000 7,000SubstratesAcrylic 2-3 25Pure gold 2.5-3 30Hard gold alloys 3-4Amalgam 4-5 90Dentin 3-4Enamel 5-6 270Glass 5-6Resin composite 5-7 200Porcelain 6-7 400
2. The particle size of an abrasive may be expressed in micrometers. By convention,particles are classified as fine (0 to 10 um), medium (10 to 100 um), and coarse (100to 500 um), according to the average particle size of the sample. Larger abrasiveparticles will abrade a surface more rapidly than will smaller particles; however, theytend to leave coarser scratches in the abraded surface than do fine particles.Equivalent-sized scratches can be produced by different sizes of particles by varyingthe applied pressure (Fig 10-2(a)).Fig 10-2 Factors affecting abrasion. (a) Large particle produces similar scratcheswith lower applied force (F1) than smaller particle with greater applied force (F2). (b)Sharp particle produces deeper abrasion than rounder particle under equal appliedforce. (c) Deeper and wider scratches are produced by increasing the applied forcefrom F1 to F2.3. The particle shape also has an effect on rate of abrasion. Sharp, irregularly shapedparticles will abrade a surface more rapidly than will more rounded particles havingduller cutting angles. Also, the former will produce deeper scratches than the latter(Fig 10-2(b)). The abrasion rate of an abrasive decreases during use; this is due partlyto rounding of the particles and partly to contamination of the abrasive with some ofthe substrate material (debris).
4. The greater the speed at which the abrasive travels across the surface of thesubstrate, the greater the rate of abrasion. The greater friction at higher speeds,however, tends to create higher temperatures at the surface of the substrate.5. The greater the pressure applied, the more rapid will be the abrasion for a givenabrasive. Greater pressure produces deeper and wider scratches (Fig 10-2(c)) andcreates higher temperatures (and patient discomfort).6. Lubricants (eg, silicone grease, water spray, glycerol) are used during abrasion fortwo purposes: to reduce heat buildup and to wash away debris to prevent clogging, orblinding, of the abrasive instrument. Too much lubrication can reduce the abrasionrate because it may prevent some of the abrasive from coming in contact with thesubstrate.Applications of abrasivesDental prophylaxis pastesProphylaxis pastes should be chosen carefully and applied to remove exogenousstains without damaging the underlying tooth structure or adjacent restorativematerials. The abrasive selected should be harder than the surface stain beingremoved and softer than the tooth surface, although this is not always practicable. Ifthe tooth structure is excessively roughened during the procedure, it should bepolished with a fine abrasive (such as zirconium silicate); otherwise, plaque and foodsubstances will easily adhere to it.The most common abrasives used in prophylaxis pastes are pumice, silica, zirconiumsilicate, and other silicates. They are usually supplied in various particle sizes (coarse,medium, fine), which produce different rates of abrasion and sizes of scratches.Sodium fluoride or stannous fluoride are incorporated into some prophylaxis pastes tohelp prevent dental caries.DentifricesDentifrice pastes are used for removing debris and minor stains from teeth and forpolishing tooth surfaces. The most commonly used abrasives are dibasic calciumphosphate dihydrate, anhydrous dibasic calcium phosphate, tricalcium phosphate,calcium pyrophospate, and hydrated alumina.Many dentifrices contain therapeutic agents, such as sodium fluoride, stannousfluoride, or sodium monofluorophosphate, to decrease the acid solubility of toothenamel, decrease hypersensitivity, and interrupt the mechanisms of plaque attachmentand calculus formation on tooth structure. Dentifrice pastes additionally may contain ahumectant to reduce evaporation of water, a surface-active detergent, binders,flavoring and sweetening agents, and a preservative.Abrasive values for dentifrice products have been reported as an abrasivity index(AI), which is a measure of the abrasion of dentin.
In selecting a dentifrice for a patient, the following factors should be considered:degree of staining, toothbrushing habits (force, stiffness of brush, method ofbrushing), presence of relatively soft restorative materials (eg, acrylic resin veneers,silicates), and the amount of exposed cementum and dentin.Denture cleanersFood debris, plaque, calculus, and stains may accumulate on denture base materials inthe same way as natural teeth and are best removed on a regular basis by the patient.Daily soaking in a denture cleanser solution or brushing with or without a paste orpowder is usually effective.Chemical cleansers may contain sodium perborate, which releases peroxide. Asperoxide decomposes, oxygen is released, resulting in effervescence. Effervescence,along with the oxidizing ability of peroxide, are assumed to be responsible for thecleaning action.Dentures may also be soaked in a dilute solution of 5% sodium hypochlorite (1:3water). Other chemical denture cleansers may contain dilute acids or enzymes.Dentures should not be soaked in hot water, which may warp the denture basematerial.Brushing may be needed to remove stains and stubborn deposits. Hard-bristle brushesor brushing with much force may abrade the plastic surface of the denture and shouldbe avoided. Dentifrices are generally too abrasive for use with dentures, althoughsome with gentle abrasives (sodium bicarbonate or acrylic resin) can be used. Organicsolvents should be avoided, as they may cause crazing and eventual cracking of thedenture material. Ultrasonic vibration has not been shown to adequately removeplaque from dentures.Handpiece instrumentsHandpiece instruments include stones, burs, rubber wheels, and disks. Bondedabrasives are available for dental use in various shapes, abrasive sizes, andhardnesses:1. Dental stones are composed of abrasive particles that have been sintered togetheror bonded with an organic resin to form a cohesive mass. These stones are available infine, medium, and coarse grades. The color of the stone is an indication of theparticular abrasive used; green stones contain silicon carbide, and white stonescontain aluminum oxide. Diamond stones generally have a higher cutting efficiencythan silicon carbide or aluminum oxide.2. Dental excavating burs have a cutting action on tooth structure that is similar togrinding and polishing. Low-speed burs are composed of either carbon tool steel ortungsten carbide. High-speed burs are almost exclusively composed of the hardertungsten carbide. Burs with eight blades can be used for gross reduction of toothstructure and removal of old restorations, and they produce a rather rough surfacetexture on the substrate. Burs with 12, 20, or 40 blades can be used for producing a
smooth surface on tooth structure and restorations. Of significance is the relativehardness values of the burs and the substrates (see Table 10-1). Hard restorativematerials (such as quartz-filled composite restorative materials and dental porcelain)will rapidly dull the sharp cutting edges of the high-speed tungsten carbide burs.Cutting efficiency and durability of the burs varies greatly among manufacturers anddesign types. Crosscut fissure burs have higher cutting efficiency than plain fissureburs, but they produce a rougher surface.3. Rubber wheels are used for fine grinding of restorative materials (removing coarsescratches from rough grinding). They are made by molding fine abrasives (such asaluminum oxide, silicon carbide, and chromium oxide) in an elastomeric matrix.4. Disks and strips are made by bonding abrasive particles onto a thin plastic backing.They generally wear out rapidly due to the loss of abrasive particles. They areparticularly useful in finishing relatively flat surfaces. Abrasives commonly used ondisks and strips are garnet, emery, aluminum oxide, and quartz (cuttle).PolishingIntroductionPolishing is the process of making a rough surface smooth to the touch and glossy(mostly specular reflection of incident light) (see Fig 10-1(a)). Polishing is usuallyperformed with very-small-particle-size (submicron-size) abrasives.To produce a smooth, lustrous surface by abrasion, successively smaller abrasivesizes must be used. Larger abrasive particles remove large amounts of material fromthe substrate, and smaller particles smooth out the roughness produced by the largerparticles. Final polishing of a surface with a very fine abrasive produces a virtuallyscratch-free surface by creating a thin microcrystalline or amorphous layer on thesurface of the substrate.It is extremely important to remove all debris and abrasive particles from the surfaceof the substrate before using a finer abrasive during the polishing sequence. Even asingle abrasive particle left on the substrate from a previous step will continue toscratch the surface during the subsequent polishing steps.Appearance and texture of polished surfacesA polished surface is important for esthetic and functional reasons. If the scratchesproduced by the abrasives are greater in width than the wavelength of visible light (ie,approximately 0.5 um), the surface will appear to have a dull finish. If the scratchesare less than about 0.5 um in width, the surface will appear shiny. In addition, it hasbeen found that the tongue can distinguish subtle differences in roughness; scratchesmore than 20 um deep feel rough, whereas those less than 2 um deep feel smooth.Techniques for polishing restorative materialsDental amalgam
A polished surface is desirable on dental amalgam to retard the collection of plaqueand help retard tarnish as well. Burnishing alone does not create as smooth a surfaceas does polishing. Although an amalgam restoration can be burnished immediatelyafter carving, most brands should be left undisturbed for at least 24 hours beforepolishing to allow the amalgam to set completely. Polishing can then be performedwith a rotary instrument (cup, brush, or felt) with a fine abrasive mixed with water oralcohol in a slurry or paste; flour of pumice (ground volcanic glass), extra-fine silex(various silicates, such as quartz or tripoli), or tin oxide may also be used for thispurpose. Care must be taken to use sufficient water or alcohol to avoid frictionalheating of the restoration, which could cause pulpal damage.Fast-setting high-copper amalgams may be successfully polished 10 to 12 minutesfollowing placement.Gold alloysGold alloys are finished by using coarse, medium, and fine abrasives in sequence.Coarse scratches are removed with fine pumice or coarse abrasive rubber wheels; thesurface is finished with a rubber wheel impregnated with a fine abrasive and finallypolished with tripoli and rouge on rag wheels. Particular care must be taken to avoidoverfinishing of contours and margins.Acrylic resin denture bases and veneersGypsum material left on the denture base following processing and deflasking may beremoved with a "shell blaster." Small blemishes and bumps on the resin surface maybe scraped off or removed with an acrylic finishing bur. Denture base material iscomparatively soft and can be finished easily with a rag wheel and fine pumicefollowed by tripoli or tin oxide. Care must be taken not to alter the contour of thedenture during finishing. Acrylic denture teeth are particularly easily abraded bypumice.Resin composite restorationsResin composite restorations present a unique polishing problem because they arecomposed of a relatively soft polymeric resin and a hard filler. Relief polishing mayresult due to unequal wear rates of the resin and filler, leaving "valleys" between thefiller particles (Fig 10-3).Fig 10-3 Uneven wear of composite surface produces valleys in the resin matrixbetween the hard filler particles.
This is particularly apparent in large-particle (conventional type) resin composites,which still look and feel rough after finishing with available dental abrasives (Fig 10-4).Fig 10-4 Scanning electron micrograph of a composite restorative material withconventional filler, finished with a 12-fluted bur. (From OBrien et al, 1984. Reprintedwith permission.)Although relief polishing still takes place during the finishing of microfilled resincomposites, the valleys and filler particles are so small that the surface appears glossy(large specular component of reflection) and feels smooth (Fig 10-5). The new typesof hybrid and small-particle resin composites also tend to appear shiny and smoothbut cannot be polished as easily as the microfilled resin composites.
Fig 10-5 Scanning electron micrograph of a composite restorative material withsmaller filler particles in the micron range, finished with the rubber-abrasivecomposite resin wheel. (From OBrien et al, 1984. Reprinted with permission.)A typical sequence for polishing resin composites would be as follows: coarsegrinding with a diamond stone or a green stone followed by a series of coarse to finequartz or aluminum oxide abrasive disks or rubber wheels. Carbide burs with 12 ormore blades have also been used to polish resin composites. Finishing instruments forresin composites are available commercially. The effects of several polishingsequences on the surface roughness of resin composites are shown in Fig 10-6, whichare tracings from the surface analyzer shown in Fig 10-7.
Fig 10-6 Roughness profiles of conventional resin composite surfaces finished with:(1) green to white stone; (2) silicon carbide disks; (3) 12-fluted bur; (4) 40-fluted bur;(5) green to white stone to alumina paste; and (6) diamond stone. For scale: A = 50um; B = 2 um. (From Tolley et al, 1978. Reprinted with permission.)
Fig 10-7 Surface analyzer using a diamond stylus to produce roughness profiles (Surfanalyzer, Gould). Porcelain The best way to obtain a smooth, glossy surface on dental porcelain is by glazing in a porcelain oven. After minor adjustments of the surface of a porcelain restoration, the porcelain can be polished using a series of coarse to fine abrasive rubber wheels (containing silicon carbide or aluminum oxide), followed by a fine-particle-size diamond paste applied on a felt wheel. Bleaching Bleaching has been used to whiten teeth since the 1800s, but with the introduction of home bleaching systems in 1989, its use has widened. Three types of bleaching treatments are currently used (Table 10-2). Table 10-2 Tooth bleaching options Home bleaching Dentist-assisted Power or bleaching combination bleachingPatient Anyone with mild Anyone with mild to Anyone with mild to selection discolorations desiring acute discolorations severe discolorations teeth a shade or two desiring a more desiring an whiter and willing to dramatic whitening immediate result. devote time to an at- effect. home regimen.Materials used Carbamide peroxide Carbamide peroxide Hydrogen peroxide (CP) (10%-22%) or (34%-44%). (30%-50%). whitening gels containing no peroxide.Location At home, 2-4 hours per Dental office. Dental office. day.
Technique A custom-fitted tray is CP is applied in a The solution is applied made in a dental office. customized tothe teeth by a The correct strength of whitening tray and dental professional solution and the tray placed in the and activated with a are taken home with the patients mouth for at special light or heat patient, who least 30 minutes per source. administers the treatment. treatment and returns Additional periodically for follow- applications are sent up. home with the patient.Outcome Takes about 3-4 weeks Some results are seen In most cases dramatic for measurable results within 30 minutes of results are seen to be seen. treatment. immediately.Average Once per day for 2-3 Can be used as a One visit. An at-home number of hours for 4-6 weeks. "jump-start" for regimen may be treatments daily home suggested depending treatments. on the stains being treated. The first is home treatment, which involves the patient using carbamide peroxide materials in a custom-fitted tray overnight or for a few hours a day. Home bleaching kits are available for daytime or nighttime use (Fig 10-8). The other two types are performed in the dental office. One method involves application of carbamide peroxide for about 30 minutes, while the other, power bleaching, employs a 30% to 50% hydrogen peroxide solution further activated by a strong light or heat. Dental office treatments may also involve microabrasion to remove superficial staining from enamel with hydrochloric acid and a fine abrasive. Fig 10-8 Home bleaching kit for nighttime use.
The results of bleaching last about a year. Deep, dark stains are better handled withporcelain veneers. Side effects of bleaching include tooth hypersensitivity, soft tissuelesions, and sore throat and nausea from swallowing the bleach. Due to the possibilityof tooth hypersensitivity, anesthesia should not be used during treatment, whichwould mask irritation of the pulp. About three office appointments are usuallyrequired for dark stains. Considerable care is needed to protect the patients eyes andto discontinue the treatment if painful. Although bleaching can be effective, manypatients have an unrealistic view of the natural color of teeth and undergo unnecessarytreatment.Glossaryabrasion The mechanical process of wear of the surface of one material by another.abrasive The material that causes the wear of another material.abrasivity index (AI) A method of rating the abrasiveness of dentifrices.amorphous Without crystalline structure; having random arrangement of atoms inspace.blinding Clogging of an abrasive wheel with debris, causing reduction of abrasiveaction.dental stones Grinding instruments composed of abrasive particles bound in a hardresin matrix or sintered together into a hard mass.disks Grinding and polishing rotary instruments composed of abrasive particlescemented to a flexible plastic backing.microcrystalline Composed of tiny (submicron) crystals.polishing The process of making a rough surface smooth and glossy.rubber wheels Grinding and polishing instruments composed of abrasive particles ina flexible rubber matrix.strips Instruments for grinding and polishing interproximal areas; composed ofabrasive particles cemented to a flexible plastic backing.substrate The material being abraded.whitening Removal of surface discoloration by polishing or bleaching.Discussion Questions
1. Since many esthetic porcelain restorations are given a final thin layer of stain glazefor color matching, how could a dentifrice cause an undesirable change in color?2. How could polishing teeth reduce the need for bleaching?3. Why is trying to obtain snow-white teeth by bleaching unrealistic?4. What are the dangers of bleaching teeth, and what are the current regulationsregarding the use of these products?Study Questions(See Appendix E for answers.)1. What is an abrasive?2. Which factors affect the rate of abrasion?3. Place the following in order of hardness: cuttle, rouge, silicon carbide, chalk, sand,diamond, aluminum oxide, and pumice.4. Rouge is used to polish gold alloys. What effect do you think it would have ondental porcelain?5. Why is it important to obtain polished surfaces on dentition?6. During grinding and polishing, what would be the effect if coarse abrasive particlesfrom a previous step were present during the final polishing step? How can this beavoided?7. How sensitive is the tongue to scratches?8. What are some common abrasives found in (a) prophylaxis pastes; (b) dentifrices;and (c) stones, rubber wheels, and disks?9. Which criteria would you use in selecting a dentifrice for a patient?10. When should you polish an amalgam restoration? Which materials would youuse?11. Why are composite restorations difficult to polish? When would a rough surfaceon a composite restoration be desirable?12. What evidence is provided regarding the performance of the large number ofbleaching products?Recommended ReadingAmerican Dental Association (1983). Dentists Desk Reference: Materials,
Instruments and Equipment, ed 2. Chicago: ADA.Ashmore H, et al (1972). The measurement in vitro of dentine abrasion by toothpaste.Br Dent J 133:60.Buehler Analyst (1975). Sections 4 and 5. Evanston: Buchler, 111.Council on Dental Therapeutics: Guidelines for the acceptance of peroxide-containingoral hygiene products (1994). J Am Dent Assoc 125:1140.Gerdin PO (1971). Studies in dentifrices. IV. Size and shape of particles incommercial dentifrices. Svensk Tandlak T 64(7):447-461.Grabenstetter RJ, et al (1958). The measurement of the abrasion of human teeth bydentifrice abrasives: a test utilizing radioactive teeth. J Dent Res 37:1060-1069.Haywood VB, et al (1994). Effectiveness, side effects and long-term status ofnightguard vital bleaching. J Am Dent Assoc 125:1219.Hefferen JJ, et al (1970). Abrasivity of dentifrice products. J Am Dent Assoc 81:1177.Norton FH (1974). Elements of Ceramics, ed 2. Reading, MA: Addison-Wesley, 260-268.OBrien WJ, et al (1984). The surface roughness and gloss of composites. J Dent Res63(5):685-688.Phillips RW (1973). Skinners Science of Dental Materials, ed 7. Philadelphia: WBSaunders, 623-640.Powers JM, Roberts JC, Craig RG (1976). Wear of filled and unfilled dentalrestorative resins. Wear 39:117-122.Reder BS, Eames WB (1976). The cutting rates and durability of diamond stones[abstract 499]. J Dent Res 55(B):186.Stookey GK, Muhler JC (1968). Laboratory studies concerning the enamel and dentinabrasion properties of common dentifrice polishing agents. J Dent Res 47(4):524-532.Tolley LG, OBrien WJ, Dennison JB (1978). Surface finish of dental compositerestorative materials. J Biomed Mater Res 12:233-240.Whitehurst JF, Stookey GK, Muhler JC (1968). Studies concerning the cleaning,polishing, and therapeutic properties of commercial prophylactic pastes. J Oral ThermPharm 4(3):181-191.
Chapter 11. Structure and Properties of Metals and AlloysIntroductionA wide variety of metals is used in dentistry, as indicated in Table 11-1. Each has amelting or solidification temperature that is characteristic of that element. Whenelements are alloyed together to change their properties, this single meltingtemperature is changed to a range of temperatures over which the liquid is inequilibrium with solid crystals nucleated in the liquid metal. Table 11-1 Metallic elements used in dentistryElement Unit cell Melting temperature (C)Mercury Rhombohedral -39Gallium Orthorhombic 30Indium Tetragonal 156Tin Face-centered cubic 419Aluminum Face-centered cubic 660Silver Face-centered cubic 960Gold Face-centered cubic 1,063Copper Face-centered cubic 1,083Manganese Cubic 1,244Beryllium Hexagonal close pack 1,284Nickel Face-centered cubic 1,452Cobalt Body-centered cubic 1,493Iron Body-centered cubic 1,535Palladium Face-centered cubic 1,552Titanium Hexagonal close pack 1,668Platinum Face-centered cubic 1,769Chromium Body-centered cubic 1,875Molybdenum Body-centered cubic 2,610The upper temperature for the liquid-solid alloy range is called the liquidustemperature, and the lower temperature limit is called the solidus temperature. When aliquid alloy melt is being cooled, the liquidus temperature is the temperature at whichsolid crystals start to nucleate. When a mixture of an alloy liquid and crystals is beingheated, the liquidus temperature is the temperature at which the crystals dissolve intoliquid. The solidus temperature is the temperature at which the last liquid solidifies oncooling or the first liquid is formed on heating.Complete melting is needed for casting and soldering and at least an additional 100Csuperheat is needed for a fluid melt to cast. Note that a gas/air torch cannot be used tocast a metal with a liquidus temperature above 1,000C because the flame does notget hot enough. Also, a reducing flame rich in gas should be used for casting or
soldering, otherwise the liquid metal will be oxidized by the oxygen in air. Oxidationkeeps the solder from wetting the surface and flowing. To provide a margin of safetyagainst melting the castings in a fixed partial denture, the liquidus temperature of thesolder should be at least 50C lower than the solidus temperature of the casting alloybeing soldered.Unit Cells of Crystal LatticesLiquid metals nucleate crystals upon cooling (Fig 11-1). The atoms joining thecrystals form a unique packing arrangement in space that is characteristic of thatmetal or alloy at equilibrium. The smallest division of the crystalline metal thatdefines the unique packing is called the unit cell. When the unit cell is repeated inspace, the repeating atomic positions form the crystal lattice structure of a crystallinesolid (Fig 11-2). The atoms at the corners of the unit cell are shared among theadjacent eight unit cells, as shown for the body-centered unit cell. Therefore, oneeighth of the corner atom is associated with the cell; there are eight corner atoms, sothey each contribute one atom to the unit cell. The body-centered atom is totallyinside the unit cell and is not shared, so it contributes the second atom to the unit cellmass. Using the lattice parameters to calculate the volume of the cubic cell, thedensity of the metal can be calculated by dividing the mass of atoms in the unit cell byits volume. The lattice parameters for metals and alloys range between 2 A and 10 Afor the different unit cells formed.Fig 11-1 Formation of crystal nuclei in liquid metal. = atoms in liquid state; =atoms in solid state.
Fig 11-2 (a) The body-centered cubic unit cell is typical of the crystal lattice of pureiron at room temperature. The lattice parameter for iron is 2.87 A. (b) A part of abody-centered cubic crystal lattice. It could extend in all directions. In this "hardsphere model," the atoms are visualized as hard spheres of a definite radius in contact.(c) The body-centered cubic space lattice can be visualized as a "point skeleton" ofthe body-centered cubic crystal lattice.It has been observed that the position of the neighboring atoms surrounding everyatom of a crystal lattice is identical in a pure crystalline metal. When the property ofidentical periodic points in space was explored mathematically, it was discovered thatthere are 14 unique ways to arrange points in space (Fig 11-3).
Fig 11-3 Unit cells of the 14 space lattice contain atoms arranged so that each one hasidentical surroundings. (From Mott, 1967. Reprinted from Scientific American.) These are called space lattices. A pure metal crystal lattice is similar to one of thespace lattices except that each mathematical point is the site of an atom. Complexcrystal lattices like amalgam alloy and enamel have the points of their space latticesreplaced by the different atoms of the material or by groups of atoms. The unit cell ofeach crystalline material, no matter how complex, corresponds with one of these 14space lattice unit cells (see Table 11-1).
Nucleation and Polycrystalline Grain StructureIntroductionAs the melt of metal is cooled, clusters of atoms come together from the liquid toform solid crystal nuclei. These nuclei will be stable and grow into crystallites orgrains if the energy of the system is favorable, that is, the energy is lowered by theprocess. The energy is lowered by an atom bonding to the solid nuclei, thereby givingup its liquid-state kinetic energy of motion. However, when an atom bonds to thenuclei, the energy can also be raised by the creation of more interfacial surface energyas a result of the increased surface area of the nuclei in contact with the liquid. Theenergy of the system is favorable for stable nuclei and growth when more energy islost by bonding than is gained by increasing the interfacial surface area (ie, energy).Nucleation can occur by two processes. The first, called homogeneous nucleation, isenhanced by rapid cooling so the nuclei are supercooled. The result for the system isthat more energy is lost when an atom of the liquid bonds to the solid. With rapidcooling (quenching in water) more nuclei are formed per unit volume. These nucleigrow together to form the irregular polycrystalline grains or crystallites that fittogether like a three-dimensional puzzle to form the bulk of the metal shape (Figs 11-4 and 11-5).Fig 11-4 Irregular polygons called grains or crystallites. An average distancemeasured across the faces of the crystal grains is called the grain size. It may be lessthan 1,000 A or more than 1 cm, depending on the number of nuclei present duringsolidification. (From Guy et al, 1971. Reprinted with permission.)
Fig 11-5 The grain structure of a metal is revealed by polishing the surface to a mirrorfinish and etching lightly in acid. To study the grain structure of metals used fordental appliances, a light or scanning electron microscope is needed for magnificationbecause of the small grain sizes. (From Guy et al, 1971. Reprinted with permission.) The more nuclei that are formed by rapid cooling, the smaller the grain size orcrystallite dimensions. Another means of decreasing the grain size (grain refining) isby adding to the melt a foreign solid particle or surface to which the atoms areattracted, such as a very fine high-melting metal or oxide powder. This process ofseeding the nuclei is called heterogeneous nucleation.Grain size and propertiesDecreasing the grain size can have a number of beneficial effects on the cast alloystructure of a crown or removable partial denture. The finer grain size can raise theyield stress, increase the ductility (percent elongation), and raise the ultimatestrength. The change in these properties with grain size is related to the processes ofplastic deformation and fracture, and to how the boundaries between grains relate tothese processes. The size of metal grains in different metals may range from less than1,000 A to more than 1 cm. Grains contain large numbers of unit cellseven grainsof only 1,000 A across. The lattices of the grains are formed in random directionswhen they grow from the melt. A boundary is formed where the grains grow intocontact, because the atoms in one grains crystal lattice are not in position to meshwith the repeating atoms in the crystal lattices of adjacent grains. These grainboundaries are layers several atoms thick that are distorted from normal atomicpositions in order to bridge the mismatch in the lattice orientations of adjacent grains.Only metals with simple body-centered or face-centered cubic unit cells have enoughdensely packed planes of atoms in their lattices to allow plastic deformation at yieldstress. These lattice types permit shearing of the densely packed planes of atoms likecards of a microscopic deck sliding over each other. However, the lattice of adjacent
grain can be viewed as a second microscopic card deck at a different angle. To get themetal to deform, it is necessary to force the cards of one deck into other decks at anangle. But the more grains per unit volume, the more difficult it is to get the planes(cards) to slide because the dislocated slipping planes run against the grain boundariessooner. Thus, a greater resistance to slippage is created by more grain boundaries, andhigher yield stress results.On the other hand, a material will fracture because a crack opens up on a grainboundary. This is more likely to occur in large-grain metals, when the planes cannotbe slipped into the adjacent grains. Many smaller grains in various orientations candivide the plastic strain among the grains more easily, with more of them oriented forslipping. Large grains must each accommodate a larger strain and will have fewerproperly oriented to slip. The result is lower ductility and lower ultimate strength forlarge-grain metals, which open cracks more readily at grain boundaries because theplastic deformation cannot be accommodated. For these reasons, grain-refined or"micrograin" alloys produced by heterogeneous nucleation are advantageous fordeveloping fixed partial denture alloys with higher yield stress, better ductility, andimproved ultimate strength.Alloy SystemsMost pure metals are miscible in the liquid state when melted together. When twometals form a solution in the liquid state so their atoms mix randomly on the atomicscale, they are said to form an alloy. As the alloy liquid freezes, the atoms mayremain randomly distributed on the unit-cell lattice sites in each crystal grain. Thisrandom distribution in the solid alloy is called a solid solution. But, if like atoms tendto prefer to bond among themselves, then as the nuclei form from the melt, the atomsof different elements may segregate in different grains. The grains of the two differentmetal elements are mixed together.Different grains may be practically pure if their elements are insoluble in each otherslattices in the solid state. Or they can have a limited solubility in the others crystallattice if the elements exhibit partial solubility in one another. Metal atoms of twodifferent metal elements are more likely to be soluble in each others lattices if they(1) have the same atomic lattice type, (2) have similar atomic radii (ie, a difference ofless than 10%), (3) have the same valence number, and (4) form bonds to other atomswith strengths similar to those they form among themselves. On the other hand, ifthese rules are not followed and the unlike atoms have a strong affinity to each other,grains of an intermetallic compound may be formed at definite ratios of the alloyingelements (eg, dental amalgam alloy Ag3Sn).The energetically stable (ie, at equilibrium) crystal lattice structures and theircompositions for an alloy that is preferred by "nature" varies with temperature andratio of the alloying elements that are melted together. It is not possible to calculatethe equilibrium composition and structures and at what temperatures these change.They must be determined experimentally by measuring the temperatures at which thelatent heat is liberated when alloy liquid solidifies or solid lattices transform todifferent crystal lattices. The type of crystal lattice is determined by x-ray diffractionfrom the crystal atomic planes. The angle and intensity of the x-ray beam reflections(ie, diffraction) are characteristic of the atomic composition, type of crystal lattice,
and position of atoms in their unit cell. Thus, experimental detection of thetemperature when heat is liberated indicates when an alloy is changing its structure,and x-ray scattering identifies what lattices are present. This information is portrayedin a binary phase diagram of the alloy system (Figs 11-6 and 11-7). The alloysystem represents all possible ratios of the elements.Fig 11-6 Copper-gold phase diagram. The disordered solid solution (softer) andordered solid solutions (harder) are produced by heat treatment. FCC = face-centeredcubic.When two elements are alloyed, the system is called a binary alloy; when threeelements are alloyed, the system is a ternary alloy, and so on. An alloy is named bylisting its elements in descending order of percent composition. For example, Ag3Snis called silver-tin alloy. If more than two elements are involved, the number of phasechanges and their representation becomes complex, but their description follows thesame principle.
Fig 11-7 Silver-copper phase diagram showing a eutectic (lowest melting) point at28.1% copper.An equilibrium phase is defined as a homogeneous body of matter that is physicallydistinct and mechanically distinguishable. For a pure material like water, the vapor,liquid, and solid phases are physically distinct because there is a definite boundarybetween the regions when they exist together. Also, they are mechanicallydistinguishable in properties like hardness, compressibility, and elastic modulus.However, when the phase definition is applied to an alloy system, it is important torecognize that if two different types of unit cells nucleate from the meltas, forexample, at the eutectic (lowest melting) point in Fig 11-7a two-phase region isformed. The two phases nucleate as separate grains. They are physically distinct, asindicated by grain boundaries that define their limits. Their mechanical propertiesdiffer, as can be measured by a microhardness tester impinging on individual grains.Note that two-phase alloys are not as corrosion resistant as like single-phase alloys,because microscopic galvanic corrosion cells are set up between the grains of thedifferent phases. Also, porcelain bonding to multiphase alloys is consideredpotentially weaker because of composition differences of the grains.Deformation in MetalsThere are three types of deformation that can occur in metals, which arise fromdifferent mechanisms. The simplest deformation, elastic strain, is the elastic stretchingof lattice in which all the atoms are shifted from their equilibrium positions by afraction of their atomic spacing. The strain is directly proportional to the appliedstress (ie, force/area or force intensity) up to the proportional limit stress. When thestress is removed, the atoms return to equilibrium atomic spacing. Compared withmost polymeric materials, metals generally have strong metallic bonds and resist
elastic stretching. This stiffness or resistance to elastic strain is indicated by the highelastic modulus of metals. Stiffness is desirable for removable partial dentures, soforces can be transmitted by the framework across an arch to better distribute the load.It is desirable for the alloy of resin-bonded fixed partial dentures to resist flexing ofthe bond.Another type of deformation is plastic deformation, a permanent deformation thatbegins when the elastic limit stress or its approximation, yield stress, is reached. Thismode of deformation requires that atoms be shifted to new atomic sites on the lattice.These lattice sites must be identical to the old sites and not far away, so the energy toshift atoms is not too great. Thus, ductility is associated with face-centered and body-centered cubic metal lattices, which have more identical sites and more closelypacked planes, so atoms do not have to slide far to reach the new lattice sites.Intermetallic compounds are usually brittle because the atomic sites are specific to thedifferent atoms of the compound and not interchangeable.The mechanism of plastic deformation is called dislocation motion and produces theslipping of the closely packed planes over each other. A dislocation (Fig 11-8a, Dx) isthe line of atoms that denotes the edge of an additional half-plane of atoms thatappears to be wedged into the lattice. The lattice is distorted (strained) by the presenceof the dislocation line of atoms.Fig 11-8a The distortion (strain) around a dislocation in a simple cubic crystal lattice.The size of the atoms has been reduced so the perspective can be seen. The row ofatoms of the dislocation is Dx. (From Ziman, 1967. Reprinted from ScientificAmerican.)Dislocation motion shifts atoms from one lattice site to the next, rather than movingall the atoms of the plane at one time, which would take much more energy (Fig 11-8b).
Fig 11-8b The crystal lattice as it would appear after the yield stress has beenexceeded and the dislocation has moved through the lattice. The solid has beendeformed to this new shape. (From Ziman, 1967. Reprinted from ScientificAmerican.)It is important to understand that any process that impedes dislocation movementtends to harden a metal, raise its yield stress and often lower its ductility. Someprocesses are reversible, allowing the hardness to be low when making an appliance,for example, after which the metal can be hardened to provide better service ifnecessary.One process for hardening metal is called cold working, or work hardeninganyplastic deformation of metal by hammering, drawing, cold forging, cold rolling, orbending. These processes produce many dislocations in the metal that cannot slipthrough each other as easily as the lattice becomes more distorted. The yield stresscan be raised more than 100% when a drawn orthodontic wire is compared to the as-cast metal. In dentistry, cold working occurs when gold foil is compacted, a dentureclasp is bent, an inlay margin is burnished, or a deformed metal layer forms on acrown during finishing and polishing.A second process for hardening a metal is precipitation hardening. In this process asecond phase of finely dispersed clusters of atoms are precipitated from a metastablesupersaturated solid solution by reheating an alloy that was quench-cooled to form themetastable supersaturated solid.Heat treatment can also be used to harden gold-copper alloys by a slightly differentprocess. In this case, because the gold-copper system forms a complete solid solutionat all compositions, the atoms can be interchanged on the lattice sites. However, as theatoms are cooled, the copper and gold atoms tend to separate on alternating planes ofthe lattice in ordered arrangement. This ordering makes dislocation motion moredifficult, raising the yield stress. These alloys are soft if quenched but hard if cooled
slowly on the bench top or held in the furnace at the ordering temperature range(350C for 30 minutes).Other heat treatments are used to homogenize the grains of an alloy that havedeveloped composition gradients by rapid cooling and crystallization of the melt.When cooled rapidly, the grains of the alloy cannot maintain an equilibrium oruniform composition in the grain. The first part of the grain to cool will be richer thanthe average composition of the higher-melting-temperature element, and the last partof the grain to solidify is richer in the low-melting alloy component. Thisinhomogeneity tends to reduce corrosion resistance of the metal because of thegalvanic cell created between the center of the grain and the grain boundary. Heatingthe solid at a temperature and for a duration that allows the atoms to reach equilibriumwill improve corrosion resistance.Diffusion in MetalsAtoms of a crystalline solid vibrate about their fixed lattice positions. As they absorbheat with increasing temperature, they vibrate at greater amplitude. Also, a smallfraction of the atom sites are vacant in a metal. As the temperature increases, an atommay momentarily experience an increase in vibrational energy, which will besufficient to permit it to jump from one lattice site to another. As the temperature andtime increase, more atoms will be able to jump or diffuse to new lattice sites. Thisrandom jumping during heat treatment allows the rearrangement of the crystal lattice.Atomic diffusion also permits rearrangement of cold-worked metals and permanentdeformation of metals at stress levels far below the yield stress if the stress lasts longenough. In general, these rearrangements by diffusion begin to occur at a significantrate as the temperature of metal exceeds one half of its absolute melting temperature.The rate of rearrangement accelerates rapidly as the metal or alloy approaches itssolidus temperature.There are several heat treatment processes for metals that utilize diffusion. Amongthem is an annealing heat treatment for release of residual stress. It allows thedislocations and atomic vacancies to move and realign to lower the internal residualstress fields in a cold-worked metal at a relatively low temperature and short heatingtime.If the temperature and heating times are extended for a cold-worked metal, the metalcan experience recrystallization, in which stress-free grains are crystallized out of thedeformed grains. A recrystallization temperature is the temperature at which it wouldtake 1 hour for the cold-worked metal to recrystallize. This temperature is betweenone third and one half of the absolute melting temperature for most metals (Fig 11-9).As the temperature and time are further extended, grain growth occurs, during whichthe stress-free grains grow larger at the expense of the disappearing small grains.
Fig 11-9 A microscopic view of the stages that a cold-worked metal, such as anorthodontic wire, goes through when subjected to prolonged heating. The higher thetemperature and the greater the cold working, the more quickly the transitions occur.This figure shows recrystallization being completed in 1 hour, which means thetemperature of heating was the recrystallization temperature as per the definition. Thechanges in properties can be compared with the structural changes. (From Jastrzebski,1959. Reprinted with permission.)The residual stress heat treatment relaxes the internal stress, which may causewarpage over time. The chance of corrosion related to residual stress differences onthe metal surface are reduced. Recrystallization heat treatment lowers the yield stressand increases the ductility. Grain growth further reduces yield stress and increasesductility yield stress. When soldering a cold-worked wire in which a high yield stressis desired (eg, a partial denture wire clasp or an orthodontic appliance), a low-meltingsolder and a short soldering time are desirable to minimize recrystallization and graingrowth.Glossaryalloy An atomic mixture of metallic elements.annealing A relatively low-temperature heat treatment for removing residual stress.binary alloy An alloy composed of two elements.
binary phase diagram A map with temperature and composition as coordinates,which displays the regions where each stable phase exists.cold working (work hardening) Deforming a metal at temperatures that are lowcompared with its melting temperature.crystal A solid with periodic arrangement of atoms in space, usually with atomicplanes forming facets on the surface.crystal lattice The periodic arrangement of atoms in three-dimensional space.crystallite A crystal with irregularly shaped surfaces instead of facets.crystallization The process of crystal and crystallite formation.deformation The process of changing the shape of a metal by applied stresses.dislocation A row of atoms displaced from their normal positions in the lattice.dislocation motion The movement of a dislocation through a crystal under an appliedstress.eutectic alloy An alloy, easily melted with respect to its component elements, that cantransform at one temperature from liquid to two phases separated as distinct grains inthe solid metal.eutectic composition The alloy composition at which the eutectic transformationoccurs.eutectic temperature The temperature at which the eutectic transformation occurs.grain Another name for crystallite.grain boundary The interface or junction of adjacent grains.grain growth Enlargement of grains by heating.hardening A process in which the yield stress and resistance to indentation areincreased.homogeneous Having uniform composition throughout.intermetallic compound An alloy phase with a composition usually near a definitefixed atomic ratio of the elements.lattice parameters The distances between corners of the unit cell.nuclei The embryos of the crystallites formed from the liquid.
phase A homogeneous body of matter that is physically distinct and mechanicallydistinguishable.polycrystalline Composed of many crystallites.recrystallization The process of forming new crystallites from existing crystallites byheating.residual stress Internal stress remaining between parts of a solid after the appliedstress is removed.solid solution An alloy phase in which one alloying element enters the lattice of theother.space lattice A pattern of points in space that satisfies the condition that each point issurrounded by the same arrangement of points.ternary alloy An alloy composed of three elements.ultimate strength The maximum stress a solid can suppo